IBFPR 11/22/2000 4:04 PM Page i
Impact behaviour of fibre-reinforced composite materials and structures
IBFPR 11/22/...

Author:
S. R. Reid

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

IBFPR 11/22/2000 4:04 PM Page i

Impact behaviour of fibre-reinforced composite materials and structures

IBFPR 11/22/2000 4:04 PM Page ii

IBFPR 11/22/2000 4:04 PM Page iii

Impact behaviour of fibre-reinforced composite materials and structures Edited by S R Reid and G Zhou

Cambridge England

IBFPR 11/22/2000 4:04 PM Page iv

Published by Woodhead Publishing Limited, Abington Hall, Abington, Cambridge CB1 6AH, England www.woodhead-publishing.com Published in North and South America by CRC Press LLC, 2000 Corporate Blvd, NW Boca Raton FL 33431, USA First published 2000, Woodhead Publishing Ltd and CRC Press LLC © 2000, Woodhead Publishing Ltd The authors have asserted their moral rights. This book contains information obtained from authentic and highly regarded sources. Reprinted material is quoted with permission, and sources are indicated. Reasonable efforts have been made to publish reliable data and information, but the authors and the publishers cannot assume responsibility for the validity of all materials. Neither the authors nor the publishers, nor anyone else associated with this publication, shall be liable for any loss, damage or liability directly or indirectly caused or alleged to be caused by this book. Neither this book nor any part may be reproduced or transmitted in any form or by any means, electronic or mechanical, including photocopying, microfilming and recording, or by any information storage or retrieval system, without permission in writing from the publishers. The consent of Woodhead Publishing and CRC Press does not extend to copying for general distribution, for promotion, for creating new works, or for resale. Specific permission must be obtained in writing from Woodhead Publishing or CRC Press for such copying. Trademark notice: Product or corporate names may be trademarks or registered trademarks, and are used only for identification and explanation, without intent to infringe. British Library Cataloguing in Publication Data A catalogue record for this book is available from the British Library. Library of Congress Cataloging in Publication Data A catalog record for this book is available from the Library of Congress. Woodhead Publishing ISBN 1 85573 423 0 CRC Press ISBN 0-8493-0847-X CRC Press order number: WP0847 Cover design by The ColourStudio Typeset by Best-set Typesetter Ltd., Hong Kong Printed by TJ International, Cornwall, England

IBFPR 11/22/2000 4:04 PM Page v

Contents

1

Preface

ix

List of contributors

xii

An overview of the impact behaviour of fibrereinforced composites n l hancox

1

1.1 1.2 1.3 1.4 1.5 1.6 1.7 1.8 1.9

Introduction Composite materials Failure processes Measurement of impact strength Theoretical prediction of impact energy The effect of the matrix on fracture toughness Crush strength Summary Final reflection Acknowledgements References

1 2 6 9 19 24 26 27 28 29 29

2

Recent developments in impact damage assessment of fibre composites j-k kim

33

Introduction Destructive techniques Nondestructive techniques Concluding remarks Acknowledgements References

33 34 37 67 69 69

2.1 2.2 2.3 2.4

v

IBFPR 11/22/2000 4:04 PM Page vi

vi

Contents

3

Modelling impact of composite structures using small specimens c ruiz and j harding

75

3.1 3.2 3.3 3.4 3.5

Introduction Small specimen testing Structural analysis of impact Modelling of impact damage Conclusions References

75 76 91 99 102 103

4

Impact damage – tolerant composite structural design r l sierakowski

106

4.1 4.2 4.3 4.4 4.5 4.6 4.7

Introduction Damage tolerance Sources of damage Damage tolerant design Impact damage Impact damage tests Summary References

106 107 109 111 114 123 126 128

5

Damage resistance and tolerance of thick laminated woven roving GFRP plates subjected to low-velocity impact g zhou and l j greaves

133

5.1 5.2 5.3 5.4 5.5 5.6

Introduction Characterisation of composite materials Experimental procedures Impact damage resistance Impact damage tolerance and assessment Conclusions Acknowledgements References

133 135 136 143 160 180 183 183

6

Elastic impact stress analysis of composite plates and cylinders s r swanson

186

Introduction Impact regimes Analysis of impact

186 186 187

6.1 6.2 6.3

IBFPR 11/22/2000 4:04 PM Page vii

Contents

vii

6.4 6.5 6.6

The quasi-static approximation Issues of scaling in impact Summary and conclusions References

204 209 210 210

7

Impact behaviour and analysis of CFRP laminated plates e wu and c z tsai

212

7.1 7.2 7.3 7.4 7.5 7.6 7.7

Introduction Experimental set-up and procedure Near-elastic impact behaviour Prediction of elastic impact response Impact beyond the delamination threshold Impact beyond the ballistic limit Conclusions Acknowledgements References

212 214 217 221 228 232 233 236 236

8

Perforation of FRP laminates and sandwich panels subjected to missile impact s r reid and h m wen

239

8.1 8.2 8.3 8.4 8.5 8.6

Introduction Experimental procedure Experimental results Model development Comparisons and discussion Conclusions References

239 242 246 263 267 277 278

9

High-velocity impact damage to polymer matrix composites r c tennyson and c g lamontagne

280

Introduction Hypervelocity impact tests on composites Entry impact damage Secondary debris cloud Conclusions Acknowledgements References

280 285 286 289 295 298 298

Index

301

9.1 9.2 9.3 9.4 9.5

IBFPR 11/22/2000 4:04 PM Page viii

IBFPR 11/22/2000 4:04 PM Page ix

Preface

The last three decades have witnessed a steady increase in the use of lightweight polymeric composites for structural applications. In addition to their excellent quasi-static mechanical properties such as high specific stiffness and strength, it has become essential for these composite structures to perform well under various types of impact loading. For example, in the aerospace industry, the residual compressive strength of an impactdamaged composite structure has become the design-limiting factor. Major aspects of current damage-tolerant design philosophies in other industrial sectors are similar to that of the aerospace industry. Consequently, this book brings together nine chapters that deal with the various aspects of impact behaviour of fibre-reinforced composite materials and structures. Contributions are provided by some of the world’s leading experts in the field. It is hoped that the detailed presentation of a wide range of topics within a single volume will form a sound basis for further studies of impact behaviour and also serve as a useful reference source. The book has a broad scope and covers both experimental and analytical approaches to understanding the impact response of fibre-reinforced composites, and the effects of impact damage and failure under conditions ranging from low velocity to hypervelocity impact. It is intended to be useful not only to practising engineers, academics, researchers and designers in the field, but also to materials scientists, postgraduate research students, and manufacturers of composite materials and structures. Numerous references are given at the end of each chapter to enable the reader to explore the topics covered in greater detail. Impact problems concerning composite structures involve diverse disciplines, and require the combined skills of engineers, materials scientists and mathematicians. Thus, a degree of overlap between the sections of some chapters is unavoidable. Since the book focuses exclusively on the impact behaviour of continuous fibrereinforced composite materials and structures, the general subject of composite materials is not covered in depth. Also, short fibre-reinforced composite materials and structures are not considered. ix

IBFPR 11/22/2000 4:04 PM Page x

x

Preface

Chapter 1 presents an overview of impact performance of various notched composite beams, assessed by Charpy and Izod impact methods. Details of various experimental approaches are explained, and the ability of the composites to absorb impact energy is discussed together with the associated failure processes. The analytical predictions of the impact energy absorbed based on these methods is presented. Chapter 2 contains a summary of the various destructive and non-destructive techniques for detecting as well as quantitatively characterising impact damage. Particular emphasis is placed on the emerging variants of some well-established techniques such as X-radiography and ultrasonics where the three-dimensional distribution of damage is demonstrated. Some examples, illustrating the capacity as well as the effectiveness of certain selected techniques, are presented. Chapter 3 provides an in-depth examination of some of the experimental techniques that have been used to characterise several composites under various uniaxial states of stresses at high strain rates. It also deals with the low velocity impact responses of beam structures. Additionally, numerical modelling of impact damage is discussed, and some of the issues regarding both stress-based and fracture mechanics-based failure criteria are examined, along with the issue of scaling. Chapter 4 serves as an introduction to impact-damage tolerant composite structural design. The concepts as well as the key issues in damage tolerant design are examined. The sources and effects of damage are described. It also discusses damage tolerant design criteria. The development of analytical and FEM-based models for characterising both the impact event and damage tolerance, respectively, is presented. Chapter 5 is a comprehensive treatise on both impact damage resistance and damage tolerance assessment of thick glass fibre-reinforced laminates subjected to low velocity and high energy impact. In this chapter, impact response and dominant damage mechanisms occurring during impact are discussed from an experimental perspective and their energy-absorbing characteristics are described. Details of compression after impact tests are also presented. Considerable discussion is devoted to the advantages and disadvantages of both conventional and newly proposed damage tolerance assessment methods, which are illustrated with numerical examples. In Chapter 6, the elastic impact stress analyses of flat plates and cylinders, both made of carbon/epoxy, are provided. Comparisons are made between an analytical model and experimental data for low velocity impact response and this is supplemented with numerical examples. The justification for the quasi-static approximation of low-velocity impact responses is presented with examples. Geometric scaling issues are discussed. Chapter 7 examines the impact responses of and associated damage in graphite/epoxy plates under impact velocities ranging from very low to above the ballistic limit. Two major aspects are covered. One is concerned with obtaining experi-

IBFPR 11/22/2000 4:04 PM Page xi

Preface

xi

mentally the plate impact response histories generated by using a gas gun. The other is concerned with predicting analytically the plate impact responses under imperfect boundary conditions by using Mindlin plate theory. The correlation between the two is discussed with numerical examples. Chapter 8 presents a detailed study on the penetration and perforation of glass/polyester laminates and glass/polyester skinned sandwich panels with foam cores under impact velocities ranging from low to above the ballistic limit. The development of two semi-empirical models is discussed, and the nose-shape effects of both indentors and projectiles are examined. One model predicts penetration and perforation energies by using a dynamic enhancement factor. The other model is developed for high velocity impacts where inertia effects dominate. The correlation between the two is discussed with numerical examples. Extensive discussion of and comparisons with experimental data are provided. Chapter 9 deals with the damage analysis of both flat plates of varying thickness and cylinders, made of graphite/epoxy, graphite/PEEK and Kevlar/epoxy, under normal as well as oblique hypervelocity impacts. The damage caused by both the direct impact of projectiles and secondary debris clouds from perforated laminates is examined in detail. Considerable discussion is devoted to the correlation between impact energy and damage crater size. We wish to express our gratitude to all the contributing authors for their efforts and outstanding cooperation, and to Mrs Patricia Morrison of Woodhead Publishing Limited for her enthusiasm and patience throughout this project. Finally, we would like to thank our wives, Susan and Juan for their support and patience. SR Reid and G Zhou

IBFPR 11/22/2000 4:04 PM Page xii

List of contributors

Greaves L G Mechanical Sciences Sector, DERA, Famborough, Hants GU14 0LX, UK Hancox N L AEA Technology, Harwell, Oxfordshire OX1 0RA, UK Harding J Department of Engineering Sciences, University of Oxford, Oxford OX1 3PJ, UK Kim J-K Department of Mechanical Engineering, Hong Kong University of Science and Technology, Clear Water Bay, Kowloon, Hong Kong Lamontagne C G Institute of Aerospace Studies, University of Toronto, Ontario M3H 5T6, Canada Reid S R Department of Mechanical Engineering, UMIST, Manchester M60 1QD, UK Ruiz C Department of Engineering Sciences, University of Oxford, Oxford OX1 3PJ, UK Sierakowski R L Department of Civil Engineering, Ohio State University, Columbus, OH 43210, USA xii

IBFPR 11/22/2000 4:04 PM Page xiii

List of contributors

xiii

Swanson S R Department of Mechanical and Industrial Engineering, University of Utah, Salt Lake City, UT 84112, USA Tennyson R C Institute of Aerospace Studies, University of Toronto, Ontario M3H 5T6, Canada Tsai C Z Institute of Applied Mechanics, National Taiwan University, Taipei 106, Taiwan Wen H M Department of Mechanical Engineering, UMIST, Manchester M60 1QD, UK Wu E Institute of Applied Mechanics, National Taiwan University, Taipei 106, Taiwan Zhou G Department of Aeronautical and Automotive Engineering, Loughborough University, Leicestershire LE11 3TU, UK

IBFPR 11/22/2000 4:04 PM Page xiv

IBF1 11/22/2000 4:13 PM Page 1

1 An overview of the impact behaviour of fibre-reinforced composites N L HANCOX

1.1

Introduction

Impact may be defined as the relatively sudden application of an impulsive force, to a limited volume of material or part of a structure. The proviso is that relatively and limited are capable of an extraordinarily wide range of interpretations. The effects of impact are widely known and yet analysing the phenomenon and relating effects to the forces acting and the materials’ properties, in order to predict the outcome of a particular event, can be very difficult. The results of an impact can be largely elastic, with some energy dissipated as heat, sound, internally in the material, etc. Alternatively there may be deformation, permanent damage, complete penetration of the body struck or fragmentation of the impacting or impacted body, or both, as demonstrated in Chapters 5, 7, 8 and 9. For fibre composite materials it is permanent damage, possibly subsurface and barely visible, penetration and fragmentation, that are of interest. There are various ways of analysing the impact process; in terms of the energy deposited and gross damage produced, micro energy dissipation or by considering the stresses acting on flaws in the material and the effects that are generated. The latter method, which is known as fracture mechanics, is extensively employed with metals but will only be alluded to here. In practice the impact behaviour of composites merges into the general area of damage mechanics. Much of the early pioneering work on the properties of composites under impact is still relevant as the concepts employed in the analysis are the same though the results, depending specifically on the materials used (fibre, resin), interface and method of fabrication, may have been superseded. For this reason many of the earlier references concerning the impact behaviour of composite materials are employed here. This is not a detailed historical treatment and references are chosen for their appropriate nature rather than for being first (or last!) in the field. In this chapter it is intended to view impact in a general way. Later 1

IBF1 11/22/2000 4:13 PM Page 2

2

Impact behaviour of composite materials and structures

contributions will focus on specific situations in which the material and/or impact process is more closely defined. The general principles set out in Chapter 1 should, however, be applicable in all situations.

1.2

Composite materials

To discuss the impact behaviour of composites it is helpful initially to consider the nature of the materials. Modern polymer composites based on glass, carbon, aramid, ceramic or polymer fibres in a polymer matrix are heterogeneous and anisotropic materials. They have a low density, high strength and stiffness and hence excellent specific properties (the ratio of the property to the density or specific gravity) in the fibre direction. They can be relatively easily formed into components with complex shapes by vacuum pressure compaction or pressing at temperatures of no more than ~200°C for 1 h or more, though post curing may be needed. Because of the need to have long fibres for optimum properties and, in many cases, easier and effective processing, composite structures are often shells. They have excellent properties within the plane of the shell, in the fibre direction in tension, and to a lesser extent, in compression. The performance transversely, through the thickness and in shear and impact, is poorer. Generally, properties which are matrix dependent are much lower than those which are governed by the fibre. Nevertheless the role of the matrix is vital in composite behaviour; protecting the fibre, transferring stresses and, in some cases, alleviating brittle failure by providing alternative paths for crack growth.

1.2.1 Properties of fibres and resins Reinforcing fibres usually have a diameter of 5–10 mm, though it may be up to ~100 mm, for certain types (e.g. boron), and a modulus and strength of the order of 70–800 GPa and 1000–7000 MPa, respectively. The failure strain is ~0.27–5.0%. Carbon and aramid fibres may exhibit an increasing modulus with increasing strain due to changes in their internal structure during stressing. The resins, whether thermosets or thermoplastics, have a modulus and strength of the order of 2–5 GPa and 50–100 MPa, respectively, and a strain to failure of ~1% upwards. It should be noted that resin failure strain is usually well in excess of the minimum figure. Properties of resins are usually strain rate dependent and markedly influenced by temperature (see a fuller treatment in Chapter 3). This occurs because the glass transition temperature, Tg, which is indicative of the upper working temperature, is ~80–200°C for most resins. This is much closer to room temperature than is the case for the melting or degradation point of most structural

IBF1 11/22/2000 4:13 PM Page 3

Impact behaviour of fibre-reinforced composites

3

Table 1.1. Some fibre and resin properties Material

Density (Mgm-3)

Tensile modulus (GPa)

Tensile strength (MPa)

Strain to failure (%)

Glass fibre Carbon fibre Aramid fibre Inorganic fibre Phenolic resin Polyester resin Epoxy resin Bismaleimide resin

2.49–2.55 1.7–2.0 1.39–1.45 2.0–3.97 1.0–1.35 1.1–1.23 1.2–1.2 1.2–1.32

73–86 160–827 73–160 152–462 3.0–4.0 3.1–4.6 2.6–3.8 3.2–5.0

3400–4500 1400–7070 2400–3400 1720–3900 60–80 50–75 60–85 48–110

3.5–5.4 0.27–1.9 1.4–4.6 ~1.8 1.0–6.5 1.5–8.0 1.5–3.3

materials. Hence creep can be a problem with polymers at relatively low temperatures. Some fibre and resin properties are summarised in Table 1.1. It should be noted that these are indicative of the property range for the materials. Individual grades/types of material, the way the property is measured, etc., might cause variations outside the limits given.

1.2.2 Composite properties Table 1.2 lists some composite properties. These are again indicative of the performance of 60 v/o (fibre volume fraction), unidirectional fibre composites. Values will vary with the type of fibre (e.g. grade of carbon fibre), method of test, matrix and way the specimens were fabricated. The important points to appreciate are the very significant differences between longitudinal and transverse properties, the lesser difference between longitudinal tensile and compressive strengths and the disparity between the interlaminar shear strength (ILSS) and tensile/compressive strengths. Shear modulus is in the range 2.5–5.0 GPa for all of the materials. Longitudinal tensile and compressive strain to failure is essentially that of the fibre.Transversely the figure may be lower, ~0.3–0.5%, and is governed by the properties of the interface and resin matrix. Laminates, containing layers of fibres with different orientations within a plane, may have higher impact, shear and transverse properties, but lower longitudinal performance. Charpy impact energy for unnotched materials, stressed in the longitudinal or fibre direction, varies widely depending on the interface, matrix and experimental details. There may also be errors due to the scaling up of results for different cross section specimens. Charpy impact strength in the transverse direction (i.e. at right angles to the fibre) can be very low. It is common to use Gc, the critical strain energy release rate, as a measure

1.8–2.0 1.54–1.66 1.36–1.4

Glass Carbon Aramid

37–53 125–330 66–107

Elt (GPa) 9.0–13.6 5.9–10 4.1

Ett (GPa) 1.2–1.9 1.76–2.9 1.29–1.5

slt (GPa) 30–80 27

stt (MPa) 0.78–1.6 0.19–0.28

slc (GPa) 53–83 70–127 38–69

t (MPa) 125–3300 60–3300 1100

G1c (J m-2) 600–1200 154–2033

G2c (J m-2)

Up to 609 8–150 20–40

Imp st. l, (k Jm-2)

Up to 28 0.2–4.0

Imp st. t, (k Jm-2)

Where r is the density, Elt and Ett are the longitudinal tensile and transverse tensile moduli, respectively, slt, stt and slc are the longitudinal tensile, transverse tensile and longitudinal compressive strengths, respectively, t is the shear strength (also known as the interlaminar shear strength or ILSS), G1c and G2c are the critical works of fracture for the 1 and 2 deformation modes and Imp st. l, and Imp st. t, are the longitudinal and transverse Charpy impact strengths.

r (Mg m-3)

Material

4

Table 1.2. Some properties of unidirectional composite materials

IBF1 11/22/2000 4:13 PM Page 4

Impact behaviour of composite materials and structures

IBF1 11/22/2000 4:13 PM Page 5

Impact behaviour of fibre-reinforced composites

5

1.1 G1c. Crack propagation parallel to the fibres. The horizontal lines show the fibre direction.

of toughness, though some workers distinguish between initiation and propagation energies for this quantity. Often Gc is equated to 2g, where g is the work of fracture or the energy required to produce a new surface in a material. It is important to remember that both g and Gc refer to a specific mode of deformation (a tensile type opening for G1c) and that the direction of the fibres in relation to the sense of deformation must be clearly defined, see Fig. 1.1. In Table 1.2, G1c refers to the extension of a crack parallel to the fibre direction and is thus analogous to the transverse Charpy impact energy. G1c defined in this way is also known as the mode 1 interlaminar shear work of fracture. More information on fibre, resin and composite properties is available, for instance, as is a simple description of the various deformation modes associated with G1c, G2c and G3c.1 A general account of composites fracture mechanics and toughening mechanisms is given in Hancox and Mayer.2 More details and descriptions of the experimental difficulties of determining the critical strain energy release rates and the influence of materials’ and testing parameters on the results have been recorded.3 For metals, figures of 4–140 kJm-2 have been reported for the work of fracture, g.4 An advantage of composites, compared with more conventional materials, is the ability of the designer/fabricator to tailor mechanical and thermal properties over a wide range by suitable choice of fibre type, orientation, loading (within limits), and possibly the resin. It is possible to reduce in-plane anisotropy to give a quasi-isotropic material and improve shear and transverse (though not through-thickness) performance by laminating. However, the specific property in a given direction is reduced as

IBF1 11/22/2000 4:13 PM Page 6

6

Impact behaviour of composite materials and structures

more ‘redundant’ material has been added. Laminates, with successive layers orientated differently, are in some ways akin to plywood. Alternatively, a wide range of woven, knitted and needled fabrics, often based on glass or aramid fibres, is available for reinforcement. The first two types of fabric possess good reinforcement in more than one direction in a plane without the need for laminating. Disadvantages are that strength and stiffness properties are reduced because of out-of-plane deviations of the fibres due to the weaving process and lower fibre volume fraction, possibly fibre/fibre wear at cross over points and physical damage to the fibre occurring during needling. It has so far been implicit that long/continuous fibre tows are used in composite construction. Many products, especially those reinforced with glass fibre, employ short (sub-micron or mm), intermediate (cm) or randomly laid, continuous fibres in a plane, or combinations of these, for reinforcement. These materials, with thermoset or thermoplastic matrices and sometimes special additives to aid processing, are known as bulk or dough moulding compounds, injection moulding feedstock and stampable mat thermoplastics. Sheet moulding compound contains, in addition to chopped fibres, continuous or woven glass fabric. These types of composite are very widely used because of the relative ease with which they can be pressed, moulded or extruded into useful components. One difficulty arising in the discussion of the properties of composites relates, ironically, to one of the virtues of the materials – the ability of the user to tailor their properties to suit the design. There is a huge number of fibre lay-ups, fibre types, combinations and forms, resin matrices, additives and cure schedules to choose from and it can be very difficult to extrapolate from, or relate, the results for one unique combination to those of another. This has the effect of making quoted property measurements appear very diverse.

1.3

Failure processes

New situations and materials tend to be judged initially by comparison with existing ones. Since the principle class of construction materials used in high performance applications is metals, composites are usually compared with them. Generally, metals tend to be dense, stiff, strong, good conductors of heat and electricity, isotropic and inexpensive. In particular many show plastic behaviour before failure and it may be possible to remove the effects of deformation/damage by annealing and/or reworking the material. Unfortunately, at least on a significant scale, polymer matrix fibre composites do not exhibit this type of behaviour – elastic deformation is followed by irreversible damage and failure. Another important influence on composite

IBF1 11/22/2000 4:13 PM Page 7

Impact behaviour of fibre-reinforced composites

7

performance, especially in failure, is the heterogeneous nature of the material on a micro/meso scale. Composites are generally strong, and have a reasonable impact resistance, if the applied stress is in the fibre direction. In other directions they tend to be weak and to have a low impact resistance. Small secondary stresses in the transverse direction or unexpected stresses due to an impact, in a weak direction, can easily cause damage. Because of the ease with which localised permanent damage can be produced and the low values of g or G1c for failure parallel to the fibres, or between plies in a laminate, G1c is sometimes regarded as critical and the focus of most attention in impact work. Fracture mechanics methods of determining G1c are favoured over traditional measurements of impact strength, from which g and arguably G1c can be determined, because of their greater accuracy and virtual elimination of extraneous energy absorption. However, the assumptions implicit in fracture energy determinations may not be true for fibre composites, where crack propagation may be dominated by crack blunting, fibre pull-out and fibre/matrix delamination. It has been suggested that in such circumstances conventional fracture toughness may not necessarily be the best measure of overall toughness.5 Impact tests can be more useful, although not so readily analysed as fracture toughness measurements, and can be conducted at strain rates more representative of the deformation rates seen in service. The topic can be a contentious one of which the reader should be aware. There are five basic mechanical failure modes that can occur in a composite after initial elastic deformation. These are: • • • • •

Fibre failure, fracture, and, for aramids, defibrillation. Resin crazing, microcracking and gross fracture. Debonding between the fibre and matrix. Delamination of adjacent plies in a laminate. Fibre pull out from the matrix and stress relaxation.

In practice, debonding and delamination are not always distinguished. A very detailed list of types of damage in composites and associated references is given in Chapter 2. Behaviour is modified by external conditions. Polymeric fibres, which depend for their properties on molecular alignment, suffer a fall-off in performance above ~100°C, aramids degrade at elevated temperatures, carbon fibres, if unprotected from air, oxidise at 300–400°C and glass will soften at 500–800°C. The environment, particularly water, causes the plasticisation of thermosets, lowering the Tg and causing microcracking and debonding and possibly corrosive effects in stressed glass fibre composites. The interface, at which mechanical keying and chemical bonding are involved, is

IBF1 11/22/2000 4:13 PM Page 8

8

Impact behaviour of composite materials and structures

very sensitive to moisture. Sometimes the effects are reversible on drying out – sometimes they are not. All these factors are of relevance to impact performance because of their influence on composite mechanical properties.

1.3.1 Why are composites prone to impact damage? The lack of plastic deformation in composites means that once a certain stress level is exceeded permanent damage, resulting in local or structural weakening, occurs. Unlike a metal, which may undergo plastic deformation but can retain its integrity (e.g. water tightness), composites stressed above a certain level, though possibly retaining some structural properties, are permanently damaged. A blow with an energy of ~1 J or less at ~2 ms-1 can cause irreversible damage in a realistic composite laminate. To summarise, the reasons for a low impact strength are: • • •

Low transverse and interlaminar shear strength. Laminar construction, which is required if the reinforcing fibres are to be used efficiently and anisotropy reduced. No plastic deformation.

1.3.2 Estimation of the stresses acting in an impact It is informative to try to estimate the stress generated by an impact. The situation is very complex and our simple approach merely indicates the order of magnitude of the stress. Consider a steel ball of radius ~25 mm and mass 0.5 kg, with an energy of 1 J impacting a surface at a velocity, V, of 2 ms-1. The compression stress generated, sc, is, given by 0.5

s c = V (Ect r)

[1.1] 6

where Ect is the transverse compressive modulus and r the density. Typical values of these quantities are 10 GPa and 2 ¥ 103 kgm-3, respectively, giving sc = 9 MPa. In practice, compressive loading could cause localised bending and transverse failure in suitably oriented plies and generate interlaminar shear stresses. The compressive stress will continue to act until the impacting body rebounds. The stress wave will propagate into the impacted material, with a decreasing amplitude, and be reflected at the back surface as a tension wave. It is possible to apply the theory of Hertzian contact stresses6 to the estimation of the impact stress. This indicates that if the diameter of the contact area is 2 a the maximum shear stress appears below the point of contact at a depth of ~a/2. The maximum contact stress, q0, for indentation on a plane surface is

IBF1 11/22/2000 4:13 PM Page 9

Impact behaviour of fibre-reinforced composites q0 = 0.7aE R

9 [1.2]

This assumes a common Poisson’s ratio of 0.3 and that the controlling modulus is that of the composite through its thickness ~10 GPa. If a = 0.25 mm and R, the radius of the impactor, is 25 mm as before, the maximum compressive stress is found to be ~70 MPa and the maximum shear stress, ~0.31 q0, is 22 MPa. Both approaches neglect, among other points, the differences in the properties of the impacting and impacted bodies, geometrical effects and the heterogeneous, anisotropic nature of the composite. In addition, whether a static theory of contact stresses can be applied to an impact situation is open to debate. In view of all these factors the results are approximate but they do indicate the potential for damage.

1.4

Measurement of impact strength

1.4.1 Izod and Charpy methods The Izod and Charpy tests have been used for many years to assess the impact performance of metals particularly with respect to the brittle/ductile transition temperature and notch sensitivity.7,8 The Izod test is still widely used for polymers. In the Izod test a rectangular or square cross section bar of specified dimensions is clamped at one end and struck towards the top of the test piece with a pendulum. For the Charpy test a beam is rested freely against two anvils and struck in the centre by a pendulum. In the former case, if the specimen is notched, the notch is at the top of the clamped section and usually faces the direction of strike. Charpy specimens may be machined with U or V notches in the centre of the beam opposite the direction of strike, see Fig. 1.2. For metal specimens, dimensions are controlled as stated in the various national standards. In either test, and with any material, the impact energy may be overestimated because energy is: • •

Stored elastically in the specimen prior to failure. Energy is dissipated acoustically, thermally, in the kinetic energy of the failed parts, etc.

Despite the somewhat arbitrary nature of the tests, difficulties of crosscorrelating information and of scaling impact energies to bodies with different cross sections, they were readily adapted by the plastics industry and national standards established. The Izod impact testing of rigid plastics9 and the impact behaviour of plastics including the effects of flow direction in moulded specimens, notching, notch tip radius and notch depth and the relation of the impact energy to the stress concentration factor10 are both covered. Also dealt with very thoroughly are the Izod and Charpy impact

IBF1 11/22/2000 4:13 PM Page 10

10

Impact behaviour of composite materials and structures

Impact

Impact

1.2 Charpy test specimens with triangular and U-shaped notches. The arrow shows the direction of impact.

procedures for plastics.11 When carbon fibres were developed, and the potential of carbon fibre composites in aerospace was realised, these test methods, especially the Charpy, were adapted for composites, including glass and aramid fibre materials. If the striking arrangement in a Charpy test is such as to load the specimen in 4 rather than 3 point bending, see Fig. 1.3, the work of fracture is increased, presumably because of the different shear stress patterns in the two cases. Sometimes the Charpy test is viewed as an accelerated static test, but there is evidence that the energy stored to maximum load differs in the static and impact cases, with laminated specimens exhibiting a reduced modulus, and hence greater energy storage, in impact.12 A similar conclusion has been reached for sandwich panel specimens with composite skins. In this case quasi-static testing gave results 50–65% less than impact measurements.13 The physical cause is probably related to differences in the transverse shear behaviour at the different strain rates in the two cases. In parallel with the work on traditional impact tests the fracture mechanics approach was developed to describe composite fracture. This method is more complex theoretically and experimentally but arguably, for some materials, is more suitable for use in design.

IBF1 11/22/2000 4:13 PM Page 11

Impact behaviour of fibre-reinforced composites

11

Impact

Support

Impact

Support

1.3 Schematic diagram of Charpy specimens impacted in 3 and 4 point loading, respectively.

To some extent the effect of the notch is to reduce the sources of error due to stored energy. In this respect a chevron notch is often used in the Charpy test. This is formed by making two opposing cuts from the base of the specimen to the top, meeting at a point on the top surface. This leaves a triangular shaped cross section of material joining the two halves of the specimen, see Fig. 1.2. The argument is that if the specimen is struck at the back failure starts at the apex before significant energy storage due to bending occurs elsewhere in the specimen.Thus the recorded impact energy is more nearly the true value. Notches are also used to determine if the material is notch sensitive. If a scratch or surface flaw, acting as a stress raiser, severely reduces the impact strength of a component, because the stress concentration at the notch tip cannot be relieved, it is important to establish this prior to use. One method of expressing impact energy, for a plastic or a composite, is in terms of the formula U = E b(d - c )

[1.3]

where U is the impact energy, and E the energy registered in the test, for a specimen of breadth b, and depth d, containing a notch of depth c. This is a simple scaling formula. By adopting a fracture mechanics approach it can be shown2 that the fracture energy may be expressed thus: U = E fb( d - c)

[1.4]

IBF1 11/22/2000 4:14 PM Page 12

12

Impact behaviour of composite materials and structures Medium toughness

Force

Brittle

Ductile

Displacement

1.4 Idealised load displacement characteristics for brittle, medium toughness and ductile material. Note that the materials will differ in elastic properties – hence the different slopes. Real characteristics will be much less smooth.

where f is a calibration factor which depends on specimen and crack dimensions and compliance. In using either the Charpy or Izod test it is most important to specify the fibre direction in relation to the main stresses applied by the impact force. A trawl through the literature reveals that the Charpy test is much more widely used for composites than the Izod method. The variety of specimen shapes and notches is large – a typical specimen might be 6 ¥ 6 mm in cross section and 60 mm in length with a U, V or chevron notch, the former up to half the thickness of the specimen and for a V notch an angular opening of 30 or 45°. In another case the specimen was a laminate 2 mm thick, 13 mm wide, with a V notch on either side in the thickness. Pendulum strike velocities are typically ~2–4 ms-1 with energies, governed by the mass of the pendulum, of 0.4–15 J, and exceptionally up to 100 J. Some idealised load displacement traces, which could be obtained from machines with an instrumented striker head or tup, are shown in Fig. 1.4. Instrumenting the striker enables the force as a function of time into the impact, or displacement, to be obtained. The characteristics are for brittle, intermediate and tough materials, respectively. The difference in the areas under the curves in the three cases is obvious. Real traces tend to be a lot less clean because of ring in the system, possibly bouncing of the striker and repeated impact and complex material behaviour. A variety of impact tests using the DYNA3D FEA code were recently analysed and it was concluded that ringing or noise is due to local bending of plies around the tip of the impactor.14

IBF1 11/22/2000 4:14 PM Page 13

Impact behaviour of fibre-reinforced composites

13

By integrating the area under the load or force displacement curve, and noting the value up to the maximum load or the load at first failure, it is possible to deduce the energy required to start or initiate damage and relate it to the energy to propagate damage and the total energy involved, as indicated in Fig. 5.4 of Chapter 5 and Fig. 8.3 of Chapter 8. The ratio of the propagation energy, Ep, to the initiation energy, Ei, is known as the ductility index, D.15 D = E p Ei

[1.5]

Values range from zero upwards. The zero value indicates that, in this type of test, the material is behaving in a completely brittle manner. The larger D, the more energy is used in propagating failure compared with that to cause initiation. Note that a high index does not imply a material with high absolute toughness. What is required in practice is a large initiation energy and a large propagation energy. The reader should be aware that some authors define D as the ratio of propagation to total energy, Et. An analogous situation arises with G1c measurements where there is a relatively low initiation energy followed possibly by a higher propagation value. Some typical figures for G1c, for unidirectional sized and untreated glass fibre epoxy composites, are given by Krawczak and Pabiot.16 For crack initiation in the sized material the figure is 87 Jm-2 and 438 Jm-2 for propagation. For unsized fibre the figures are 224 and 185 Jm-2, respectively, indicating that in this case once a crack is initiated it propagates more easily.

1.4.2 Other methods of determining impact energy An increasingly popular method of assessing impact energy is the falling dart test,17 which was originally developed for rigid plastics. The standard covers both instrumented and uninstrumented testing procedures. The test piece, either 60 mm in diameter or 60 ¥ 60 mm square, and 1–4 mm thick, is supported on a hollow steel cylinder with an inside diameter of 40 mm. It may be clamped in position. The steel striker has a polished hemispherical head, either 10 or 20 mm in diameter, and is allowed to fall from a height of up to 2 m onto the specimen (equivalent to a maximum velocity of 6.3 ms-1). For a puncture test on a composite, a strike velocity of 4.4 ms-1 and a total striker mass of 5–20 kg (equivalent to energies of 48–193 J) are preferred. Many variants of the dropped weight test are described in the literature, with specimens ranging in size from 127 ¥ 127 mm square to 100 mm in diameter, and impactors with tip radii of 5–12.7 mm. Other variants are noted in Chapters 5 and 8. The impact velocity can be varied, within reason, to suit a particular requirement. Details of the impact testing of skinned sandwich panels, sometimes using specially shaped impactors, are

IBF1 11/22/2000 4:14 PM Page 14

14

Impact behaviour of composite materials and structures

1.5 C-scan of a laminated carbon fibre composite panel impacted at 50 ms-1 with a 6 mm diameter indenter. Note damage development along a diagonal.

given in Hildebrand.13 It was noted that pyramidal and hemispherical indenters gave different results and it was concluded that these different test methods are not even qualitatively comparable. Another way of assessing the impact energy in a Charpy, or falling weight, test is to repeatedly impact the same specimen, until failure occurs, under conditions which do not cause immediate failure, or to increase the impact energy on each successive blow until failure occurs. While this may be acceptable for ranking materials or designs, the build up of damage, which is not quantified before failure, makes the absolute interpretation of the results uncertain. To increase the impact velocity it is necessary to fire the projectile at the specimen. This may involve a conventional bullet, an anti-tank shell, a small ball ~1–40 g in weight fired by a gas gun, a soft projectile,18 or a liquid drop.19,20 See Chapters 7–9 for further details. The impact velocity can range from 20–100 ms-1 to 6000 ms-1 plus. Under certain conditions the projectile may penetrate the specimen cleanly or it may cause overall flexing, fibre break out at the back surface or considerable delamination. The latter can be assessed ultrasonically. In laminated specimens the damage pattern may show greater development in certain directions corresponding to less favourably oriented plies, see Fig. 1.5. One problem is having a specimen which is sufficiently large that the damage does not interact with the boundaries. One study of soft body impact involved firing a 3 g gelatine pellet at 90–190 ms-1 at a carbon thermoplastic matrix target. The damage was assessed by measuring the extent of delamination ultrasonically. The

IBF1 11/22/2000 4:14 PM Page 15

Impact behaviour of fibre-reinforced composites

15

damage was similar in form to that due to an aluminium projectile, though less extensive. The erosion, or impact damage of composites by repeated liquid impact, has been studied at velocities of 90 ms-1 upwards. A liquid or a soft body behaving compressibly exerts a pressure of rcV on the surface it strikes, where r is the density, V the impact velocity and c the stress wave velocity in the liquid. Liquid flowing outwards from under a curved surface causes considerable localised shear damage, particularly if the initial pressure has ruptured the surface. At high velocities, ~1000 ms-1, the compression wave generated by the liquid drop, on being reflected as a tension wave from the back surface of the specimen, causes scabbing, or the removal of material, if the transverse tensile strength is low. This has been observed in carbon fibre composite specimens. Fibres end-on to the direction of impact have an increased resistance to liquid erosion, probably due to the much better compressive properties of the fibre in the longitudinal, as compared with the transverse, direction. Practically, elastomer coatings (e.g. polyurethanes) are used to protect surfaces from liquid and solid particle erosion. In many of the cases involving high velocity impacts, with either hard or soft bodies, the experiment has been set up to test a special combination of projectile and material/design and the object is to determine the behaviour of the specimen rather than to derive a more fundamental impact energy; see Chapter 9. Three other areas of impact study involve: • • •

Barely visible impact damage (BVID). The measurement of a property after impact. The impacting of stressed bodies.

All are somewhat specialised and are related to damage tolerance, and the latter to the effects of superimposed stresses on impact behaviour. A general discussion of damage tolerant structural design is given in Chapter 4. BVID occurs when an object, such as a tool, is dropped accidentally onto a composite structure. For example, a thin shell-like, highly stressed aerospace component is particularly vulnerable in this respect. The danger is that the damage is so slight that it is not readily noticed by the naked eye but nevertheless compromises the load bearing capacity of the component. Apart from the obvious step of avoidance, possible solutions to this problem are the incorporation of sensitive sensors in the component and the use of damage tolerant matrices. An FEA analysis14 attributes back surface tensile damage in an impacted laminate, with little or no evidence of damage at the front, to localised bending in the vicinity of the impactor. If the back of the specimen is not visible this would be classified as a type of BVID. Since many crucial aerospace composite components are stressed in compression it is usually the compression strength that is evaluated after

IBF1 11/22/2000 4:14 PM Page 16

16

Impact behaviour of composite materials and structures

the impact. If the composite suffers debonding as a result of impact the compression strength will be affected because plies can act independently; limited microbuckling could occur on loading in compression and the strength would be reduced. Broken fibres would be an additional cause of a reduction in compression strength, possibly because of the complex stress field in the vicinity of the break. The compression strength after impact, CAI, is related to BVID, though the impact energies involved are probably greater than in the latter case. The approach to evaluating the damage is different, however. The crucial parameter is now how much a given energy or velocity impact reduces the strength of the material or component. Clearly the greater the strength retention, for given conditions, the better the material. As an illustration of the effect, a drop weight test with an impact energy of 30 J causes a reduction in the compressive stress of a laminate of ~30–40%.21 The authors developed a model based on the assumption that the change in compressive strength is related to the degradation of flexural stiffness in the impacted laminate. Fitting parameters are required and have to be determined experimentally but the model then gives a good fit to the data for the complete range of impact energies involved. Another, typical, account of the evaluation and analysis of the process for carbon fibre laminates is given in Ishai and Shragai.22 Generally the resulting degradation is influenced by clamping conditions and specimen geometry, since these can determine the nature of the damage produced under impact (e.g. shear delamination vs fibre failure). For similar studies see Chapter 5. The study of the impact of pre-stressed materials was initiated23 and more recently explored in a lengthy programme whose results have been summarised.24,25 The aim is to establish the combined effects of impact and a superimposed tensile or compressive stress. The combination is usually more damaging than either factor on its own. In the earlier work unidirectionally reinforced carbon and glass fibre specimens were stressed in tension up to 1.5–2.0 GPa and impacted with a wedge-shaped pendulum with a maximum energy of 4 J. The form of the results is shown in Fig. 1.6. The stress to cause failure, after impact in the unstressed state, falls linearly with increasing impact energy. This is equivalent to an ordinary notch sensitivity tensile test. Specimens stressed at the time of impact, however, require a lower stress to cause complete failure when tested to destruction after impact. It was noted that generally a high fibre strength and low fibre modulus lead to a higher impact performance. Later work investigated the effect of the wedge radius and role of delamination on the onset of failure – a low transverse strength could decrease the impact response. Rigidly supporting the back of the specimen caused different behaviour. Now the specimen could not bend when struck and no compressive fracture was

IBF1 11/22/2000 4:14 PM Page 17

17

0

Stress (GPa)

2

Impact behaviour of fibre-reinforced composites

0

Impact energy (J)

4

1.6 Effects of tensile prestress on impact energy. The upper line is for specimens impacted unstressed and then tested to failure in tension. The lower curve is for specimens impacted in the stressed state. In practice the prestress had to be adjusted to get impact on failure. The material was an intermediate modulus, unidirectional, carbon fibre/epoxy composite.

observed running in from the impacted face. There was also an optimum fibre volume loading ~67 v/o for maximum toughness. In the later work,24,25 carbon and glass fibre epoxy and thermoplastic laminates, prestrained in tension or compression up to 0.5%, were impacted at velocities ranging from a few meters per second up to 2.78 kms-1 using pendula, small projectiles and rifle bullets. The corresponding impact energies could be as high as 2.69 kJ. Damage was assessed visually and by using ultrasonic C scanning. Generally, impact with or without prestraining caused delamination, breakout of rear plies and sometimes complete penetration. The damage diameter, as determined by C scan, for different types of carbon fibre laminate as a function of prestrain, is shown in Fig. 1.7. Similar results were obtained with glass and aramid fibre panels. Compressive prestrain appeared more damaging than tensile prestrain, probably because the initial delamination allows the individual plies to buckle more easily under compression. Simultaneous strain and impact lowered the failure strain below that observed in the sequential case, see Fig. 1.8. Reasonable success was achieved in modelling the behaviour of cross ply laminates using the VEC-DYNA3D FEA code. It was possible to account for

C scan damage diameter (mm)

60

IBF1 11/22/2000 4:14 PM Page 18

More brittle resin

0

Less brittle resin –0.5

0

+0.5

Prestrain (%)

1.7 Delamination diameter, determined by C-scan, for carbon fibre composite laminated panels impacted at 50 ms-1 with a 6 mm diameter impacter at an energy of 1.1 J. Tensile prestrain has a minimal effect but compressive prestrain, combined with a more brittle epoxy resin leads to considerable damage.

Failure strain (%)

0.5

Woven

0

Unidirectional

0

0.25

0.5

Prestrain (%)

1.8 Effects of prestress on failure strain of a carbon fibre laminate. The figure shows the failure strain of the material impacted whilst prestrained and then, if required, strained to failure. The highest result is for a woven material. The impact velocity was 80 ms-1 and the impact energy 2.8 J.

IBF1 11/22/2000 4:14 PM Page 19

Impact behaviour of fibre-reinforced composites

19

penetration and the type and extent of damage. Overall it is important to use the correct boundary conditions. Potential failure mechanisms are complicated and interrelated and if one is not correctly assigned this may effect the predictions. Although much information on impact has been generated experimentally it is frequently very difficult to compare results because of differing specimen dimensions, boundary conditions, testing procedures, etc. The reader may be forgiven for thinking that the subject is poorly regulated and somewhat arbitrary. It has been suggested26 that specimen details seem to be resolved by a process of random choice. Certainly anyone perusing much of the literature on the impact properties of composites is struck by the way in which most papers approach the experimental side, appearing to use whatever materials and equipment are to hand rather than making a choice which fits in with other work. Having said that, the present author must confess to having tested specimens, 1 ¥ 1 m square ¥ 100 mm or more in thickness, by dropping steel cylinders, weighing up to 500 kg, onto the surface from a height of about a meter. The problem is that in many cases the modelling of the behaviour of a structure in an impact situation is so difficult that the best way to tackle the problem is to test the real structure in the most realistic way possible. No doubt as our knowledge and computational ability progress this will become less necessary but at present there is often nothing like a field trial.

1.5

Theoretical prediction of impact energy

Having discussed the methods for measuring impact energy and indicated the spread of results obtained it is necessary to develop a theoretical framework to describe the impact process. There are three approaches: • • •

Evaluate the bulk stored strain energy. Micromechanics – calculate the energy stored or dissipated in the fibre, resin and interface and in other failure processes. Linear elastic fracture mechanics (LEFM).

The first approach considers the elastically stored strain energy, while the second method covers dissipative processes. As was previously mentioned, because of energy storage in a specimen at the extremities, the first method will overestimate the energy required to create the two new surfaces resulting from the fracture of the specimen. LEFM is more mathematical and fibre composites do not always meet the assumptions made because of conditions at the crack tip leading to stress relief. While we shall mention fracture mechanics this approach will not be developed here.

IBF1 11/22/2000 4:14 PM Page 20

20

Impact behaviour of composite materials and structures

1.5.1 Strain energy If a body is stressed in tension, compression, flexure or shear, a simple strength of materials method27 can be used to calculate the stored strain energy. The area under a stress strain curve, up to the strain e, is equal to the energy, U, stored in the body, or e

U = Ú sde

[1.6]

0

If the material obeys Hooke’s law, s = Ee, the energy, per unit volume, is U = Ee 2 2 or s 2 2E

[1.7]

A similar expression applies for the energy in shear, per unit volume, viz.: U = t 2 2G

[1.8]

The following expressions for the strain energy in a rectangular beam of breadth, b, depth, d, and length, l, are useful: U t , U c = s lt2 bdl 2Elt , s lc2 bdl 2Elc (tension, compression)

[1.9]

U bc = 1 9 ¥ s bdl 2Elt (cantilever, beam 3 point loading)

[1.10]

U s = 4 15 ¥ t 2 bdl G (shear, 3 point loading)

[1.11]

2 lt

Note that in all of the formulae it is the maximum stress that is specified. A short span to depth ratio, Fmax > Fi F Fi

t Stage III-1: Fult = Fmax > Fi Fult F

t Stage III-2: Fult < Fmax F

t (a)

(b)

(c)

5.7 Three-stage damage sequence in thick laminate plates under lowvelocity impact described by (a) deformation sketches, (b) impact response curves and (c) C-scan graphs.

If a greater IKE was supplied, the top ply right underneath the impactor would be sheared through when the plate reached the maximum bending, as discussed earlier on the small plates and illustrated in Fig. 5.7. Because of this membrane stretching, the impacted large plates have shown much

IBF5 11/22/2000 4:54 PM Page 148

148

Impact behaviour of composite materials and structures

Table 5.2. Geometric effects on impact load-bearing capabilities of laminated composites Material

Laminate thickness (mm)

Impact force small plate (kN)

Impact force large plate (kN)

Percentage increase (%)

E-glass/polyester

10 25 150%

61 ± 1 124 ± 6 103%

92 144 57%

51 16

14 19 36%

117 ± 1 146 ± 2 25%

157 164 5%

34 12

Increased by S-glass/phenolic Increased by

greater load-bearing capability than the small plates as will be seen from Table 5.2. 5.4.1.2 Dominant damage mechanisms The use of the experimental techniques and processes described in Section 5.3.3 revealed that there were four types of damage mechanisms, on a macroscopic scale, operating during impact loading: matrix cracking, delamination, ply shear-out and fibre fracture. These failure modes would occur when stresses had exceeded the relevant strength values of the material. As these failure modes corresponded to strengths of very different magnitudes, they would be likely to occur sequentially and fibre breakage occurred only when a high IKE was provided. For example, matrix cracking usually took place first because its tensile strength in the region of 40– 90 MPa was the lowest and this was followed by delamination because of its low ILS strength, as shown in Fig. 5.4(b–c). Obviously, the damage mechanism such as matrix cracking dominated only at the lower end of the IKE spectrum. The other damage mechanisms were dominant at the central region and the upper end of the spectrum. Of course, the perforation of the laminate plates occurred at the upper end. In most of the impact and quasi-static tests, delamination and ply shear-out were the two dominant damage mechanisms. In order to ascertain these observations, extensive cross examination was carried out involving ultrasonic C-scanning, cross-sectioning and the use of impact force-time and/or quasi-static load-strain curves. Additional diagnostic impact as well as quasi-static tests on the small specimens were also conducted at several selected IKE levels aiming at generating the maximum forces slightly below and above the thresholds as identified previously. All

IBF5 11/22/2000 4:54 PM Page 149

Thick laminated woven roving GFRP plates

149

5.8 A through-the-thickness view of a single delamination in a 25 mm thick impacted E-glass/polyester panel (cut for CAI test).

these painstaking efforts19–21 have confirmed the following failure sequence for both composite systems, which is illustrated schematically in Fig. 5.7(a–d). Localised matrix cracking occurred in the contact area before the onset of delamination but it was insufficient to have a noticeable effect on the impact response curves.The initial load drop as indicated in Fig. 5.4(b–c) was caused by the onset of delamination and the final load drop in Fig. 5.4(c) corresponded to ply shear-out. After this load drop, shearing of plies continued through the thickness resulting in the growth of a truncated cone of sheared-out material. Ultimately this cone forced the remaining plies, close to the distal face, to fracture with an explosive bang as illustrated at the bottom of Fig. 5.7(a). The sequence of damage development is similar to observations on various CFRPs, reported in22–27 though some authors presented only quasi-static load-displacement curves. Because of the nature of woven roving reinforcement in a single ply, the current thick laminates were more likely to have a single delamination than those made of unidirectional prepregs, especially when impacted at low up to medium level of IKE. Such a single delamination usually occurred between one-quarter and three-quarters of the way through the laminate thickness as shown in a photograph taken from a sectioned impacted specimen in Fig. 5.8. Moreover, the projected contour of the delamination was usually close to a circle as a C-scan graph in Fig. 5.9 shows, though the difference of ILS strengths between the warp and the fill direction was around 20%. Obviously, at high IKE more than one delamination could be generated (see Fig. 5.26(a–b)), especially when the IKE was sufficient to induce ply shear-out. The through-thickness distribution of delamination was not investigated in all cases, but it is thought that a single, nearly circular delamination was the normal form of damage, at least in the early

IBF5 11/22/2000 4:54 PM Page 150

150

Impact behaviour of composite materials and structures

5.9 A C-scan graph showing a delamination in a 14 mm thick impacted S-glass/phenolic panel.

stages of the impact. In some thin UD-based quasi-isotropic carbon/epoxy laminates, it was often reported28–30 that a projected delamination of a nearly circular shape was due to an overlapping of multiple ‘peanut-shaped’ delaminations of similar sizes. This morphology results from the tendency of UD composites to delaminate along fibre directions, which seems not to apply to the woven rovings in the present investigation. Therefore, for the dominant damage mechanisms identified above, IDR comprises two separate elements: the resistance to the onset of delamination and its subsequent propagation and the resistance to ply shear-out or ultimate failure. In particular, resistance to delamination propagation in terms of IKE, as presented in Figs 5.10(a–b), is very much desired in the conventional impact damage tolerance assessment, as will be discussed in Section 5.5.4.

5.4.2 Effects of other parameters on impact damage resistance Since both composite systems could be strain-rate sensitive even at low impact velocities, the loading rate in addition to laminate geometry may affect the nature of the damage and thus the damage tolerance. Therefore the effect of varying these parameters on damage must be understood in terms of IKE, impact force and absorbed energy. Because of the different thicknesses used for the different composite systems, a direct comparison between them remains qualitative. Discussion on the strain-rate effect under high impact velocities is available in Chapter 3.

IBF5 11/22/2000 4:54 PM Page 151

Thick laminated woven roving GFRP plates

151

Damage area (mm2)

240 000 10 mm thick plates

200 000

25 mm thick plates 160 000 120 000 80 000 40 000 0 0

400

(a)

800

1200

1600

2000

2400

2800

3000

3500

Incident kinetic energy, IKE (J) 240 000

Damage area (mm2)

14 mm thick plates 200 000

19 mm thick plates

160 000 120 000 80 000 40 000 0

0

500

1000

1500

2000

2500

Incident kinetic energy, IKE (J)

(b)

5.10 (a) Damage area as a function of IKE for E-glass/polyester plates. (b) Damage area as a function of IKE for S-glass/phenolic plates.

5.4.2.1 Loading rate effect The effect of loading rate on damage was examined phenomenologically in two ways. One was to examine the variation of impactor mass (inertia) with impact velocity being kept constant; the other was to examine the variation of impact velocity by using the same impactor. The former has been neglected in most low-velocity impact investigations either due possibly to assumption that inertia effect plays no part in low-velocity impact or possibly because it is just easier to ignore it. The inertia effect examined

IBF5 11/22/2000 4:54 PM Page 152

152

Impact behaviour of composite materials and structures

Initial threshold impact force (kN)

100 10 mm thick 25 mm thick

80

14 mm thick 19 mm thick

60

40

20

0 0

10

20

30

40

50

60

70

80

Impactor mass (kg)

5.11 Initial threshold impact forces as a function of impactor mass for small E-glass/polyester and S-glass/phenolic plates.

here addressed half the problem as it arose only from the variation of impactor mass. The mass of the laminate plate during impact was not directly studied. Figure 5.11 presents the variation with impactor mass of the threshold forces corresponding to the onset of delamination for both composite systems. In this diagram, a higher impact force at specific impact mass corresponds to a higher impact velocity (thus IKE). It seems to show that the force at the onset of delamination was independent of impactor mass for both composite systems irrespective of laminate thickness, even when impactor mass was increased by nearly nine times. This finding seems also in accordance with one of the analytical predictions given.30 The inertia effect on delamination propagation was examined by increasing impactor mass while keeping impact velocity constant.As seen in Fig. 5.12, the growth of delamination area was sensitively related to an increase of impactor mass (and hence IKE) for both composite systems. Since IKE also increased with impactor mass in Fig. 5.12, this inertia effect on delamination area is further examined later by varying impactor mass and impact velocity simultaneously with IKE being kept constant. The effect of impact velocity on resistance to specific damage mechanisms has been examined using two methods.31 The effect was examined, in addition to the usual method in which impact velocity is varied, by directly comparing impact data with quasi-static. For delamination propagation, the examination procedure was quite involved as will be explained later. For the onset of delamination and ply shear-out, direct comparisons of the

IBF5 11/22/2000 4:54 PM Page 153

Thick laminated woven roving GFRP plates

153

Delamination area (mm2)

14 000 10 mm thick E-glass/polyester with 5.3ms-1 25 mm thick E-glass/polyester with 4.3ms-1 14 mm thick S-glass/phenolic with 4.3ms-1

12 000 10 000 8 000 6 000 4 000 2 000 0 0

100

200 300 400 500 600 700 Incident kinetic energy, IKE (J)

800

5.12 Delamination areas as a function of IKE with constant impact velocity for large laminate plates.

90 10 mm thick glass/polyester 25 mm thick glass/polyester 14 mm thick glass/phenolic 19 mm thick glass/phenolic

Initial threshold force (kN)

80 70 60 50 40 30 20 10 0 0

1

2

3

4

5

Impact velocity

6

7

8

9

(m s-1)

5.13 Initial threshold force for the onset of delamination as a function of impact velocity.

threshold forces were made between quasi-static and impact cases. In Fig. 5.13, both the quasi-static and impact threshold forces corresponding to the onset of delamination are plotted against velocity, which was varied from 8.3 ¥ 10-5 ms-1 (i.e. 5 mm/min) to 8 ms-1. It can be observed that the Eglass/polyester system seemed to be independent of impact velocity irre-

IBF5 11/22/2000 4:54 PM Page 154

154

Impact behaviour of composite materials and structures

Maximum force (kN)

180 160

Static data

140

Impact data 22%

120

19% 18%

100 80

36%

60 40 20 0

10 mm E-gl/po

25 mm E-gl/po

14 mm S-gl/ph

19 mm S-gl/ph

5.14 Comparison of load-bearing capabilities of small plates subjected to static and impact loadings.

Delamination area (mm2)

8000 10 mm thick E-glass/polyester 14 mm thick S-glass/phenolic 6000

4000

2000

0 0

30 60 90 120 Incident kinetic energy, IKE (J)

150

5.15 Delamination areas as a function of IKE with constant impactor mass of 8 kg.

spective of laminate thickness. However, the S-glass/phenolic system did show a modest increase in the threshold forces (over 20%) for both thicknesses with reference to the quasi-static values. For ply shear-out or laminate load-bearing capability, the results as summarised in Fig. 5.14 show that the effect of impact velocity was significant for the E-glass/polyester and was modest for the S-glass/phenolic. The effect of impact velocity on delamination propagation was examined with a constant impactor mass and the results are shown in Fig. 5.15. There, delamination area is seen to increase with impact velocity and thus IKE, as

IBF5 11/22/2000 4:54 PM Page 155

Thick laminated woven roving GFRP plates

155

Delamination area (mm2)

240 000 25mm thick large E-glass/polyester plates

200 000

68kg impactor mass 105kg impactor mass

160 000 120 000 80 000 40 000 0 0

500

1000

1500

2000

2500

Incident kinetic energy, IKE (J)

(a)

Delamination area (mm2)

240 000

68kg mass for 14mm thick plates 105kg mass for 14mm thick plates 68kg mass for 19mm thick plates 105kg mass for 19mm thick plates

200 000 160 000

S-glass/phenolic plates

120 000 80 000 40 000 0 0

(b)

500

1000

1500

2000

2500

Incident kinetic energy, IKE (J)

5.16 (a) and (b) Delamination areas as a function of two combinations of impactor mass and impact velocity for identical IKE.

expected. In order to separate out the effects of velocity, inertia and energy, it was also necessary to vary both impact velocity and impactor mass simultaneously while IKE was kept constant. In some cases appreciable variation of delamination area can occur.31 However, in the present investigation, as shown in Fig. 5.16(a–b), differences in delamination area produced in this way were small. In conjunction with the results in Fig. 5.12–15, this could be attributed to one of the following two reasons. One is that the 20% variation of impact velocity associated with a change of impactor mass from 68 kg to 105 kg was insufficient due to the physical constraints of the present drop-weight impact rig. The other is that, for an identical IKE, the effect of impact velocity on delamination propagation was likely to cancel out the inertia effect. That is, increasing impact velocity while holding impactor

IBF5 11/22/2000 4:54 PM Page 156

156

Impact behaviour of composite materials and structures Delamination area (mm2)

14 000 10 mm thick 25 mm thick

12 000 10 000 8 000 6 000 4 000 2 000 0 0

30

60

90

120

150

Impact force (kN)

5.17 Delamination area as a function of impact force for small E-glass/polyester plates.

mass constant may have produced a trend of delamination areas similar to that caused by increasing impactor mass while holding impact velocity constant. Consequently, the net effect caused by these combinations on delamination area for identical IKE would be small. 5.4.2.2 Laminate thickness effect In the present impact tests, the geometry of the laminate plates was varied to allow an examination of its effect on impact response and IDR over a large range of IKE for each composite system. The test results are summarised in Table 5.2 which shows clearly that, for specimens of a constant diameter, the impact resistance to ply shear-out increased with an increase of thickness as expected for both composite systems. In Fig. 5.13, the impact resistance to the onset of delamination increased by 216% with a thickness increase of 150% for small E-glass/polyester plates. For small S-glass/phenolic plates, a smaller increase of 36% in impact resistance was observed which was identical to the increase in thickness (36%). This appears to be independent of impact velocity. In Fig. 5.17, the thicker E-glass/polyester plates are seen to provide the greater impact resistance to delamination propagation for the same delamination area. In other words, for identical impact force, the delamination areas of the thicker plates were much smaller than those of the thin ones. Obviously, the penalty paid for this superior impact resistance was 150% weight increase. For Sglass/phenolic plates, however, there was little difference in the impact resistance to delamination propagation irrespective of plate diameter, as seen in Fig. 5.18(a–b). Interestingly, the resistance of this material to delamina-

IBF5 11/22/2000 4:54 PM Page 157

Thick laminated woven roving GFRP plates

157

Delamination area(mm2)

15 000 14 mm thick 19 mm thick

12 000 9 000 6 000 3 000 0 0

20

40

(a)

60 80 100 120 140 160 Impact force (kN)

Delamination area (mm2)

200 000 14 mm thick 19 mm thick

160 000 120 000 80 000 40 000 0 0

20

40

(b)

60 80 100 120 140 160 180 Impact force (kN)

5.18 (a) Delamination areas as a function of impact force for small S-glass/phenolic plates. (b) Delamination areas as a function of impact force for large S-glass/phenolic plates.

tion propagation, if measured by IKE, seemed to become lower for the thicker plates, as shown in Fig. 5.10(b). 5.4.2.3 Plate diameter effect Exploring the effect of plate diameter32 is possibly of greater practical importance than that of thickness. A realistic thickness is easily obtained in laboratory conditions for most full-scale composite structures. On the other hand, the in-plane dimensions of real structures normally need to be scaled down for test specimens. Scaling in impact testing is discussed elsewhere.32 A more general discussion is available, and33 relevant quasi-static data can also be found.34–36

IBF5 11/22/2000 4:54 PM Page 158

158

Impact behaviour of composite materials and structures

When the diameter of a laminate plate was increased from 100 mm to 500 mm, the increased membrane stretching was expected to contribute to IDR, especially in the relatively thin plates. In Table 5.2, the laminate loadbearing capabilities are clearly seen to increase rather than decrease as predicted by the static plate theory, while other experimental data based on carbon/epoxy plates34–36 have shown insensitivity to a change in plate diameter. The present dynamic enhancement of load-bearing capability was believed to be due to a change in the state of three-dimensional stresses in the contact area. This resulted from a significant contribution of membrane stretching to the in-plane stress components, manifested in part by the compression-to-tension switching of an impact strain gauge response in Fig. 5.6. The effect of this appears to be either a reduction in the local shear stress component which was responsible for ply shear-out, or possibly an increase in effective strength resulting from the triaxial stresses. Obviously, the thicker a laminate plate became, the less significant this enhancement would be, as shown in the table. Although an increase in plate diameter increased the degree of membrane stretching in the plate behaviour, it did not seem to affect the threshold forces corresponding to the onset of delamination17,27 and thus not the initial impact resistance. Moreover, the size of delamination areas from the small plates did not overlap in any way with that of the large plates, so unfortunately direct comparison of their impact resistance to delamination propagation was not feasible.

5.4.3 Energy-absorbing characteristics of damage mechanisms It was very likely that the damage mechanisms absorbing more IKE (such as delamination) had a greater effect on IDR and thus on damage tolerance. The onset of delamination was an unstable process associated with the sudden load drop and the jump in delamination area as described in Figs 5.17 and 5.18(a). Its subsequent propagation has been identified as the primary energy-absorbing damage mechanism. It appears to be a more desirable failure mode than ply shear-out, which could potentially lead to the plate perforation as illustrated in Fig. 5.19. In other words, the most effective process for completely absorbing a specified IKE in an impact event was through delamination propagation (OABCD) before the loadbearing capability was reached (at C or B¢). This was preferable to absorbing the energy by fibre fracture (OAB¢C¢), because more energy is absorbed and the delaminated plate still possessed a considerable amount of residual load-bearing capability as will be discussed later. It is not difficult to see that the region CDC¢E ought to be much greater than the region AB¢EB, although the position of C¢ is speculative. In Fig. 5.20(a–b) which sum-

IBF5 11/22/2000 4:54 PM Page 159

Thick laminated woven roving GFRP plates

159

A - Onset of delamination

Impact force

Fibre breakage

B¢

C

E A B

O

C¢

D

Time

5.19 Illustration of energy absorption with and without delamination.

marises the results of groups of impact tests, the IDR corresponding to delamination propagation increased nearly linearly with an increase of energy absorption (AE). When ply shear-out occurred, the IDR started to level off so that some of the IKE was absorbed by continued ply shear-out. It was shown that,37 when ply shear-out did not occur, an amount of AE (EAE) could be expressed by EIKE - ER = EAE = Emc + Eod + Epd = Emc + GIIcA

[5.1]

in which ER is rebound energy, Emc, Eod, and Epd denote an amount of AE from localised matrix cracking, onset of delamination, propagation of delamination, GIIc is mode-II strain energy release rate and A is delamination area with the assumption of a single delamination. If rebound velocity in an impact test was measured so that ER as well as EIKE (IKE) were known, the corresponding delamination area would be approximately estimated providing that GIIc was available and Emc was negligible. In the present case with GIIc = 4.2 kJ/m2 and 3.8 kJ/m2 for the E-glass/polyester and S-glass/phenolic systems, respectively, the predictions of equation [5.1] are demonstrated in Fig. 5.20(a–b) with arbitrary Emc as the latter was believed to be small and was impossible to quantify under the present impact conditions. When delamination areas were less than three-quarters of the small plate area, the predicted overall trends agreed reasonably well with the experimental data for both composite systems. An additional interesting feature was the effect of varying thickness on the relationship between delamination propagation and absorbed energy. For a given plate

IBF5 11/22/2000 4:54 PM Page 160

160

Impact behaviour of composite materials and structures

Delamination area (mm2)

14 000

Predictions of equation [5.1] with an arbitrary amount of matrix cracking

12 000 10 000 8 000 6 000 4 000

10 mm thick plate 25 mm thick plate

2 000 0 0

50 100 150 200 250 300 350 400 450 500 Absorbed energy, AE (J)

(a) 16 000

Predictions of equation [5.1] with an arbitrary amount of matrix cracking

Delamination area (mm2)

14 000 12 000 10 000 8 000 6 000 4 000

14 mm thick plate 19 mm thick plate

2 000 0 0

(b)

200 400 600 800 1000 1200 1400 1600 1800

Absorbed energy, AE (J)

5.20 (a) Delamination area as a function of AE for small Eglass/polyester plates. (b) Delamination area as a function of AE for small S-glass/phenolic plates.

diameter, delamination area seemed to decrease with increasing laminate thickness for identical AE. This suggested that some of the IKE in the thicker laminate was dissipated in other deformation mechanisms so that not all the IKE was absorbed in initiating and propagating delamination. A detailed discussion for the effect of GIIc on energy absorption is available in Chapter 1.

5.5

Impact damage tolerance and assessment

Naturally, for in-service load-bearing composite structures which also have a high risk of impact load, their damage tolerance holds the key to success.

IBF5 11/22/2000 4:54 PM Page 161

Thick laminated woven roving GFRP plates

161

The essence of damage tolerance is that the damaged composite structures are still capable of providing the desired performance, as defined by a set of mechanical requirements. As discussed in Section 5.1, the main measure of impact damage tolerance is the retention rate of compressive strength relative to the strength of the intact composite structure. The energy-based IDR alone provides only limited information. For a general damage tolerant structural design philosophy, see Chapter 4.

5.5.1 Compressive behaviour of intact and damaged panels In-plane compressive strength and stiffness were determined by testing rectangular panels quasi-statically. Generally, either damaged or intact panels needed to be supported laterally by using the anti-buckling device as described in Section 5.3.4 to avoid a premature buckling. The back-to-back strain gauges were bonded at a number of selected locations and an examination of their responses provided an important physical insight into the development of panel deformation mechanisms leading to ultimate failure. For intact panels, at least seven pairs of strain gauges were bonded across the panel width with one row (either two or three pairs per row) close to each end and one on the middle section. For damaged panels, three pairs were used, as shown in Fig. 5.3(b–c).The gauge response in terms of bending strain (i.e. difference between gauges on opposite sides of the panel at the same point) and mean strains was used to characterise panel behaviour. A positive panel bending strain here means that a panel buckles towards the distal surface while a negative panel bending strain corresponds to buckling toward the impact surface. The mean strain is relatively small if buckling occurs and is relatively large if delamination opening occurs. Equipped with this understanding, four major deformation mechanisms were identified in the compression of the present panels as illustrated in Fig. 5.21.38 Typical load-panel bending strain and load-mean strain curves are shown in Fig. 5.22(a–b) from a damaged 10 mm thick E-glass/polyester panel. Assuming a circular shape (as can be seen in Fig. 6 of Zhou17), the delamination area of 8961 mm2 was converted to a circle of 107 mm in diameter as shown in the inset of Fig. 5.22(a). Examining the 1/4 pair of strain gauges indicates that global buckling did not occur as the panel bending strain remained more or less zero until the ultimate failure was approached. Also, the fact that both panel bending and mean strains for the 2/5 pair were relatively large suggested that local buckling and delamination opening could have occurred simultaneously (case (2) in Fig. 5.21). The response of the 3/6 pair shows the similar behaviour to that of the 1/4 pair. The continuing local buckling eventually led to compression failure with a kink shear band as a photograph in Fig. 5.23 shows. This development must have been assisted

IBF5 11/22/2000 4:54 PM Page 162

162

Impact behaviour of composite materials and structures Pair 1/4

Pair 2/5

Pair 3/6

Bending Mean Bending Mean Bending Mean strain strain strain strain strain strain (1) Euler buckling

Large Small

Large Small

Large Small

(2) Delamination opening

Small Large

Small Large

Small Large

(3) Global-local mechanism

Large Small

Large Small

Small Large

Small Large

Large Small

(4) Compression with kink shear band

Small Large

5.21 Illustration of failure mechanisms of damaged panels in CAI tests with back-to-back strain gauges.

IBF5 11/22/2000 4:54 PM Page 163

Thick laminated woven roving GFRP plates

163

10 000

Bending microstrain

8 000

SG 1/4 SG 2/5 SG 3/6

1/4 3/6

6 000

2/5

4 000 2 000 0 -2 000 0

40

80

120

160

200

240

280

240

280

Compressive load (kN)

(a) 8000

SG 1/4 SG 2/5 SG 3/6

Mean microstrain

7000 6000 5000 4000 3000 2000 1000 0 0

(b)

40

80

120

160

200

Compressive load (kN)

5.22 (a) Compressive load-bending strain curves of a 10 mm thick damaged E-glass/polyester panel. (b) Compressive load-mean strain curves of a 10 mm thick damaged E-glass/polyester panel.

by the presence of the increased curvature of local fibres which made the damaged panel unsymmetrical locally thereby favouring local buckling. Sideways propagation of delamination was not very noticeable, but this may have been due to the fact that the orientation of the 2/5 and 3/6 pairs of the strain gauges was in the loading direction. With the benefit of hindsight, it may be speculated that additional strain gauges in the direction of the panel width could have been more useful for detecting width-wise delamination growth. In Fig. 5.24(a–b) from a damaged 14 mm thick S-glass/phenolic panel, some global buckling is visible though the response of all the strain gauges

IBF5 11/22/2000 4:54 PM Page 164

5.23 Compression failure with a kink shear band in a 10 mm thick Eglass/polyester CAI panel.

5.25 Compression failure with a kink shear band in a 14 mm thick Sglass/phenolic CAI panel.

IBF5 11/22/2000 4:54 PM Page 165

Thick laminated woven roving GFRP plates

165

30 000

Bending microstrain

25 000

1/4

SG 2/5

20 000

3/6 2/5

15 000 10 000

SG 3/6

5 000 0 -5 000

SG 1/4

-10 000 0

40

80

120

160

200

240

280

320

Compressive load (kN)

(a) 10 000 SG 1/4 SG 2/5 SG 3/6

Mean microstrain

8 000 6 000 4 000 2 000 0 0

(b)

50

100

150

200

250

300

Compressive load (kN)

5.24 (a) Compressive load-bending strain curves of a 14 mm thick damaged S-glass/phenolic panel. (b) Compressive load-mean strain curves of a 14 mm thick damaged S-glass/phenolic panel.

was similar. Judging from the developing trend of the 2/5 and 3/6 pairs, local buckling and delamination opening again occurred simultaneously. The final panel failure is shown in Fig. 5.25 with a clear kink shear band. This in conjunction with all three pairs of strain gauge readings suggested that the damaged panel twisted during loading in the form of the second buckling mode. Photographs in Fig. 5.26(a–b) show typical failed thicker damaged panels for both E-glass/polyester and S-glass/phenolic laminates. The only difference is that these thicker panels had multiple delaminations so that each sublaminate failed in compression through its own kink shear band. Therefore, the adjacent shear bands with often different orientations coalesced

IBF5 11/22/2000 4:54 PM Page 166

166

Impact behaviour of composite materials and structures

5.26 Compression failure with a kink shear band in (a) a 25 mm thick E-glass/polyester and (b) a 19 mm thick S-glass/phenolic CAI panels.

to form a saw-tooth shaped failure zone through the thickness. Other noticeable features are that the E-glass/polyester panel had a much greater shear angle formed between the loading direction and major kink band than the S-glass/phenolic panel. Also that the kink band was more jagged in the E-glass/polyester than in the S-glass/phenolic, possibly due to a stronger fibre/matrix interfacial bonding. As a whole, it seemed that compression failure with a kink shear band was predominant in the tests of the damaged panels. Ideally, both the intact and damaged compressive strengths used to calculate strength retention factor ought to be measured from panels which fail by similar mechanisms or at least at the middle section. Although the present damaged panels indeed failed consistently at the middle section with the combined mechanism of local buckling and shear as demonstrated, the intact panels always failed close to one end as shown in Fig. 5.27(a–b). Therefore the use of the compressive strengths from the intact panels as a

IBF5 11/22/2000 4:54 PM Page 167

Thick laminated woven roving GFRP plates

167

5.27 Compression failure with a kink shear band in (a) a 25 mm thick E-glass/polyester and (b) a 19 mm thick S-glass/phenolic intact panels.

reference was probably subject to a degree of systematic error. Nevertheless, this inherent feature is present in most of the published impact damage tolerance research works. Residual compressive stiffness could also be measured on the load-mean strain curve. This is important not only for a stiffness-sensitive structural component but also for its contribution to potential further propagation of impact damage.

5.5.2 Factors affecting strength retention factor Obviously, the strength retention factor decreased steadily as a severity of impact damage increased. Less obvious was its possible dependence on the panel geometry and local changes of fibre curvature in the vicinity of the impact contact area. Very little information exists on the panel geometry effect on residual and intact compressive strengths. In addition, an understanding of the contribution of local fibre curvature to a reduction of com-

IBF5 11/22/2000 4:54 PM Page 168

168

Impact behaviour of composite materials and structures

pressive strength may shed light on the true nature of compressive strength degradation. For example, it may provide an interesting physical insight into why a panel with an open hole (indirect assessment of residual strength) provided greater compressive strength than the impact-damaged panel with delamination area identical to the hole.39 Impact damage induced in the large plates had both local and global effects.40–41 Local damage consisted of matrix cracking, fibre/matrix debonding, surface microbuckling and fibre breakage (including both shear-out and tensile fracture for some plates), all surrounding the slightly dented impact contact area. Global damage refers to the extensive internal delamination or multiple delaminations, although, strictly, these are still local, but on a much larger scale. The local deformation (especially induced at relatively high IKE and involving ply shear-out) resulted in a local change in fibre curvature, which in turn acted as a pre-introduced misalignment, or region of fibre waviness, in the panel. In compressive loading this contributed to the initiation of local compression failure with a kink shear band. Another contribution to the loss in compressive strength was clearly the breakage of load-bearing fibres, but the failure mode is dominated by the impactinduced internal delamination. The delamination effectively divided the laminate locally into two or more sublaminates so that local flexural stiffness of these sublaminates was significantly reduced. As a result, these sublaminates may buckle locally causing an overall failure of the panel at a load level considerably lower than that of the intact panel.42 For thin damaged panels as demonstrated earlier, impact-induced delamination did not seem to propagate much in compressive loading. It is therefore thought that the large strains in the post-buckled part of the plate triggered in-plane compression failure. An increase of panel thickness by two and half times did not much alter either deformation mechanism or residual compressive strength as shown in Fig. 5.28(a–b). This finding is consistent with compression-after-impact (CAI) results of carbon/epoxy panels measured by Boeing method.43–44 Because failure is initiated locally, residual strength should not be affected by panel length. This was not investigated in the present study but work elsewhere on carbon/epoxy45 found a reduction of the length of damaged panels by 17% did not result in any significant change in residual compressive strength determined by the NASA method. On the other hand, variation of the geometry of intact panels, especially length, can have a greater effect on compressive strength so as to significantly affect strength retention factor. This was found, for example in.44 In the present investigation, the two-and-a-half-times increase of panel thickness between the two E-glass/polyester laminates led to a 12% decrease in undamaged compressive strength. This may partially account for the higher strength retention factors observed in the thicker plate.

IBF5 11/22/2000 4:54 PM Page 169

Thick laminated woven roving GFRP plates

169

18 000 SG 1/4 SG 2/5 SG 3/6

Bending microstrain

15 000 12 000 9 000 6 000 3 000 0 -3 000 -6 000 0

100

200

300

400

500

600

500

600

Compressive load (kN)

(a) 12 000

SG 1/4 SG 2/5 SG 3/6

Mean microstrain

10 000 8 000 6 000 4 000 2 000 0 -2 000 0

100

200

300

400

Compressive load (kN)

(b)

5.28 (a) Load-bending strain curves of a 25 mm thick damaged Eglass/polyester panel. (b) Load-mean strain curves of a 25 mm thick damaged E-glass/polyester panel.

5.5.3 Damage measures IKE, delamination area and depth of surface indent have all been used as the measures of damage in the tolerance assessment of impact damage. While the depth of a surface indent has been proved46 to bear no relation to the magnitude of interior damage and thus to a strength retention factor, IKE and delamination area also have inherent limitations, all involving the nature of impact damage. The only advantage of using IKE is its convenience as it can be readily defined to represent a degree of threat before an impact test is conducted. Disadvantages are that individual contributions

IBF5 11/22/2000 4:54 PM Page 170

170

Impact behaviour of composite materials and structures

of impact velocity (including quasi-static case) and impactor mass to damage and thus to damage tolerance cannot easily be examined separately. Therefore, an impact energy value could potentially yield a range of different strength retention factors. As discussed earlier, combinations of low velocity with large mass and high velocity with small mass have proved to result in two different delamination areas. Different orientations with regard to the loading direction of a single irregular delamination area of a given size have also been demonstrated both experimentally47 and numerically48 to be responsible for different strength retention factors. For example, residual compressive strength was shown to be higher when an elliptical damage area had the major axis in the loading direction. The reliability of using delamination area to assess likely residual strength is therefore questionable. The use of absorbed energy was suggested as a more relevant measure of damage.49 Quite recently, the use of impact force was shown to be a useful additional measure of damage17, 40–41 as it brought out some features of the panel compressive behaviour, which were less obvious when the other measures of damage were used. In particular, the identifiable impact force thresholds on a force-time history curve could be not only related to the dominant damage mechanisms occurring in laminate during impact but also compared directly to the static ones for examining the effect of loading rate in damage tolerance assessment.

5.5.4 Conventional damage tolerance assessment As described in Section 5.1, damage tolerance should embrace not only a load level or an IKE which a structure can sustain without suffering appreciable damage (IDR) but also a minimum level of residual load-bearing capability which the damaged structure can retain at the specified IKE or delamination area. The first part of the damage tolerance concept has already been established by the damage force and energy maps in the discussions of IDR (i.e. Figs 5.10(a–b), 5.17 and 5.28(a–b)). This is the idea of initial threshold force or IKE, below which there should be no damage. The estimated threshold will appear in the later diagrams as the end of the initial strength plateau on the grounds that if there is no damage, there should be no loss in residual compressive strength. The second part of the concept is addressed in the following through the variations of strength retention factor with IKE, delamination area and impact force. Figures 5.29–31 show the variations of strength retention factor for all four laminates in terms of damage area, IKE and impact force. As can be seen, once damage area started to increase or the initial threshold value of IKE or impact force was exceeded, residual strength was reduced very rapidly due to the presence of extensive delamination or multiple

IBF5 11/22/2000 4:54 PM Page 171

Thick laminated woven roving GFRP plates

171

1.1 1.0

10 mm glass/polyester 25 mm glass/polyester 14 mm glass/phenolic 19 mm glass/phenolic

Strength retention factor

0.9 0.8 0.7 0.6 0.5 0.4 0.3 0.2 0.1 0.0 0

40 000

80 000

120 000

160 000

200 000

Damage area (mm2)

5.29 Compressive strength retention factors as a function of damage area for composite panels.

1.1 1.0

10 mm glass/polyester 25 mm glass/polyester 14 mm glass/phenolic 19 mm glass/phenolic

Strength retention factor

0.9 0.8 0.7 0.6 0.5 0.4 0.3 0.2 0.1 0.0 0

400

800

1200 1600 2000 2400 2800 3200

Incident kinetic energy, IKE (J)

5.30 Compressive strength retention factors as a function of IKE for composite panels.

delaminations, prompting compression failure. It is noted that both types of the laminates could still retain 30% and 20% compressive strengths, respectively, even when they were completely delaminated. These asymptotes were largely due to the fact that the current panel width of 250 mm or the

IBF5 11/22/2000 4:54 PM Page 172

172

Impact behaviour of composite materials and structures 1.2 10 mm glass/polyester 25 mm glass/polyester 14 mm glass/phenolic 19 mm glass/phenolic

Strength retention factor

1.0 0.8 0.6 0.4 0.2 0.0 0

20

40

60

80

100

120

140

160

180

Impact force (kN)

5.31 Compressive strength retention factors as a function of impact force for composite panels.

equivalent circular area of 49 087 mm2 was not capable of differentiating compressive strengths from the panels containing a delamination area greater than that. Thickness did not seem to have much effect on residual strengths plotted against damage area or IKE once damage occurred or the initial IKE threshold was exceeded. However, plotting against impact force did reveal an effect of thickness. Another advantage of using impact force is that the initial plateau established in the damage force maps is readily recognised in the retained strength plots. The overall trends in degradation of residual strengths for the Sglass/phenolic laminates were similar to that of the E-glass/polyester laminates. The best performance from the 25 mm thick glass/polyester differed from the worst from the 14 mm thick glass/phenolic by less than 20%. For the same type of laminate, the thicker plates had fractionally higher residual strengths. The thickness effect on residual strength therefore did not seem to be significant on the basis of the present data. Sometimes the residual far-field compressive strain rather than strength is favoured in the conventional assessment of impact damage tolerance. Thus, the far-field compressive strain data for all four laminates are presented in terms of IKE in Figs 5.32–33(a–b), which also include strength retention data for comparison. These results indicate that both the overall downward trends were similar in magnitude and that the residual far-field compressive strain data gave higher retention factors than the residual strength data (except for the 10 mm thick E-glass/polyester panels). This

IBF5 11/22/2000 4:54 PM Page 173

1.2 Strain data Strength data

1.0 0.8 0.6 0.4 0.2 0.0 0

300

(a)

900

1200

1500

1800

1.2 Strain data

1.0

Strength data 0.8 0.6 0.4 0.2 0.0 500

1000

1500

2000

2500

Compressive strength retention factor

Compressive strain retention factor

Incident kinetic energy, IKE (J)

0

(b)

600

173

Compressive strength retention factor

Compressive strain retention factor

Thick laminated woven roving GFRP plates

3000

Incident kinetic energy, IKE (J)

5.32 (a) Comparison of far-field strain and strength retention factor data for 10 mm thick E-glass/polyester panels. (b) Comparison of far-field strain and strength retention factor data for 25 mm thick E-glass/polyester panels.

would be expected if the damage caused a reduction in stiffness and may indicate that the gauges were not truly in the far field. The impact damage did indeed cause a degradation in stiffness. For the present thick laminate panels, the reduction in compressive stiffness as shown in Figs 5.34–35 was much less severe than that in strength, as expected. The rate of degradation was nearly linear and the thicker panels suffered a lesser reduction. For example, the 25 mm thick E-glass/polyester panel suffered almost no loss in compressive stiffness after being impacted with an IKE of 334 J and having a delamination area of 163 mm in diameter, and lost only about 10% of stiffness at an IKE of 2000 J.

IBF5 11/22/2000 4:54 PM Page 174

1.2 Strain data Strength data

1.0 0.8 0.6 0.4 0.2 0.0 0

600

1800

2400

3000

3600

Compressive strain retention factor

1.2 Strain data Strength data

1.0 0.8 0.6 0.4 0.2 0.0 0

600

1200

1800

2400

3000

Compressive strength retention factor

Incident kinetic energy, IKE (J)

(a)

(b)

1200

Compressive strength retention factor

Impact behaviour of composite materials and structures Compressive strain retention factor

174

3600

Incident kinetic energy, IKE (J)

5.33 (a) Comparison of far-field strain and strength retention factor data for 14 mm thick S-glass/phenolic panels. (b) Comparison of far-field strain and strength retention factor data for 19 mm thick S-glass/phenolic panels.

5.5.5 Impact-force data based damage tolerance assessment As discussed earlier, the conventional assessment of impact damage tolerance is a complex, costly and time-consuming process. The use of strength retention factor in this process has been shown to have several inherent limitations, for example, sensitivity to different local topographic features around the impact contact area and different failure characteristics in addition to the uncertain effect of anti-buckling support on residual compressive strength. Therefore, it seems necessary to seek a simpler and more cost-effective alternative on both cost and lead time grounds.

IBF5 11/22/2000 4:54 PM Page 175

Compressive stiffness retention factor

Thick laminated woven roving GFRP plates

175

1.2 1.0 0.8 0.6 0.4 10 mm thick 0.2

25 mm thick

0.0 0

400

800

1200

1600

2000

2400

2800

Incident kinetic energy, IKE (J)

Compressive stiffness retention factor

5.34 Stiffness retention factor as a function of IKE for Eglass/polyester panels.

1.2 14 mm thick 1.0

19 mm thick

0.8 0.6 0.4 0.2 0.0 0

600

1200

1800

2400

3000

3600

Incident kinetic energy, IKE (J)

5.35 Stiffness retention factor as a function of IKE for S-glass/phenolic panels.

A novel method proposed recently50–51 was to use the ratio of two impact force thresholds identified on the recorded impact force-time history curves. One was the initial threshold force corresponding to the onset of delamination whereas the other was a peak impact force. It is advantageous if the data from the impact tests can be used directly for a preliminary assessment of damage tolerance. This method was developed on the basis of the fact that the dominant damage mechanisms such as delamination and

IBF5 11/22/2000 4:54 PM Page 176

Ratio of initial threshold force to max force

1.2 Force data of small plates Force data of large plates CAI data

1.0 0.8 0.6 0.4 0.2 0.0 0

2 000 4 000 6 000 8 000 10 000 12 000 14 000 Delamination area (mm2)

(a)

Ratio of initial threshold force to max force

1.2 Force data of small plates Force data of large plates CAI data

1.0 0.8 0.6 0.4 0.2 0.0 0

(b)

Compressive strength retention factor

Impact behaviour of composite materials and structures

40 000

80 000

Compressive strength retention factor

176

120 000 160 000 200 000

Delamination area (mm2)

5.36 (a) Comparison of force ratio and strength retention factor data for 10 mm thick E-glass/polyester panels. (b) Comparison of force ratio and strength retention factor data for 25 mm thick Eglass/polyester panels. (c) Comparison of force ratio and strength retention factor data for 14 mm thick S-glass/phenolic panels. (d) Comparison of force ratio and strength retention factor data for 19 mm thick S-glass/phenolic panels.

fibre breakage took place at different stages of impact loading and could be identified easily as demonstrated in Section 5.4.1. Consequently, the impact force-time curves from either large or small plates could be used for this purpose. In addition, the quasi-static force data may also be used. Figures 5.36–37(a–d) show impact force ratio data plotted against delamination area and IKE, respectively, for both large and small plates from all four laminates. Impact force ratio is defined here as initial damage

IBF5 11/22/2000 4:55 PM Page 177

Ratio of initial threshold force to max force

1.2 Force data of small plates Force data of large plates CAI data

1.0 0.8 0.6 0.4 0.2 0.0 0

177

Compressive strength retention factor

Thick laminated woven roving GFRP plates

20 000 40 000 60 000 80 000 100 000 120 000

Ratio of initial threshold force to max force

1.2 Force data of small plates Force data of large plates CAI data

1.0 0.8 0.6 0.4 0.2 0.0 0

Compressive strength retention factor

Delamination area (mm2)

(c)

30 000 60 000 90 000 120 000 150 000 180 000 Delamination area (mm2)

(d) 5.36 (cont.)

threshold divided by the maximum force that occurred during the impact, thus a low value of this ratio indicates a high maximum force. Compressive strength retention factor is also plotted on the same graphs. Two features can be readily observed from these diagrams. One is that the small plate data are in reasonably good agreement with the large plate data. The other is that impact force ratio and strength retention factor are approximately equal to each other for the 10 mm thick E-glass/polyester and both Sglass/phenolic panels. For the large 25 mm thick E-glass/polyester panels, the strength retention ratio is about 35% below the force ratio over the whole spectrum of damage. This difference is believed to be associated with the existence of a substantial amount of localised matrix cracking which contributed to a weakening of the panels.

IBF5 11/22/2000 4:55 PM Page 178

Ratio of initial threshold force to max force

1.2 CAI data of large plates Force ratio data of large plates Force ratio data of small plates

1.0 0.8 0.6 0.4 0.2 0.0 0

200 400 600 800 1000 1200 1400 1600 1800 Incident kinetic energy, IKE (J)

(a)

Ratio of initial threshold force to max force

1.2 CAI data of large plates Force ratio data of large plates Force ratio data of small plates

1.0 0.8 0.6 0.4 0.2 0.0 0

(b)

Compressive strength retention factor

Impact behaviour of composite materials and structures

400

800

Compressive strength retention factor

178

1200 1600 2000 2400 2800

Incident kinetic energy, IKE (J)

5.37 (a) Comparison of force ratio with strength retention factor in terms of IKE for 10 mm thick E-glass/polyester panels. (b) Comparison of force ratio with strength retention factor in terms of IKE for 25 mm thick E-glass/polyester panels. (c) Comparison of force ratio with strength retention factor in terms of IKE for 14 mm thick S-glass/phenolic panels. (d) Comparison of force ratio with strength retention factor in terms of IKE for 19 mm thick S-glass/phenolic panels.

Alternatively, as mentioned earlier, impact damage tolerance can be assessed in terms of the residual far-field compressive strain rather than strength. Strain retention factor is compared with force ratio and strength retention factor, all plotted against IKE in Fig. 5.38(a–d). It is noticeable from these diagrams that the far-field compressive strain factors are close to, but generally higher than, the force ratios. Therefore to assume that the

IBF5 11/22/2000 4:55 PM Page 179

Ratio of initial threshold force to max force

1.2 CAI data of large plates Force ratio data of large plates Force ratio data of small plates

1.0 0.8 0.6 0.4 0.2 0.0 0

179

Compressive strength retention factor

Thick laminated woven roving GFRP plates

400 800 1200 1600 2000 2400 2800 3200 3600

Ratio of initial threshold force to max force

1.2 CAI data of large plates Force ratio data of large plates Force ratio data of small plates

1.0 0.8 0.6 0.4 0.2 0.0 0

Compressive strength retention factor

Incident kinetic energy, IKE (J)

(c)

400 800 1200 1600 2000 2400 2800 3200 3600 Incident kinetic energy, IKE (J)

(d) 5.37 (cont.)

two were equal would normally give a conservative estimate of the strain retention factor. It should be noted that these results are based on only one size of CAI specimen, but the failure is thought to be controlled by the local damage and should therefore be independent of panel size. This observation that impact force ratio can be used as an estimate of strength retention ratio could have significant practical implications such that damage tolerance could be assessed by using the impact response curves of small plates alone. It would be necessary neither to carry out impact tests on large plates, nor to resort to expensive CAI tests. In addition, the use of the impact force data can allow the development of a unified effective scheme to assess simultaneously both IDR for the development of composite materials and impact damage tolerance for structural

IBF5 11/22/2000 4:55 PM Page 180

Ratio of initial threshold force to max force

1.2 Force data CAI data Far-field strain data

1.0 0.8 0.6 0.4 0.2 0.0 0

300

600

900

1200

1500

Compressive strength retention factor

Impact behaviour of composite materials and structures

1800

Incident kinetic energy, IKE (J)

(a)

Ratio of initial threshold force to max force

1.2 Force data CAI data Far-field strain data

1.0 0.8 0.6 0.4 0.2 0.0 0

500

1000

1500

2000

2500

Compressive strength retention factor

180

3000

Incident kinetic energy, IKE (J)

(b)

5.38 (a) Comparison of force ratio with strength and far-field strain retention factors for 10 mm thick large E-glass/polyester panels. (b) Comparison of force ratio with strength and far-field strain retention factors for 25 mm thick large E-glass/polyester panels. (c) Comparison of force ratio with strength and far-field strain retention factors for 14 mm thick large S-glass/phenolic panels. (d) Comparison of force ratio with strength and far-field strain retention factors for 19 mm thick large S-glass/phenolic panels.

analysis and design. This could lead to a considerable further saving of both time and experimentation cost. Further verification on different laminate systems would, however, be necessary.

5.6

Conclusions

Thick woven roving glass fibre-reinforced laminated plates of various dimensions were subjected to low-velocity and high-energy impact as well

IBF5 11/22/2000 4:55 PM Page 181

Ratio of initial threshold force to max force

1.2 Force data CAI data Far-field strain data

1.0 0.8 0.6 0.4 0.2 0.0 0

600

1200

1800

2400

3000

181

Compressive strength retention factor

Thick laminated woven roving GFRP plates

3600

(c)

Ratio of initial threshold force to max force

1.2 Force data CAI data Far-field strain data

1.0 0.8 0.6 0.4 0.2 0.0 0

600

1200

1800

2400

3000

Compressive strength retention factor

Incident kinetic energy, IKE (J)

3600

Incident kinetic energy, IKE (J)

(d) 5.38 (cont.)

as quasi-static loading. Their resistance and tolerance to impact damage have been thoroughly investigated. Delamination and ply shear-out were found to be the dominant damage mechanisms. The effect of varying impact velocity, impactor mass, plate thickness and diameter on these damage mechanisms was examined by using the recorded impact response curves, ultrasonic C-scanning and cross-sectioning. The resistance to (i.e. the threshold force for) the onset of delamination was shown to be insensitive to a change in either impactor mass or plate diameter for both E-glass/polyester and S-glass/phenolic systems. It was also insensitive to a change in velocity for the E-glass/polyester system but increased modestly with increasing velocity for the S-glass/phenolic system. Moreover, it was very sensitive to plate thickness and increased significantly for the thicker plates of the same diameter. The impact resistance to ply

IBF5 11/22/2000 4:55 PM Page 182

182

Impact behaviour of composite materials and structures

shear-out was enhanced significantly by an increase of velocity for the E-glass/polyester and modestly for the S-glass/phenolic and was found to be significantly affected by the variation of geometry especially for the E-glass/polyester system. The plate diameter-related enhancement was due to a significant contribution from membrane stretching which diminished considerably with an increase of thickness. It was demonstrated that an examination of the impact resistance to delamination propagation posed a very complex picture, being dependent on the parameter used to characterise the intensity of the impact. When impact force was used to characterise the impact, the resistance to delamination propagation was found to be insensitive to plate thickness for the S-glass/phenolic system, but it was much more sensitive for the thicker Eglass/polyester plates of the same diameter.When IKE was used, the thicker large plates had greater delamination areas. It was also found that the impacts of similar IKE gave similar amounts of delamination, regardless of whether the energy came from a high mass at low velocity or low mass at high velocity. Also, delamination propagation was found to be the primary energy-absorbing mechanism. The residual compressive strength of impact-damaged panels was found to deteriorate very rapidly due to a combined effect of a change of local fibre curvature in the vicinity of the contact area and the presence of extensive delamination(s) once the initial threshold value of IKE or impact force was exceeded. It was not sensitive to either panel thickness or variations of impact velocity and impactor mass (at fixed IKE). In addition, strength suffered more than residual stiffness or residual far-field strains. It was also found that the characteristic failure mechanism of the damaged panels in the compression tests was different from that of the intact. The damaged panels failed by a combination of local delamination buckling and kink band formation, while a near-end compression failure with a shear mechanism was found for the intact panels. The use of compressive strength retention factor along with IKE and delamination area in conventional impact damage tolerance assessment was reasonably satisfactory but was also complex, time-consuming and costly. In addition, strength retention factor, IKE and delamination area were all shown to have respective limitations. The novel alternative based on force data was demonstrated to be useful for the assessment of impact damage tolerance through direct comparisons with the conventional method in terms of both strength and far-field strain retention factors. In particular, it appeared possible to obtain a reasonable prediction of compression after impact performance using data from only impact tests on plates of an arbitrary size. If the composite system is not very strain rate sensitive, it should be possible to use quasi-static rather than impact loading. In addition, the use of impact force data can allow the development of a unified effective

IBF5 11/22/2000 4:55 PM Page 183

Thick laminated woven roving GFRP plates

183

scheme to assess simultaneously both IDR for the development of composite materials and impact damage tolerance for structural analysis and design. This could result in a considerable saving of both time and experimentation cost before resorting to the expensive conventional method.

Acknowledgements The authors are grateful to Professor G A O Davies of Imperial College (IC) for extensive and valuable interaction. The authors are also grateful to Mr J Churchward (Aeronautics of IC) for assistance and to Dr J M Hodgkinson and Mr E W Godwin (the Centre for Composite Materials of IC) for their generous assistance and discussions in the testing of mechanical properties and C-scanning. The work described here was supported by the Ministry of Defence.

References 1 Anon, ‘Joint airworthiness requirements’, JAR 25, ACJ 25.603, 1994. 2 Johnson A F and Marchant A, ‘Design and analysis of composite structures’, in Polymers and Polymer Composites in Construction, ed L C Hollaway, Thomas Telford, London, 1990. 3 Evans R E and Masters J E, ‘A new generation of epoxy composites for primary structural applications: materials and mechanics’, ASTM, 1985 STP 876 413–36. 4 Masters J E, ‘Correlation of impact and delamination resistance in interleafed laminates’, 6th ICCM/2nd ECCM, London, 3, 1987. 5 Mouritz A P, Leong K H and Herszberg I, ‘A review of the effect of stitching on the in-plane mechanical properties of fibre-reinforced polymer composites’, Composites, 1997 28A 979–91. 6 Freitas G, Magee C, Dardzinski P and Fusco T, ‘Fiber insertion process for improved damage tolerance in aircraft laminates’, J Advan Mater, 1994 36. 7 Dorey G, ‘Damage tolerance and damage assessment in advanced composites’, in Advanced Composites, ed I K Partridge, Elseview Applied Science Pub, Chapter 11, 369–98, 1989. 8 Abrate S, ‘Impact on laminated composite materials’, Appl Mech Rev, 1991 44(4) 155–90. 9 Cantwell W J and Morton J, ‘The impact resistance of composite materials – a review’, Composites, 1991 22(5) 347–62. 10 Abrate S, ‘Impact on laminated composites – recent advances’, Appl Mech Rev, 1994 47(11) 517–44. 11 Cantwell W J, Curtis P T and Morton J, ‘Post impact fatigue performance of carbon fibre laminates with non woven and mixed woven layers’, Composites, 1983 14 301–5. 12 Vedula M and Koczak M J, ‘Impact resistance of cross-plied polyphenylene sulfide composites’, J Thermoplastic Composite Materials, 1989 2 154–63. 13 Zhou G and Davies G A O, ‘Experimental determination of interlaminar shear strengths of thick GFRPs’, 6th ECCM – CTS2, Hamburg, 1994.

IBF5 11/22/2000 4:55 PM Page 184

184

Impact behaviour of composite materials and structures

14 Zhou G and Davies G A O, ‘Characterisation of thick glass woven roving/ polyester laminates: Part I, tension, compression and shear’, Composites, 1995 26(8) 579–86. 15 Zhou G and Davies G A O, ‘Characterisation of thick glass woven roving/ polyester laminates: Part II, flexure and statistical consideration’, Composites, 1995 26(8) 587–96. 16 Hodgkinson J M, Ayache S and Matthews F L, ‘In-plane and out-of-plane property measurements on thick woven glass/polyester laminates’, 5th ECCMCTS 1, Amsterdam, 1992. 17 Zhou G, ‘Static behaviour and damage of thick composite plates’, Composite Struct, 1996 36(1–2) 12–33. 18 Davies G A O, Hitchings D and Zhou G, ‘Impact damage and residual strengths of woven fabric glass/polyester laminates’, Composites, 1996 27A(8) 1147–56. 19 Zhou G and Davies G A O, ‘Impact response of thick glass fibre reinforced polyester laminates’, Int J of Impact Eng, 1995 16(3) 357–74. 20 Zhou G, ‘Damage mechanisms in composite laminates impacted by a flat-ended impactor’, Composites Sci and Tech, 1995 54(3) 267–73. 21 Zhou G, ‘Prediction of Impact damage thresholds in glass fibre reinforced laminates’, Composite Struct, 1995 31 185–93. 22 Sjoblom P, ‘Simple design approach against low-velocity impact damage’, 32nd Int SAMPE Symp, Anaheim, 529–39, 1987. 23 Lagace P A, Williamson J E, Tsang P H W, Wolf E and Thomas S, ‘The use of force as a (impact) damage resistance parameter’, 7th Tech Conf of American Society of Composites, PA, 1992. 24 Jakson W C and Poe Jr. C C, ‘The use of impact force as a scale parameter for the impact response of composite laminates’, J Composite Technol Res, 1993 15 282–9. 25 Lesser A J and Filippov A G, ‘Mechanisms governing the damage resistance of laminated composites subjected to low-velocity impacts’, Int J Damage Mech, 1994 3 408–32. 26 Rydin R W, Bushman M B and Karbhari V M, ‘The influence of velocity in low-velocity impact testing of composites using the drop weight impact tower’, J Reinforced Plastics Composites, 1995 14 113–27. 27 Delfosse D, Poursartip A, Coxon B R and Dost E F, ‘Non-penetrating impact behaviour of CFRP at low and intermediate velocities’, ASTM, 1995 STP 1230 333–50. 28 Liu D, ‘Impact induced delamination – a view of bending stiffness mismatching’, J Composite Mater, 1988 22 674–92. 29 Hull D and Shi Y B, ‘Damage mechanism characterization in composite damage tolerance investigations’, Composite Struct, 1993 23 99–120. 30 Davies G A O and Zhang X, ‘Impact damage prediction in carbon composite structures’, Int J Impact Eng, 1995 15(3) 357–74. 31 Zhou G, ‘Impact velocity effect on damage in laminated composites’, 7th ECCM – High Performance Composites, London, 1, 1996. 32 Zhou G, Impact damage resistance of thick glass woven roving fibre reinforced composites – geometric effects, Int Conf on Advanced Materials, Beijing, 1996. 33 Morton J, ‘Scaling of impact-loaded carbon fiber composites’, AIAA Journal, 1988 26 989–94.

IBF5 11/22/2000 4:55 PM Page 185

Thick laminated woven roving GFRP plates

185

34 Kwon Y S and Sankar B V, ‘Indentation-flexure and low-velocity impact damage in graphite epoxy laminates’, J Composite Technol Res, 1993 15 101. 35 Lee S W R and Sun C T, ‘Dynamic penetration of graphite/epoxy laminates impacted by a blunted-ended projectile’, Composites Sci Technol, 1993 49 369–80. 36 Zhou G, Lloyd J C and McGuirk, J J, ‘Experimental evaluation of geometric factors affecting damage mechanisms in carbon/epoxy plates’, accepted by Composites Part A. 37 Zhou G, ‘Characteristics of impact energy absorption during damage development in laminated composites’, 4th Int Conf Deformation and Fracture of Composites, Manchester, 1997. 38 Zhou G, ‘Compressive behaviour of large undamaged and damaged thick composite panels’, Composite Struct, 1997 38(1–4) 589–97. 39 Horton R E and McCarty J E, ‘Damage tolerance of composites’, in Engineering Materials Handbook, T J Reinhart, Ohio, USA, 1, ASM, 1987. 40 Zhou G and Davies G A O, ‘Damage tolerance of thick glass fibre reinforced laminate structures subjected to low-velocity impact’, ASME-WAM, Chicago, MD-vol. 51, 1994. 41 Zhou G, ‘Effect of impact damage on residual compressive strength of GFRP laminates’, Composite Struct, 1996 35(2) 171–81. 42 Lagace P A, ‘On delamination failures in composite laminates’, in Composite Structures Testing, Analysis, and Design, eds J N Reddy and A V K Murty, New Delhi, Spinger-Verlag/Narosa Publications, 1992. 43 Manders P W and Harris W C, ‘A parametric study of composite performance in compression-after-impact testing’, SAMPE J, 1986 Nov. 47–51. 44 Vedula M, Lee W M, Benedetto E E and Groleau M R, ‘Screening test for compression after impact strength evaluation of composites’, 7th Tech Conf of American Society of Composites, PA, 1992. 45 Ishikawa T, Sugimoto S, Matsushima M and Hayashi Y, ‘Some experimental findings in compression-after-impact (CAI) tests of CF/PEEK (APC-2) and conventional CF/epoxy flat plates’, Composites Sci Technol, 1995 55 349–63. 46 Wardle B L and Lagace P A, ‘On the use of dent depth as an impact damage metric for thin composite structures’, J Reinforced Plastics Composites, 1997 16 1093–110. 47 Lameris J, BRITE-EURAM 3159 CR, National Aerospace Lab., The Netherlands, 1993. 48 Xiong Y and Poon C, ‘Prediction of residual compressive strength of impactdamaged composite laminates’, 9th ICCM, Madrid, 1993. 49 Pintado P, Vogler T J and Morton J, ‘Impact damage tolerance of thick graphiteepoxy composite material systems’, 8th ICCM, Hawaii, 1993. 50 Zhou G, ‘The use of experimentally-determined impact force as a damage measure in impact damage resistance and tolerance of composite structures’, Composite Struct, 1998 42(4) 375–82. 51 Zhou G, ‘Replacing residual compressive strengths by impact force data in the damage tolerance assessment of composite structures’, 8th ECCM, Naples, 1998. © Crown copyright 2000. Published with the permission of the Defence Evaluation and Research Agency on behalf of the Controller of HMSO.

IBF6 11/22/2000 6:34 PM Page 186

6 Elastic impact stress analysis of composite plates and cylinders S R SWANSON

6.1

Introduction

Impact is a complicated topic, involving both structural and material response and damage formation. However, the stress analysis of the impact is fundamental to understanding the entire problem. The analysis can take many forms, such as nonlinear numerical analysis or linear analysis with closed form solutions, as some examples show in Chapter 7. In the following, the fundamentals of primarily linear analysis of laminated plates and cylinders will be discussed, and examples of work in the literature on these topics will be presented.

6.2

Impact regimes

It is possible to classify impact into various categories, depending on the characteristics of the impactor and target. A major category is those impact events where through-the-thickness stress wave effects are important. In impact of a structure by a foreign body, a through-the-thickness compressive stress wave will be initiated. In some circumstances, this wave will be reflected as a tensile wave from the free surface on the back side, introducing the possibility of through-the-thickness tensile failure.1 Calculation of the characteristics of the through-the-thickness wave may in general be difficult and require numerical treatment, however some limit cases will be informative. If the impactor is large with respect to the thickness of the target and both the target and impactor have parallel surfaces, the stressstate is that associated with one dimensional strain, and the wave speed will be in the order of c = Q33 r

and s = -aQ33v c

[6.1]

where Q33 is the diagonal term of the three-dimensional stress–strain matrix for the composite in the through-the-thickness direction, a is a constant depending on the properties of the impactor and target, and v is the 186

IBF6 11/22/2000 6:34 PM Page 187

Elastic impact stress analysis of composite plates and cylinders

187

impact velocity. For many composites Q33 is not greatly different from the through the thickness modulus, which is also comparable to the in-plane modulus E22 in a direction transverse to the fibers. The magnitude of the stress wave depends linearly on the ratio of the impactor velocity to the wave speed. Substituting values shows that through-the-thickness stress waves will be important in ballistic events and many simulations such as air-gun driven impactors, but are not likely to be significant in dropweight impacts. However the impactor and target surfaces are often not parallel, and the impactor may not be large. In this case the indentation of the impactor into the target will smear out the transverse wave so that detailed numerical computation is required, e.g. as carried out by Joshi and Sun.2 For those impact events in which through-the-thickness stress waves are not considered to be important, a further division is possible. Events in which the distributed mass of the target is negligible relative to the impactor mass are termed quasi-static. This assumption greatly simplifies the analysis of the impact event, as the target can then be characterised only by its static stiffness properties. Impact events that do not fall into this category will respond in a much more complex fashion, that can be considered to be a synthesis of a large number of natural frequencies and mode shapes of the target. Because of the simplicity of the quasi-static analysis, it is important to be able to determine when this assumption is applicable, and this topic is addressed further in the following. Impacts in which the quasistatic assumption is assumed to hold are sometimes termed ‘low-velocity’ impacts, but this is questionable terminology as the division between the structural dynamic and the quasi-static regimes is completely independent of the impact velocity itself, but depends on other characteristics of the impact.

6.3

Analysis of impact

The analysis of the stresses and strains resulting from impacts on laminated plates, beams, and cylinders will be discussed in this section, for impacts in which the structural dynamics of the target are important, but through-thethickness stress waves are not. The local deformations associated with the indentation of the target are first described, followed by several schemes for solving the dynamics problem of impact on plates and cylinders.

6.3.1 Contact stiffness and deformation The projectile indents the target to a greater or lesser extent, and this additional compliance influences the response. The usual treatment follows that of Sun et al.,3–5 who adapted the usual Hertz solution for contact between

IBF6 11/22/2000 6:34 PM Page 188

188

Impact behaviour of composite materials and structures

two bodies to the impact problem. The contact force is assumed to be related to the contact indentation by the following equation F = ka 3 2

with

k=

4 Rs E22 3

[6.2]

where F is the total contact force on the target, a is the local indentation, Rs is the radius of the spherical impactor, and E22 is the transverse Young’s modulus of the laminated target. The contact force is then related to the motion of the projectile by assuming rigid body dynamics for the projectile, that is F = -mü

[6.3]

where m is the mass and u is the displacement of the projectile. The relationship between the local indentation, projectile displacement and plate displacement at impact center is expressed by a(t ) = u(t ) - w(t , x, h)

[6.4]

where ξ and h give the location of the center of impact.

6.3.2 Structural dynamics of impact for plates The analysis of static and dynamic loadings of laminated composite plates has seen considerable development recently. Lekhnitskii,6 and Whitney and Leissa7 have presented analyses with infinite transverse rigidity while Whitney and Pagano8 have presented a theory including transverse shear deformations. The dynamic problems considered involved vibration of plates. Sun and Chattopadhyay3 and Dobyns9 used the plate equations developed by Whitney and Pagano8 to analyse a simply supported orthotropic plate subject to center impact. Dobyns assumed that the lateral force history was known, while Sun and Chattopadhyay noted that in impact by a foreign body, the force history must be computed as part of the problem. Thus Sun and Chattopadhyay integrated the equations of motion numerically. Birman and Bert10 obtained a closed-form solution for laminated angle-ply simply supported plates subject to blast loading, which again considers that the force history is known. Solutions of the impact problem for plates have been displayed in the literature, that solve for the force history as well as the resulting stresses, strains, and deformation. An analytical solution is available for plates with simply supported boundary conditions, using Fourier series expansion techniques combined with Laplace transform techniques. However, the contact stiffness must be linearised to permit this analytical solution. The solution for other boundary conditions has been addressed using Ritz solutions,

IBF6 11/22/2000 6:34 PM Page 189

Elastic impact stress analysis of composite plates and cylinders

189

combined with numerical time integration. These analysis techniques are illustrated in the following.

6.3.2.1 Equations of motion for plates The plate equations of motion developed by Whitney and Pagano8 reduced to specially orthotropic form (Bij = 0, A16 = A26 = D16 = D26 = 0), are given by Dobyns9 as D11

3 2 ∂2 yx ∂2 yx ∂ 2 yy Ê y + ∂w ˆ = rh ∂ y x ( ) + D + D + D kA 12 66 55 66 x Ë ∂x ∂ y ∂x ¯ 12 ∂t 2 ∂x 2 ∂ y2

( D12 + D66 ) [6.5] kA55

∂2 yx ∂ 2 yy ∂ 2 yy ∂w ˆ rh3 ∂ 2 yy + D66 + D22 - kA44 Ê y y + = 2 2 Ë ∂x ∂ y ∂y ¯ 12 ∂t 2 ∂x ∂y

2 ∂2w ˆ ∂2w Ê ∂y x ∂ w ˆ Ê ∂yy ( ) + + kA + + q x y t h , , = r 44 Ë ∂x Ë ∂y ∂x 2 ¯ ∂ y2 ¯ ∂t 2

[6.5]

where Dij and Aij are the stiffnesses, as defined by Whitney and Pagano,8 h is the plate thickness, t is time, r is material density, w is the plate displacement in the z direction at the plate midplane, yx and yy are the rotations in the x and y directions and k is a shear correction factor that is often taken to be p2/12.

6.3.2.2 Solution for simply-supported boundary conditions For plates with boundary conditions of simple support on all four edges, it is possible to use standard Fourier series expansion techniques to determine the response. Christoforou and Swanson11,12 have shown that it is possible to obtain an analytical solution to the impact problem by using Laplace transform techniques, if the nonlinear contact indentation is approximated by a linearised version. The solution is based on expansions of the loads, displacements, and rotations in Fourier series which satisfy the end boundary conditions of simple support. Each expression is assumed to be separable into a function of time and a function of position. Furthermore, following Bert and Birman,13 by neglecting in-plane and rotary inertia the problem becomes a second order ordinary differential equation in time for the Fourier coefficients of the lateral deflection. In the case of impact, the impact force is computed from the deceleration of the impactor mass. This involves the equilibrium equation between the impactor and the plate during contact. For a given dynamic load, solutions of the governing equations [6.5] that satisfy the boundary conditions of simple support are given by

IBF6 11/22/2000 6:34 PM Page 190

190

Impact behaviour of composite materials and structures F(t)/(uv)

x

h

U v

b

¡

a

y

6.1 Illustration of plate geometry used for analysis of simply supported plates.

yx = Â Â Amn (t ) cos m

n

yy = Â Â Bmn (t ) sin m

n

w = Â Â Wmn (t ) sin m

n

mpx npy sin a b

mpx npy cos a b

[6.6]

mpx npy sin a b

with the load function represented by q(x, y, t ) =

Â ÂQ

mn

m

n

(t ) sin

mpx npy sin a b

[6.7]

Equations [6.6] and [6.7] are the Fourier series representation of the rotations, lateral displacement and load. The coordinate system and geometry are illustrated in Fig. 6.1. The terms of the Fourier series representation for a uniform load over the rectangular area u, v with center at z, h is shown in Fig. 6.1 are Dobyns’.9 Qmn (t ) =

16F (t ) mpz nph mpu npv sin sin sin sin 2 a b 2a 2b p mn uv

[6.8]

Following the results of Bert and Chen,14 rotary inertia effects are neglected. Thus substituting equations [6.6] and [6.7] into equation [6.5]

IBF6 11/22/2000 6:34 PM Page 191

Elastic impact stress analysis of composite plates and cylinders

191

results in the independent sets of three equations for each set of modal parameters m and n: ÈC11 C12 C13 ˘ Ï Amn (t ) ¸ Ô Ô ÍC C 22 C 23 ˙ Ì Bmn (t ) ˝ = Í 12 ˙Ô ÍÎC13 C 23 C33 ˙˚ ÓWmn (t ) Ô˛

0 Ï ¸ Ô Ô 0 Ì ˝ ÔÓQ (t ) - rhW Ô ˙˙ mn mn (t ) ˛

[6.9]

where the elements of the symmetric matrix Cij are 2

2

mp ˆ np C11 = D11 Ê + D66 Ê ˆ + kA55 Ë a ¯ Ë b¯ mp ˆ Ê np ˆ C12 = (D12 + D66 )Ê Ë a ¯Ë b ¯ mp ˆ C13 = kA55 Ê Ë a ¯ 2

2

mp ˆ np C 22 = D66 Ê + D22 Ê ˆ + kA44 Ë a ¯ Ë b¯ np C 23 = kA44 Ê ˆ Ë b¯ 2

mp ˆ Ê np ˆ C33 = kA55 Ê + kA44 Ë b¯ Ë a ¯

[6.10]

2

Following Bert and Birman,13 equation [6.9] can be reduced to a single differential equation by the following transformation: Amn (t ) = K A Wmn (t ); Bmn (t ) = K BWmn (t )

[6.11]

where KA = KB =

C12C 23 - C13C 22 2

C11C 22 - C12 C12C13 - C11C 23 C11C 22 - C12

[6.12]

2

Substitution of equation [6.8] reduces the set [6.9] into the following: ab F (t ) 2 ˙˙ mn (t ) + w mn W Wmn (t ) = Pmn uv m1

[6.13]

C13 K A + C 23 K B + C33 are the squared fundamental frequenrh cies of the plate, and m1 is its mass. where w 2mn =

IBF6 11/22/2000 6:34 PM Page 192

192

Impact behaviour of composite materials and structures

For zero initial displacement and velocity, the solution of equation [6.13] is obtained using the convolution integral: Wmn (t )

Pmn ab uvm1w mn

t

Ú F (t) sin w 0

mn

(t - t )dt

[6.14]

The deflection of the plate at any point is given by w(x, y, t ) =

ab uvm1

Pmn

ÂÂw m

n

sin

mn

mpx npy t sin F (t ) sin w mn (t - t )dt a b Ú0

[6.15]

The response of a plate to impact by a foreign object may be computed from the transient response, equation [6.15], by computing the impact force from the deceleration of the impactor mass. The integral equilibrium equation between the impactor and the plate during contact is given by a b 1 wÊ , , t ˆ = V0 t Ë2 2 ¯ m2

t

Ú F ( t)(t - t)dt 0

F (t ) K2

[6.16]

Êa b ˆ where V0 is the initial velocity of the impactor with mass m2, w , , t is Ë2 2 ¯ the lateral deflection of the plate evaluated at the impact point as a function of time, F(t) is the impact force and K2 is the linearised contact area stiffness. As mentioned above, the contact problem must be linearised in order to be treated analytically using the present approach. This involves both replacing the nonlinear contact stiffness with an appropriate linearised value, as well as approximating the time varying contact area by a constant area. Combining equations [6.15] and [6.16] yields 1 t F (t ) F (t )(t - t )dt Ú 0 m2 K2 ab Pmn mp np t = sin sin F (t ) sin w mn (t - t )dt Â Â uv m1 m n w mn 2 2 Ú0

V0 t -

[6.17]

Taking the Laplace transform of equation [6.17] and after some rearranging yields F (s) =

m2 V0 m2 2 abm2 1+ s + K2 uvm1

mp np s2 Pmn sin sin Â Â 2 2 2 s 2 + w mn m n

[6.18]

Using the inverse theorem for Laplace transforms and following the procedure of Christoforou and Swanson11,12 yields

IBF6 11/22/2000 6:34 PM Page 193

Elastic impact stress analysis of composite plates and cylinders

193

0.0010 75 terms

Strain Ep X

0.0008

51 terms 25 terms

0.0006

0.0004

0.0002

0.0000 0

100

200

300

Time (ms)

6.2 Convergence of solution for strain behind the impact point. (After Christoforou and Swanson12.)

F (t ) =

Â F sinw t j

[6.19]

j

j

where ωj are the response frequencies or poles of expression [6.18] and Fj =

m2 V0 È m2 ab m2 w jÍ + Î K 2 uv m1

˘ w 2mn mp np sin Pmn sin ˙ Â Â 2 2 2 (w 2mn - w 2j ) ˚ m n

[6.20]

The impact response can be determined by combining the Laplace transforms of equations [6.14] and [6.19] Wmn (s) =

Pmn ab F jw j Â 2 2 m1uv j (s + w mn )(s 2 + w 2j )

[6.21]

Inverting as above gives Wmn (t ) =

Pmn ab Fj (w j sin w mnt - w mn sin w j t ) Â m1uv j w mn (w 2j - w 2mn )

[6.22]

The deflection and strain at any point can then be obtained by substituting [6.22] into equations [6.11] and [6.6]. An illustration of the convergence of the solution for strain is shown in Fig. 6.2, taken from Christoforou and Swanson.12 Further results will be shown subsequently.

IBF6 11/22/2000 6:34 PM Page 194

194

Impact behaviour of composite materials and structures

6.3.2.3 Plates with other boundary conditions As is the case with the static analysis of plates, boundary conditions other than simple support require techniques other than the double Fourier series expansion. An approximate but general technique is to use a Ritz analysis, combined with a numerical integration of the time variable. It is possible to include the nonlinear contact stiffness with this approach.The analysis shown here has been displayed by Cairns and Lagace15 and Qian and Swanson.16 The analysis is based on Lagrange’s equation of motion with the Lagrangian function L = T - V: d ∂L ∂L [6.23] =0 dt ∂ x ∂ x where x is the modal amplitude. Consider a laminated plate under dynamic lateral loading. The potential energy is given as V=

T 1 1 T k] [ D][k]dA + Ú Ú [ g ] [ A][ g ]dA - Ú Ú p(t , x, y) w(t , x, y)dA [ Ú Ú A 2 A 2 A [6.24]

where the first two terms are bending and transverse shear strain energy, respectively, and the third is the work done by the lateral load. The kinetic energy of the plate is given by T=

rh 2 w˙ (t , x, y) dA. Ú Ú A 2

[6.25]

Here again the in-plane and rotary inertia effects have been neglected, as suggested by Birman and Bert10 and Dobyns.9 The problem considered in Qian and Swanson16 has clamped boundary conditions on two opposing edges of the plate and free boundaries on the other two edges to correspond with experiments. The procedure followed is based on choosing two series of functions, or ‘mode shapes’, which satisfy the boundary conditions and give suitable expressions for deflection curves in x and y directions separately. The assumed deformed shape of the rectangular plate is then taken as a product of these functions. Therefore the series approximation for the planar rotations and transverse displacement can be taken as a (t , x, y) =

ÂÂA

(t ) X m¢ ( x)Yn ( y)

[6.26]

ÂÂB

(t ) X m ( x)Yn¢( y)

[6.27]

(t ) X m ( x)Yn ( y)

[6.28]

mn

m

b (t , x, y) =

mn

m

w(t , x, y) =

n

n

Â ÂC m

n

mn

IBF6 11/22/2000 6:34 PM Page 195

Elastic impact stress analysis of composite plates and cylinders

195

where Amn, Bmn, and Cmn are the modal amplitudes of the plate and are to be determined. Substituting the assumed mode shapes in the expressions for potential and kinetic energy, and then using Lagrange’s equation [6.23] gives three sets of equations with unknowns Amn, Bmn, and Cmn. Substituting Amn, Bmn in terms of Cmn yields a system of second order ordinary differential equations for the modal amplitudes Cmn

[ S ]{C˙˙} + [T ]{C} = {P}

[6.29]

In Qian and Swanson16 the assumed mode shapes were taken as beam functions, which are solutions for mode shapes of beams under the appropriate boundary conditions.17 The beam functions are orthogonal, permitting expansion of the load in terms of these functions. This expansion is of the form p(t , x, y) =

ÂÂ p

mn

m

(t ) X m ( x)Yn ( y)

[6.30]

n

with pmn (t ) =

ÚÚ

A

p(t , x, y)X m (x)Yn ( y)dxdy

ÚÚ

A

X m2 (x)Yn2 ( y)dxdy

[6.31]

The {P} in the right hand of equation [6.29] is a force term, and each component comes from taking the derivative of the work done by the lateral load to the relative mode amplitude, that is Pmn =

∂W = pmn Ú Ú X m2 (x)Yn2 ( y)dxdy A ∂ C mn

[6.32]

The contact force is assumed to be related to the contact indentation using the relations given previously above. The contact pressure p(t, x, y) is simply taken as the uniform distribution of the total contact force F(t) over a square area Ac. This area is determined by

[

Ac = p Rs2 - (Rs - a )

2

]

[6.33]

The equations above along with the contact laws were solved simultaneously. Due to the nonlinearity of the contact deformation relationship, the above equations were solved numerically, using the Newmark method with b = 1/4, which gives an unconditionally stable solution. A typical comparison of calculation with experimentally measured strain is shown in Fig. 6.3, taken from Qian and Swanson.16 It can be seen that the agreement is very reasonable.

IBF6 11/22/2000 6:34 PM Page 196

196

Impact behaviour of composite materials and structures 7000 Experiment Analysis

6000

e x at A (microstrain)

5000 4000 3000 2000 1000 0 -1000

0

200

400

600

800

1000

Time (ms)

6.3 Comparison of Ritz analysis with experiment for strain in impact of plate. (After Qian and Swanson16.)

6.3.2.4 Comparison of solution techniques It is possible to apply the second solution technique described above, that of using a Ritz analysis in conjunction with numerical time integration, to the problem of impact of a plate with simply-supported boundary conditions, and thus permit a comparison with the first technique, which used Laplace transforms. This comparison of solution techniques has been carried out by Qian and Swanson,18 and is reviewed in the following. The basic problem chosen to illustrate the techniques is based on geometry and properties used previously by Sun and Chen,19 and consists of center impact of a simply supported square composite plate. The material properties and geometry are given in Table 6.1. Analyses were also carried out on plates with two and four times the standard thickness. As mentioned above, the Rayleigh–Ritz technique used the Newmark method for time integration, and incorporated the nonlinear contact law with the contact area changing at each time step. The analytical solution with Laplace transforms was restricted to a linearisation of the contact law, with a constant contact area throughout the solution. The results of the computations presented in Qian and Swanson18 show the importance of using a sufficiently small time step in the numerical time integration used with the Ritz solution, and a time step of 0.1 ms was

IBF6 11/22/2000 6:34 PM Page 197

Elastic impact stress analysis of composite plates and cylinders

197

Table 6.1. Data for the plate impact problem used for comparison Plate:

[0/90/0/90/0]s T300/934 carbon/epoxy plate, simply supported plate size: 200 mm by 200 mm plate thickness: (a) h = 2.69 mm (0.269 mm/layer) (b) 2 h = 5.38 mm (0.538 mm/layer) (c) 4 h = 10.76 mm (1.076 mm/layer) E22 = 7.9 GPa E11 = 120 GPa υ12 = υ23 = 0.30 G12 = G23 = 5.5 GPa r = 1580 kg m-3

Impactor: 12.7 mm diameter steel ball, r = 7960 kg m-3 mass = 8.537 g, impact velocity = 3.0 m s-1 Hertzian contact stiffness kh = 8.394 ¥ 108 N m-3/2 Linearised contact stiffness kl = 5.866 ¥ 106 N m-1 Source: Qian and Swanson.18

employed. Comparisons of the contact force, and target displacement and strain between the two solution techniques were in general good. When the linearised contact law was used with both techniques, the agreement between the two methods was excellent. Using the nonlinear contact law with the Ritz technique and the linearised contact law with the Fourier series expansion technique gives results as shown in Fig. 6.4. Computations for the nominal plate thickness of the example problem showed reasonable agreement, but plates with thickness of two and four times this showed less good agreement, indicating the relative error involved in the linearisation of the contact law. A comparison with the dynamic finite element calculations of Sun and Chen19 is shown in Fig. 6.5, which shows reasonable agreement for displacement.

6.3.3 Impact of a cylinder Ramkumar and Thakar20 have presented an analysis of the dynamic response of curved laminated plates subjected to low-velocity impact. They use Donnell’s equations for thin shells, assume that the impact force varies linearly with time, and follow Dobyns’s9 procedure to solve for the response. Vinson and Chou21 presented a double Fourier series solution of an orthotropic cylindrical shell subjected to a lateral concentrated static load. A solution technique for impact of laminated cylinders has been presented by Christoforou and Swanson,11 and a comparison with experimental data has been given by Swanson et al.22 The solution uses Fourier series expansions and Laplace transform techniques, and requires linearisation of the contact stiffness. A review of this approach is given in the following.

IBF6 11/22/2000 6:34 PM Page 198

198

Impact behaviour of composite materials and structures 1400 Analytical solution

1200

Rayleigh–Ritz solution

Strain ex (microstrain)

1000 h 800

600

400 2h 200 0

4h

-200 0

50

100

150

200

250

Time (ms)

6.4 Comparison of Fourier series–Laplace transform solution with Ritz solution with numerical time integration, for strain behind the impact point in plate impact. (After Qian and Swanson18.)

This analysis is based on an expansion of the load, displacements, and rotations in a double Fourier series that satisfies the end boundary conditions of simple support. Each expansion is assumed to be separable into a function of time and a function of position. Furthermore, by neglecting in-plane and rotary inertia the problem becomes a second order ordinary differential equation in time for the Fourier coefficients of the radial deflection. On the right hand side of the differential equation are the Fourier coefficients of the loading function. For a given loading impulse the solution can be found by invoking the convolution integral. In the case of impact, the impact force is computed from the deceleration of the impactor mass.This basically involves the equilibrium equation between the impactor and the shell during contact. By neglecting the local contact area deformation, the resulting integral equation can be solved algebraically for the impact force by using Laplace transforms. The expressions for the impact response and force in time are obtained by using the inversion theorem of the Laplace transforms in conjunction with the Cauchy residue theorem.

IBF6 11/22/2000 6:34 PM Page 199

Elastic impact stress analysis of composite plates and cylinders

199

0.45 0.40

Plate centre displacement (mm)

0.35 0.30 0.25 0.20 0.15 0.10 Rayleigh–Ritz solution 0.05

Finite element solution6

0.00 0

400

800

1200

1600

Time (ms)

6.5 Comparison of Ritz solution with numerical time integration with dynamic finite solution,19 for center displacement in plate impact. (After Qian and Swanson18.)

6.3.3.1 Governing equations for cylinders Love’s equations of motion for a circular cylindrical shell of length L, radius R, and thickness h subject to lateral loads generalised to include shear deformations, combined with the constitutive equations for a specially orthotropic material, result in the equations given by Bert and Birman13 as: A66 A12 + A66 ˆ A12 u,qq + Ê v, xq + w, x = rhu˙˙ 2 Ë ¯ R R R Ê A12 + A66 ˆ u + A v + A22 v - A44 v 66 , xx ,qq Ë ¯ , xq R R2 R2 A22 + A44 ˆ A44 w ,q + +Ê bq = rhv˙˙ 2 Ë ¯ R R A12 A44 + A22 ˆ A44 A22 u, x - Ê v,q + A55 w , xx + 2 w ,qq - 2 w 2 Ë ¯ R R R R A44 ˙˙ + A55b x,x + bq,q + q( x, q, t ) = rhw R A11u, xx +

IBF6 11/22/2000 6:34 PM Page 200

200

Impact behaviour of composite materials and structures F z, w A l1

x, u

q, v bx

bq

l

Loaded area

A

2f1 t

Support conditions v = w = bq = 0 Nx = Mx = 0

R

Support conditions v = w = bq = 0 Nx = Mx = 0

6.6 Geometry of cylinder under transverse impact. (After Christoforou and Swanson11.)

D66 bx,qq - A55bx R2 D12 + D66 ˆ rh3 ˙˙ +Ê bq , xq = bx Ë ¯ R 12 A44 A44 D12 + D66 ˆ vw ,q + Ê b + D66bq , xx Ë ¯ x, xq R R R

- A55 w, x + D11bx, xx +

+

[6.34]

D22 rh3 ˙˙ b A b = bq q , qq 44 q 12 R2

where u, v, and w are the displacements along the axial x axis, circumferential θ axis and radial z axis, bx and bθ are bending slopes in the x - z and θ - z planes, q is lateral pressure loading, r is the mass per unit area, Aij and Dij are the standard lamination theory constants, and t is time. A comma denotes differentiation with respect to the space variables, and a dot denotes differentiation with respect to time. The geometry considered is illustrated in Fig. 6.6. The constitutive equations for a specially orthotropic

IBF6 11/22/2000 6:34 PM Page 201

Elastic impact stress analysis of composite plates and cylinders

201

material (Bij = 0, A16 = A26 = D16 = D26 = 0) have been used to relate the stress, moment, and shear resultants to the midsurface strains e0i , curvatures ki, and average transverse shear strains gxz and gθz. 6.3.3.2 Solution procedure for impact of cylinders A closed-form solution of the governing equations is given as follows. The boundary conditions for a cylindrical shell that is freely supported (simplysupported without in-surface restraint) along its curved edges are given by N x ( 0, q, t ) = N x (L, q, t ) = M x ( 0, q, t ) = M x (L, q, t ) = 0 w( 0, q, t ) = w(L, q, t ) = v( 0, q, t ) = v(L, q, t ) = 0 bq ( 0, q, t ) = bq (L, q, t ) = 0

[6.35]

For a given load, the solution to equation [6.34] that satisfies the boundary conditions, equation [6.35], can be separated into a function of time and a function of position as follows: mpx L mpx v = Vmn (t ) sin nq sin L mpx w = Wmn (t ) cos nq sin L mpx b x = Tmn (t ) cos nq cos L mpx bq = Bmn (t ) sin nq sin L u = U mn (t ) cos nq cos

[6.36]

and the load as q(x, q, t ) = Qmn (t ) cos nq sin

mpx L

[6.37]

Equations [6.36] and [6.37] are the double Fourier series expansions of the displacements, rotations and load, which are similar to the static case developed by Vinson and Chou.21 The effects of in-surface and rotary inertia will be assumed to be negligible. Bert and Birman13 mentioned these effects to be negligible in dynamic stability studies, while Dobyns,9 by referring to Mindlin’s23 finding made the same assumptions for the impact response of orthotropic plates. Thus, substituting equations [6.36] and [6.37] into equation [6.34] and neglecting in-surface and rotary inertia yields the following set of equations:

IBF6 11/22/2000 6:34 PM Page 202

202

Impact behaviour of composite materials and structures

ÈC11 Í Í Í Í Í Î

C13 C14 C15 ˘ ÏU mn (t ) ¸ C 23 C 24 C 25 ˙ ÔVmn (t ) Ô ˙ ÔÔ Ô C33 C34 C35 ˙ ÌWmn (t ) ˝ = sym C 44 C 45 ˙ Ô Bmn (t ) Ô Ô ˙Ô C55 ˚ ÔÓTmn (t ) Ô˛ C12 C 22

0 Ï ¸ Ô Ô 0 ÔÔ Ô ˙˙ mn (t ) - Qmn (t ) Ô˝ ÌrhW Ô Ô 0 Ô Ô ÔÓ Ô˛ 0

[6.38]

where Cij are given as 2

mp ˆ n C11 = - A11 Ê - A66 Ê ˆ Ë L ¯ Ë R¯ C12 = C 21

2

C 25 = C52 = 0

Ê n ˆ Ê mp ˆ = ( A12 + A66 ) Ë R¯Ë L ¯

C13 = C31 =

A12 Ê mp ˆ R Ë L ¯

C34

C14 = C15 = 0

C35 2

C 22 C 23

2

mp ˆ n A44 = - A66 Ê - A22 Ê ˆ - 2 Ë L ¯ Ë R¯ R A22 + A44 ˆ Ê n ˆ = -Ê Ë ¯Ë R¯ R

C 24 = C 42 =

A44 R

C33

C 44

2

2

2

2

mp ˆ n A22 = - A55 Ê - A44 Ê ˆ - 2 Ë L ¯ Ë R¯ R n = C 43 = A44 Ê ˆ Ë R¯ mp ˆ = - A55 Ê Ë L ¯ mp ˆ n = - D66 Ê - D22 Ê ˆ - A44 Ë L ¯ Ë R¯

Ê n ˆ Ê mp ˆ C 45 = -(D66 + D12 ) Ë R¯Ë L ¯ 2

2

mp ˆ n C55 = - D11 Ê - D66 Ê ˆ - A55 Ë L ¯ Ë R¯ [6.39]

Bert and Birman13 obtained equations similar to [6.38] for a dynamic stability problem, and showed that they can be reduced to a single linear second-order differential equation by the following transformation: U mn (t ) = KU Wmn (t ); Vmn (t ) = K V Wmn (t ) Bmn (t ) = K BWmn (t ); Tmn (t ) = KT Wmn (t ) where the coefficients Ki are given by Bert and Birman13 as KU = S1 + S 2 K B + S3 KT ; K V = S 4 + S5 K B + S 6 KT K B = D B D ; KT = D T D D B = (C35 + C15 S1 + C 25 S 4 )(C 45 + C14 S3 + C 24 S 6 ) - (C34 + C14 S1 + C 24 S 4 )(C55 + C15 S3 + C 25 S 6 ) D T = (C 45 + C15 S 2 + C 25 S5 )(C34 + C14 S1 + C 24 S 4 ) - (C 44 + C14 S 2 + C 24 S5 )(C35 + C15 S1 + C 25 S 4 )

[6.40]

IBF6 11/22/2000 6:35 PM Page 203

Elastic impact stress analysis of composite plates and cylinders D = (C 44 + C14 S 2 + C 24 S5 )(C55 + C15 S3 + C 25 S 6 ) - (C 45 + C14 S3 + C 24 S 6 )(C 45 + C15 S 2 + C 25 S5 ) S1 = (C12C 23 - C 22C13 ) S S 2 = (C12C 24 - C 22C14 ) S S3 = (C12C 25 - C 22C15 ) S S 4 = (C12C13 - C11C 23 ) S S5 = (C12C14 - C11C 24 ) S S 6 = (C12C15 - C11C 25 ) S

203

[6.41]

S = C11C 22 - C122 Substituting equation [6.40] into the third equation in [6.38] yields ˙˙ mn (t ) + K mn Wmn (t ) = 1 Qmn (t ) W rh rh

[6.42]

where the coefficients Kmn are given by K mn = -(C13 KU + C 23 K V + C33 + C34 K B + C35 KT )

[6.43]

The terms of the Fourier series representation for the load, applied uniformly over a small rectangular area, 2Rf1(l2 - l1), at the center of the cylindrical shell (L/2, 0) are Qmn (t ) = Pmn

F (t ) 2Rf1 (l 2 - l1 )

[6.44]

where Pmn =

mp mp 8 (l 2 + l1 ) sin (l 2 - l1 ) sin nf1 sin 2 2L 2L mnp

[6.45]

Substituting equation [6.44] into [6.42] and rearranging yields Pmn pRL F (t ) 2 ˙˙ mn (t ) + w mn W Wmn (t ) = Rf1 (l 2 - l1 ) m1

[6.46]

where ω2mn = Kmn/rh are the fundamental frequencies of the shell and m1 is the mass of the shell. For zero initial displacement and velocity, the solution of equation [6.46] is Wmn (t ) =

Pmn pRL Rf1 (l 2 - l1 )m1w mn

t

Ú F (t) sin w 0

mn

(t - t )dt

[6.47]

Using equations [6.47] and [6.40] with [6.36] results in expressions for the deformations in a shell under transverse loading, for example, the transverse deflection at any point of the shell is given by

IBF6 11/22/2000 6:35 PM Page 204

204

Impact behaviour of composite materials and structures w(x, q, t ) =

pRL Rf1 (l 2 - l1 )m1 ¥

Ú

t

0

Pmn

ÂÂw m

n

mn

sin

mpx cos nq L

[6.48]

F (t ) sin w mn (t - t )dt

6.3.3.3 Impact loading The response of a cylindrical shell to impact loading may be computed from the transient response, equation [6.48], by computing the impact force from the deceleration of the impactor mass. This procedure parallels that given previously above for plates in Section 3.2.2. The solution for the coefficients of the radial displacement are finally given by Wmn (t ) =

Pmn pRL Rf1 (l 2 - l1 ) m1

Âw j

Fj (w j sin w mnt - w mn sin w j t ) 2 2 mn (w j - w mn )

[6.49]

and by combining the above equations, the deflection and strain histories at any point of the shell can be evaluated. A series of impact experiments with transverse impact of laminated cylinders has been reported by Swanson et al.22 A typical comparison of a calculation made using the theory described above with three replicate experiments is shown in Fig. 6.7. It is seen that the comparison of calculated and measured strain is very reasonable.

6.4

The quasi-static approximation

The quasi-static calculation procedure involves treating the impact problem as an equivalent static problem with a static load applied to the impact site. By treating the impact mass and structure as a simple spring-mass system (neglecting the mass of the structure in comparison to the impact mass), the impact force can be obtained from the formula F = vi K st M i

[6.50]

where vi and Mi are velocity and mass of the impactor, and Kst is the static stiffness of the structure. This formula can equivalently be obtained by equating the kinetic energy of the impactor to the strain energy of the structure. The stresses and strains in the structure are then obtained from the static solution, using the force from equation [6.50]. It is possible to include the Hertzian contact law as developed by Sun et al.4,5 for anisotropic materials, to refine the above procedure.

IBF6 11/22/2000 6:35 PM Page 205

Elastic impact stress analysis of composite plates and cylinders

205

1000

500

Strain (10E-06)

0

-500

C6AV0D2 C8AV0D2

-1000 C9AV0D2 Predicted

-1500

-2000 -0.2

-0.0

0.2

0.4

0.6

0.8

1.0

1.2

1.4

1.6

Time (ms)

6.7 Comparison of analysis with strain gauge readings in impact of cylinders. The axial strains near the impact point in three separate experiments are shown. (After Swanson et al.22)

Clearly the quasi-static solution is much simpler to use than the structural dynamics solution. The question that arises is whether it is possible to determine the limits of applicability of the quasi-static solution, without recourse to a more complicated dynamic solution. A dimensionless parameter consisting of the ratio of the mass of the impactor to the ‘effective’ structure mass has been developed24 that permits identification of the range of applicability of the quasi-static solution. This procedure is briefly reviewed in the following.

6.4.1 Limits of quasi-static analysis An often employed rule-of-thumb is that the quasi-static approximation is valid if the frequency of the impact (say as defined by the contact duration) is less than 1/3 the lowest natural frequency of the structure.25 When dynamic effects in the structure do become important, the impact force and the resulting peak values of stresses and strains in the structure typically become larger than they would be for a given impact energy under quasistatic loading. This will be illustrated in calculations to be shown subsequently for impacts of plates and cylinders.

IBF6 11/22/2000 6:35 PM Page 206

206

Impact behaviour of composite materials and structures

The rule-of-thumb cited above does seem to be a reasonable method of ascertaining the limit of the quasi-static solution. However, it entails knowing at least the lowest natural frequency of the structure. This may be a significant drawback in some cases, as the point of the quasistatic approximation is to be able to analyse the impact event without knowledge of the dynamic solution. While it is easier to get a natural frequency of the structure than the entire dynamic response, there is still motivation for developing an alternative rule for the limits of the quasi-static approximation without knowing the structure’s natural frequency. This objective is pursued in the next section, following the work of Swanson.24

6.4.2 Alternative rule for limits of quasi-static approximation Intuitively it can be seen that if the impact mass is large with respect to the structure mass, the impact event can be treated as quasi-static. This idea can be simply related to the conventional rule for the ratio of natural frequencies given above. The approach taken is to develop an expression for an equivalent lumped mass, that can be used in conjunction with the static stiffness to approximate the lowest natural frequency of the structure. The definition of the equivalent mass will be given subsequently. The first premise to be advanced is that the lowest natural frequency of the structure can be approximated as wnª

K st meq

[6.51]

The impact frequency is given by wiª

K st meq + M i

[6.52]

Using the rule-of-thumb given above for the limits of quasi-static impact in terms of frequencies leads directly to the rule for the limits of validity of the quasi-static approximation as Mi ≥ 8meq 10meq

[6.53]

Thus a rule-of-thumb for the limits of the quasi-static approximation for impact problems has been formulated in terms of the ratio of impact mass to equivalent structure mass, which can be easily determined. The equivalent structure mass is defined here implicitly by the following formula,

IBF6 11/22/2000 6:35 PM Page 207

Elastic impact stress analysis of composite plates and cylinders 1 1 meq nc2 = Ú rn2 dVol 2 2 Vol

207 [6.54]

where meq is the equivalent lumped mass of the structure, vc is the peak velocity of the contact point for the impact, v is the peak velocity distribution throughout the impacted structure, and the integral is taken over the entire structure. The above expression is based on equating the energy of the equivalent lumped mass to the energy of the structure. If the assumption is made that the structure is undergoing motion in the mode determined by the quasi-static approximation, then the peak velocities are proportional to peak displacements, and the displacements are those calculated from a static application of load at the contact point.Thus, the above can be replaced by 1 1 meqd c2 = Ú rw 2 dVol 2 2 Vol

[6.55]

where here dc is the displacement at the point of impact, and w is the transverse displacement throughout the body as calculated by a static analysis. It is important to note that equation [6.55] enables the equivalent mass to be calculated from a knowledge of the static deformation of the body alone, without requiring access to a dynamic solution. The procedure given in [6.55] has been suggested for calculating lumped mass approximations, as presented by Steidel,26 for example, as an approximate method of calculating natural frequencies for beams and rods. The central issue at present is whether the equivalent lumped mass can be used to estimate the limits of suitability of a quasi-static solution for an impact problem. This is addressed in the following by comparing dynamic calculations with quasi-static calculations for various impact problems.

6.4.3 Comparison of dynamic and quasi-static impact response The calculations shown in this section will use solutions for impact problems of orthotropic plates and cylinders with various boundary conditions. Various example solutions for the impact response of structures were calculated using the procedures described above, for various values of impact mass. The equivalent masses of the structures were calculated using static solutions.55 The response quantities examined were the contact force, normal strains behind the impact point, and peak interlaminar shear stress values. In general, all of these response values start to increase relative to

IBF6 11/22/2000 6:35 PM Page 208

208

Impact behaviour of composite materials and structures

Ratio of dynamic to quasi-static solution

5

4

quasi-static (rule based on mass ratio = 10)

3

2

1

0 -2

-1

0

1

2

3

4

5

Log (projectile mass/effective structure mass)

6.8 Transition from quasi-static to dynamic response in impact of composite plates and cylinders. The variables shown are peak contact force, strain behind the impact point, and interlaminar shear stress. Plates are both simply supported and clampedclamped, free-free, and cylinders are of two lengths. (After Swanson24.)

the quasi-static solution when impact energy is held constant, as dynamic effects in the structure start to become important. A typical set of results for two different lengths of an orthotropic cylinder and plate solutions for two different sets of boundary conditions, using the calculational procedures discussed above, are shown in Fig. 6.8. These results have been normalised by dividing by the quasi-static solution, holding impact energy constant, and plotted as a function of the ratio of impact mass to equivalent structure mass as calculated by equation [6.55]. The critical ratio of impact mass to equivalent structure mass has been taken as 10 from [6.53], and is also shown. It can be seen that this rule is in fact a reasonable estimate of the limit of the validity of the quasi-static approximation. Qualitatively the results are quite comparable, as the value of 10 for the ratio of impact mass to equivalent structure mass appears to represent the limit of the quasi-static approximation for both the plates and cylinders reasonably well.

IBF6 11/22/2000 6:35 PM Page 209

Elastic impact stress analysis of composite plates and cylinders

209

3000 l=1 l=2 l=3 l=4 l=5

2500

ey at A (microstrain)

2000

1500

1000

500

0

-500 0

100

200

300

400

500

Time/l (ms)

6.9 Comparison of strain response in impact tests on five different plate sizes. Plates are scaled geometrically by the parameter l, and the analysis shows that time is also scaled by l. (After Qian and Swanson16.)

6.5

Issues of scaling in impact

The question of scaling, i.e. extrapolating from tests on small laboratory specimens to larger structures, is an important issue in impact. This issue has been addressed by a number of authors, including Morton,27 Sankar,28 Qian et al.,29 Qian and Swanson,16 Swanson et al.,22 and others. Analytical solutions such as those discussed in the above are very helpful in understanding the issues of scaling, as the governing equations can be manipulated to reveal the dimensionless parameters involved.An approach taken16,22,29 was to use geometric scaling, which also dictated the scaling of time. A typical result of scaled impact experiments on plates is shown in Fig. 6.9, where the linear response is found to scale within the basic reproducibility of the experiments for five sizes of plates. Scaling of the damage formation resulting from impact is more complicated. For example, Swanson30 found that the scaling associated with delamination resulting from impact is that characteristic of fracture mechanics. Christoforou and Yigit31,32 also address

IBF6 11/22/2000 6:35 PM Page 210

210

Impact behaviour of composite materials and structures

scaling of impact, and in addition develop dimensionless numbers characterising impact with respect to the relative importance of indentation, and the conditions for quasi-static analysis to be applicable.

6.6

Summary and conclusions

The fundamental equations and some solution procedures have been presented for elastic impact of laminated plates and cylinders. Issues of convergence and accuracy have been addressed, and comparisons with experimental data have been given. The results show that the linear response of these fundamental structural elements is reasonably well understood.

References 1 Zukas J A, et al., Impact Dynamics, New York, Wiley, 1982. 2 Joshi S P and Sun C T, ‘Impact induced fracture in a laminated composite’, J Composite Mater, 1985 19 51–66. 3 Sun C T and Chattopadhyay S, ‘Dynamic response of anisotropic laminate plates under initial stress to impact of a mass’, J Appl Mech, 1975 42 693–8. 4 Yang S H and Sun C T, ‘Indentation law for composite laminates’, Composite Materials: Testing and Design (Sixth Conference), ASTM STP 787, pp 425–49, 1982. 5 Tan T M and Sun C T, ‘Use of statical indentation laws in the impact analysis of laminated composite plates’, J Appl Mech, 1985 52 6–12. 6 Lekhnitskii S G Anisotropic Plates, transl S W Tsai and T Cheron, New York, Gordon and Breach Science, 1968. 7 Whitney J M and Leissa A W, ‘Analysis of a simply-supported laminated anisotropic rectangular plate’, AIAA J, 1970 7 28. 8 Whitney J M and Pagano N J, ‘Shear deformation in heterogeneous anisotropic plates’, J Appl Mech, 1970 37 1031. 9 Dobyns A L, ‘Analysis of simply-supported orthotropic plates subject to static and dynamic loads’, AIAA J, 1981 19 642. 10 Birman V and Bert C W, ‘Response of composite plates to blast loading’, in Proc ICCM & ECCM Conf, 5, Imperial College of Science and Technology, London, July 20–24, 5.192, 1987. 11 Christoforou A P and Swanson S R, ‘Analysis of simply-supported orthotropic cylindrical shells subject to lateral impact loads’, J Appl Mech, 1990 57 376–82. 12 Christoforou A P and Swanson S R, ‘Analysis of impact response in composite plates’, Intl J Solids Struct, 1991 27 161–70. 13 Bert C W and Birman V, ‘Dynamic stability of thick, orthotropic, circular cylindrical shells’, in Lecture Notes in Engineering: Refined Dynamic Theories of Beams, Plates and Shells and Their Applications, Springer-Verlag, Berlin, 235, 1987. 14 Bert C W and Chen T L C, ‘Effect of shear deformation on vibration of antisymmetric angle-ply laminated rectangular plates’, Int J Solid Struct, 1978 14 465.

IBF6 11/22/2000 6:35 PM Page 211

Elastic impact stress analysis of composite plates and cylinders

211

15 Cairns D S and Lagace P A, ‘Transient response of graphite/epoxy and kevlar/epoxy laminates subjected to impact’, presented at 29th Structures, Structural Dynamics and Materials Conference (not published in Proceedings), 1988. 16 Qian Y and Swanson S R, ‘Experimental measurement of impact response in carbon/epoxy plates’, AIAA J, 1990 28 1069–74. 17 Timoshenko S and Young D H, Vibration Problems in Engineering, 3rd edn, Van Nostrand, New York, 1955. 18 Qian Y and Swanson S R, ‘A comparison of solution techniques for impact response of composite plates’, Composite Struct, 1990 14 177–92. 19 Sun C T and Chen J K, ‘On the impact of initially stressed composite laminates’, J Composite Mater, 1985 19 490. 20 Ramkumar R L and Thakar Y R, ‘Dynamic response of curved laminated plates subjected to low velocity impact’, ASME J Eng Mater Technol, 1987 109 67–71. 21 Vinson J R and Chou T W, Composite Materials and Their Use in Structures, Applied Science, London, 1975. 22 Swanson S R, Smith N L and Qian Y, ‘Analytical and experimental strain response in impact of composite cylinders’, Composite Struct, 1991 18 95–108. 23 Mindlin R D, ‘Influence of rotary inertia and shear on flexural motions of isotropic elastic plates’, ASME J Appl Mech, 1951 18 31–8. 24 Swanson S R, ‘Limits of quasi-static solutions in impact of composite structures’, Composites Eng, 1992 2 261–7. 25 Cook R D, Malkus D S and Plesha M E, Concepts and Applications of Finite Element Analysis, 3rd edn, New York, Wiley, 1989. 26 Steidel R F, An Introduction to Mechanical Vibrations, 3rd edn, New York, Wiley, 1989. 27 Morton J, ‘Scaling of impact-loaded carbon-fiber composites’, AIAA J, 1988 26 989–94. 28 Sankar B V, ‘Scaling of low-velocity impact for symmetric composite laminates’, J Reinforced Plastics Composites, 1992 11 296–309. 29 Qian Y, Swanson S R, Nuismer R J and Bucinell R B, ‘An experimental study of scaling rules for impact damage in fiber composites’, J Composite Mater, 1990 24 559–70. 30 Swanson S R, ‘Scaling of impact damage in fiber composites from laboratory specimens to structures’, Composite Struct, 1993 25 249–55. 31 Yigit A S and Christoforou A P, ‘Impact dynamics of composite beams’, Composite Struct, 1995 32 187–95. 32 Christoforou A P and Yigit A S, ‘Characterization of impact in composite plates’, Composite Struct, 1998 43 15–24.

IBF7 11/22/2000 6:42 PM Page 212

7 Impact behaviour and analysis of CFRP laminated plates ENBOA WU AND CHENG-ZORN TSAI

7.1

Introduction

The low-velocity impact behaviour of composite laminates has been studied extensively in recent decades. As described in two review papers,1,2 experimental results reported in the literature have mainly focused on impactinduced damage mechanisms, such as matrix cracking, delamination and fiber breakage in different impact stages; on the other hand, most of the analytical methods have focused on elastic impact on laminates with perfect boundaries. Aside from direct investigation of the laminate damage using the naked eye, such as for glass/epoxy laminates that are partially light transparent,3–5 C-scan or X-ray has mostly been employed in damage assessment.6,7 A focused treatment of this topic is available in Chapter 2. The apparatus that has provided the impact energy has usually been a drop weight tower. Due to the limitation of the tower height, almost all the impact events have been conducted using a heavy impactor at a velocity of less than 10 m/s. The impact force has usually been recorded by a force transducer embedded in the impactor. The corresponding histories of energy, velocity, and displacement were then derived once the onset of contact between the impactor and the target was detected by Cantwell and Morton8 and others in Chapters 5 and 8. On the other hand, the higher-speed impact results published in the literature have been far fewer than those for lower-speed impact. One reason has been the need for a gas gun to provide the initial kinetic energy of the impactor. In this category, impact has generally been conducted using a lighter impactor, most of the time called a projectile, at a much higher initial velocity. Further, because it is very difficult to mount a sensor in a flying projectile,9,10 the data recorded during such an impact event has usually been only the initial and the final states of the projectile and the target. The history of impact, even if a high-speed camera was employed, was very hard to record. For example, Gupta and Davids back in 196611 used a rifle to launch projectiles which struck glass/epoxy laminates at impact speeds from 212

IBF7 11/22/2000 6:42 PM Page 213

Impact behaviour and analysis of CFRP laminated plates

213

305 to 387 m/s and found a linear relationship between the projectile energy loss and the target thickness.Takeda et al.12,13 studied the delamination crack propagation phenomena of glass/epoxy laminates for projectiles at initial speeds up to 83 m/s. Cantwell and Morton investigated the effects of laminate thickness, dimensions, and stacking sequence on the penetration energy threshold.14–16 Zhu et al. reported the impact phenomena for kevlar/polyester composites struck by cylindrically-conical projectiles.17 The results of impact on graphite/epoxy laminates by blunt projectiles were reported by Lee and Sun.18,19 The effect of the strain rate on the penetration behaviour was also uncovered by Jenq et al.20 and Wu and Chang.5 Other high-velocity impact studies can be found in Chapters 8 and 9. Meanwhile, as the composite laminated structures used in modern industry have rapidly increased, the need to more accurately predict the impact response of such advanced structures has become inevitable. In the past, most of the studies focused on the development of analytical or numerical methods to predict the elastic response of laminated beams,21 plates22–25 and shells,26 and the relationship between the impactor and the struck laminate was frequently modelled using the modified Hertz contact law,27 which was verified experimentally7,28 and analytically.29,30 A further example is available in Chapter 6. On the other hand, the inverse method was found to be able to detect the impact force, location, impactor mass and velocity using the response, which sometimes was even incomplete, of the struck plate.31–35 This method was also found to be able to reconstruct forces in bar-to-bar impact problems.36 However, most, if not all, of the experimental results reported in the literature for impact on graphite/epoxy composite laminates involving a gas gun, i.e. high-velocity impact, described only the final state, and in the analytical predictions, the laminates were all assumed to have perfect boundary conditions. In this chapter, the goal is to obtain the impact history of such advanced structures when they are struck by projectiles in a velocity range that is from very low to way above the ballistic limit of the targets, and to present an analytical method that can take boundary imperfection into consideration. In the experimental investigation, a gas gun was employed to launch a hemispherically tipped projectile to strike a 32-layered quasiisotropic graphite/epoxy laminate. Transient laser Doppler anemometry (TLDA), which was developed at the National Taiwan University and is a noncontact measurement method having a 1.0 ms sampling rate, was employed to extract the velocity history of the projectile while it was striking the target. This excellent technique has been successfully employed to uncover the impact process of metallic targets,37,38 glass/epoxy laminates39,40 and honeycombs.41 The force and the displacement histories were then subsequently derived. Thus, the terminal velocity, impact energy, absorbed energy, peak force and momentum change were obtained. The impact

IBF7 11/22/2000 6:42 PM Page 214

214

Impact behaviour of composite materials and structures

response of this laminated structure will be discussed in detail using these data and the measured laminate damage area. On the other hand, the Ritz method along with the Mindlin plate theory was employed to construct the governing equations of a laminated plate under impact conditions. In order to predict the impact response of a laminate under ‘imperfect’ boundary conditions, two beam functions, one satisfying simply supported conditions and the other satisfying fixed conditions, were employed, and a non-dimensional constant that represents the rotational spring constant of the physical clamp was used. The actual value of the rotational spring constant was obtained from the quasi-static contact test result. The correlation between the prediction and the measured data will be used to verify the presented method.

7.2

Experimental set-up and procedure

7.2.1 Specimen Fiberite Hy-E 1076E T300/976 graphite/epoxy prepregs were employed to fabricate the specimens using an autoclave. All the specimens were 32-ply (0/45/90/–45)4S quasi-isotropic laminates. The nominal thickness was 4.3 ± 0.1 mm. The in-plane dimensions were 152.4 mm by 101.6 mm. The 0° laminae were along the long dimension. Two types of boundary conditions were employed. In the first type, the plates were suspended by two light strings attached to two adjacent corners of the plate to simulate the free boundary condition, and was used for verification of the presented analytical method as the boundary can easily be made to be perfect. On the other hand, in most of the test runs, the laminates were tightly clamped on two opposite edges with the other two free of support, resulting in a clamped span of 101.6 mm and leaving the original short dimension of 101.6 mm as the free span. After the specimens were struck, they were C-scanned to uncover the delamination damage profile. In this study, the delamination area was defined as the area that was enclosed by the outermost crack fronts in all the interfaces along the thickness direction of the laminate.

7.2.2 Experimental procedure The transient laser Doppler anemometer (TLDA), which was developed in the Impact and Precision Measurement Laboratory of National Taiwan University, was employed for extraction of the quickly changing velocity history of a projectile during impact and penetration.38 This is a backscattering arrangement. It allows the Doppler signals to scatter backward to the optical devices through which the laser beams originally passed. The principle of laser Doppler anemometry is to intersect two coherent light beams to form a small measuring volume in an ellipsoidal shape, whose

IBF7 11/22/2000 6:42 PM Page 215

Impact behaviour and analysis of CFRP laminated plates

215

size depends upon the beam diameter and the light intersection angle, 2k, and is usually only a few mm in all three ellipsoidal axes. Because of light interference, fringes of spacing df are formed inside the measuring volume. When particles on the surface of a projectile travel across the fringes inside the measuring volume, light is scattered. By recording the history of this scattered light, the velocity history of the surface of the projectile can be obtained using the following equation:42,43 V=

l fD 2 sin k

[7.1]

where l is the wave length of the coherent light and fD is the frequency of the Doppler signal. In this study, l = 632.8 nm and k = tan-1 (1/20). Thus, df = l/(2 sin k) = 6.336 mm and V = 6.336 ¥ 10-6 fD m/s. A detailed description of the LDA principle can be found in Durst et al.42 and Drain.43 The experimental set-up for the impact test is schematically shown in Fig. 7.1. A gas gun was employed to launch a hemispherically tipped projectile, made of hard steel, of 12.7 mm diameter. The mass of the projectile was 35.6 g, and its length was 38.0 mm. The projectile was hardened to Rc60 to avoid possible plastic deformation during impact. The transient laser Doppler anemometer (TLDA) system included a 35 mW He–Ne laser light source, a series of optical devices for passage of the laser light and the scattered Doppler signals, a photomultiplier for conversion of the scattered Doppler signals into electric current, and a bandpassed filter for filtering out noises and pedestal signals carrying the Doppler signals. To simplify the process, the zero-crossing method was employed to extract the velocity history from the recorded Doppler signals. This was similar to the method used by Wu and Chang for impact on glass/epoxy laminates.4,5 On the other hand, a complete description of the implementation procedure for TLDA can be found in Tsai and Wu.38 After the velocity data were obtained, the acceleration history could be retrieved, in principle, by means of differentiation. In order to avoid errors from being induced in the acceleration due to direct differentiation, the smoothing cubic-spline method was employed. This method was a modification of the cubic-spline interpolation method, in which a function, f(x), in the following form is usually used:44 2

3

f (x) = a i + bi (x - x i ) + c i (x - x i ) + di (x - x i ) x i £ x £ x i+1 i = 1, 2, . . . , n - 1

[7.2]

where (xi, yi), i = 1, 2, . . . , n; n > 3 are the recorded discrete data points set and yi = f(xi). To suppress the noise, an objective function E is defined as i= N

E(a i , S ) =

Â (y i=1

2

i

- ai) + S Ú

xN

x1

2

[ f ¢¢(x)] dx

[7.3]

IBF7 11/22/2000 6:42 PM Page 216

Impact behaviour of composite materials and structures

7.1 A schematic of the experimental set-up for impact on composite laminates.

216

IBF7 11/22/2000 6:42 PM Page 217

Impact behaviour and analysis of CFRP laminated plates

217

where S is the smoothing parameter. The first term in [7.3] represents the deviation between f and the data point, and the second term is the smoothing level of f. A detailed description of the smoothing cubic-spline method can be found in de Boor.44 This method acts as a low-pass filter to the velocity data extracted from Doppler signals. The acceleration history was then obtained by means of direct differentiation of the function f. A detailed description of the implementation procedure can also be found in Tsai45 and examples shown in later sections. On the other hand, the displacement history was obtained by means of direct integration of the velocity data. The time for the onset of contact between the projectile and the target was precisely determined using a piezo-film attached at the center of the distal side of the laminated plate.37

7.3

Near-elastic impact behaviour

In this velocity range, no damage was found in laminates using both visual inspection by means of the naked eye and C-scan. The impact velocity of the projectile was lower than 20 m s-1. Typical velocity and force histories for the struck laminates in this category are shown in Fig. 7.2(a) and (b), which shows projectile impact results at 8.3 and 14.5 m s-1, respectively. Before the onset of contact, the velocity remained constant. This value dropped drastically once the projectile hit the target, and caused the projectile to indent the laminate in the contact region. The amount of indentation was equal to the difference of movement between the target and the projectile, and could be related to the impact force using the modified type of Hertz contact law.7 Thus, this indentation caused the impact force to increase drastically. In the meantime, the impact neighbourhood of the target started to move forward owing to the action of the projectile. This movement immediately decreased the indentation value, and the force dropped almost as sharply as in the rising part, thus forming the first peak. As impact proceeded, the velocity of the impact neighbourhood of the struck laminate was reduced due to the action of the bending stiffness of the laminate. As a result, the value of the indentation increased again. This resulted in a drastic increase of the force value. In this study, the second force peak was always observed when the laminate was not significantly damaged and occurred when the projectile velocity decreased to approximately zero, as typically shown in Fig. 7.2(a) and (b). It is interesting to note that a third force peak was also observed, and that the projectile physically separated from the target before the third peak occurred. Further, this phenomenon occurred when the projectile velocity was negative. Apparently, the projectile was hit by the target when the target bounced back. Due to the force exerted by the bouncing target,

IBF7 11/22/2000 6:42 PM Page 218

Impact behaviour of composite materials and structures 2.5 Vi = 8.3 ms–1 Vt = –6.4 ms–1 Fp = 2.30kN

2.0 1.5

0 1.0 –5

0.5

–10 –0.2

–0.0

0.2 0.4 Impact time (ms) (a)

0.6

0.0 0.8

4.0 Vi = 14.5 ms–1 Vt = –10.7 ms–1 Fp = 3.70kN

10 0

2.0

–10

1.0

–20 –0.2

–0.0

0.2 0.4 Impact time (ms) (b)

0.6

30 Velocity (ms–1)

3.0

Force (kN)

Velocity (ms–1)

20

0.0 0.8

5.0 Vi = 22.2 ms–1 Vt = –13.8 ms–1 Fp = 4.29kN

20 10

4.0 3.0

0

2.0

–10

1.0

–20 –0.2

–0.0

0.2 0.4 Impact time (ms) (c)

0.6

0.0 0.8

4.0

30 Velocity (ms–1)

Force (kN)

5

Force (kN)

Velocity (ms–1)

10

Vi = 24.4 ms–1 Vt = –15.2 ms–1 Fp = 3.27kN

20 10

3.0 2.0

0 1.0

–10 –20 –0.2

–0.0

0.2 0.4 Impact time (ms) (d)

0.6

Force (kN)

218

0.0 0.8

7.2 Velocity and force histories for laminates struck at (a) 8.3 m s-1; (b) 14.5 m s-1; (c) 22.2 m s-1; (d) 24.4 m s-1; (e) 31.8 m s-1; and (f) 36.2 m s-1.

IBF7 11/22/2000 6:42 PM Page 219

Impact behaviour and analysis of CFRP laminated plates 5.0 Vi = 31.8 ms–1 Vt = –5.1 ms–1 Fp = 4.23kN

30 20

4.0 3.0

10

2.0

0

1.0

–10 –0.4

–0.0

0.4

0.8

1.2

Force (kN)

Velocity (ms–1)

40

219

0.0 1.6

Impact time (ms) (e) 4.0 Vi = 36.2 ms–1 Vt = 10.0 ms–1 Fp = 3.63kN

30

3.0

20

2.0

10

1.0

0 –0.4

Force (kN)

Velocity (ms–1)

40

0.0 –0.0

0.4

0.8

1.2

1.6

Impact time (ms) (f)

7.2 (cont.)

the absolute value of the projectile velocity increased again, but in the negative direction.The impact process terminated when the bouncing target was pulled again in the forward direction due to its bending stiffness, at which point the projectile gained enough momentum from the bounced target and started to separate permanently from the target. The relationship between the impact and the terminal velocities for the event in which the struck laminates showed no delamination damage is illustrated in Fig. 7.3. A straight line was found to fit the relationship fairly well. Thus, the relationship between the absorbed energy, DE, and the impact velocity, Vi, was found to be quadratic, as shown in Fig. 7.4. On the other hand, a straight-line relationship is also observed in Fig. 7.5 between the impact velocity and the maximum force peak for each test run. Note that, in Fig. 7.2(a) and (b), the first peak in the multi-peak impact event always has the highest magnitude. This is because the largest indentation value between the projectile and the target always occurred very shortly after the onset of first contact. During this very short period the target did not deform extensively. As a result, the target response to impact was not similar to the target response to quasi-static loading because the peak force in the latter case always occurred when the deflection was largest.

IBF7 11/22/2000 6:43 PM Page 220

Impact behaviour of composite materials and structures 100 Measured Predicted

Terminal velocity (ms–1)

80

60

40

20

0 0

20

40

60

80

100

120

Impact velocity (ms ) -1

7.3 The relationship between the impact velocity, Vi and the terminal velocity, Vt of the projectile.

25

20 Absorbed energy (J)

220

15

10

5

0 0

20

40

60

80

100

120

Impact velocity (m s -1)

7.4 The relationship between the impact velocity, Vi of the projectile and the absorbed energy of the struck laminates.

IBF7 11/22/2000 6:43 PM Page 221

Impact behaviour and analysis of CFRP laminated plates

221

6

Peak impact force (kN)

5

4

3

2

1

0 0

20

40

60

80

100

120

Impact velocity (m s ) -1

7.5 The relationship between the impact velocity, Vi and the peak impact force of the projectile.

7.4

Prediction of elastic impact response

7.4.1 Governing equations The method presented in this section was derived using the Ritz method, and the Mindlin plate theory was adopted. The displacement field, by neglecting the in-plane deformation of the plate, reads u1 (x, y, z, t ) = za (x, y, t ) u2 (x, y, z, t ) = z b (x, y, t )

[7.4]

u3 (x, y, z, t ) = w (x, y, t ) where u1, u2 and u3 are the displacements in the x, y and z directions of the plate; a ¯ and b¯ are the rotations of the plate in the x and y directions, respectively; and w is the lateral deflection of the plate. The strain-displacement relations become Ê e xx ˆ Ê e1 ˆ Ê a ,x ˆ Á e yy ˜ = Á e 2 ˜ = zÁ b,y ˜ Á ˜ Á ˜ Á ˜ Ë 2 e xy ¯ Ë e 6 ¯ Ë a ,y + b, x ¯ Ê 2 e yz ˆ Ê e 4 ˆ Ê b + w ,y ˆ = = Ë 2 e zx ¯ Ë e 5 ¯ Ë a + w , x ¯

[7.5]

IBF7 11/22/2000 6:43 PM Page 222

222

Impact behaviour of composite materials and structures

For each lamina, the constitutive relations are Ê s xx ˆ Ê s1 ˆ ÈQ11 Q12 Q16 ˘ Ê e1 ˆ Á s yy ˜ = Á s 2 ˜ = ÍQ12 Q22 Q26 ˙ Á e 2 ˜ ˙Á ˜ Á ˜ Á ˜ Í Ë t xy ¯ Ë s 6 ¯ ÍÎQ16 Q26 Q66 ˙˚ Ë e 6 ¯

[7.6]

ÈQ44 Ê t yz ˆ Ê s 4 ˆ = = kÍ Ë t zx ¯ Ë s 5 ¯ ÎQ45

[7.7]

Q45 ˘ Ê e 4 ˆ Q55 ˙˚ Ë e 5 ¯

where Qij is the reduced elastic constant under the plane-stress conditions and k is the shear correction factor, whose value was taken to be 5/6. The kinetic and strain energy for the laminate is, respectively, h

T=

1 b a 2 r(u˙ 12 + u˙ 22 + u˙ 32 )dzdxdy 2 Ú0 Ú0 Ú-2h

V=

1 b a 2 (s1 e1 + s 2 e 2 + s 6 e 6 + s 4 e 4 + s 5 e 5 )dzdxdy 2 Ú0 Ú0 Ú-2h

[7.8]

and h

[7.9]

where r is the density of the laminate. On the other hand, the work done by the external force, P(x, y, t), applied normally to the plate is W =Ú

b

0

Ú

a

0

P(x, y, t )u3 dxdy.

[7.10]

In order to apply the Ritz method, beam functions that satisfy the geometric boundary conditions of the plate were adopted, and the three independent variables are expressed by the series expansion: a (x, y, t ) =

Âa

b (x, y, t ) =

Â b (t )x (x)h¢ ( y)

w (x, y, t ) =

Âw

ij

ij

ij

ij

(t )x ¢i (x)h j ( y)

ij

i

ij

j

[7.11]

(t )x i (x)h j ( y)

where x(x) and h(y) are beam functions in the x and y directions, respectively. Note also that x¢(x) and h¢(y) are included in the above equation in order to avoid the erroneous shear locking phenomenon when the plate becomes very thin.31 The governing equation in the form of

[ M ]{q˙˙} + [ K ]{q} = {P *}

[7.12]

can be derived by applying the Hamilton principle of t2

d Ú (T - V )dt = 0 t1

[7.13]

IBF7 11/22/2000 6:43 PM Page 223

Impact behaviour and analysis of CFRP laminated plates

223

where the generalised coordinates, q, are in the form of T

{q} = {a11 , a12 , . . . , a 21 , . . . ; b11 , b12 , . . . b 21 , . . . ; w11 , w12 , . . . , w 21 , . . .}. [7.14] On the other hand, the generalised force, P*, can be obtained from P. In this study, the area of contact between the projectile and the plate was small. Thus, a point load assumption is justified, and [7.10] is simplified as b

a

Â Ú Ú P(t )d(x - x )d( y - y ) ◊ w = P(t )(Â w (t )x (x )h ( y ))

W=

ij 0

0

0

ij

ij

0

i

T

0

ij

(t )x i (x)h j ( y)dxdy [7.15]

0

j

T

= P(t ){q} {Y *} = {q} {P *} where T

{Y *} = {0, 0, . . . , 0, 0, . . . , x1 h1 , . . . , x1 h2 , . . . , x 2 h1 , . . .}( x 0 ,y 0 ) . [7.16] Equation [7.12] can be further simplified by neglecting the effect of rotational inertia:31 È0 ÍÎ 0

0 ˘Ê q˙˙1 ˆ È K11 + M 22 ˙˚Ë q˙˙ 2 ¯ ÍÎ K 21

K12 ˘Ê q1 ˆ Ê 0 ˆ = K 22 ˙˚Ë q 2 ¯ Ë P2 ¯

[7.17]

* ]{q 2 } = {P2 } [ M22 ]{q˙˙ 2 } + [ K 22

[7.18]

where T

-1

[ K 22* ] = [ K 22 ] - [ K12 ] [ K11 ] [ K12 ]

[7.19]

and -1

{q1} = -[ K11 ] [ K12 ]{q 2 } T

{q 2 } = {a11 , a12 , . . . , a 21 , . . . ; b11 , b12 , . . . , b 21 . . .}

[7.20]

T

{q 2 } = {w11 , w12 , . . . , w 21 , . . .} T

{P2 } = P(t ){x1 h1 , x1 h2 , . . . , x 2 h1 , . . .}( x 0 ,y 0 ) = P(t ){Y }

T

7.4.2 Solution scheme The response of the projectile, on the other hand, is expressed in the form of mS˙˙(t ) = - P(t )

[7.21]

where m is the mass of the projectile and S is the projectile movement. The modified Hertz contact law, by assuming the projectile to be rigid, is then employed:7,28

IBF7 11/22/2000 6:43 PM Page 224

224

Impact behaviour of composite materials and structures f (a ) =

4 3 2 REz (a ) 3

[7.22]

where R is the radius of the projectile head and Ez is the Young’s modulus of the laminate in the thickness direction. In this equation, the indentation, a, is defined as the difference between s(t) and w0(t), and the impact force P(t) is equal to f(a), where w0(t) is the laminate deformation in the thickness direction at the contact location. In this study, the central difference method was employed. Thus, equations [7.18] and [7.21] can be expressed in the following discrete forms: 2

-1

2

-1

* ]{q 2 } {q 2 } j+1 = Pj (Dt ) [ M22 ] {Y } - (Dt ) (M22 ) [ K 22 j + 2{q 2 } j - {q 2 } j-1 2

S j+1 = Pj (Dt ) m + 2 S j - S j-1

[7.23] [7.24]

Comparisons between the prediction and the test results are shown in Fig. 7.6(a) and (b), in which the histories of the velocity and force are plotted. The initial striking velocity was 7.46 m s-1. The overall correlation is considered to be very satisfactory. Thus, the presented method has been demonstrated to be suitable for impact prediction of laminated structures.

7.4.3 Modeling of physically clamped boundaries As stated in the Introduction, the boundary of a laminated plate, except for one under free-free boundary conditions, can hardly be considered as being perfect due to elastic deformation and material and geometric imperfection of both the laminate and the clamped pads. Figure 7.7(a) and (b) shows typical results for a laminate that was physically clamped on two opposite sides and struck by a 35.6 g projectile at an impact velocity of 4.3 m/s. Also shown in these figures are two predictions made under the assumption that the boundary was simply supported and fully clamped. It is found that neither correlates with the experimental data. Thus, it is essential to develop a method that takes the physical boundary condition into consideration. In order to model the boundary of a laminated plate that is physically clamped on its two opposite sides with the other two free of support, this nearperfect clamped boundary was modeled as a simple support with an elastic restrained edge; i.e. a finite rotational angle was allowed on the clamped sides. Thus, using the Ritz approach, where the displacement field was constructed by means of a series of orthogonal beam functions, the eigenfunction of such a beam can be derived from the following equation: mü + EIu≤≤ = 0

[7.25]

IBF7 11/22/2000 6:43 PM Page 225

Impact behaviour and analysis of CFRP laminated plates

225

8 Experimental data Prediction

7

Impact velocity (m s -1)

6 5 4 3 2 1 0 -0.2

-0.1

-0.0

0.1

0.2

0.3

0.4

0.5

0.6

0.5

0.6

Impact time (ms) (a) 2.0 Experimental data Prediction

1.8

Impact force (kN)

1.5 1.3 1.0 0.8 0.5 0.3 0.0 -0.2

-0.1

-0.0

0.1

0.2

0.3

0.4

Impact time (ms) (b)

7.6 (a) The velocity history and (b) the force history for a 35.6 g projectile striking at 7.46 m s-1. Both the measurement data and the prediction using the Ritz method are plotted.

IBF7 11/22/2000 6:43 PM Page 226

226

Impact behaviour of composite materials and structures 6 Experimental data Prediction (Simple support) Prediction (Fixed-end)

Impact velocity (m s -1)

4

2

0

-2

-4 -0.1

-0.0

0.1

0.2

0.3

0.4

0.5

0.6

0.7

0.8

0.6

0.7

0.8

Impact time (ms) (a) 1.6 Experimental data Prediction (Simple support) Prediction (Fixed-end)

Impact force (kN)

1.2

0.8

0.4

0.0 -0.1

-0.0

0.1

0.2

0.3

0.4

0.5

Impact time (ms) (b)

7.7 The measured (a) velocity and (b) force histories for a laminated plate that was struck by a 35.6 g projectile at 4.3 m s-1 and was physically clamped on two opposite sides with the other two sides free of support. Also shown are the Ritz predictions, which treat the boundary as being simply supported and fully clamped.

IBF7 11/22/2000 6:43 PM Page 227

Impact behaviour and analysis of CFRP laminated plates

227

The corresponding boundary conditions are u(0, t ) = u(l , t ) = 0 u ¢¢(0, t ) =

K u ¢(0, t ) EI

u ¢¢(l , t ) = -

[7.26]

K u ¢(l , t ) EI

where m is the mass per unit length, u(x, t) is the transverse displacement, and E and I are the Young’s modulus and the moment of inertia, respectively, of such a beam. On the other hand, K is the stiffness of the rotational spring, and l is the length of the beam. The value of K represents the rotational stiffness of the boundary. In the two extreme cases when K reaches zero and infinity, the simply supported and the fixed end conditions are obtained, whose beam functions are f s (x) =

2 EIa (sinh al sin ax - sinh ax sin al ) (sinh al - sin al )

[7.27]

and f c (x) = (cosh ax - cos ax) -

cosh al - cos al (sinh ax - sin ax) sinh al - sin al [7.28]

respectively. On the other hand, when the value of K falls in between the two extremes, the beam function becomes a combination having the following form: f(x) = f s (x) K + f c (x)

[7.29]

and note that a must satisfy the following characteristic equation: 2

2

Ê K ˆ (cosh al cos al - 1) + 2Ê K ˆ (cos al sinh al - sin al cosh al ) Ë EIa ¯ Ë EIa ¯ [7.30] - 2 sinh al sin al = 0 By selecting a proper value of K, a real boundary condition that reflects the physically clamped condition can be obtained. In this study, the K value was determined from a quasi-static test result, in which the boundary conditions, the shape of the indentor, and the laminate being tested remained identical to those tested under impact conditions. The optimal K, by which the correlation between the predicted Ritz

IBF7 11/22/2000 6:43 PM Page 228

228

Impact behaviour of composite materials and structures

method and the experimental result was the best, was then searched. For analysis purposes, a non-dimensional value was employed: S Kl = 1 - S EI

0£S£1

[7.31]

Note that S ranges between 0 and 1. In this study, S = 0.93 was found to be optimal. The predictions obtained using S = 0.93 and the measured data are shown in Fig. 7.8(a) and (b). It is found that the correlation is much better. Other similar comparisons can be found in Tsai.45 This demonstrates that the developed method is capable of predicting the impact response of a laminate under physically clamped boundaries. On the other hand, the deviation between the measurement and the prediction is more noticeable in Fig. 7.8(a) and (b) as compared with the example shown in Fig. 7.6(a) and (b), in which the plate is subject to free-free boundary conditions. This might to be due to the assumption of the uniform boundary condition along the clamped boundary. Other factors contributing to the deviation include the assumptions that the boundary behaviours due to the quasi-static and to the impact loads are identical, that S remains unchanged during loading and unloading processes, etc.

7.5

Impact beyond the delamination threshold

7.5.1 Delamination damage Delamination damage was observed when the impact velocity increased to 20.3 m s-1, at which point the terminal velocity was -13.8 m s-1 and the area calculated based on the C-scan run was 2.90 cm2. Under this impact condition, no damage was found on either the front or the distal surfaces of the struck laminate. Thus, delamination should be the only observed damage mechanism. However, because the absorbed energy ratio of DE/Ei = 0.48 remained essentially identical to that for impact at Vi = 14.5 m s-1, under which condition no delamination damage was observed, this damage alone did not absorb a significant amount of the impact energy. As a result, the impact histories of the force and velocity have profiles very similar to the results shown in Fig. 7.2(a) and (b) and, thus, are not plotted again. Similarly, the impact velocity versus the terminal velocity of the projectile, shown in Fig. 7.3, continuously follows the same linear relationship, and the absorbed energy, shown in Fig. 7.4, follows the same quadratic curve. From these revealed impact results, it is found that the responses of the projectile remained the same regardless of whether or not the impact was beyond the delamination threshold of the laminates.

IBF7 11/22/2000 6:43 PM Page 229

Impact behaviour and analysis of CFRP laminated plates 6 Experimental data Ritz method, S = 0.93

Impact velocity (m s -1)

4

2

0

-2

-4 -0.1

0.1

0.5

0.3

0.7

Impact time (ms) (a)

1.2 Experimental data Ritz method, S = 0.93

Impact force (kN)

0.8

0.4

0.0 -0.1

-0.0

0.1

0.2

0.3

0.4

0.5

0.6

0.7

Impact time (ms) (b)

7.8 The (a) velocity and (b) force histories measured using the developed TLDA and predicted using the Ritz method with S = 0.93. The experimental data are identical to those shown in Fig. 7.7.

229

IBF7 11/22/2000 6:43 PM Page 230

230

Impact behaviour of composite materials and structures

16

Delamination area (cm 2)

12

8

4

0 0

10

20

30

40

50

60

Impact velocity (m s ) -1

7.9 The relationship between the projectile initial velocity and the delamination damage area.

7.5.2 Spalling damage When the impact velocity increased slightly to 22.2 m s-1, a patch of the lamina layers on the distal side of the struck specimen started to separate from the laminate. This phenomenon was different from that observed under the quasi-static loading condition. Thus, the damage was considered to have been induced by the reflected tensile waves that were induced by the dynamic loads applied by the striking projectile. This phenomenon, designated as spalling damage, was similarly observed for a brittle target, such as one made of concrete, under projectile impact. In this test run, the delamination area was found to enlarge to 4.52 cm2, as plotted in Fig. 7.9. This shows that graphite/epoxy laminates are brittle, and that the difference in the thresholds between the delamination damage and the spalling damage of such a laminated specimen is not significant. On the other hand, the absorbed energy ratio, DE/Ei, was found to jump significantly from 0.48 in a previous run to 0.61. This indicated that the spalling damage along with the enlargement of the delamination area consumed a significant amount of the impact energy. Still no damage was observed at the initial contact point between the projectile and the target. The velocity and the force histories for impact at 22.2 m s-1 are shown in

IBF7 11/22/2000 6:43 PM Page 231

Impact behaviour and analysis of CFRP laminated plates

231

Fig. 7.2(c). Compared to the results shown in Fig. 7.2(a) and (b) for the case that involved no impact-induced damage as revealed by both C-scan and visual inspection, the phenomenon is found to be significantly different. For example, the second force peak disappeared due to stiffness degradation of the struck laminate, which, in turn, was due to damage on the distal surface of the laminates. This degradation in laminate stiffness also prevented separation of the projectile from the struck target during impact. However, the residual stiffness of the struck laminate was still large enough to cause the laminate to strike the projectile when its velocity was close to zero during the impact process. This resulted in a peak force at around 0.4 ms after the onset of impact, and the projectile gained enough velocity in the negative direction to escape from contact with the struck target that bounced back due to the action of the residual stiffness. The terminal velocity was found to be Vt = -13.8 m s-1. Its absolute value, as expected, was found to be lower than that in the previous impact run of Vt = -14.7 m s-1 due to the more severe reduction of the stiffness in the struck laminate. Meanwhile, as shown in Fig. 7.3, the terminal velocity, Vt, was found to decrease as the impact velocity continuously increased. Thus, the spalling damage was considered to have caused significant degradation in laminate stiffness. It is found from Fig. 7.5 that the maximum force peak was 5.34 kN when the impact velocity was 20.3 m s-1. The force peak dropped and remained at a constant level as the impact velocity further increased. One possible explanation for this peculiar phenomenon was the occurrence of spallation, which reduced the stiffness of the laminate. Once spalling damage occurred on the distal side of the laminates, due to the sudden reduction of the laminate stiffness, the laminate moved much more easily with the projectile. As a result, the maximum indentation between the projectile and the laminate during the impact process, which corresponded to the maximum force peak, for the impact test run that involved spallation was smaller as compared to the test runs in which spallation was not observed.

7.5.3 Permanent indentation damage Permanent indentation damage on the impact side of the struck laminates was observed when the impact velocities became higher, and layers on the distal side of the laminates broke more seriously and separated from the remainder of the laminate. Two typical velocity and force histories for Vi = 24.4 m s-1 and Vi = 31.8 m s-1 are shown in Fig. 7.2(d) and (e). Due to the higher impact velocity, such as in the test run conducted at Vi = 31.8 m s-1, the laminate was damaged more seriously. As a result, it was not able to vibrate effectively enough to push the projectile further back in the reverse direction. Thus, the previously observed multiple force peak phenomenon

IBF7 11/22/2000 6:43 PM Page 232

232

Impact behaviour of composite materials and structures

was diminished, and there existed essentially only a single peak in the force history at the very beginning of the impact stage. The terminal velocity, Vt, was found to decrease at an approximately constant rate as the impact velocity became higher, as shown in Fig. 7.3. This value dropped finally to zero at the ballistic limit. On the other hand, as shown in Fig. 7.4, the absorbed energy, DE, was found to continuously follow the quadratic relationship and to reach the highest value also at the ballistic limit. Close investigation of the struck laminate reveals that the area of fiber bundle breakage increased when the impact velocity was slightly higher than the threshold, and that on the impact side of the fiber bundle, there was breakage due to permanent indentation of the laminate by the projectile. As the impact velocity became even higher, the fiber bundle breakage areas on both sides of the laminate remained approximately the same. However, comparing these areas with the delamination area, shown in Fig. 7.9, it was surprising to find that the delamination area was still proportional to the impact velocity even when the velocity was higher than the threshold corresponding to spalling damage. This demonstrates that it was not the delamination area that governed the residual stiffness of the struck laminate. Thus, the fiber bundle breakage associated with the spalling damage on the distal side of the laminate was considered to be the mechanism that affected the most of the residual stiffness of laminate.

7.6

Impact beyond the ballistic limit

7.6.1 Perforation The ballistic limit occurred when the projectile was struck at the laminate after impact, at which point the terminal velocity was equal to zero, and the impact period lasted forever. The force and velocity histories at the ballistic limit were very similar to that shown in Fig. 7.2(e) for Vi = 31.8 m s-1 except that the terminal velocity was equal to zero. When the impact velocity became higher than the ballistic limit, the terminal velocity was in the same direction as that of the impact velocity. Figure 7.2(f) shows a typical result for the case in which Vi = 36.2 m s-1. The velocity and force profiles were very similar to those shown in Fig. 7.2(e). The single force peak occurred right after the onset of contact between the projectile and the target, as expected. As impact proceeded, the velocity dropped quickly, but its rate of decrease became slower. It was found that the rate of decrease of the projectile velocity could be divided into two portions. In the first portion of the impact process, during roughly the first 0.5 ms after the onset of contact, the rate of decrease was very sharp. As the hemispherical part of the projectile perforated the laminate, the rate of decrease became much smaller, and the corresponding force was only several hundred Newtons.

IBF7 11/22/2000 6:43 PM Page 233

Impact behaviour and analysis of CFRP laminated plates

233

This force was considered to be the dynamic friction force between the projectile and the laminate, and was much smaller than the peak impact force. Meanwhile, the terminal velocity increased drastically again when the projectile velocity became even higher, as shown in Fig. 7.3. A simple equation was adopted to predict the terminal velocity of the projectile, Vt, when the initial striking velocity, Vi, was higher than the ballistic limit:19,20,46 0.5

Vt = (V02 - 2 * Es m)

[7.32]

where Es is the energy needed for an indentor to perforate a laminate under the quasi-static loading condition and m is the mass of the projectile. The predicted result is also plotted in Fig. 7.3. The correlation is considered to be satisfactory. As shown in Fig. 7.8, the absorbed energy was found to remain approximately the same regardless of the increasing velocity of the projectile. Thus, the laminate did not absorb extra energy in a perforated test run even if it was struck at a higher velocity.

7.6.2 Comparison with the quasi-static results To investigate the effect of the loading rate on the CFRP laminate when it is under lateral loading, results from both the impact test at the ballistic limit and the quasi-static contact test are plotted in Fig. 7.10. A similar comparison is also given in Fig. 8.5 of Chapter 8. A double peak phenomenon is observed in the quasi-static case. This is similar to the result observed by Lee and Sun and is attributed to delamination and the globally excessive deflection which occurred during the test.19 In Fig. 7.10, there is only a single peak for the impact test, and it is seen that the force increased at a much faster displacement rate before it reached the peak value. This is because the laminate deflection was very local when the laminate was struck by a projectile at a much higher loading rate. On the other hand, the relatively lower force peak shown for the impact case, as compared to the quasi-static counterpart, was considered to be due to the occurrence of spallation damage that reduced the laminate stiffness. This damage was induced by stress waves that reflected back from the distal side of the struck laminate immediately after the onset of contact between the projectile and the target. Thus, the loading rate effect is also considered to be noticeable for graphite/epoxy laminates under laterally applied loading.

7.7

Conclusions

A general overview for the impact behaviour of a projectile striking on a graphite/epoxy composite laminate has been reported. The laminates used were 6 inch ¥ 4 inch in their in-plane dimensions and 4.3 mm in thickness.

IBF7 11/22/2000 6:43 PM Page 234

234

Impact behaviour of composite materials and structures 5 Quasi-static Impact

Force (kN)

4

3

2

1

0 0

5

10

15

20

Displacement (mm)

7.10 The force vs displacement relationships for laminates under impact at the ballistic limit and under quasi-static loading conditions.

The projectiles employed had a hemispherical tip weighing 35.6 g in mass. The impact speeds were from 3.0 to 101.8 m s-1, where the ballistic limit of the laminates was found to be 35.5 m s-1. The kinetic energy of the projectile was provided by a gas gun. Two different boundary conditions were employed. The first one, which is considered to be perfect, was a free-free boundary. On the other hand, the second was clamping on two opposite sides of the laminate with the other two sides left free of support.This physically clamped boundary only approximated the perfect fixed-end condition although the boundary had been tightly clamped. When the laminate was struck, the velocity signals were measured in a non-contact manner by a developed transient laser Doppler anemometer (TLDA) system. The force and displacement histories for each impact run were then derived from the recorded velocity history, from which the initial and terminal velocities, the initial and the absorbed energy, and the force peak of the projectile were obtained.The struck laminates were then C-scanned to measure the delamination area. On the other hand, an analytical model has been presented in this chapter to predict the impact response of the projectile, and the effect of boundary imperfection was accounted for. Following is a summary of the revealed impact phenomena:

IBF7 11/22/2000 6:43 PM Page 235

Impact behaviour and analysis of CFRP laminated plates 1

235

Near elastic impact. When the impact velocity was low so that no damage was observed under visual inspection, even if a delamination damage area small in size was observed under C-scan when the velocity became higher, a multiple impact phenomenon was observed. The force history showed three peaks. The first had the highest value and occurred after the onset of contact between the projectile and the target, the second peak occurred when the projectile velocity reached zero, and the third peak happened when the laminate bounced back and struck the projectile. The terminal velocity of the projectile was linear to its impact velocity. Further, the maximum peak impact force in each test run also had a linear relationship with the impact velocity. 2 Prediction of projectile response under an imperfect boundary. An analytical method using the Ritz method along with the Mindlin plate theory was employed to predict the response of a laminated plate struck by projectiles at low velocities. The displacement field of the plate was represented by means of a series of beam functions that satisfied the boundary conditions of the plate. When the boundary conditions were perfect, such as a plate with a free boundary, the method could be experimentally verified, and the correlation was found to be very satisfactory. Then, when the laminated plate was physically clamped at two opposite sides, it has been found that the clamped boundary was neither fixed nor simply supported.To take this boundary imperfection into consideration, two beam functions corresponding to simple and fixed boundary conditions were combined, and a normalised rotational spring constant was employed to represent the actual rotational stiffness of the physically clamped boundary. In this study, this spring constant was obtained from the results of a quasi-static contact test. The satisfactory correlation between the prediction and the measured results demonstrates that the presented method is capable of predicting the impact response of a laminate with near-perfect boundaries. 3 Impact beyond the spallation threshold. When the impact velocity was higher than the spallation threshold, the laminae on the distal side of the struck laminates started to separate. This damage mechanism was considered to be due to stress waves reflected from the free surface on the distal side of the laminate, and was designated as spalling damage in this study. As the impact velocity continued to increase, a permanent indentation damage mechanism at the contact location was also observed in addition to spalling damage on the laminate distal side. A further increase of the impact velocity caused these two damage mechanisms to coincide, and the ballistic limit was observed at a speed of 35.5 m s-1. The three-force-peak phenomenon was found to gradually change to a single-force-peak impact phenomenon. This force peak occurred

IBF7 11/22/2000 6:43 PM Page 236

236

4

Impact behaviour of composite materials and structures

immediately after the onset of contact between the projectile and the target. The friction force between the cylindrical portion of the projectile and the perforated laminate was found to be only a small fraction of the peak impact force. On the other hand, the terminal velocity gradually decreased to zero as the impact velocity increased to the ballistic limit, whereas the force peak was found to remain essentially unchanged, and a linear relationship was observed between the delamination area and the impact velocity. Perforated impact. When the impact velocity became higher than the ballistic limit, perforation occurred. It was found that, whereas the terminal velocity increased drastically and approached the initial velocity of the projectile, other phenomena, such as the peak impact force and the delamination area, all remained the same regardless of the increase of the impact velocity. A simple equation was found to accurately predict the terminal velocity of the projectile.

In this study, the force versus the displacement relationships for laminates under impact and quasi-static loading conditions were also compared. The force peak for the laminate under impact occurred at a much lower displacement level. These different phenomena were considered to be mainly due to the more localised laminate response under impact conditions. Thus, the graphite/epoxy laminate was also sensitive to the rate of applied loading.

Acknowledgements This work was supported by the National Science Council of Taiwan, under Contract Numbers NSC 84-0424-E-002-004 and NSC 86-2212-E-002-087. It also represents a portion of the doctoral dissertation of the second author written in partial fulfillment of the requirements for the PhD degree at National Taiwan University. Supply of specimens and help in conducting the C-scan test provided by the Aeronautical Research Laboratory of the Chung-Shan Institute of Science and Technology, and especially by Mr Ming-Fa Shu, are gratefully acknowledged.

References 1 Abrate S, ‘Impact on laminated composite materials’, ASME Appl Mech Rev, 1991 44(2) 155–90. 2 Abrate S, ‘Impact on laminated composites: recent advances’, ASME Appl Mech Rev, 1994 47(11) 517–44. 3 Wu E and Liau J, ‘Impact of unstitched and stitched laminates by line loading’, J Composite Mater, 1994 28(17) 1640–58.

IBF7 11/22/2000 6:43 PM Page 237

Impact behaviour and analysis of CFRP laminated plates

237

4 Wu E and Wang J, ‘Behavior of stitched laminates under in-plane tensile and transverse impact loading’, J Composite Mater, 1995 29(11) 2254–79. 5 Wu E and Chang L C, ‘Loading rate effect on woven glass laminated plates by penetration force’, J Composite Mater, 1998 32(8) 702–21. 6 Liu D, ‘Impact-induced delamination – a view of bending stiffness mismatching’, J Composite Mater, 1988 22 674–92. 7 Wu E and Shyu K, ‘Response of composite laminates to contact loads and relationship to low-velocity impact’, J Composite Mater, 1993 27 1443–64. 8 Cantwell W J and Morton J, ‘The impact resistance of composite materials – a review’, Composites, 1991 22(5) 347–62. 9 Virostek S P, Dual J and Goldsmith W, ‘Direct force measurement in normal and oblique impact of plates by projectiles’, Int J Impact Eng, 1987 6 247–69. 10 Delfosse D, Pageau G, Bennett R and Poursartip A, ‘Instrumented impact testing at high velocities’, J Composites Technol Res, 1993 15(1) 38–45. 11 Gupta B P and Davids N, ‘Penetration experiments with fiberglass-reinforced plastic’, Exp Mech, 1966 6(9) 445–50. 12 Takeda N, Sierakowski R L and Malvern L E, ‘ Wave propagation experiments on ballistically impacted composite laminates’, J Composite Mater, 1981 15 157–74. 13 Takeda N, Sierakowski R L, Ross C A and Malvern L E, ‘ Delamination-crack propagation in ballistically impacted glass/epoxy composite laminates’, Exp Mech, 1982 22 19–25. 14 Cantwell W J and Morton J, ‘The influence of target geometry on the high velocity impact response of CFRP’, Composite Struct, 1988 10 247–65. 15 Cantwell W J and Morton J, ‘Comparison of the low and high velocity impact response of CFRP’, Composites, 1989 20(6) 545–55. 16 Cantwell W J and Morton J, ‘Impact perforation of carbon fibre-reinforced plastic’, Composites Sci Technol, 1990 38 119–41. 17 Zhu G, Goldsmith W and Dharan C K H, ‘Penetration of laminated kevlar by projectiles (I) experimental investigation’, Int J Solids Struct, 1992 29(4) 399–420. 18 Lee S-W R and Sun C T, ‘A quasi-static penetration model for composite laminates’, J Composite Mater, 1993 27 251–71. 19 Lee S-W R and Sun C T, ‘Dynamic penetration of graphite/epoxy laminates impacted by a blunt-ended projectile’, Composites Sci Technol, 1994 49 369–80. 20 Jenq S T, Jing H S and Chung C, ‘Prediction of the ballistic limit for plain woven glass/epoxy composite laminate’, Int J Impact Eng, 1994 15(4) 451–64. 21 Schonberg W P, Keer L M and Woo T K, ‘Low velocity impact of transversely isotropic beams and plates’, Int J Solids Struct, 1987 23(7) 871–96. 22 Cairns D S and Lagace P A, ‘Thick composite plates subjected to lateral loading’, ASME J Appl Mech, 1987 54 611–16. 23 Cairns D S and Lagace P A, ‘Transient response of graphite/epoxy and kevlar/epoxy laminates subjected to impact’, AIAA J, 1989 27(11) 1590–6. 24 Chao C C, Tung T P, Sheu C C and Tseng J H, ‘A consistent higher-order theory of lamimated plate with nonlinear impact modal analysis’, ASME J Vibrat Acoust, 1994 116 371–8. 25 Wu H Y T and Chang F K, ‘Transient dynamic analysis of laminate composite plates subjected to transverse impact’, Computer Struct, 1989 31(3) 453–66. 26 Lin H J and Lee Y J, ‘Impact-induced fracture in laminated plates and shells’, J Composite Mater, 1990 24 1179–99.

IBF7 11/22/2000 6:43 PM Page 238

238

Impact behaviour of composite materials and structures

27 Hertz H, ‘Uber die Beruhrung fester Elastischer Korper’, 1881 92 156–71, transl by Jones D E and Schott G A, London, MacMillan, 1896. 28 Tan T M and Sun C T, ‘Use of statical indentation laws in the impact analysis of laminated composite plates’, J Appl Mech, 1985 52 6–12. 29 Wu E, Chao J C and Yen C S, ‘Smooth contact of orthotropic laminates by rigid cylinders’, AIAA J, 1993 31(10) 1916–21. 30 Wu E and Yen C S, ‘The contact behavior between laminated composite plates and rigid spheres’, ASME J Appl Mech, 1994 61 60–6. 31 Yen C S and Wu E, ‘On the inverse problems of rectangular plates subjected to elastic impact, part 1: method development and numerical verification’, ASME J Appl Mech, 1995 62 692–8. 32 Yen C S and Wu E, ‘On the inverse problems of rectangular plates subjected to elastic impact, part 2: experimental verification and further applications’, ASME J Appl Mech, 1995 62 699–705. 33 Wu E, Yeh J C and Yen C S, ‘Impact on composite laminated plates: an inverse method’, Int J Impact Eng, 1994 15(4) 417–33. 34 Wu E, Yeh J C and Yen C S, ‘Identification of impact forces at multiple locations on laminated plates’, AIAA J, 1994 34(12) 2433–9. 35 Wu E, Tsai T D and Yen C S, ‘Two method for determining impact force history on elastic plates’, Exp Mech, 1995 35(1) 11–18. 36 Wu E, Tsai C Z and Tseng L H, ‘A deconvolution method for force reconstruction in rods under axial impact’, J Acoust Soc Am, 1998 104(3) 1418–26. 37 Wu E, Sheen H J, Chen Y C and Chang L C, ‘Penetration force measurement of thin plates by laser Doppler anemometry’, Exp Mech, 1994 38 93–9. 38 Tsai C Z and Wu E, ‘A transient laser Doppler anemometry to measure rapidly changed velocities of solid bodies’, Exp Mech, 1998 38 261–9. 39 Wu E, Tsai C Z and Chen Y C, ‘Penetration into glass/epoxy composite laminates’, J Composite Mater, 1994 28(18) 1783–802. 40 Wu E and Chang L C, ‘Woven glass/epoxy laminates subject to projectile impact’, Int J Impact Eng, 1995 16(4) 607–19. 41 Wu E and Jiang W S, ‘Axial crush of metallic honeycombs’, Int J Impact Eng, 1997 19(5–6) 439–56. 42 Durst F, Melling A and Whitelaw J M, Principles and Practice of Laser Doppler Anemometry, New York, Academic Press, 1976. 43 Drain L E, The Laser Doppler Technique, New York, Wiley, 1980. 44 de Boor C, A Practical Guide to Splines, Berlin, Springer, 1978. 45 Tsai C Z, ‘Development of the transient laser Doppler anemometry and applications to impact force measurements’, PhD dissertation, Institute of Applied Mechanics, National Taiwan University, Taiwan 1995. 46 Backman M E and Goldsmith W, ‘The mechanics of penetration of projectiles into targets’, Int J Engng Sci, 1978 16 1–99.

IBF8 11/22/2000 6:51 PM Page 239

8 Perforation of FRP laminates and sandwich panels subjected to missile impact S R REID AND H M WEN

8.1

Introduction

Composite structures such as fibre-reinforced plastic (FRP) laminates and sandwich panels made with such laminate skins and light-weight cores have great potential for use in aggressive environments. The high specific strength of composites can offer weight savings and their corrosion resistance gives advantage over traditional metallic materials. Such components, however, could be subjected to high speed impact by fragments resulting from the effects of the disintegration of nearby items of plant as well as low-velocity impact by dropped objects. Their response to such loading in the context of offshore applications has been studied extensively by the authors in recent years as part of the UK collaborative research programme on the Cost Effective Use of Fibre-Reinforced Composites Offshore. Most of this work has been summarised by the authors and their co-workers.1–3 Fibre-reinforced plastic laminates have also been considered for armour applications,4,5 glass fibres being more popular than other types of fibre such as Kevlar due to their cost advantage. The mechanics of deformation and failure of FRP laminates subjected to local impact loads is understood only for a few cases of simple geometrical form.4,5 Static indentation of thick composites with fibres in the form of woven fabrics by conical indenters has been modelled by Rutherford6 (see Reid et al.10) who used an energy approach to relate the force at a certain level of indentation to two strength parameters representing the in-plane and through-thickness strengths of the composites, respectively. A similar problem was also examined by Zhao et al.7 who employed transversely isotropic elastic analysis and rigid, perfectly-plastic material models. They showed that the latter led to a formula depending only on the in-plane strength of the material. This formula showed good agreement with tests on Scotch-ply laminates. The deformation mechanisms which occur during dynamic penetration and perforation of laminates have been examined by a number of authors.1–3,8–14 As indicated in Reid et al.,10 Greaves8,9 studied the deforma239

IBF8 11/22/2000 6:51 PM Page 240

240

Impact behaviour of composite materials and structures

tion mechanisms during ballistic perforation of thick S-2 glass/phenolic laminates by flat-faced projectiles and found that the failure can be divided into two phases. Phase 1 involves compression, shear, indentation and expulsion of debris. In phase 2 the formation of a cone of delaminations, fibre stretching and fracture occur and the projectile exits the back face. It was noted that the phase 1 indentation mechanism, said to be dominated by the through-thickness compressive resistance of the material, absorbed most of the impact energy and was therefore worthy of more detailed study. To this end, an investigation into the impact force-indentation characteristics of laminates at velocities of up to 200 m/s has been carried out by Reid et al.10 Zhu et al.11 investigated experimentally the penetration of laminated Kevlar29/polyester plates by conical-nosed projectiles and proposed a range of models for the various energy-absorbing mechanisms to estimate the target resistance to the projectile motion.12 The event of ballistic impact was divided into three consecutive stages: indentation, perforation and exit. The global structural deformations were determined using laminated plate theory. Dissipative mechanisms including indentation of the projectile tip, bulging of the back surface of the laminate, fibre failure, delamination and friction were described utilising certain simplifying assumptions. Good agreement was obtained between the model predictions and the experimental results. Lee and Sun13 carried out a combined experimental and numerical study on the dynamic penetration of clamped circular CFRP laminates by a 30 g, 14.5 mm diameter flat-ended projectile in the velocity range 24–91 m/s. The composite material examined was Hercules AS4/3501-6 graphite/epoxy and the stacking sequence of all the laminates was based on a basic pattern, namely [0/90/45/-45]s. Three types of impact tests were conducted on the graphite/epoxy laminates which had two thicknesses, 2 mm and 4 mm, and the ballistic limits were determined. The penetration process of composite laminates by a flat-ended missile consisted of three stages: predelamination, post-delamination before plugging and post-plugging. Based upon these three stages, a finite element model was established to simulate the static punch process. The material was modelled using effective moduli so that the details of the stacking sequence were not included in the model. The simulated static load-punch displacement curve was subsequently employed in the dynamic penetration analysis, and the displacements at certain specific checkpoints were adopted as the penetration criteria. It was shown that the computational results were in good agreement with the limited experimental data. More recently, Mines et al.14 conducted an experimental investigation into the high-velocity perforation behaviour of fully-clamped 200 mm ¥ 200 mm polymeric composite laminates at impact velocities of up to 571 m/s. Woven

IBF8 11/22/2000 6:51 PM Page 241

Perforation of FRP laminates and sandwich panels subjected

241

roving, z-stitched and through-thickness z-stitched glass polyester laminates for a number of laminate thicknesses (6, 12, 24 ply), three types of impactors (flat, hemispherical and conical), and two missile masses (6 g, 12 g) were examined. The results were presented in terms of static and impact perforation energies, and energy absorption mechanisms during high-velocity perforation were also discussed with a view to identifying improved combinations of materials. It was found that all types of construction behave in a similar manner. As far as sandwich structures are concerned, Moriarty and Goldsmith15 have recently conducted an experimental investigation into the dynamic energy absorption characteristics of sandwich shells, this work representing an extension of earlier work on flat sandwich panels.16 Aluminium or ABS (acrylonitrile–butadiene–styrene) were used for the skins and a variety of honeycomb materials for the cores of the sandwich constructions. The specimens were subjected to non-perforating impact by a 0.7045 kg, 76.2 mm diameter projectile with a slightly curved impact surface. The projectiles were fired pneumatically at speeds ranging from 16.5 to 19.05 m/s. At these low velocities, it was found that the core material dominates the response in the case of fully-clamped specimens. For the simply-supported samples, the skins (faceplates) dominated the performance characteristics, with the thicker aluminium skin giving significantly poorer results than either the thinner metal or the ABS facing. The effect of the core was more diffuse and was coupled more to the nature of the skin than for fully-clamped specimens. Other relevant investigations have been concerned primarily with the analysis and design of sandwich structures for quasi-static loading17–19 although Bernard and Lagace20 examined the impact resistance of composite sandwich panels and Kosza and Sayir21 studied failure patterns in the cores of sandwich beams and plates under impact loading. It is noted however that all of these studies of sandwich panels and components relate to relatively low impact velocities. This chapter presents some of the results of our own detailed study on the penetration and perforation of sandwich panels made of composite material skins with polymeric foam cores. Emphasis is placed on ballistic test results and associated deformation mechanisms are contrasted with those found in quasi-static penetration. General empirical models are given that provide the perforation energies of FRP laminates and sandwich panels consisting of FRP laminate skins and foam cores under lowvelocity impact by flat-faced, hemispherical-ended and conical-nosed indenters. A new model is developed for the so-called wave-dominated response/perforation of FRP laminates and sandwich panels with such laminates as skins and foam cores subjected to high-velocity impact by the three types of missile (flat, hemispherical and conical). The model predictions and the available test data are compared and discussed. The development

IBF8 11/22/2000 6:51 PM Page 242

242

Impact behaviour of composite materials and structures

of the high velocity perforation model complements and extends the discussion on the ballistic impact on FRP laminates and sandwich panels given recently in references.1–3

8.2

Experimental procedure

8.2.1 Materials and specimens E-glass woven roving (WR) cloth of 600 g/m2 area density with polyester resin (Crystic 491PA and Butanox M50 (1%) hardener) were chosen for the skins and expanded polymeric foam (e.g. PVC) cores were used, these being purchased in slab/sheet form. The manufacture of panels and preparation of specimens by hand lay-up and assembly are described in Wen et al.1 Square laminates and sandwich panels with side lengths of 0.9 m were prepared and some smaller panels of 0.3 m ¥ 0.3 m were cut from the larger panels for testing. Several triple-skinned (i.e. with a central laminate as well as the other skins) panels were manufactured using the same procedures. The behaviour of these latter panels is not discussed extensively herein (see Wen et al.1) but some of the test data will be included in the appropriate figures. Some of the properties of the materials used are given in Table 8.1 in which su, Es1, se and t13 are the tensile strength, Young’s modulus for inplane tension, the elastic limit for through-thickness compression and the transverse shear strength of the laminates, respectively, and sc, Ec, Gc and t are the compressive strength, Young’s modulus in compression, shear modulus and shear strength of the core materials, respectively. Typical nominal stress-strain curves for both GRP laminates and foam core are given in Fig. 8.1.

8.2.2 Loading and data recording In all the tests, panels were supported in specially designed frames, one with a 0.85 m square aperture (for the larger 0.9 m square panels) and the other with a 0.2 m square window (for smaller 0.3 m square panels). The supports were such that the out-of-plane movement of the edges of the panels was restrained but their in-plane movement was allowed (see Wen et al.1). Quasi-static indentation tests were conducted on a screw driven (RDP) testing machine operating under displacement control. Flat-ended, hemispherical-ended and conical-nosed indenters with different diameters (ranging from 5.25 mm up to 150 mm) were used in the experiments. All the indenters were case-hardened. The panels were loaded normal to their planes at the centre and the load versus punch displacement curves were

Source Scott Bader Source Strand Source Barracuda Barracuda Tensile tests

Resins Isopthalic polyester

Reinforcement E-Glass WR

Core material Divinycell H130 Divinycell HCP100

GRP skins

Table 8.1. Materials for sandwich panels

Average volume fraction = 43%

Density, thickness 130 kg m-3, 25 mm 400 kg m-3, 20 mm

Weight 600 g m-2

Type Crystic 491 PA

Ec 175 MPa 340 MPa Es1 = 24 GPa

sc 2.5 MPa 10.4 MPa su = 345 MPa se = 225 MPa

Cloth Woven roving

Catalyst/hardener Butanox M50 (1%)

t13 = 45 MPa

Gc 50 MPa 180 MPa

t 2 MPa 7.4 MPa

IBF8 11/22/2000 6:51 PM Page 243

Perforation of FRP laminates and sandwich panels subjected 243

IBF8 11/22/2000 6:51 PM Page 244

244

Impact behaviour of composite materials and structures 500

Stress (MPa)

400

300

200

100

0

1.6

0.8

2.4 3.2 Strain (%)

(a) 4

Stress (MPa)

3

2

1

0

0.1

0.2

0.3

0.4

0.5

0.6

Strain (b)

8.1 Nominal stress-strain curves: (a) GRP laminates in tension; (b) Divinycell H130 foam in compression; (c) GRP laminates in through-thickness compression.

recorded. The movements of the centres of the lower skins were also recorded on the larger panels during the tests using a suitable arrangement with an LVDT. The cross-head speed was 3 mm/minute for all the tests. Low-velocity impact tests were carried out using a drop weight apparatus. The tup was instrumented with an accelerometer (Bruel and Kjaer, type 4382) and the deceleration-time history was recorded using a Kontron digital event recorder (WW700) operating at a sampling rate of 106 samples

IBF8 11/22/2000 6:51 PM Page 245

Perforation of FRP laminates and sandwich panels subjected

245

500 450 400

Stress (MPa)

350 300 250 200 150 100 50 0 0.00

0.05

0.10

0.15

0.20

0.25

Strain (mm/mm) (c)

8.1 (cont.)

Pressure vessel

Solenold valve

Gun barrel

Specimen

Photocell unit

Holder Screens

Projectile catcher

Timer counters

8.2 Schematic diagram of the pneumatic gun facility.

per second. The direction of motion of the tup was controlled by pretensioned vertical guide ropes. The initial impact velocity was measured by means of a photocell system. Details of the results of these tests have been described elsewhere1 but some of the data are included in the relevant graphs to indicate the consistency in the behaviour of panels over a wide range of impact velocities. The fixtures for high speed ballistic impact tests and the pneumatic gun facility for firing the projectiles are shown schematically in Fig. 8.2. Three types of projectile end geometries referred to above were used but only two projectile diameters (10.5 mm and 45 mm) were chosen, the projectiles

IBF8 11/22/2000 6:51 PM Page 246

246

Impact behaviour of composite materials and structures

weighing approximately 18.0 g and 1.30 kg, respectively (see Wen et al.1 and Reddy et al.2 for details).

8.3

Experimental results

8.3.1 Quasi-static tests 8.3.1.1 Range of tests and general observations Details of the results of the quasi-static indentation experiments are given by Wen et al.1 It was found that most of the specimens failed by local indentation, penetration and perforation under the punches. One exception was the case of larger (0.9 m square) sandwich panels with 3.25 mm thick GRP skins and higher density foam core (Divinycell H100, density 400 kg/m3) loaded by 50 mm diameter flat or hemispherical indenters and those loaded by larger (150 mm) diameter indenters, all of which failed in a global bending mode. The other exception was the case of smaller (0.3 m square) sandwich panels with 3.25 mm thick GRP skins and higher density foam core (HCP100) loaded by a 20 mm flat-faced punch which failed by core shear. It was also found that sandwich panels loaded quasi-statically by hemispherical-ended indenters with radii equal to or greater than the thickness of the core required the least energy for complete penetration and for this reason particular emphasis was placed upon the results for this nose geometry.2 The details of the response to flat-ended indenters/projectiles are sufficiently different to warrant separate discussion and this has been given elsewhere.1,3 When the radii of the indenters were smaller than the core thickness, the energies for perforation by hemispherical, flat and conical punches were approximately the same. Flat-faced indenters Figure 8.3(a) shows typical quasi-static load-displacement characteristics for a 0.9 m square sandwich panel with 3.25 mm thick GRP skins and 25 mm thick Divinycell H130 foam core loaded centrally by a 50 mm diameter flatfaced indenter, which first failed by indentation. The load-punch displacement curve and the vertical moment of the bottom skin of the panel are indicated in the figure. The first part of the load-punch displacement trace (up to the top skin failure at the first peak load) is bilinear. Core crushing as evidenced by the difference between the punch and the bottom skin displacement starts just after the knee of this bilinear part. After top skin failure (by shear along the periphery of the punch) at the peak load, the load drops to about a third of its peak value, there was considerable further

IBF8 11/22/2000 6:51 PM Page 247

40 Flat

30

Load (kN)

Lower skin

20 Punch

10

0 0

20

40

60

80

100

120

Displacement (mm) (a) 40

Hemispherical

Load (kN)

30

Lower skin

Punch

20 F 10

0

20

40

60

80

100

Displacement (mm) (b)

8.3 Load-displacement characteristics for 0.9 m square 3.25 mm thick GRP skin sandwich panels loaded quasi-statically by 50 mm diameter indenters: (a) Twin-skinned panel with 25 mm thick H130 foam core; (b) twin-skinned panel with 25 mm thick H130 foam core; (c) twin-skinned panel with 50 mm thick H130 foam core; (d) triple-skinned panel with 25 mm thick H130 foam cores; (e) twinskinned panel with 25 mm thick H130 foam core; (f) cross-sectional view of identical panels loaded by flat-faced, hemispherical-ended and conical-nosed indenters (from bottom to top).

IBF8 11/22/2000 6:51 PM Page 248

248

Impact behaviour of composite materials and structures 20 Hemispherical Lower skin

15 Load (kN)

F

Punch

10

5

0

20

40

60

80

100

Displacement (mm) (c) Hemispherical B Lower skin

C Punch

Load (kN)

20

A 10

0

20

40

60 Displacement (mm) (d)

8.3 (cont.)

80

100

120

IBF8 11/22/2000 6:51 PM Page 249

Perforation of FRP laminates and sandwich panels subjected

249

30 Conical

Load (kN)

20 Punch

Lower skin

10

F

0 0

20

40

60

Displacement (mm) (e)

(f)

8.3 (cont.)

80

100

IBF8 11/22/2000 6:51 PM Page 250

250

Impact behaviour of composite materials and structures

deformation characterised by progressive core crushing, lower skin debonding and bending. The lower skin of the panel debonded gradually from the core and failed by fracturing due to bending of the debonded skin. Hemispherical-ended indenters Typical load-displacement characteristics for 0.9 m square sandwich panels with 3.25 mm thick GRP skins and 25 mm and 50 mm thick H130 foam cores loaded quasi-statically by a 50 mm diameter hemispherical-ended indenter are presented in Fig. 8.3(b) and (c), respectively. It can be seen that core crushing starts very soon after loading begins. The top skins failed by a central puncture causing four cruciform cracks, at points indicated by F in these two load-displacement curves. It is clear that the load-punch displacement responses are different. In Fig. 8.3(b) after the top skin failure, the load did not fall but rather increased steadily. This corresponded to the crushing of the core material, the lengthening of cracks in the top skin as well as bending of the flaps resulting from cracks. This was then followed by a more rapid rise in load until the bottom skin failed in bending. It should be noted here that in this test the core thickness was equal to the radius of the indenter so that the applied force directly acted on the lower skin before the indenter had completely penetrated the upper skin. By contrast the load-displacement curve in Fig. 8.3(c) shows double hump response. This response is associated with the larger ratios of core thickness, c, to punch diameter, D, (c/D > 0.5) which allows the top skin penetration to be completed before the bottom skin is loaded directly by the indenter through a layer of densified foam (Reddy et al.2). Good repeatability was observed for identical sandwich panels in terms of their load-displacement response. A typical example is shown in Fig. 8.3(b) in which the solid and broken lines represent the load versus punch displacement characteristics of two nominally identical panel tests. Figure 8.3(d) shows the load-displacement curve for a triple-skinned sandwich panel with three six-layer laminate skins of E-glass WR cloth reinforced polyester resin and two 25 mm thick H130 foam cores, loaded quasistatically by the 50 mm diameter hemispherical-ended indenter. Like the twin-skinned sandwich panels described above, core crushing occurs from the beginning of the loading process as can be seen from Fig. 8.3(d). The top skin failed by a central puncture causing four cruciform cracks at point A in the curve. After the top skin failure, the load dropped slightly and then increased steadily which corresponded to the crushing of the core, the lengthening of the cracks as well as the bending of the resulting petals in the top skin. This was then followed by a more rapid rise in load until the middle skin failed at point B. It is interesting to note here that up to the middle skin failure the load-displacement response of the triple-skinned

IBF8 11/22/2000 6:51 PM Page 251

Perforation of FRP laminates and sandwich panels subjected

251

panel was very similar to that of the double-skinned panel as shown in Fig. 8.3(c). After the middle skin failure, there was considerable further deformation which was characterised by progressive core crushing and the lower skin bending. At point C the lower skin fractured with the formation of four major cruciform cracks and perforation ensued. Conical-nosed punches Figure 8.3(e) shows typical load-displacement characteristics for a 0.9 m square sandwich panel with 3.25 mm thick GRP skins and 25 mm thick H130 foam core loaded quasi-statically by a 50 mm diameter conical-nosed indenter. After top skin failure just underneath the 2 mm radius nose tip (denoted by F in the figure), the load dropped slightly and then increased steadily to the maximum value. This second region was associated with the formation of major cruciform cracks and bending of the resulting flaps with bending hinges moving away from the loading point through the propagation of fractures and also overcoming the friction between the panel and the conical punch, all of which dissipated energy at an increasing rate. The bottom skin failed in bending accompanied by a small area of debonding. Figure 8.3(f) shows photographs of the cross-sectional views of the three identical 0.9 m square sandwich panels with 3.25 mm thick GRP skins and 25 mm thick H130 foam cores loaded quasi-statically by 50 mm diameter flat-faced, hemispherical-ended and conical-nosed indenters (from bottom to top). The top skin shear plugging and core crushing are evident with a flat punch, the other two look very similar to each other. All these cases are categorised as indentation failures. 8.3.1.2 Discussion Energies associated with three critical events in the penetration process of a twin-skinned sandwich panel loaded by flat-faced, hemispherical-ended and conical-nosed indenters can be found from the load-displacement curves as shown in Fig. 8.3(a), (b,c) and (e). These critical events are: (i) the energy to penetrate the top skin; (ii) the energy to penetrate (fracture) the bottom skin; and (iii) the energy to perforate the whole panel. It was found (Wen et al.1) that both the peak load at the failure of the top skin and the corresponding energy absorbed are approximately proportional to the weight of glass fibres in a skin, or equivalently, the thickness of the skin if the volume fraction is maintained the same. Similarly, the energies absorbed up to the failure (fracture) of the bottom skins of sandwich panels which fall into the same category (defined below) were also found to be linearly related to the weight of fibres or the thickness of skin (Wen et al.1 and

IBF8 11/22/2000 6:51 PM Page 252

252

Impact behaviour of composite materials and structures

Reddy et al.2). These observations indicate that laminate skins play a very important role in the failure and energy absorption of GRP skinned sandwich panels with foam cores, whilst the core thickness controls which category of behaviour occurs. The experimental results obtained for sandwich panels loaded quasistatically by hemispherical-ended indenters are presented in Fig. 8.4(a), which shows the plot of the non-dimensional penetration energy (Ef /suTD2) versus the non-dimensional geometric property (L/D). It is clear from Fig. 8.4(a) that, irrespective of panel side length (L), the quasistatic tests conducted on the sandwich panels using hemispherical-ended punches may be categorised into two groups, one group with H/D > 2, the other with H/D < 2, here H and D are the total panel thickness and the punch diameter, respectively. In the former case considerably more energy was absorbed as can be seen from Fig. 8.4(a). In order to dilineate the difference, panels were sectioned to study the mechanisms. The only obvious difference appeared to be that for the panels with H/D > 2 relatively more debonding between the lower skin and the foam core had occurred. This was found (Wen et al.1) generally to be one of the mechanisms enhancing the quasi-static energy absorbing capacity. On the other hand, the experimental data obtained for sandwich panels loaded quasi-statically by flat-faced punches are given in Fig. 8.4(b), which shows the plot of the non-dimensional global energy (Eg/suTD2) against the non-dimensional geometric property (L/D). It can be seen from Fig. 8.4(b) that all the data points follow the same trend irrespective of the ratios of H/D. Closer examination reveals that the plots of the non-dimensional global energy (Eg/suTD2) against the non-dimensional geometric property (L/D) for sandwich panels loaded quasi-statically by both flat-faced punches and hemispherical-ended indenters with H/D > 2 are almost identical, as can be deduced from Fig. 8.4(a) and (b). It may also be inferred from Fig. 8.4(b) that the energy absorbed by the global deformations of panels loaded by flat-faced punches is also approximately proportional to the thickness of the skin laminates. It should be mentioned here that the experimental results obtained for sandwich panels loaded quasi-statically by hemispherical-ended indenters can also be presented in terms of the plot of the non-dimensional global energy (Eg/suTD2) against the nondimensional geometric property (L/D), which is very similar to that given in Fig. 8.4(a). How to distinguish the global energy from the total penetration energy is discussed in Section 8.4.

8.3.2 Low-velocity impact tests Low-velocity tests will not be described or discussed in detail in this chapter (for details, see Wen et al.1). However, Fig. 8.5 shows a typical low-velocity

IBF8 11/22/2000 6:51 PM Page 253

Perforation of FRP laminates and sandwich panels subjected

253

Ef su TD 2 0.5

0.4

: t = 1.75 mm : t = 3.25 mm : t = 7.0 mm : Triple-skinned panel Open symbols: H/D < 2 Solid symbols: H/D > 2

0.3

Equation [8.5]

0.2

0.1

0

20

10

30

L D

40

(a) Eg su TD 2

0.6

D: t = 1.75 mm : t = 3.25 mm : t = 7.0 mm Open symbols: H D < 2 Solid symbols: H D > 2

0.4 Equation [8.7b]

0.2

0

10

20

30

40

L D

(b)

8.4 Variation of the non-dimensional penetration/global energies with the ratio of panel span to indenter diameter for sandwich panels loaded quasi-statically at the centre: (a) hemispherical-ended indenters; (b) flat-faced punches.

IBF8 11/22/2000 6:51 PM Page 254

254

Impact behaviour of composite materials and structures

30

Impact Load (kN)

20

10 Quasi-static

0

10

20

30

40

50

60

Displacement (mm)

8.5 Comparison between quasi-static and impact load-displacement characteristics for 0.9 m square sandwich panels with 3.25 mm thick GRP skins and 25 mm thick H130 foam core loaded by a 50 mm diameter hemispherical-ended punch.

impact load-displacement curve for a 3.25 mm thick GRP skin sandwich panel with 25 mm thick H130 foam core struck at 6.23 m/s by a 42.5 kg tup mass with an attached 50 mm diameter hemispherical indenter.1 Also shown in the figure is the corresponding quasi-static load-displacement curve for an identical panel. The lower skin of the panel subjected to dropped object loading fractured but was not completely penetrated. It was found that the fracture patterns as well as the load-deflection characteristics of the GRP skin sandwich panels loaded dynamically were similar to those observed in the corresponding quasi-static cases. It was also found that the extent of damage (judged by the extent of lower skin perforation) under dropped object loading was less than that observed in the identical panel under quasi-static loading even though the impact energy was about 20% higher than the corresponding quasi-static perforation energy. However, the extent of debonding between the lower skin and the core was larger in the impact tests. The dynamic load required to cause a given deflection is higher than the load required to cause the same deformation under quasi-static loading

IBF8 11/22/2000 6:51 PM Page 255

Perforation of FRP laminates and sandwich panels subjected

255

conditions (see Fig. 8.5). The changes are presumably the result of enhanced strengths and stiffnesses of the components due to rate-dependent material properties and inertia effects. The interplay between these and the core-skin bond strength will influence the balance between the various failure mechanisms in the panel and their respective contributions to energy absorption.

8.3.3 Ballistic impact tests 8.3.3.1 Range of tests and observations Ballistic impact tests were performed on 0.3 m square GRP laminates as well as sandwich panels with H130 foam core using 10.5 mm diameter projectiles with masses of approximately 19.0 g at impact velocities up to 305 m/s. Ballistic impact tests were also carried out on 0.9 m square twinskinned (as well as triple-skinned) panels using projectiles with a 45 mm diameter and masses of approximately 1.3 kg at impact velocities up to 102 m/s. Many tests were performed. Here we concentrate on presenting data for the critical impact conditions associated with the ballistic limit (velocity for full perforation of the projectile nose through the panel) for flat-faced, hemispherical-ended and conical-tipped projectiles. Figure 8.6(a) and (b) shows respectively the effects of total laminate skin thickness on the ballistic limits for 0.3 m and 0.9 m square sandwich panels struck by hemispherical-ended and conical-nosed missiles while Fig. 8.6(c) and (d) show respectively the same effects for 0.3 m and 0.9 m square sandwich panels struck by flat-faced projectiles. Plots of the variation in the residual velocity with impact velocity for 0.3 m square sandwich panels struck by hemispherical-ended conical-nosed projectiles are given in Fig. 8.6(e). It is seen from Fig. 8.6(a) to (d) that the ballistic limit is an increasing function of the total laminate thickness. Figure 8.6(a), (b) and (e) illustrates that the perforation processes for the hemispherical-ended and the conical-tipped projectiles used in the study are essentially the same in terms of ballistic limits and residual velocities. In order to observe the influence of skin thickness on the ballistic performance of sandwich panels, panels were sectioned. Figure 8.7(a) shows the cross-sectional view of 0.3 m square sandwich panels with 1.75 mm, 3.25 mm and 7.0 mm thick GRP skins and 25 mm thick H130 foam core, perforated by the 10.5 mm diameter hemispherical-ended missile at initial velocities well above their ballistic limits. It is evident from this figure that debonding between the lower skins and the core decreases with an increase in laminate thickness while delamination in the lower skins in particular increased with increasing laminate thickness. This is the reverse of the

IBF8 11/22/2000 6:51 PM Page 256

Vb (m s-1) D: conical : hemispherical

200

Equation [8.17] with G = 1.5

Equation [8.17] with G = 1.414 150 Equation [8.13] 100

50

0

4

8

12

16

T (mm) (a) Vb (m s-1) 100

: conical : hemispherical : triple-skinned panel

Equation [8.17] with G = 1.5

Equation [8.17] with G = 1.414

75

Equation [8.13] 50

25

0

4

8

12

16

T (mm) (b)

8.6 (a) Effects of total laminate thickness on the ballistic limits for 0.3 m square sandwich panels with GRP skins and 25 mm thick H130 foam core struck by 10.5 mm diameter hemispherical-ended and conical-nosed missiles. (b) Effects of total laminate thickness on the ballistic limits for 0.9 m square sandwich panels with GRP skins and 25 mm thick H130 foam core (two in the case of tripleskinned panel) struck by 10.5 mm diameter hemispherical-ended and conical-nosed missiles.

IBF8 11/22/2000 6:51 PM Page 257

Vb (ms-1) Flat 200

Equation [8.17]

Equation [8.13] 150

100

50

0

4

8

12

16

T (mm) (c) Vb (m s-1)

100

Flat

Equation [8.17]

70

Equation [8.13]

50

25

0

4

8

12

16

T (mm) (d)

8.6 (cont.) (c) Effects of total laminate thickness on the ballistic limits for 0.3 m square sandwich panels with GRP skins and 25 mm thick H130 foam core struck by a 10.5 mm diameter flat-faced projectile. (d) Effects of total laminate thickness on the ballistic limits for 0.9 m square sandwich panels with GRP skins and 25 mm thick H130 foam core struck by a 45 mm diameter flat-faced missile.

IBF8 11/22/2000 6:51 PM Page 258

258

Impact behaviour of composite materials and structures

Vr (ms-1)

200

D: t = 1.75 mm : t = 3.25 mm : t = 7.0 mm Open symbols: hemispherical Solid symbols: conical

150

100

50

0

50

100

150 Vi

200

250

300

(m s-1) (e)

8.6 (cont.) (e) Variation of the residual velocity with the initial impact velocity for 0.3 m square sandwich panels with GRP skins and 25 mm thick H130 foam core struck by 10.5 mm diameter hemispherical-ended and conical-nosed missiles.

behaviour of identical panels loaded quasi-statically by the same diameter punch, as shown in Fig. 8.7(b). The photographs in Fig. 8.8 show the effects of initial impact velocity on the behaviour of 0.3 m square sandwich panels with 1.75 mm thick GRP skins and 25 mm thick H130 foam core tested using the 10.5 mm diameter hemispherical-ended missile with impact velocities at and above the ballistic limit (approximately 100 m/s), as indicated in the figure. It is clear from this figure that debonding between the lower skins and the core decreased with increasing impact velocity whereas delamination within the lower skins increased with an increase in impact velocity. At an impact velocity of 163.9 m/s the delamination area was roughly circular in shape and its diameter was about eight times that of the missile, as can be seen from Fig. 8.8(d). 8.3.3.2 Discussion It was observed from the experiments described briefly in the previous sections that the dynamic perforation energies are higher than those under

IBF8 11/22/2000 6:51 PM Page 259

Perforation of FRP laminates and sandwich panels subjected

259

(a)

(b) 8.7 Cross-sectional views of 0.3 m square sandwich panels with GRP skins and 25 mm thick H130 foam core tested with a 10.5 mm diameter hemispherical-ended punch: (a) ballistic loading; (b) quasi-static loading, indicating the extent of delamination in the skins and debonding between the core and the bottom skin.

IBF8 11/22/2000 6:51 PM Page 260

260

Impact behaviour of composite materials and structures

(a)

(b)

(c)

(d)

8.8 Photographs of 0.3 m square sandwich panels with 1.75 mm thick GRP skins and 25 mm thick H130 foam core struck by a 10.5 mm diameter hemispherical-ended missile at different velocities. (a) Vi = 98 m s-1; (b) Vi = 120.5 m s-1; (c) Vi = 143.9 m s-1; (d) Vi = 163.9 m s-1.

quasi-static loading conditions. Figure 8.9(a), (b) and (c) shows plots of the dynamic enhancement factor, f, against impact velocity, Vi, for sandwich panels struck by hemispherical-ended projectiles for H/D ratios less than and greater than 2, and by flat-faced missiles (irrespective of the ratios of H/D), respectively. f is defined here as the ratio of the dynamic perforation energy for a panel to the energy absorbed up to the fracture of the lower skin of an identical panel under quasi-static loading. What it reflects is changes in energy absorbing mechanisms due to dynamic effects including inertia. Closer examination of Fig. 8.4(a) and Fig. 8.9(a) and (b) reveals that the products of the quasi-static penetration energy and the dynamic enhancement factor are nearly the same for sandwich panels with H/D > 2 and H/D < 2 especially at higher impact velocities. This means that at higher impact velocities the energy absorbing mechanisms are the same for sand-

IBF8 11/22/2000 6:51 PM Page 261

Perforation of FRP laminates and sandwich panels subjected f

261

: t = 1.75 mm : t = 3.25 mm : t = 7.0 mm Hemispherical

5

4

Equation [8.10]

3

2

1

0

25

50

75

100

125

Vi (m s-1) (a) f

D: t = 1.75 mm : t = 3.25 mm : t = 7.0 mm Hemispherical

3

Equation [8.10]

2

1

0

100

200 Vi ( m s

-1

)

(b)

8.9 Variation of the dynamic enhancement factors, f, with the initial impact velocity, Vi for sandwich panels. (a) Hemispherical-ended projectiles with H/D < 2; (b) hemispherical-ended projectiles with H/D > 2; (c) flat-faced missiles.

IBF8 11/22/2000 6:51 PM Page 262

262

Impact behaviour of composite materials and structures f

: t = 1.75 mm : t = 3.25 mm : t = 7.0 mm Flat

Equation [8.10]

3

2

1

0

150 Vi

300

(m s-1) (c)

8.9 (cont.)

wich panels irrespective of the H/D ratios and that the kinetic energy is mainly dissipated by the FRP laminate skins. The ratios of dynamic to quasi-static perforation energies versus impact velocity (in this case for 0.3 m square sandwich panels as noted above) are also given in Fig. 8.9(b) as open symbols. The latter illustrates the difference in the fracture and perforation energies for the smaller panels struck by hemispherical-ended projectiles when H/D > 2 which is why the fracture energies are used. It should be noted that for all the 0.9 m square panels loaded quasi-statically by a 50 mm diameter hemispherical-headed indenter the perforation energy and the energy absorbed up to the fracture of the lower skin of the panels are almost identical (Wen et al.1). Therefore, these two ratios are equivalent to each other in Fig. 8.9(a) as designated by the solid symbols. The half-solid symbols in this figure represent the experimental data for the 0.9 m square sandwich panels subjected to low speed impact (dropped object) loading, where the panels were not totally perforated, while the open symbol in Fig. 8.9(c) represent the test result for a 0.9 m square sandwich panel under dropped object loading, where the lower skin of the panel was not penetrated but debonded from the core in a large area (Wen et al.1). It is apparent from Fig. 8.9(a) and (c) that initially the dynamic enhancement factor increases with increasing impact velocities, while it is seen from Fig. 8.9(b) (where only the results of higher velocity impact tests are shown) that the dynamic enhancement factor is independent of the impact veloci-

IBF8 11/22/2000 6:51 PM Page 263

Perforation of FRP laminates and sandwich panels subjected

263

ties. These results imply that there exists a transition velocity below which the dynamic enhancement factor is linearly related to initial impact velocity and above which it is a constant. For the tests performed this velocity is approximately 80 m/s. It should be mentioned here that similar observations can be made for conical-nosed projectiles.

8.4

Model development

Based on the experimental observations and discussions made in the previous sections and elsewhere,1–3 ballistic impact on fibre-reinforced polymer laminates and sandwich panels with such laminates as skins and foam cores may be categorised into two regimes, namely, low velocity impact and wavedominated response. In the former case global response as well as local deformations/failure are simultaneously present while in the latter case local deformations/failure dominate. Two semi-empirical modelling methods are described. One uses the dynamic enhancement factor to scale the quasi-static behaviour and encompass the whole range of perforation/ballistic data. The other (wave-dominated) model is based upon a local mechanism alone and incorporates inertial effects in a simplified manner.

8.4.1 Low-velocity impact 8.4.1.1 Empirical formulas for quasi-static penetration energy The principle of dimensional analysis is used here to derive the empirical formulas for quasi-static penetration energies. Based on the observations made on the experimental data, it is reasonable to assume that the energy absorbed up to the fracture (penetration) of the lower skin by a sandwich panel with FRP laminate skins and foam core loaded quasi-statically by an indenter can be divided into two parts, in a similar manner to the procedure suggested by Wen and Jones.22 One part is associated with the energy absorbed by local deformations, El, and the other, Eg, is related to the energy dissipated by global deformations of the panel. Thus1–3 Ef = El + Eg

[8.1]

where Ef is the energy absorbed up to the fracture (penetration) of the lower skin of the sandwich panel. Hemispherical-ended indenters It is assumed that, in the case of a sandwich panel loaded by a hemispherical-ended indenter, the local energy, El, can be estimated by the fragmentation energy given by

IBF8 11/22/2000 6:51 PM Page 264

264

Impact behaviour of composite materials and structures E1 =

pD2Ts u e f 8

[8.2]

in which su, ef, D and T are the failure stress (UTS) and the fracture strain of the laminates in tension, indenter diameter and total laminate thickness, respectively. If the indenter diameter, D, is taken as a characteristic length, then standard techniques of dimensional analysis indicate that the energy absorbed by global structural response, Eg, when normalized with respect to suD3 can be related to the geometric properties of the punch and the panel by a relationship of the following form1–3 b1

Eg L T = AÊ ˆ Ê ˆ 3 Ë ¯ Ë D D¯ suD

b2

[8.3]

Substituting El and Eg in equations [8.2] and [8.3] into equation [8.1] and rearranging gives b1

Ef L T pe f Ê T ˆ = + AÊ ˆ Ê ˆ 3 Ë ¯ Ë ¯ Ë 8 D D D¯ suD

b2

[8.4]

here A, b1 and b2 are constants which are to be determined from experiments. For FRP skin sandwich panels with foam cores loaded quasi-statically by hemispherical-ended indenters it is found (Wen et al.,1 also see discussion in Section 8.3.1.2) that Ef is linearly related to the thickness of the skin laminates. Hence, b2 in equation [8.4] can be taken as unity. Equation [8.4] can thus be rewritten in the following form Ef L pe f = + AÊ ˆ 2 Ë 8 D¯ s uTD

b1

[8.5]

Flat-faced punches It is assumed that, in the case of a sandwich panel loaded by a flat-faced punch, the local energy, viz. the first term on the right hand side of equation [8.1], can be estimated by the following expression 2

E1 p Ks c ˆ Ê c ˆ p t13 ˆ Ê T ˆ Ê t ˆ pe f Ê t ˆ = Ê ed + Ê + 2 Ë ¯ Ë ¯ Ë ¯ Ë ¯ Ë ¯ 4 s T 2 s D T 8 ËT ¯ s uTD u u

[8.6]

in which the first, second and last terms on the right hand side of equation [8.6] represent the energies dissipated by the core crushing, the upper skin shear plugging and the fragmentation energy of the lower skin of the panel, respectively. K is the constraint factor usually taken to be 2 (Wen et al.1) and t13 and sc are the transverse shear strength of the skin laminates and

IBF8 11/22/2000 6:51 PM Page 265

Perforation of FRP laminates and sandwich panels subjected

265

the compressive strength of the core, respectively. ed is a measure of densification of the foam core, which may be determined experimentally, as discussed in Section 8.5. The energy dissipated by the global deformations of the panel may be estimated in a similar manner to that described above for a hemisphericalended indenter. Thus, b3

Eg L T = BÊ ˆ Ê ˆ 3 Ë ¯ Ë D D¯ suD

b4

[8.7a]

here B, b3 and b4 are constants which are to be determined from experiments. For FRP skin sandwich panels with foam cores loaded quasi-statically by flat-faced punches it is found (see discussion in Section 8.3.1.2) that Eg is approximately proportional to the thickness of the skin laminates. Therefore, b4 in equation [8.7a] can be taken as unity. Equation [8.7a] can thus be recast into the following form Eg L = BÊ ˆ Ë D¯ s uTD2

b3

[8.7b]

Substituting equations [8.6] and [8.7b] into equation [8.1] yields Ef p Ks c ˆ Ê c ˆ p t13 ˆ Ê T ˆ Ê t ˆ = Ê ed + Ê 2 4 Ë su ¯Ë T ¯ 2 Ë s u ¯ Ë D¯ Ë T ¯ s uTD +

pe f Ê t ˆ L + BÊ ˆ Ë ¯ Ë 8 T D¯

2

b3

[8.8]

8.4.1.2 Dynamic enhancement factor On the basis of the observations made regarding the experimental results (Section 8.3.3.2), the impact perforation energy, Epi, of a sandwich panel struck transversely by a projectile may be written as Epi = fEf

[8.9]

where f is the dynamic enhancement factor which may be expressed in the following form Vi f = 1 + bÊ ˆ Ë Vo ¯

(Vi < Vo )

[8.10a]

f = 1+b

(Vi > Vo )

[8.10b]

where b is an empirical constant. Here, Vo is the transition velocity. The data acquired in the test programme suggest that this is given by

IBF8 11/22/2000 6:51 PM Page 266

266

Impact behaviour of composite materials and structures Es1 ef rt

Vo = Ce f =

[8.10c]

in which C is the speed of sound in the laminates along the fibre direction; rt and Es1 are the density and the in-plane Young’s modulus of the laminates, respectively. Equation [8.10c] is the Karman critical velocity, the uniaxial impact velocity above which tensile deformation cannot be transmitted away from the loading point because the material has fractured and, perhaps coincidentally, is approximately 80 m/s for the material properties of the laminates used. The rationale for using this critical velocity for transverse impacts needs to be explored further. Combining equations [8.5], [8.8] and equation [8.9] yields Epi p L = e f + AÊ ˆ 2 Ë 8 D¯ fs uTD

b1

[8.11]

for hemispherical-ended projectiles, and Epi p Ks c ˆ Ê c ˆ p Ê t13 ˆ Ê T ˆ Ê t ˆ = Ê ed + 2 Ë ¯ Ë ¯ 4 su T 2 Ë s u ¯ Ë D¯ Ë T ¯ fs uTD L pe f Ê t ˆ + + BÊ ˆ Ë ¯ Ë 8 T D¯

b3

2

[8.12]

for flat-faced missiles. Finally, from the above equations an approximate expression can be obtained for the ballistic limit, Vb, by assuming that the critical projectile kinetic energy is equal to Epi, the energy for perforation. Thus, 1

2 Epi ˆ 2 Vb = Ê Ë G ¯

[8.13]

where G is the projectile mass.

8.4.2 Wave-dominated response 8.4.2.1 Assumption about the resistive pressure As discussed previously, for the wave-dominated response the deformations will be localised and the through-thickness strength of the FRP laminates will be enhanced by dynamic effects such as inertia and wave propagation. The nose shape of missiles also has an effect on the ballistic perforation process. In the following, a simple model is proposed for the high speed perforation of FRP laminates by missiles with different nose shapes. It is assumed that the mean pressure (s) applied normally to the surface of the missile provided by an FRP laminate target material to resist penetration

IBF8 11/22/2000 6:51 PM Page 267

Perforation of FRP laminates and sandwich panels subjected

267

and perforation by a missile can be decomposed into two parts, one part is the cohesive static resistive pressure (ss) due to the elastic-plastic deformations of the laminate material and the other is the dynamic resistive pressure (sd) arising from velocity effects. Thus23 s = ss + sd

[8.14]

If it is further assumed that the cohesive static resistive pressure is equal to the static linear elastic limit (se) in through-thickness compression of the FRP laminates,1,10 i.e. ss = se, and that the dynamic resistive pressure (sd) is a function of the parameter (rt/se)1/2Vi and is taken to be sd = G(rt/se)1/2Vise,23 then equation [8.14] can be rewritten as rt ˘ È s = Í1 + G Vi s e s e ˙˚ Î

[8.15]

Here rt and Vi are the density of the FRP laminates and the initial impact velocity of the missile, respectively. G is a constant which is determined empirically. In Wen,23 by curve-fitting the perforation data, G has been evaluated to be 2, 1.5 and 2 sin(q/2) for flat-faced, hemispherical-ended and conical-nosed missiles, respectively. Here q is the cone angle of a conical-nosed projectile.

8.4.2.2 Perforation of FRP laminates/sandwich panels The ballistic limit condition for FRP laminates and sandwich panels with such laminates as skins and with foam core struck transversely by a rigid missile with different nose shapes can be estimated from energy consideration. It is easy to show that Ek =

pD2Ts pD2T È rt ˘ = Vb s e 1+ G s e ˙˚ 4 4 ÍÎ

[8.16]

Substituting Ek = (1/2)GVb2 into the above equation and rearranging yields Vb =

pG r t s e D2T 4G

8G È ˘ ÍÎ1 + 1 + pG 2 r D2T ˙˚ t

[8.17]

where Vb is the critical impact velocity or ballistic limit.

8.5

Comparisons and discussion

The four constants, viz. A, b1 in equation [8.5] and B, b3 in equation [8.7] are determined by a curve-fitting technique using the test data obtained from the experimental programmes. As noted earlier in Section 8.3.1, all the quasi-static tests performed on sandwich panels by hemispherical-

IBF8 11/22/2000 6:51 PM Page 268

268

Impact behaviour of composite materials and structures

ended indenters thus far can be classed into two groups (see Fig. 8.4(a)) depending upon the ratio of the total panel thickness to punch diameter, H/D. ef in equation [8.5] is taken to be 0.021.1 For H/D < 2, A = 0.05, b1 = 1/3; for H/D > 2, A = 0.016, b1 = 1. Figure 4(a) shows how equation [8.5] correlates with the experimental data with these values of A and b1. On the other hand, all the quasi-static tests conducted on sandwich panels by flat-faced punches, as shown in Fig. 8.4(b), followed the same trend irrespective of the ratios of H/D. The data points for the global energy (Eg) presented in Fig. 8.4(b) are calculated using equation [8.1] and equation [8.6]. ed in equation [8.6] is taken to be 0.8 for H130 foam core employed in the tests, which may be estimated from the load-displacement characteristics as shown in Fig. 8.3(a) (from which it can be seen that the 25 mm thick foam core crushed about 20 mm when the bottom skin of the sandwich panel failed. Hence, ed = 20/25 = 0.8). It can be shown that the two constants, namely, B and b3 in equation [8.7] can be estimated to be B = 0.016 and b3 = 1. It should be noted here that these two values are the same as those for sandwich panels loaded by hemispherical-ended indenters with H/D > 2. It is seen from Fig. 8.4(b) that equation [8.7] with these two values is in good correlation with the experimental data. Equation [8.10] has been fitted to the available experimental results presented in Fig. 9(a), (b) and (c). rt and Es1 in equation [8.10c] are taken to be 1650 kg/m3 and 24 GPa, respectively (Wen et al.1). Substituting these values and ef = 0.021 into equation [8.10c] gives Vo = 80 m/s. The empirical constant, b, in the equation has been evaluated to be b = 4.5 and 1.5 for sandwich panels struck by hemispherical-ended projectiles with H/D < 2 and H/D > 2, respectively. For sandwich panels impacted by flat-faced missiles b has been evaluated to be b = 1.5. As can be seen from Fig. 8.9, with these values for b, there is good correspondence between equation [8.10] and the test data. Comparisons are made in Fig. 8.6(a) and (b) between the model predictions (equations [8.13 and [8.11]) and the experimental results obtained for GRP skin sandwich panels with H/D > 2 and H/D < 2 struck normally by hemispherical-ended projectiles. In Fig. 8.6(a) the solid line is the predictions of equation [8.13] with A = 0.016, b1 = 1 and b = 1.5, whilst in Fig. 8.6(b) the solid line represents equation [8.13] with A = 0.05, b1 = 1/3 and b = 4.5. It is clear from these two figures that the model predictions (equations [8.13] and [8.11]) fit the experimental results with good accuracy. Comparisons are also made in Fig. 8.6(c) and (d) between the model predictions (equations [8.13] and [8.12]) and the test data obtained for sandwich panels impacted by flat-faced missiles. The solid lines are the predictions of equation [8.13] with B = 0.016, b3 = 1 and b = 1.5. It is seen

IBF8 11/22/2000 6:51 PM Page 269

Perforation of FRP laminates and sandwich panels subjected

269

from Figs. 8.6(c) and (d) that the model (equations [8.13] and [8.12]) fits well with the experimental data. Figure 8.6(e) shows the experimental plots of the residual velocity versus impact velocity for 0.3 m square sandwich panels with H130 foam core impacted by a 10.5 mm diameter hemispherical-headed missile with a mass of 17.9 g at velocities up to 305 m/s. Also shown in Fig. 8.6(e) as solid lines are predictions based upon 1

Vr = (V 2i - V b2 ) 2

[8.18]

where Vr and Vi are the residual and incident impact velocities of the missile, respectively and Vb is the ballistic limit which is determined by equation [8.13]. It is evident from Fig. 8.6(e) that the model predictions are in good accord with the experimental observations. As noted earlier, the difference of the energies absorbed by identical sandwich panels loaded by hemispherical-ended indenters and conicalnosed punches are negligibly small and therefore the equations derived above for hemispherical indenters may also be applicable for conical punches. Indeed, as can be seen from Fig. 8.6(a), (b) and (e), good agreement is also obtained between the model predictions and the experimental data for sandwich panels struck by conical-nosed projectiles which are represented by the triangle (D) in Fig. 8.6(a) and (b) and the solid symbols in Fig. 8.6(e). Figures 8.10(a) and (b) show photographs of two identical panels with 7.0 mm thick GRP skins and 25 mm thick H130 foam core tested with 10.5 mm diameter hemispherical-ended and conical-nosed missiles at impact velocities of 199 m/s and 197 m/s, respectively which lend further support to the above argument. To a first approximation, the equations developed above may also be applied or adapted to monolithic FRP laminates subjected to missile impact and have been checked against published data on FRP laminates. For hemispherical-ended and conical-nosed projectiles the empirical constants in the appropriate equations are found to be A = 0.05, b1 = 1/3, b = 4.5 for simply-supported single laminates using the data presented above for panels with H/D < 2 and A = 0.016, b1 = 1, b = 4.5 for fully-clamped monolithic laminates using the data reported by Zhu et al.11 Figure 8.11(a) shows comparisons between equation [8.13] (solid line) and the test data for simply-supported GRP single laminates struck transversely by the 10.5 mm diameter hemispherical-ended projectile of 17.9 g mass. It is evident from Fig. 8.11(a) that the model predictions are in good agreement with the experimental data. Figure 8.11(b) demonstrates the comparison between equation [8.13] (solid line) and the experimental results for fully-clamped KFRP single laminates subjected to impact by a 12.7 mm diameter conical-nosed missile with a mass of 28.9 g, reported by

IBF8 11/22/2000 6:51 PM Page 270

(a)

(b) 8.10 Photographs of two 0.3 m square sandwich panels with 7.0 mm thick GRP skins and 25 mm thick H130 foam core tested with 10.5 mm diameter projectiles. (a) hemispherical-ended projectile at an impact velocity of 199 m s-1; (b) conical-nosed missile at an impact velocity of 197 m s-1.

IBF8 11/22/2000 6:51 PM Page 271

Perforation of FRP laminates and sandwich panels subjected

271

Vb (m s-1) Hemispherical

180

Equation [8.17]

120

Equation [8.13]

60

0

2

4

6

T (mm) (a) Vb (m s-1)

Conical

180

Equation [8.13]

Equation [8.17]

120

60

0

2

4

6

8

10 T (mm)

12

14

(b)

8.11 (a) Comparison of the model predictions with the experimental results for simply-supported GRP single laminates struck by a 17.9 g, 10.5 mm diameter hemispherical-ended missile. (b) Comparison of the model predictions with the test data for fully-clamped KFRP monolithic laminates impacted by a 28.9 g, 12.7 mm diameter conical-nosed missile. (After Zhu et al.11) (c) Comparison of the model predictions with the experimental data for simply-supported GRP single laminates struck by a 20.4 g, 10.5 mm diameter flat-faced missile.

IBF8 11/22/2000 6:51 PM Page 272

272

Impact behaviour of composite materials and structures Vb (m s-1) Flat

Equation [8.17]

100

Equation [8.13] 50

0

1

2

3 T (mm)

4

(c)

8.11 (cont.)

Zhu et al.11,12 It is seen from Fig. 8.11(b) that equation [8.13] gives a good fit to the test data reported by those authors when A = 0.016, b1 = 1 and b = 4.5 are used. For flat-faced missiles the appropriate equations developed previously for sandwich panels may be adapted directly to single FRP laminates. It has been observed experimentally that, depending upon the ratio of laminate thickness to missile diameter, either shear plugging (plus delamination) or shear plus tensile fracture (plus delamination) are the predominant failure mechanisms in the perforation of monolithic FRP laminates subjected to impact by flat-ended projectiles. It is further assumed that this critical value for T/D is to be determined empirically and may be taken as 1/4. Thus, one obtains Epi L p t13 ˆ Ê T ˆ = Ê + 0.016Ê ˆ 2 Ë ¯ Ë ¯ Ë 2 su D D¯ fs uTD

[8.19]

for T/D £ 1/4 (i.e. thin single FRP laminates), and Epi p t13 ˆ È 1 1 Ê D ˆ ˘ p e f = Ê + 2 2 Ë s u ¯ ÍÎ 2 16 Ë T ¯ ˙˚ 8 fs uTD

1 Ê Dˆ ˘ È Ê Lˆ ÍÎ1 - 4 Ë T ¯ ˙˚ + 0.016Ë D ¯ [8.20]

for T/D >1/4 (viz. thick monolithic FRP laminates). Figure 8.11(c) shows the comparison of equation [8.13] which incorporates equation [8.19] (solid line) with the limited test data obtained for simply-supported single GRP laminates struck by a 20.4 g, 10.5 mm diame-

IBF8 11/22/2000 6:51 PM Page 273

Perforation of FRP laminates and sandwich panels subjected

273

ter flat-faced projectile. It is seen from Fig. 8.11(c) that the model predictions are in good agreement with the limited experimental data. Figures 8.12–8.14 show comparisons of equation [8.13] with the recently obtained high velocity perforation data for glass fibre-reinforced polymeric laminates struck transversely by flat-faced, hemispherical-ended and conical-nosed (90° cone) missiles, respectively. It is seen from Fig. 8.12 that equation [8.13] incorporating equation [8.20] (solid line) predicts well the ballistic limits at relatively low velocities but underpredicts the ballistic limits at higher velocities for the GRP laminates subjected to impact by flat-faced missiles. It is also seen from Fig. 8.13 and 8.14 that equation [8.13] incorporating equation [8.11] (solid line) overpredicts the ballistic limits compared to the experimentally obtained values for the GRP laminates when struck by hemispherical-ended and conical-nosed projectiles. The predictions by the newly developed wave-dominated model for high velocity perforation of FRP laminates/sandwich panels are also presented in Fig. 8.6(a–d), Fig. 8.11(a) and (c) and Figs. 8.12–8.14. In the theoretical calculation,1 rt = 1650 kg/m3, se = 225 MPa and G has been evaluated to be G = 2, 1.5 and 2 sin(q/2) for flat-faced, hemispherical-ended and conicalnosed missiles, respectively.23 Here q is the cone angle of a conical-nosed missile. It is clear from Fig. 8.5(a–d) and Fig. 11(a) and (c) that the high velocity perforation model, equation [8.17], is in reasonable agreement with the experimental data.1 It is also clear from Fig. 8.12–8.14 that equation [8.17] predicts well the high velocity perforation of the GRP laminates examined in Mines et al.14 The high velocity perforation model is also compared in Fig. 8.11(b) with the ballistic perforation of KFRP laminates impacted by a 28.9 g, 12.7 mm diameter conical-nosed missile investigated in Zhu et al.11 In the theoretical calculation, rt = 1231 kg/m3, se = 145 MPa and q = 60°.11 It is seen from Fig. 8.11(b) that the model predictions (equation [8.17]) are in good agreement with the test results. The applicability of the models is dictated by the range of impact parameters examined in the present investigations. For example, the range of impact velocities studied lies between 0 and 305 m/s from which the empirical models have been derived. Furthermore, the empirical constants in the models have mainly been determined from the present experiments conducted on GRP laminates and sandwich panels with such laminates as skins and with foam cores and, strictly speaking, these constants are valid only for the material systems investigated. Therefore, care should be exercised when the model with these empirical constants is applied to other material systems though it has been shown to give good representation for KFRP laminates. From the comparisons between the empirical models and the high veloc-

IBF8 11/22/2000 6:51 PM Page 274

274

Impact behaviour of composite materials and structures

6 g Flat woven

700

6 g Flat Z-stitch

Vb (m s-1)

600 500

Equation [8.17]

400 300

Equation [8.13]

200 100 0

0

0.5

1.0

1.5 T/D

2.0

2.5

(a) 12 g Flat woven

500

12 g Flat Z-stitch

Vb (m s-1)

400

Equation [8.13]

300

200 Equation [8.17] 100

0

0

0.5

1.0

1.5

2.0

2.5

T/D (b)

8.12 Comparison of the model predictions with the experimental data for fully-clamped GRP single laminates struck by a 7.6 mm diameter flat-faced missile. (a) G = 6 g; (b) G = 12 g. (After Mines et al.14)

IBF8 11/22/2000 6:51 PM Page 275

Perforation of FRP laminates and sandwich panels subjected

700

275

6 g Hemisphere woven 6 g Hemisphere Z-stitch

600 Equation [8.13]

Vb (m s-1)

500 400

Equation [8.17]

300 200 100 0 0

0.5

1.0

1.5

2.0

2.5

T/D (a)

12 g Hemisphere woven

500

12 g Hemisphere Z-stitch

Vb (m s-1)

400

Equation [8.13]

300

200 Equation [8.17] 100

0 0

0.5

1.0

1.5

2.0

2.5

T/D (b)

8.13 Comparison of the model prediction with the experimental data for fully-clamped GRP single laminates struck by hemispherical missiles. (a) D = 10 mm; G = 6 g; (b) D = 7.6 mm, G = 12 g. (After Mines et al.14)

IBF8 11/22/2000 6:52 PM Page 276

276

Impact behaviour of composite materials and structures

700

6 g Cone woven 6 g Cone Z-stitch

600 Equation [8.13] Vb (m s-1)

500 400 300

Equation [8.17]

200 100 0

0

0.5

1.0

1.5

2.0

2.5

T/D (a)

12 g Cone woven 12 g Cone Z-stitch

500

Vb (m s-1)

400

Equation [8.13]

300

200 Equation [8.17] 100

0 0

0.5

1.0

1.5

2.0

2.5

T/D (b)

8.14 Comparison of the model predictions with the experimental data for fully-clamped GRP single laminates struck by a 7.6 mm diameter conical-nosed missile. (a) G = 6 g; (b) G = 12 g. (After Mines et al.14)

IBF8 11/22/2000 6:52 PM Page 277

Perforation of FRP laminates and sandwich panels subjected

277

ity perforation model and the available experimental data there exists a critical condition at which a change takes place in the mode of deformation from global response (low velocity impact) to localized deformation (wave-dominated response). It is very difficult to determine the critical condition either theoretically or experimentally, and this needs to be further investigated in a future study.

8.6

Conclusions

The results of quasi-static, drop-weight and ballistic impact tests performed on triple- as well as twin-skinned sandwich panels and single laminate skins using flat-faced, hemispherical-ended and conical-nosed indenters/projectiles with initial impact velocities up to 305 m/s have been briefly reported and discussed. Typical load-displacement characteristics under quasi-static and dropped object loading have been presented. Ballistic limits (perforation energies) have been determined and a classification of the responses deduced from the test data obtained. Experimental evidence has shown that ballistic impact on FRP laminates and sandwich panels with such laminates as skins and with foam cores may be categorized into two regimes, viz. low velocity impact and wavedominated response. Based on the experimental observations, dimensional analysis has been used to derive empirical equations that predict the penetration and perforation energies of fibre-reinforced plastic (FRP) laminates and sandwich panels with such laminates as skins and with foam cores subjected to quasistatic and impact loading by flat-faced and hemispherical-ended indenters. It is shown that the empirical formulas correlate well with the available data from experiments carried out by the authors and others. It is also shown that, to a first approximation, the formula obtained for hemisphericaltipped indenters is applicable to conical-nosed punches. A new model has also been developed for the high velocity perforation of FRP laminates and sandwich panels struck transversely by flat-faced, hemispherical-ended and conical-nosed missiles. It is found that the model predictions are in good agreement with the recently published14 high velocity perforation data. Future investigation should be directed towards clearly defining the respective ranges of impact parameters for which the models developed in Sections 8.4.1 (i.e. low velocity impact) and 8.4.2 (wave-dominated response/high velocity perforation) apply and engaging in detailed modelling of the range of failure mechanisms which control the failure of the laminates. Such investigation should lead to a methodology for optimising the design of FRP laminates and sandwich panels against impact loading.

IBF8 11/22/2000 6:52 PM Page 278

278

Impact behaviour of composite materials and structures

References 1 Wen H M, Reddy T Y, Reid S R and Soden P D, ‘Indentation penetration and perforation of composite laminates and sandwich panels under quasi-static and projectile loading’, Key Eng Mater, 1988 141–143 501–52. 2 Reddy T Y, Wen H M, Reid S R and Soden P D, ‘Penetration and perforation of composite sandwich panels by hemispherical and conical projectiles’, Trans ASME, J Pres Ves Technol, 1988 120 186–94. 3 Reid S R, Wen H M, Soden P D and Reddy T Y, ‘Response of single skin laminates and sandwich panels to projectile impact’, in Composite Materials for Offshore Operation – 2, (S S Wang, J J Williams and K H Lo, eds), pp 593–617. American Bureau of Shipping, 1999. 4 Abrate S, ‘Impact on laminated composite materials’, Appl Mech Rev, 1991 44(4) 155–90. 5 Abrate S, ‘Impact on laminated composites: recent advances’, Appl Mech Rev, 1994 47(11) 517–43. 6 Rutherford K L, ‘Indentation and penetration resistance of composite materials to pointed projectiles’, unpublished UK DRA Report, 1992. 7 Zhao Y, Pang S S and Griffin S A, ‘Force-indentation study of transversely isotropic composite materials using a conical-tip indenter’, Composites Eng, 1991 1(6) 393–402. 8 Greaves L J, ‘Failure mechanisms in GFRP armour’, unpublished UK DRA Report, 1992. 9 Greaves L J, ‘Progress in modelling the perforation of GFRP by ballistic projectiles’, unpublished UK DRA Report, 1994. 10 Reid S R, Reddy T Y, Ho H M, Crouch I G and Greaves L J, ‘Dynamic indentation of thick fibre-reinforced composites’, in High Rate Effects on Polymer, Metal and Ceramic Matrix Composites and Other Advanced Materials (Y D S Rajapakse and J R Vinson, eds), AD-Vol 48 ASME, 71–9, 1995. 11 Zhu G, Goldsmith W and Dharan C K H, ‘Penetration of laminated Kevlar by projectiles – I. Experimental investigation’, Int J Solids Struct, 1992 29(4) 399–420. 12 Zhu G, Goldsmith W and Dharan C K H, ‘Penetration of laminated Kevlar by projectiles – II. Analytical model’, Int J Solids Struct, 1992 29(4) 421–36. 13 Lee S-W R and Sun C T, ‘Dynamic penetration of graphite/epoxy laminates impacted by a blunt-ended projectile’, Composites Sci Technol, 1993 49 369– 80. 14 Mines R A W, Roach A M and Jones N, ‘High velocity perforation behaviour of polymer composite laminates’, Int J Impact Eng, 1999 22 561–88. 15 Moriarty K and Goldsmith W, ‘Dynamic energy absorption characteristics of sandwich shells’, Int J Impact Eng, 1993 13(2) 293–317. 16 Goldsmith W and Sackman J L, ‘An experimental study of energy absorption in impact on sandwich plates’, Int J Impact Eng, 1992 12 241–61. 17 Evans K E, ‘Design of doubly curved sandwich panels with honeycomb cores’, Composite Struct, 1990 17 95–111. 18 Allen H G, Analysis and Design of Sandwich Structures, Oxford, Pergamon Press, 1969. 19 Vinson J R, ‘Optimum design of composite sandwich panels subjected to uniaxial compression’, AIAA J, 1988 24 1690–6.

IBF8 11/22/2000 6:52 PM Page 279

Perforation of FRP laminates and sandwich panels subjected

279

20 Bernard M L and Lagace PA, ‘Impact resistance of composite sandwich panels’, J Reinforced Plastic Composites, 1989 8 432–45. 21 Kosza P and Sayir M B, ‘Failure patterns in the core of sandwich structures under impact loading’, Int J Impact Eng, 1994 15(4) 501–17. 22 Wen H M and Jones N, ‘Semi-empirical equations for the perforation of plates by a mass’, in Structures Under Shock and Impact – II, (P S Bulson, ed), pp 369–80. Computational Mechanics Publications, Southampton and Boston, Thomas Telford, London, 1992. 23 Wen H M, ‘Predicting the penetration and perforation of FRP laminates struck normally by a projectile with different noseshapes’, Composite Structures, 2000 49 321–9.

IBF9 11/22/2000 6:57 PM Page 280

9 High-velocity impact damage to polymer matrix composites R C TENNYSON AND C G LAMONTAGNE

9.1

Introduction

One of the major concerns involving the use of light-weight fibre-reinforced composites is their susceptibility to impact damage. Delamination (or interlaminar fracture), surface spallation and laminate penetration constitute various modes of failure resulting from impact loads. Low-velocity impacts are associated with delamination damage, especially that caused by bluntheaded projectiles. This inter-laminar debonding primarily reduces the local bending stiffness and thus can affect the bending and buckling behaviour of the structure. In the latter case, local buckling can induce further delamination growth which can lead to overall global weakening of the structure. Such damage has been reported to cause as much as a 40% reduction in static and fatigue strength.1,2 Low-velocity impacts have also been shown to reduce cylindrical shell buckling strengths by as much as 25 ~ 35%.3 As impact energy is increased, delamination coupled with surface spallation can occur, followed by penetration of the laminate. Figure 9.1 shows photomicrographs of front and rear face spallation damage to a graphite/PEEK laminate. An enlarged view of the damage associated with surface spallation and through-thickness delamination can be seen in Fig. 9.2. The ‘ballistic limit’ defines that energy which is required for a projectile to penetrate to the rear face of the laminate. Such cases are characterised by front face spallation, localised delamination below the surface (easily detected by ultrasonic C-scan) and an ‘impact hole’ just reaching the rear face. Beyond the ballistic limit, higher energy impacts produce all of the above features coupled with a crater hole, rear face spallation and ejecta plumes emanating from both sides of the laminate. Figure 9.3 presents photomicrographs of a crater hole viewed from the front and rear faces of a graphite/epoxy tube due to an actual micrometeoroid hypervelocity impact recorded on an experiment aboard a NASA satellite (LDEF, 1984–1990). Again, spallation damage is visible. 280

IBF9 11/22/2000 6:58 PM Page 281

High-velocity impact damage to polymer matrix composites

9.1 Impact damage on front/back faces.

281

IBF9 11/22/2000 6:58 PM Page 282

282

Impact behaviour of composite materials and structures

9.2 Impact damage on back face and through-thickness of graphite/epoxy laminate.

IBF9 11/22/2000 6:58 PM Page 283

High-velocity impact damage to polymer matrix composites

283

9.3 SEM Photographs of micrometeoroid/debris impact/exit holes for graphite/epoxy tube (SP-288/ T300, [±43°]4s).

IBF9 11/22/2000 6:58 PM Page 284

284

Impact behaviour of composite materials and structures

One of the dangerous features of hypervelocity impact is the debris plume emanating from the rear face. These ejecta particles can impact adjacent structures and components within the interior of the impacted structure. This of course includes human occupants residing inside a containment vessel such as the cylindrical habitat structures of the International Space Station (ISS), presently being deployed over the next several years. The ejecta from such hypervelocity impacts (i.e. at typical orbital velocities ≥7 km s-1) also travel at comparable speeds and can thus penetrate other structures causing much enhanced damage.4 Whereas the hypervelocity impacting particle produces an irregular shaped ‘hole’ or crater (typically 2.5–3 times larger than the particle diameter) on first hitting a laminate, the subsequent fracture of the particle and composite material at the impact site results in a debris plume containing 10–100 fold more particles that spread in a spherical or tear-drop pattern. Depending on the distance traveled and ‘cone’ angle, these particles produce an impact pattern and damage zone many times larger than the original crater. For composite shell structures, this secondary damage from the debris plume can lead to major structural failure.4 Hypervelocity impact conditions are most likely to occur on spacecraft in low earth orbit (LEO, 200–1000 km altitude). They are vulnerable to impact damage resulting from collisions with natural micrometeoroids (£1 cm diameter) and orbital debris (known as the MOD environment). Micrometeoroids originate from planetary or asteroidal collisions and cometary ejecta. Artificial space debris consists of everything from spent satellites and rockets to aluminum oxide fuel particles, paint chips and fragmentation objects from collisions of these bodies in orbit. A plot of the MOD environment as a function of altitude and particle size is presented in Fig. 9.4. This chart does not depict the enhanced micrometeoroid fluxes that occur when the earth passes through periodic ‘showers’ that can produce flux increases of 5–10 times that of the ‘natural’ background. In some isolated cases, these fluxes can reach as high as 105 times the background (such as the Leonid meteor storms in November 1998 and 1999). Fibre-reinforced polymer matrix composites are used extensively in spacecraft structures and satellite components such as antenna struts, panels and low distortion frames. The largest composite structure in space is the Canadian robot arm mounted on all of the Space Shuttles. A much more complex robot consisting of graphite IM7/PEEK cylinders has been assembled for the ISS Remote Manipulator System. Perhaps the greatest spacecraft application of composites is the Iridium telecommunications satellite constellation currently in orbit (~66 satellites) which employs carbon/epoxy laminates on the satellite exterior panels. Clearly, with the high cost of replacement of spacecraft, and particularly with the presence of humans in

IBF9 11/22/2000 6:58 PM Page 285

High-velocity impact damage to polymer matrix composites

285

1e3 1e2

Particle flux (#/m2 yr)

1e1 1e0 1e-1 Debris altitude (km)

1e-2 1e-3 1e-4 1e-5

100

0

Micrometeoroids 100–1000 km altitude

500 400 300

1e-6

100

1e-7 1e-8 0.001

0.01

0.1

1

10

Particle diameter (cm)

9.4 Micrometeoroid and orbital debris flux as a function of altitude (NASA CR # BB000883A, January 1991).

some cases, it is essential that the effects of hypervelocity impacts on materials and structures must be understood in order to evaluate risks and provide for the safe and reliable design of these systems. This is particularly true for composite materials where the data base is scarce and their utilisation is increasing. This chapter reviews hypervelocity impact damage to composites, with special emphasis on test data obtained on graphite epoxy and PEEK laminates. Sufficient data have been obtained to provide some insight on the major parameters governing the initial impact and debris damage that occurs.

9.2

Hypervelocity impact (HVI) tests on composites

Studies of HVI damage to composite materials and structures can be classified into three categories: flat plate laminates, tubes/cylinders, and composite laminate/sandwich structures. In the first category, a large number of graphite/epoxy, graphite/PEEK and Kevlar®/epoxy laminates have been investigated.5–13 Early work by Yew et al.5,6 on graphite/epoxy plates was done at the NASA Johnson Space Center (JSC), USA using their light gas gun facilities. A wide range of plate thicknesses was studied, including quasi-isotropic configurations. Later, Christiansen13 reported on a more detailed series of tests in which both high and low modulus graphite/epoxy laminates were tested, including tubes. Again, various target thicknesses were used and different impact angles

IBF9 11/22/2000 6:58 PM Page 286

286

Impact behaviour of composite materials and structures

employed. It was found that fibre modulus has a greater effect than lay-up. Lower energy impact tests were conducted on both graphite/epoxy and PEEK laminates,8 but the parametric range was small. A subsequent study focusing on PEEK/IM7 and AS-4 flat plates was reported,9 where varying thickness laminates of different lay-ups were tested. These experiments were conducted at JSC covering a wide range of projectile energies, including some cylinder tests as well. Most of the data reported to-date are for normal impact conditions, although some results have been obtained for oblique angles.12,13 In Lamontagne et al.,12 the experiments were undertaken at the University of Kent, UK using their light gas gun. It was observed that for oblique angle impacts, the debris cloud does not follow the line of flight of the projectile. Moreover, the cone angle associated with the debris cloud is not symmetric about the projectile impact velocity vector. Design charts derived from much of the test data reported in the above references will be described later. In comparison, HVI tests on composite tubes and cylinders are few in number.13–16 Of particular interest in these studies is the effect of the debris plume on the damage to the opposing wall. As noted earlier, the energy associated with the ejecta particles at orbital impact velocities is sufficiently high that structural failure of a cylinder under compressive loading can occur when the damage zone is large enough.4 Studies of HVI damage to composite laminate/sandwich panels have been reported for honeycomb17–20 and various heat shield materials.21 An extensive data base has been compiled for normal and oblique impacts on honeycomb/woven carbon fibre/epoxy structures.20 This data has been used to determine the ballistic limit which showed a strong dependence on impact angle. Additional data were published21 for graphite/epoxy laminates bonded to different types of heat shield material combinations subjected to normal hypervelocity impact conditions. Substantial data were obtained on the correlation of entry hole size and impactor energy. This chapter focuses on HVI damage to composite laminates only, with special emphasis on graphite/epoxy and PEEK materials.

9.3

Entry impact damage

The entry crater or hole size produced by the impact of a particle with a composite laminate can be correlated with the parameter (as suggested by Christiansen13) [Etrt/Dprp]1/3 where E is the projectile’s energy (J), t is the target thickness (mm), Dp is the projectile diameter (mm), rt and rp are the densities of the target and projectile, respectively.The entry crater is defined as Dc which is the equivalent diameter of a circle that encompasses the same area as the irregularly shaped hole. The projectile energy E is calculated as 1/2 m V n2 where Vn is the normal velocity component of the projectile

IBF9 11/22/2000 6:58 PM Page 287

High-velocity impact damage to polymer matrix composites Auburn GRE (SiC)

Auburn PEEK (SiC)

JSC PEEK (Al)

SwRl PEEK (Al)

USAF #1 PEEK (Al/Nylon)

Austin GRE (Al)

Eagle GRE (low E & Al)

USAF PEEK #2 (steel)

MSFC PEEK (Al)

SSRMS PEEK (Al)

UKC PEEK (Al)

Regression

287

Crater diameter (mm)

25 20 15 10 D c = 1.05

3

E

t rt Dp r p

5 0 0

5

10 3

15 t rt E Dp r p

20

[ J] 3

9.5 Equivalent crater diameter as a function of impact energy parameter.

velocity V and is given by V cos q, where q is the angle of V relative to the surface normal. Based on the AS-4 and IM7graphite/PEEK laminate test data described in Tennyson and Shortliffe,4,11 Fig. 9.5 illustrates the correlation between Dc and the energy parameter using a regression line forced to pass through zero. A variety of laminate lay-ups and thicknesses were tested under normal impact conditions using aluminum spheres of different diameters. Included in this plot are test results on AS-4graphite/PEEK cylinders16 and graphite/epoxy plates.13,8,5 In the latter case, some data from unpublished contract reports are also included. These results were obtained for a broad range of projectile diameters (0.4–9.13 mm), travelling at velocities from 4 to 7.5 km/s, for a variety of materials including glass, nylon, steel and SiC. More recent oblique angle impact tests were conducted on AS-4 graphite/PEEK flat plate laminates12 of different thicknesses using aluminum spheres of diameter 1–2 mm over a velocity range of 4.5–5.5 km/s. Impact angles of 0°, 30° and 45° were investigated. These results (UKC) are also plotted in Fig. 9.5 where it can be seen that reasonable correlation with normal impact data was found based on the normal velocity component.

IBF9 11/22/2000 6:58 PM Page 288

288

Impact behaviour of composite materials and structures

NASA JSC HIT-F shot #A2704 Target: SSRMS boom #1 Projectile diameter: 3.2 mm Velocity: 6.4 km s -1 Impact angle: 0°

9.6 Photograph of crater and front face spallation damage due to hypervelocity impact on graphite/PEEK laminate.

From a structural design point of view, the entry damage on the front face is an important parameter for assessing the overall reduction in stiffness, strength or long-term fatigue life due to crack propagation from this damaged region. The entry damage zone includes the crater hole and associated delamination/surface cracking area, as can be seen in the photograph shown in Fig. 9.6. As in the case of the hole diameter calculation, this region can also be defined by an ‘equivalent entry damage diameter’ parameter. Using earlier data,4,8,11 the entry damage diameter is plotted as a function of a reduced energy parameter in Fig. 9.7. Included in this graph is the regression curve based on C-scan measurements of the sub-surface damage zones. It can be seen that even though the delamination lies below the surface, the enhanced area is only about 20% greater than the visible surface area. To estimate probable damage for a given projectile impactor size, it is

IBF9 11/22/2000 6:58 PM Page 289

High-velocity impact damage to polymer matrix composites Auburn GRE (SiC)

Auburn PEEK (SiC)

JSC PEEK (AI)

SwRI PEEK (AI)

USAF #1 PEEK (AI/SiC)

Regression

C-Scan regression

UKC PEEK (AI)

289

Entry damage diameter (mm)

50 40 D C -scan = 4.043 E 30

t Dp

20 Dentry damage = 3.733 E 10

t Dp

0 0

2

4 3

E

6 t Dp

8

10

[ J] 3

9.7 Equivalent entry damage diameter as a function of impact energy parameter (visible and C-Scan).

useful to correlate the measured crater diameters with the known impactor diameters. Figure 9.8 presents this plot based on the above experiments. The regression curve was constructed only through the PEEK data. There appears to be no energy dependence when one considers complete penetration tests. However, for projectile diameters below 1 mm, it is apparent that the hole diameter can be taken as equal to the particle diameter. Rear face spallation damage on the impacted laminate is also an important parameter for assessing overall entry damage. Using the same data base, Fig. 9.9 illustrates the correlation of the equivalent damage diameter with the reduced energy parameter. The regression analysis indicates that this damage area is comparable to that observed on the front face for a given energy parameter.

9.4

Secondary debris cloud

Once the projectile has impacted and penetrated the laminate, two debris clouds are formed. These clouds or plumes of ejecta, formed by the disintegration of the wall material and the projectile, emanate from both the front and rear faces of the laminate. For high-velocity impacts, it has been found that the velocity of the ejecta is comparable to that of the impactor

IBF9 11/22/2000 6:58 PM Page 290

290

Impact behaviour of composite materials and structures

Auburn GRE (SiC)

Auburn PEEK (SiC)

JSC PEEK (Al)

SwRl PEEK (Al)

USAF #1 PEEK (Al/nylon)

Austin GRE (Al)

Eagle GRE (low E & Al)

Regression

UKC PEEK (Al)

Crater diameter (mm)

10 8 6 4 Dc = 2.67Dp 2 0 0

0.5

1

1.5 2 Projectile diameter (mm)

2.5

3

9.8 Equivalent crater diameter as a function of projectile diameter.

JSC PEEK (AI)

SwRI PEEK (AI)

Regression

UKC PEEK (AI)

USAF #1 PEEK (AI/SiC)

Spall damage diameter (mm)

30 25 20 15 10 Dspall = 3.123 E 5

t Dp

0 0

2

4 3

E

6 t Dp

8

10

[ J] 3

9.9 Equivalent rear face spall diameter as a function of impact energy parameter.

IBF9 11/22/2000 6:58 PM Page 291

High-velocity impact damage to polymer matrix composites

291

for the range of parameters studied.16 Consequently, the ejecta energy in the secondary debris cloud emanating from the rear face can be sufficiently high as to penetrate another adjacent composite laminate. Depending on the separation distance and the plume cone angle, damage areas much larger than the impact crater hole can occur. To demonstrate this process, consider the high speed photographs (Fig. 9.10) of an aluminum projectile (~9 mm diameter) impacting a composite cylindrical shell constructed of IM7/PEEK material, 19 plies thick (~2.7 mm) and 33 cm in diameter. The cylinder is a symmetric, balanced laminate (+/-43° with a single 0° centre ply). A Cordin high speed camera capable of snapping 80 frames over an elapsed time of 100 ms was used to record this impact.16 These frames show the early formation of the debris cloud and the subsequent growth of the spherical shaped plume of ejecta. Impact of the debris cloud with the rear wall of the cylinder results in the large damage area visible in the photograph of Fig. 9.11. Analysis of the debris plume velocity reveals that the cloud tip travelled at approximately the same velocity as the projectile. The damage resulting from this debris cloud impact (Fig. 9.11) contains many holes in the rear wall. This region is defined by a 200 mm diameter circle, thus yielding a damage cone angle of ~69.5°. Because of the multiple penetrations, cracks and spallation damage, the cylinder can be regarded as having a circular ‘cutout’ for structural analysis purposes. Analysis performed4 showed a compressive buckling strength loss for this cylinder of over 50%. Similar results were found in the flat plate IM7/PEEK tests.11 Using composite witness plates located 330 mm behind the primary impact sites, detailed mapping of the major debris impacts was performed to evaluate the ejecta plume damage and cone angles associated with the various laminate configurations tested. A plot of the semi-angles is presented in Fig. 9.12 as a function of the energy parameter. It is apparent that an average semi-cone angle of ~12.3° can be attributed to these experiments. Figure 9.13 depicts a schematic of one such plume impact where 87 craters were counted within a 120 mm diameter circle. The fact that these craters define holes in the laminate with associated spallation damage testifies to the ejecta energy. The typical projectile used in these tests was 2 mm in diameter and traveled at 6–7 km s-1. A series of oblique angle impact tests were conducted on 16 and 24-ply AS-4/PEEK plates12 to investigate plume damage using aluminum projectiles (1 and 2 mm in diameter) at velocities of 4.5–5.5 km/s. Analysis of the debris cloud impacts on adjacent aluminum witness plates showed that in fact there are two classes of damage. A primary damage zone was identified by large craters associated with projectile fragments, with a secondary area containing a larger number of smaller craters having carbon fibres imbedded in the aluminum plate. Figures 9.14 and 9.15 illustrate the

IBF9 11/22/2000 6:58 PM Page 292

292

Impact behaviour of composite materials and structures

9.10 High speed photographs of debris plume from hypervelocity impact on graphite/PEEK cylinder.

primary (a) and secondary (b) damage cone angles for normal and oblique impacts, respectively. In the latter case, the debris cloud exiting from the rear face of the laminates does not follow the line of flight of the projectile. Thus, a ‘turning’ angle (e) was defined as the angle between the initial

IBF9 11/22/2000 6:58 PM Page 293

High-velocity impact damage to polymer matrix composites

293

NASA JSC HIT-F shot #B934 Target: SSRMS boom #6 (Nextel AF-62 cable wrap) Projectile diameter: 9.13 mm Velocity: 6.55 km/s Impact angle: 0°

9.11 Photograph of crater, front face spallation and debris plume damage to rear wall due to hypervelocity impact on graphite/PEEK cylinder.

projectile velocity vector and the centre of mass of the primary damage zone (see Fig. 9.15). Furthermore, it was also observed that the primary and secondary cone angles for the oblique tests were not symmetric about the projectile flight line, thus accounting for the introduction of angles g and d in Fig. 9.15. Based on these experiments, a plot of the cone angles a and b are presented in Fig. 9.16 as a function of projectile impact angle. In addition, the cylinder secondary cone angle results are included for the normal impact case (~69.5°). In those experiments, one could not identify primary from secondary impacts. However, using the flat plate results from Fig. 9.12 for

IBF9 11/22/2000 6:58 PM Page 294

294

Impact behaviour of composite materials and structures

9.12 Plot of semi-cone angle of debris plume as a function of impact energy parameter.

87 distinct craters catalogued

Semi-cone angle = 11.6°

rinfluence ª 60 mm

9.13 Plot of secondary debris impact sites on flat plate.

IBF9 11/22/2000 6:58 PM Page 295

High-velocity impact damage to polymer matrix composites

295

Witness plate b a Primary damage cone Secondary damage cone

Guide rods

Target plate

Initial projectile vector

9.14 Schematic defining primary and secondary cone angles for debris plume (normal impact).

primary normal impacts (i.e. only those full penetration cases were plotted), an average primary cone angle of ~23.2° was also plotted. Thus, within the scatter indicated, all normal impact tests correlate reasonably well. Note that for the oblique tests on the 16-ply laminates using a 1 mm projectile, no evidence of primary impact debris was found. Figure 9.17 illustrates the variation of cone angles with the energy parameter using the normal projectile velocity component. Figure 9.18 presents a plot of the turning angle (e) as a function of the impact angle. For the limited data available, it appears that e is independent of ply thickness. This ‘turning’ effect, although small in magnitude, may well be important in predicting major impact damage relative to the location of critical spacecraft components and determining what protective measures it is necessary to implement.

9.5

Conclusions

This chapter presents an overview of high-velocity impact damage to composite laminates, with specific reference to test data obtained by UTIAS researchers using gun facilities at various laboratories in the USA and UK. Emphasis is placed on graphite/carbon fibre-reinforced epoxy/PEEK laminates of varying thickness and ply orientations. Where possible, pub-

IBF9 11/22/2000 6:58 PM Page 296

Witness plate

e

Center of mass, primary damage

Secondary damage cone

d

Primary damage cone

b Target plate

a g

Guide rods Initial projectile vector

9.15 Schematic defining oblique angle impact geometry associated with debris plume damage.

90 80

Cone angle (∞)

70 60 50 a, 16 ply, 1 mm a, 16 ply, 2 mm a, 24 ply, 2 mm b, 16 ply, 1 mm b, 16 ply, 2 mm b, 24 ply, 2 mm a, plate b, cylinder

40 30 20 10

0

10

20

30

40

50

Impact angle, qi (deg.)

9.16 Plot of primary and secondary debris cone angles for normal and oblique impacts on graphite/PEEK laminates.

IBF9 11/22/2000 6:58 PM Page 297

High-velocity impact damage to polymer matrix composites

297

90 80 70

Cone angle (∞)

60

b = 59.92E ¢ -164.72E ¢ 2 +182.41E ¢3 - 90.03E ¢ 4 +16.49E ¢5

50 40 30 a = -87.74E ¢ + 189.07E ¢ 2 -129.45E ¢3 + 29.02E ¢4

20

a b

10 0 2.2

3.2

4.2

(E ¢t

Dp )

(1/3 )

5.2

6.2

1/3

(J )

9.17 Plot of primary and secondary debris cone angles as a function of impact energy parameter.

14 16 ply 24 ply

12

Turning angle, e (∞)

10 8 e = 0.01e ( 0.16q ) i

6 4 2 0 0

10

20

30

40

50

Impact angle, qi (deg.)

9.18 Plot of primary turning angle as a function of impact angle.

IBF9 11/22/2000 6:58 PM Page 298

298

Impact behaviour of composite materials and structures

lished data from other researchers are included, although no results are presented on composite/sandwich construction. A variety of projectile materials are noted in the studies, but the bulk of the test data presented is based on aluminum spheres covering a wide range of impact energies. Most of the test results are derived from normal impact experiments, with a limited number of oblique tests also included. Despite the data base available from these studies, no predictive models are proposed. However, a number of observations can be made which might prove useful in the design of composite structures subject to hypervelocity impacts. First, a linear correlation of crater size and entry damage with an energy parameter has been established, which appears to be independent of laminate lay-up and valid for graphite/epoxy/PEEK materials. The damage resulting from secondary debris clouds has been amply demonstrated when the ejecta impact another laminate structure. Primary and secondary cone angles describing this debris plume have been identified for both normal and oblique angle impacts. Knowledge of the cone angles is essential in predicting the size of the plume impact area on adjacent structures. It has been shown that the energy of the debris particles can be sufficiently high as to result in major structural damage. Future research is necessary to enhance the data base, particularly for oblique impacts, and to develop predictive models capable of analysing the damage resulting from hypervelocity impacts on composite structures.

Acknowledgements The authors wish to acknowledge the significant contributions to the research referenced in this work by Mr G Shortliffe, Mr G Manuelpillai and Dr E A Taylor. It would have been impossible to undertake these studies without the collaboration of Dr J Crews, Dr E Christiansen, Mr J Kerr of the NASA Johnson Space Center, USA; Dr A Nolan of the NASA Marshall Space Flight Center, USA; and Dr J A M Mcdonnell of the University of Kent at Canterbury, UK.

References 1 Christoforou A P and Swanson S R, ‘Strength loss in composite cylinders under impact’, Trans ASME, 1988 110(2) 180–4. 2 Poe C C and Illg W, ‘Strength of a thick graphite/epoxy rocket motor case after impact by a blunt object’, 1987, NASA TM 89099. 3 Tennyson R C and Krishna Kumar S, ‘Delamination damage and its effect on buckling of laminated cylindrical shells’, AGARD Conf. Proc 530, Debonding/Delamination of Composites, 1989. 4 Tennyson R C and Shortliffe G, ‘MOD impact damage on composite materials in space’, Proc 7th Inter Symp, SP-399, Materials in Space Environment, 1997.

IBF9 11/22/2000 6:58 PM Page 299

High-velocity impact damage to polymer matrix composites

299

5 Yew C H, Yang C Y and Crews J, ‘A phenomenological study of the effect of hypervelocity impacts on graphite/epoxy plates’, Engineering Mechanics, University of Texas at Austin, and NASA JSC, 1986. 6 Yew C H and Kendrick R B, ‘A study of damage in composite panels produced by hypervelocity impact’, Int J Impact Eng, 1987. 7 Schonberg W P, ‘Hypervelocity impact response of spaced composite material structures’, Int J Impact Eng, 1990. 8 Tennyson R C, Manuelpillai G and Zimcik D G, ‘Model for predicting micrometeoroid/debris impacts and damage to composite materials’, 1st Eur Conf Orbital Debris SD-01, 1993. 9 Tennyson R C and Manuelpillai G, ‘Prediction of space hypervelocity impact damage in composite materials’, 8th CASI Conf Astronautics, 1994. 10 Silvestrov V V, Plastinin A V and Gorshkov N N, ‘Hypervelocity impact on laminate composite panels’, Int J Impact Eng, 1995. 11 Tennyson R C and Shortliffe G, ‘Hypervelocity impact damage to composite structures’, 1st Int Conf Composite Science and Technology, 1996. 12 Lamontagne C G, Manuelpillai G N, Taylor E A and Tennyson R C, ‘Normal and oblique hypervelocity impacts on carbon fibre/PEEK composites’, Proc Hypervelocity Impact Symp, 1998, Int J Impact Eng, 1999. 13 Christiansen E L, ‘Investigation of hypervelocity impact damage to space station truss tubes’, Int J Impact Eng, 1990. 14 Unda J, Weisz J, Uriarte A and Capitano R S, ‘Residual strength of CFRP tubes subjected to hypervelocity debris impact’, 45th Congr of the IAF, 1994. 15 Yasaka T, Meguro A and Watanabe M, ‘Debris impact damage and fragmentation of antenna structure in geostationary orbit’, 45th Congr of the IAF, 1994. 16 Shortliffe G D and Tennyson R C, ‘Hypervelocity impact tests on composite boom structures for space robot applications’, J Can Aeronauti Space Inst, 1997. 17 Taylor E A, Herbert M K, Gardner D J, Thomson R and Burchell M J, ‘Hypervelocity impact on spacecraft carbon fibre-reinforced plastic/aluminum honeycomb’, Proc Inst Mech Eng, 1997 211. 18 Taylor E A, Herbert M K and Kay L, ‘Hypervelocity impact on carbon fibrereinforced plastic/aluminum honeycomb at normal and oblique angles’, Proc 2nd Eur Space Debris Conf, ESA SD-02, 1997. 19 Frost C L and Rodriguez P I, ‘AXAF hypervelocity impact test results’, Proc 2nd Eur Space Debris Conf, ESA SD-02, 1997. 20 Taylor E A, Herbert M K, Vaughan A M and Mcdonnell J A M, ‘Hypervelocity Impact on carbon fibre-reinforced plastic/aluminum honeycomb: comparison with Whipple bumper shields’, Proc Hypervelocity Impact Symp, 1998. 21 Robinson J H, ‘Orbital debris impact damage to reusable launch vehicles’, Proc Hypervelocity Impact Symp, 1998.

IBF9 11/22/2000 6:58 PM Page 300

IBFINDEX 11/22/2000 7:03 PM Page 301

Index

accelerometer, 244 acoustic techniques backscattering, 51 emission, 60 microscopy, 52 adhesive bonding, 92–3 aerospace application, 280 ballistic, 266, 280 ballistic limit, 232, 255 barely visible impact damage, see damage beam, 9, 91 beam theory, 20 boundary conditions clamped, 123, 139, 194, 224, 242 simply supported, 189 brittle behaviour, 12, 17 buckling, 160–2 C-scan graph, 14, 150 carbon/epoxy, 17, 33, 86, 123, 197, 285 carbon/PEEK, 123 Charpy impact test, 9 classical plate theory, 189, 221 compression after impact (CAI) strength, see residual compressive strength compression after impact test, 123, 141 contact stiffness, 187–8 crater diameter, 287 critical strain energy release rate, 3–4, 102, 126, 159 cross-sectional micrograph, 36, 59, 281–3 crush strength, 26 damage, 6–8, 114 curing effects, 56–8 detection, 33, 140 indentation, 140, 231, 251 lay-up effects, 54 map, 37, 122, 151 measures, 169 mechanisms, 7, 148, 228–32, 246–63, 280–4

mechanics, 116 modelling, 99, 116 prediction, 114–23 source, 109 tolerance, 107, 160 tolerance assessment, 163, 172 damage tolerant structural design, 111 de-bonding, 7, 110, 255, 280 debris, 289 deflection-time curve, 97, 118, 199 delamination, 7, 33, 91–5, 148, 228, 258, 280–5 depth, 54 extent, 35–6, 54 propagation, 57, 151–9, 230 shape, 35, 150 de-ply technique, 34, 41 destructive techniques, 34, 140 drop weight impact test, 94, 123, 138, 186, 252 ductility index, 13 durability, 108 dynamic enhancement factor, 260 dynamic fracture, 1, 75 energy absorption, 13, 157, 220, 263 balance, 21, 157, 263 Charpy impact, 3 fracture, 21–2 perforation, 100, 246–66 entry diameter, see crater diameter failure criterion, 101 indentation, see damage modes, 6–7, 162 falling dart, see drop weight impact test fibre optics, 66 finite element modelling, 100, 117 foam core, 242 force-time curve, 96, 121, 144, 225–9

301

IBFINDEX 11/22/2000 7:03 PM Page 302

302

Index

fracture energy, see energy fracture mechanics, 22, 102 fracture toughness, 24 gas gun, 215, 245, 285 glass/epoxy, 17, 86 glass/phenolic, 133 glass/polyester, 133, 242 glass transition temperature, 2, 7 graphite/epoxy, 214, 285 graphite/PEEK, 285 Hertz contact law, 188, 224 high velocity impact, 212, 239 hybrid laminates, 87 hypervelocity impact, 285 impact damage, see damage damage resistance, 143 energy, see kinetic energy force ratio, 176–81 mass effects, 152 parameters, 134, 286 pre-stressed materials, 16 response, 91, 94, 143, 221 stress analysis, 91, 186 strength, 9 velocity effects, 153–4, 233, 254 impactor ball, 197 conical, 242–6 flat-ended, 139, 242–6 hemispherical, 242–6 wedge-ended, 95 incident kinetic energy, see kinetic energy indentation plates, 137 sandwich panels, 246 indentor conical, 251 flat-ended, 138, 246 hemispherical, 250 inertia effect, 152, 263 infrared thermography, 64 in-plane tests compression, 77 shear, 80 tension, 79 interface effect, 91 Izod impact test, 9

low velocity impact, 94, 123, 138, 186, 252 mass effects, see impact mass effects mechanical properties Aramid/epoxy, 4 carbon/epoxy, 4, 86, 197 carbon/glass hybrid, 86 E-glass/epoxy, 4, 86 E-glass/polyester, 137, 243 fibres, 2–3 foam core, 243 resins, 2–3 S-glass/phenolic, 137 membrane effect, 157 micromechanics, 19, 21 military application, 133 missile impact, 239 model development, 125, 263 nondestructive techniques, 33, 140, 214 nose shape, see impactor, indentor and projectile notch sensitivity, 10–12 oblique angle impact tests, 291 offshore application, 239 panel failure modes, 162 penetration process, 251 perforation, 232, 254, 283 plates circular, 137 diameter effect, 156 rectangular, 214 square, 197, 242 prediction of impact energy, 19 projectile characteristics, 96, 290 conical, 245 flat-ended, 245 gelatine pellet, 14 hemispherical, 215, 245 sphere, 14, 287 punch, see indentor quasi-static approximation, 204–7 tests, see indentation

Kevlar/epoxy, 285 kinetic energy, 21, 97, 287 kink shear band, 164–7

residual compressive properties, 113–14 stiffness, 175 strength, 16, 57, 115, 126, 170 residual impact velocity, 269

laser holography, 61 laser Doppler anemometry, 214–15 loading rate effect, see impact velocity effects

sandwich panels, 239 scaling, 99–100, 209 sensitivity of inspection techniques for impact damage, 68

IBFINDEX 11/22/2000 7:03 PM Page 303

Index shear out, 145–50 shearography, 63 skins, 242 spalling, 230, 290 split Hopkinson bar, 76–8 spring mass model, 204 stiffness retention factor, 127, 175 strain-gauged load cell, 95, 140 strain-time response, 146, 193–209 strain rate effects, 82 strain retention factor, 173–4 strength retention factor, 58, 165 stress-strain curve, 83–8, 244–5 striker, see impactor and projectile tap test, 38 terminal velocity, 233 thickness effects, 155, 253–7 threshold absorbed energy, 159 impact force, 156, 158, 171

impact velocity, 230 kinetic energy, 57, 145, 152–4 stiffness, 175 through-thickness tests compression, 81 interlaminar shear, 181 tension, 81 tube, 197, 287 tup, see impactor ultrasonic, 47 A-scan, 49 B-scan, 49 C-scan, 49, 140 wave propagation, 47, 77, 186, 266 weave pattern, 83–4, 135 woven fabrics, 82–3, 135 X-radiography, 39, 45

303

Impact behaviour of fibre-reinforced composite materials and structures

IBFPR 11/22/2000 4:04 PM Page ii

IBFPR 11/22/2000 4:04 PM Page iii

Impact behaviour of fibre-reinforced composite materials and structures Edited by S R Reid and G Zhou

Cambridge England

IBFPR 11/22/2000 4:04 PM Page iv

Published by Woodhead Publishing Limited, Abington Hall, Abington, Cambridge CB1 6AH, England www.woodhead-publishing.com Published in North and South America by CRC Press LLC, 2000 Corporate Blvd, NW Boca Raton FL 33431, USA First published 2000, Woodhead Publishing Ltd and CRC Press LLC © 2000, Woodhead Publishing Ltd The authors have asserted their moral rights. This book contains information obtained from authentic and highly regarded sources. Reprinted material is quoted with permission, and sources are indicated. Reasonable efforts have been made to publish reliable data and information, but the authors and the publishers cannot assume responsibility for the validity of all materials. Neither the authors nor the publishers, nor anyone else associated with this publication, shall be liable for any loss, damage or liability directly or indirectly caused or alleged to be caused by this book. Neither this book nor any part may be reproduced or transmitted in any form or by any means, electronic or mechanical, including photocopying, microfilming and recording, or by any information storage or retrieval system, without permission in writing from the publishers. The consent of Woodhead Publishing and CRC Press does not extend to copying for general distribution, for promotion, for creating new works, or for resale. Specific permission must be obtained in writing from Woodhead Publishing or CRC Press for such copying. Trademark notice: Product or corporate names may be trademarks or registered trademarks, and are used only for identification and explanation, without intent to infringe. British Library Cataloguing in Publication Data A catalogue record for this book is available from the British Library. Library of Congress Cataloging in Publication Data A catalog record for this book is available from the Library of Congress. Woodhead Publishing ISBN 1 85573 423 0 CRC Press ISBN 0-8493-0847-X CRC Press order number: WP0847 Cover design by The ColourStudio Typeset by Best-set Typesetter Ltd., Hong Kong Printed by TJ International, Cornwall, England

IBFPR 11/22/2000 4:04 PM Page v

Contents

1

Preface

ix

List of contributors

xii

An overview of the impact behaviour of fibrereinforced composites n l hancox

1

1.1 1.2 1.3 1.4 1.5 1.6 1.7 1.8 1.9

Introduction Composite materials Failure processes Measurement of impact strength Theoretical prediction of impact energy The effect of the matrix on fracture toughness Crush strength Summary Final reflection Acknowledgements References

1 2 6 9 19 24 26 27 28 29 29

2

Recent developments in impact damage assessment of fibre composites j-k kim

33

Introduction Destructive techniques Nondestructive techniques Concluding remarks Acknowledgements References

33 34 37 67 69 69

2.1 2.2 2.3 2.4

v

IBFPR 11/22/2000 4:04 PM Page vi

vi

Contents

3

Modelling impact of composite structures using small specimens c ruiz and j harding

75

3.1 3.2 3.3 3.4 3.5

Introduction Small specimen testing Structural analysis of impact Modelling of impact damage Conclusions References

75 76 91 99 102 103

4

Impact damage – tolerant composite structural design r l sierakowski

106

4.1 4.2 4.3 4.4 4.5 4.6 4.7

Introduction Damage tolerance Sources of damage Damage tolerant design Impact damage Impact damage tests Summary References

106 107 109 111 114 123 126 128

5

Damage resistance and tolerance of thick laminated woven roving GFRP plates subjected to low-velocity impact g zhou and l j greaves

133

5.1 5.2 5.3 5.4 5.5 5.6

Introduction Characterisation of composite materials Experimental procedures Impact damage resistance Impact damage tolerance and assessment Conclusions Acknowledgements References

133 135 136 143 160 180 183 183

6

Elastic impact stress analysis of composite plates and cylinders s r swanson

186

Introduction Impact regimes Analysis of impact

186 186 187

6.1 6.2 6.3

IBFPR 11/22/2000 4:04 PM Page vii

Contents

vii

6.4 6.5 6.6

The quasi-static approximation Issues of scaling in impact Summary and conclusions References

204 209 210 210

7

Impact behaviour and analysis of CFRP laminated plates e wu and c z tsai

212

7.1 7.2 7.3 7.4 7.5 7.6 7.7

Introduction Experimental set-up and procedure Near-elastic impact behaviour Prediction of elastic impact response Impact beyond the delamination threshold Impact beyond the ballistic limit Conclusions Acknowledgements References

212 214 217 221 228 232 233 236 236

8

Perforation of FRP laminates and sandwich panels subjected to missile impact s r reid and h m wen

239

8.1 8.2 8.3 8.4 8.5 8.6

Introduction Experimental procedure Experimental results Model development Comparisons and discussion Conclusions References

239 242 246 263 267 277 278

9

High-velocity impact damage to polymer matrix composites r c tennyson and c g lamontagne

280

Introduction Hypervelocity impact tests on composites Entry impact damage Secondary debris cloud Conclusions Acknowledgements References

280 285 286 289 295 298 298

Index

301

9.1 9.2 9.3 9.4 9.5

IBFPR 11/22/2000 4:04 PM Page viii

IBFPR 11/22/2000 4:04 PM Page ix

Preface

The last three decades have witnessed a steady increase in the use of lightweight polymeric composites for structural applications. In addition to their excellent quasi-static mechanical properties such as high specific stiffness and strength, it has become essential for these composite structures to perform well under various types of impact loading. For example, in the aerospace industry, the residual compressive strength of an impactdamaged composite structure has become the design-limiting factor. Major aspects of current damage-tolerant design philosophies in other industrial sectors are similar to that of the aerospace industry. Consequently, this book brings together nine chapters that deal with the various aspects of impact behaviour of fibre-reinforced composite materials and structures. Contributions are provided by some of the world’s leading experts in the field. It is hoped that the detailed presentation of a wide range of topics within a single volume will form a sound basis for further studies of impact behaviour and also serve as a useful reference source. The book has a broad scope and covers both experimental and analytical approaches to understanding the impact response of fibre-reinforced composites, and the effects of impact damage and failure under conditions ranging from low velocity to hypervelocity impact. It is intended to be useful not only to practising engineers, academics, researchers and designers in the field, but also to materials scientists, postgraduate research students, and manufacturers of composite materials and structures. Numerous references are given at the end of each chapter to enable the reader to explore the topics covered in greater detail. Impact problems concerning composite structures involve diverse disciplines, and require the combined skills of engineers, materials scientists and mathematicians. Thus, a degree of overlap between the sections of some chapters is unavoidable. Since the book focuses exclusively on the impact behaviour of continuous fibrereinforced composite materials and structures, the general subject of composite materials is not covered in depth. Also, short fibre-reinforced composite materials and structures are not considered. ix

IBFPR 11/22/2000 4:04 PM Page x

x

Preface

Chapter 1 presents an overview of impact performance of various notched composite beams, assessed by Charpy and Izod impact methods. Details of various experimental approaches are explained, and the ability of the composites to absorb impact energy is discussed together with the associated failure processes. The analytical predictions of the impact energy absorbed based on these methods is presented. Chapter 2 contains a summary of the various destructive and non-destructive techniques for detecting as well as quantitatively characterising impact damage. Particular emphasis is placed on the emerging variants of some well-established techniques such as X-radiography and ultrasonics where the three-dimensional distribution of damage is demonstrated. Some examples, illustrating the capacity as well as the effectiveness of certain selected techniques, are presented. Chapter 3 provides an in-depth examination of some of the experimental techniques that have been used to characterise several composites under various uniaxial states of stresses at high strain rates. It also deals with the low velocity impact responses of beam structures. Additionally, numerical modelling of impact damage is discussed, and some of the issues regarding both stress-based and fracture mechanics-based failure criteria are examined, along with the issue of scaling. Chapter 4 serves as an introduction to impact-damage tolerant composite structural design. The concepts as well as the key issues in damage tolerant design are examined. The sources and effects of damage are described. It also discusses damage tolerant design criteria. The development of analytical and FEM-based models for characterising both the impact event and damage tolerance, respectively, is presented. Chapter 5 is a comprehensive treatise on both impact damage resistance and damage tolerance assessment of thick glass fibre-reinforced laminates subjected to low velocity and high energy impact. In this chapter, impact response and dominant damage mechanisms occurring during impact are discussed from an experimental perspective and their energy-absorbing characteristics are described. Details of compression after impact tests are also presented. Considerable discussion is devoted to the advantages and disadvantages of both conventional and newly proposed damage tolerance assessment methods, which are illustrated with numerical examples. In Chapter 6, the elastic impact stress analyses of flat plates and cylinders, both made of carbon/epoxy, are provided. Comparisons are made between an analytical model and experimental data for low velocity impact response and this is supplemented with numerical examples. The justification for the quasi-static approximation of low-velocity impact responses is presented with examples. Geometric scaling issues are discussed. Chapter 7 examines the impact responses of and associated damage in graphite/epoxy plates under impact velocities ranging from very low to above the ballistic limit. Two major aspects are covered. One is concerned with obtaining experi-

IBFPR 11/22/2000 4:04 PM Page xi

Preface

xi

mentally the plate impact response histories generated by using a gas gun. The other is concerned with predicting analytically the plate impact responses under imperfect boundary conditions by using Mindlin plate theory. The correlation between the two is discussed with numerical examples. Chapter 8 presents a detailed study on the penetration and perforation of glass/polyester laminates and glass/polyester skinned sandwich panels with foam cores under impact velocities ranging from low to above the ballistic limit. The development of two semi-empirical models is discussed, and the nose-shape effects of both indentors and projectiles are examined. One model predicts penetration and perforation energies by using a dynamic enhancement factor. The other model is developed for high velocity impacts where inertia effects dominate. The correlation between the two is discussed with numerical examples. Extensive discussion of and comparisons with experimental data are provided. Chapter 9 deals with the damage analysis of both flat plates of varying thickness and cylinders, made of graphite/epoxy, graphite/PEEK and Kevlar/epoxy, under normal as well as oblique hypervelocity impacts. The damage caused by both the direct impact of projectiles and secondary debris clouds from perforated laminates is examined in detail. Considerable discussion is devoted to the correlation between impact energy and damage crater size. We wish to express our gratitude to all the contributing authors for their efforts and outstanding cooperation, and to Mrs Patricia Morrison of Woodhead Publishing Limited for her enthusiasm and patience throughout this project. Finally, we would like to thank our wives, Susan and Juan for their support and patience. SR Reid and G Zhou

IBFPR 11/22/2000 4:04 PM Page xii

List of contributors

Greaves L G Mechanical Sciences Sector, DERA, Famborough, Hants GU14 0LX, UK Hancox N L AEA Technology, Harwell, Oxfordshire OX1 0RA, UK Harding J Department of Engineering Sciences, University of Oxford, Oxford OX1 3PJ, UK Kim J-K Department of Mechanical Engineering, Hong Kong University of Science and Technology, Clear Water Bay, Kowloon, Hong Kong Lamontagne C G Institute of Aerospace Studies, University of Toronto, Ontario M3H 5T6, Canada Reid S R Department of Mechanical Engineering, UMIST, Manchester M60 1QD, UK Ruiz C Department of Engineering Sciences, University of Oxford, Oxford OX1 3PJ, UK Sierakowski R L Department of Civil Engineering, Ohio State University, Columbus, OH 43210, USA xii

IBFPR 11/22/2000 4:04 PM Page xiii

List of contributors

xiii

Swanson S R Department of Mechanical and Industrial Engineering, University of Utah, Salt Lake City, UT 84112, USA Tennyson R C Institute of Aerospace Studies, University of Toronto, Ontario M3H 5T6, Canada Tsai C Z Institute of Applied Mechanics, National Taiwan University, Taipei 106, Taiwan Wen H M Department of Mechanical Engineering, UMIST, Manchester M60 1QD, UK Wu E Institute of Applied Mechanics, National Taiwan University, Taipei 106, Taiwan Zhou G Department of Aeronautical and Automotive Engineering, Loughborough University, Leicestershire LE11 3TU, UK

IBFPR 11/22/2000 4:04 PM Page xiv

IBF1 11/22/2000 4:13 PM Page 1

1 An overview of the impact behaviour of fibre-reinforced composites N L HANCOX

1.1

Introduction

Impact may be defined as the relatively sudden application of an impulsive force, to a limited volume of material or part of a structure. The proviso is that relatively and limited are capable of an extraordinarily wide range of interpretations. The effects of impact are widely known and yet analysing the phenomenon and relating effects to the forces acting and the materials’ properties, in order to predict the outcome of a particular event, can be very difficult. The results of an impact can be largely elastic, with some energy dissipated as heat, sound, internally in the material, etc. Alternatively there may be deformation, permanent damage, complete penetration of the body struck or fragmentation of the impacting or impacted body, or both, as demonstrated in Chapters 5, 7, 8 and 9. For fibre composite materials it is permanent damage, possibly subsurface and barely visible, penetration and fragmentation, that are of interest. There are various ways of analysing the impact process; in terms of the energy deposited and gross damage produced, micro energy dissipation or by considering the stresses acting on flaws in the material and the effects that are generated. The latter method, which is known as fracture mechanics, is extensively employed with metals but will only be alluded to here. In practice the impact behaviour of composites merges into the general area of damage mechanics. Much of the early pioneering work on the properties of composites under impact is still relevant as the concepts employed in the analysis are the same though the results, depending specifically on the materials used (fibre, resin), interface and method of fabrication, may have been superseded. For this reason many of the earlier references concerning the impact behaviour of composite materials are employed here. This is not a detailed historical treatment and references are chosen for their appropriate nature rather than for being first (or last!) in the field. In this chapter it is intended to view impact in a general way. Later 1

IBF1 11/22/2000 4:13 PM Page 2

2

Impact behaviour of composite materials and structures

contributions will focus on specific situations in which the material and/or impact process is more closely defined. The general principles set out in Chapter 1 should, however, be applicable in all situations.

1.2

Composite materials

To discuss the impact behaviour of composites it is helpful initially to consider the nature of the materials. Modern polymer composites based on glass, carbon, aramid, ceramic or polymer fibres in a polymer matrix are heterogeneous and anisotropic materials. They have a low density, high strength and stiffness and hence excellent specific properties (the ratio of the property to the density or specific gravity) in the fibre direction. They can be relatively easily formed into components with complex shapes by vacuum pressure compaction or pressing at temperatures of no more than ~200°C for 1 h or more, though post curing may be needed. Because of the need to have long fibres for optimum properties and, in many cases, easier and effective processing, composite structures are often shells. They have excellent properties within the plane of the shell, in the fibre direction in tension, and to a lesser extent, in compression. The performance transversely, through the thickness and in shear and impact, is poorer. Generally, properties which are matrix dependent are much lower than those which are governed by the fibre. Nevertheless the role of the matrix is vital in composite behaviour; protecting the fibre, transferring stresses and, in some cases, alleviating brittle failure by providing alternative paths for crack growth.

1.2.1 Properties of fibres and resins Reinforcing fibres usually have a diameter of 5–10 mm, though it may be up to ~100 mm, for certain types (e.g. boron), and a modulus and strength of the order of 70–800 GPa and 1000–7000 MPa, respectively. The failure strain is ~0.27–5.0%. Carbon and aramid fibres may exhibit an increasing modulus with increasing strain due to changes in their internal structure during stressing. The resins, whether thermosets or thermoplastics, have a modulus and strength of the order of 2–5 GPa and 50–100 MPa, respectively, and a strain to failure of ~1% upwards. It should be noted that resin failure strain is usually well in excess of the minimum figure. Properties of resins are usually strain rate dependent and markedly influenced by temperature (see a fuller treatment in Chapter 3). This occurs because the glass transition temperature, Tg, which is indicative of the upper working temperature, is ~80–200°C for most resins. This is much closer to room temperature than is the case for the melting or degradation point of most structural

IBF1 11/22/2000 4:13 PM Page 3

Impact behaviour of fibre-reinforced composites

3

Table 1.1. Some fibre and resin properties Material

Density (Mgm-3)

Tensile modulus (GPa)

Tensile strength (MPa)

Strain to failure (%)

Glass fibre Carbon fibre Aramid fibre Inorganic fibre Phenolic resin Polyester resin Epoxy resin Bismaleimide resin

2.49–2.55 1.7–2.0 1.39–1.45 2.0–3.97 1.0–1.35 1.1–1.23 1.2–1.2 1.2–1.32

73–86 160–827 73–160 152–462 3.0–4.0 3.1–4.6 2.6–3.8 3.2–5.0

3400–4500 1400–7070 2400–3400 1720–3900 60–80 50–75 60–85 48–110

3.5–5.4 0.27–1.9 1.4–4.6 ~1.8 1.0–6.5 1.5–8.0 1.5–3.3

materials. Hence creep can be a problem with polymers at relatively low temperatures. Some fibre and resin properties are summarised in Table 1.1. It should be noted that these are indicative of the property range for the materials. Individual grades/types of material, the way the property is measured, etc., might cause variations outside the limits given.

1.2.2 Composite properties Table 1.2 lists some composite properties. These are again indicative of the performance of 60 v/o (fibre volume fraction), unidirectional fibre composites. Values will vary with the type of fibre (e.g. grade of carbon fibre), method of test, matrix and way the specimens were fabricated. The important points to appreciate are the very significant differences between longitudinal and transverse properties, the lesser difference between longitudinal tensile and compressive strengths and the disparity between the interlaminar shear strength (ILSS) and tensile/compressive strengths. Shear modulus is in the range 2.5–5.0 GPa for all of the materials. Longitudinal tensile and compressive strain to failure is essentially that of the fibre.Transversely the figure may be lower, ~0.3–0.5%, and is governed by the properties of the interface and resin matrix. Laminates, containing layers of fibres with different orientations within a plane, may have higher impact, shear and transverse properties, but lower longitudinal performance. Charpy impact energy for unnotched materials, stressed in the longitudinal or fibre direction, varies widely depending on the interface, matrix and experimental details. There may also be errors due to the scaling up of results for different cross section specimens. Charpy impact strength in the transverse direction (i.e. at right angles to the fibre) can be very low. It is common to use Gc, the critical strain energy release rate, as a measure

1.8–2.0 1.54–1.66 1.36–1.4

Glass Carbon Aramid

37–53 125–330 66–107

Elt (GPa) 9.0–13.6 5.9–10 4.1

Ett (GPa) 1.2–1.9 1.76–2.9 1.29–1.5

slt (GPa) 30–80 27

stt (MPa) 0.78–1.6 0.19–0.28

slc (GPa) 53–83 70–127 38–69

t (MPa) 125–3300 60–3300 1100

G1c (J m-2) 600–1200 154–2033

G2c (J m-2)

Up to 609 8–150 20–40

Imp st. l, (k Jm-2)

Up to 28 0.2–4.0

Imp st. t, (k Jm-2)

Where r is the density, Elt and Ett are the longitudinal tensile and transverse tensile moduli, respectively, slt, stt and slc are the longitudinal tensile, transverse tensile and longitudinal compressive strengths, respectively, t is the shear strength (also known as the interlaminar shear strength or ILSS), G1c and G2c are the critical works of fracture for the 1 and 2 deformation modes and Imp st. l, and Imp st. t, are the longitudinal and transverse Charpy impact strengths.

r (Mg m-3)

Material

4

Table 1.2. Some properties of unidirectional composite materials

IBF1 11/22/2000 4:13 PM Page 4

Impact behaviour of composite materials and structures

IBF1 11/22/2000 4:13 PM Page 5

Impact behaviour of fibre-reinforced composites

5

1.1 G1c. Crack propagation parallel to the fibres. The horizontal lines show the fibre direction.

of toughness, though some workers distinguish between initiation and propagation energies for this quantity. Often Gc is equated to 2g, where g is the work of fracture or the energy required to produce a new surface in a material. It is important to remember that both g and Gc refer to a specific mode of deformation (a tensile type opening for G1c) and that the direction of the fibres in relation to the sense of deformation must be clearly defined, see Fig. 1.1. In Table 1.2, G1c refers to the extension of a crack parallel to the fibre direction and is thus analogous to the transverse Charpy impact energy. G1c defined in this way is also known as the mode 1 interlaminar shear work of fracture. More information on fibre, resin and composite properties is available, for instance, as is a simple description of the various deformation modes associated with G1c, G2c and G3c.1 A general account of composites fracture mechanics and toughening mechanisms is given in Hancox and Mayer.2 More details and descriptions of the experimental difficulties of determining the critical strain energy release rates and the influence of materials’ and testing parameters on the results have been recorded.3 For metals, figures of 4–140 kJm-2 have been reported for the work of fracture, g.4 An advantage of composites, compared with more conventional materials, is the ability of the designer/fabricator to tailor mechanical and thermal properties over a wide range by suitable choice of fibre type, orientation, loading (within limits), and possibly the resin. It is possible to reduce in-plane anisotropy to give a quasi-isotropic material and improve shear and transverse (though not through-thickness) performance by laminating. However, the specific property in a given direction is reduced as

IBF1 11/22/2000 4:13 PM Page 6

6

Impact behaviour of composite materials and structures

more ‘redundant’ material has been added. Laminates, with successive layers orientated differently, are in some ways akin to plywood. Alternatively, a wide range of woven, knitted and needled fabrics, often based on glass or aramid fibres, is available for reinforcement. The first two types of fabric possess good reinforcement in more than one direction in a plane without the need for laminating. Disadvantages are that strength and stiffness properties are reduced because of out-of-plane deviations of the fibres due to the weaving process and lower fibre volume fraction, possibly fibre/fibre wear at cross over points and physical damage to the fibre occurring during needling. It has so far been implicit that long/continuous fibre tows are used in composite construction. Many products, especially those reinforced with glass fibre, employ short (sub-micron or mm), intermediate (cm) or randomly laid, continuous fibres in a plane, or combinations of these, for reinforcement. These materials, with thermoset or thermoplastic matrices and sometimes special additives to aid processing, are known as bulk or dough moulding compounds, injection moulding feedstock and stampable mat thermoplastics. Sheet moulding compound contains, in addition to chopped fibres, continuous or woven glass fabric. These types of composite are very widely used because of the relative ease with which they can be pressed, moulded or extruded into useful components. One difficulty arising in the discussion of the properties of composites relates, ironically, to one of the virtues of the materials – the ability of the user to tailor their properties to suit the design. There is a huge number of fibre lay-ups, fibre types, combinations and forms, resin matrices, additives and cure schedules to choose from and it can be very difficult to extrapolate from, or relate, the results for one unique combination to those of another. This has the effect of making quoted property measurements appear very diverse.

1.3

Failure processes

New situations and materials tend to be judged initially by comparison with existing ones. Since the principle class of construction materials used in high performance applications is metals, composites are usually compared with them. Generally, metals tend to be dense, stiff, strong, good conductors of heat and electricity, isotropic and inexpensive. In particular many show plastic behaviour before failure and it may be possible to remove the effects of deformation/damage by annealing and/or reworking the material. Unfortunately, at least on a significant scale, polymer matrix fibre composites do not exhibit this type of behaviour – elastic deformation is followed by irreversible damage and failure. Another important influence on composite

IBF1 11/22/2000 4:13 PM Page 7

Impact behaviour of fibre-reinforced composites

7

performance, especially in failure, is the heterogeneous nature of the material on a micro/meso scale. Composites are generally strong, and have a reasonable impact resistance, if the applied stress is in the fibre direction. In other directions they tend to be weak and to have a low impact resistance. Small secondary stresses in the transverse direction or unexpected stresses due to an impact, in a weak direction, can easily cause damage. Because of the ease with which localised permanent damage can be produced and the low values of g or G1c for failure parallel to the fibres, or between plies in a laminate, G1c is sometimes regarded as critical and the focus of most attention in impact work. Fracture mechanics methods of determining G1c are favoured over traditional measurements of impact strength, from which g and arguably G1c can be determined, because of their greater accuracy and virtual elimination of extraneous energy absorption. However, the assumptions implicit in fracture energy determinations may not be true for fibre composites, where crack propagation may be dominated by crack blunting, fibre pull-out and fibre/matrix delamination. It has been suggested that in such circumstances conventional fracture toughness may not necessarily be the best measure of overall toughness.5 Impact tests can be more useful, although not so readily analysed as fracture toughness measurements, and can be conducted at strain rates more representative of the deformation rates seen in service. The topic can be a contentious one of which the reader should be aware. There are five basic mechanical failure modes that can occur in a composite after initial elastic deformation. These are: • • • • •

Fibre failure, fracture, and, for aramids, defibrillation. Resin crazing, microcracking and gross fracture. Debonding between the fibre and matrix. Delamination of adjacent plies in a laminate. Fibre pull out from the matrix and stress relaxation.

In practice, debonding and delamination are not always distinguished. A very detailed list of types of damage in composites and associated references is given in Chapter 2. Behaviour is modified by external conditions. Polymeric fibres, which depend for their properties on molecular alignment, suffer a fall-off in performance above ~100°C, aramids degrade at elevated temperatures, carbon fibres, if unprotected from air, oxidise at 300–400°C and glass will soften at 500–800°C. The environment, particularly water, causes the plasticisation of thermosets, lowering the Tg and causing microcracking and debonding and possibly corrosive effects in stressed glass fibre composites. The interface, at which mechanical keying and chemical bonding are involved, is

IBF1 11/22/2000 4:13 PM Page 8

8

Impact behaviour of composite materials and structures

very sensitive to moisture. Sometimes the effects are reversible on drying out – sometimes they are not. All these factors are of relevance to impact performance because of their influence on composite mechanical properties.

1.3.1 Why are composites prone to impact damage? The lack of plastic deformation in composites means that once a certain stress level is exceeded permanent damage, resulting in local or structural weakening, occurs. Unlike a metal, which may undergo plastic deformation but can retain its integrity (e.g. water tightness), composites stressed above a certain level, though possibly retaining some structural properties, are permanently damaged. A blow with an energy of ~1 J or less at ~2 ms-1 can cause irreversible damage in a realistic composite laminate. To summarise, the reasons for a low impact strength are: • • •

Low transverse and interlaminar shear strength. Laminar construction, which is required if the reinforcing fibres are to be used efficiently and anisotropy reduced. No plastic deformation.

1.3.2 Estimation of the stresses acting in an impact It is informative to try to estimate the stress generated by an impact. The situation is very complex and our simple approach merely indicates the order of magnitude of the stress. Consider a steel ball of radius ~25 mm and mass 0.5 kg, with an energy of 1 J impacting a surface at a velocity, V, of 2 ms-1. The compression stress generated, sc, is, given by 0.5

s c = V (Ect r)

[1.1] 6

where Ect is the transverse compressive modulus and r the density. Typical values of these quantities are 10 GPa and 2 ¥ 103 kgm-3, respectively, giving sc = 9 MPa. In practice, compressive loading could cause localised bending and transverse failure in suitably oriented plies and generate interlaminar shear stresses. The compressive stress will continue to act until the impacting body rebounds. The stress wave will propagate into the impacted material, with a decreasing amplitude, and be reflected at the back surface as a tension wave. It is possible to apply the theory of Hertzian contact stresses6 to the estimation of the impact stress. This indicates that if the diameter of the contact area is 2 a the maximum shear stress appears below the point of contact at a depth of ~a/2. The maximum contact stress, q0, for indentation on a plane surface is

IBF1 11/22/2000 4:13 PM Page 9

Impact behaviour of fibre-reinforced composites q0 = 0.7aE R

9 [1.2]

This assumes a common Poisson’s ratio of 0.3 and that the controlling modulus is that of the composite through its thickness ~10 GPa. If a = 0.25 mm and R, the radius of the impactor, is 25 mm as before, the maximum compressive stress is found to be ~70 MPa and the maximum shear stress, ~0.31 q0, is 22 MPa. Both approaches neglect, among other points, the differences in the properties of the impacting and impacted bodies, geometrical effects and the heterogeneous, anisotropic nature of the composite. In addition, whether a static theory of contact stresses can be applied to an impact situation is open to debate. In view of all these factors the results are approximate but they do indicate the potential for damage.

1.4

Measurement of impact strength

1.4.1 Izod and Charpy methods The Izod and Charpy tests have been used for many years to assess the impact performance of metals particularly with respect to the brittle/ductile transition temperature and notch sensitivity.7,8 The Izod test is still widely used for polymers. In the Izod test a rectangular or square cross section bar of specified dimensions is clamped at one end and struck towards the top of the test piece with a pendulum. For the Charpy test a beam is rested freely against two anvils and struck in the centre by a pendulum. In the former case, if the specimen is notched, the notch is at the top of the clamped section and usually faces the direction of strike. Charpy specimens may be machined with U or V notches in the centre of the beam opposite the direction of strike, see Fig. 1.2. For metal specimens, dimensions are controlled as stated in the various national standards. In either test, and with any material, the impact energy may be overestimated because energy is: • •

Stored elastically in the specimen prior to failure. Energy is dissipated acoustically, thermally, in the kinetic energy of the failed parts, etc.

Despite the somewhat arbitrary nature of the tests, difficulties of crosscorrelating information and of scaling impact energies to bodies with different cross sections, they were readily adapted by the plastics industry and national standards established. The Izod impact testing of rigid plastics9 and the impact behaviour of plastics including the effects of flow direction in moulded specimens, notching, notch tip radius and notch depth and the relation of the impact energy to the stress concentration factor10 are both covered. Also dealt with very thoroughly are the Izod and Charpy impact

IBF1 11/22/2000 4:13 PM Page 10

10

Impact behaviour of composite materials and structures

Impact

Impact

1.2 Charpy test specimens with triangular and U-shaped notches. The arrow shows the direction of impact.

procedures for plastics.11 When carbon fibres were developed, and the potential of carbon fibre composites in aerospace was realised, these test methods, especially the Charpy, were adapted for composites, including glass and aramid fibre materials. If the striking arrangement in a Charpy test is such as to load the specimen in 4 rather than 3 point bending, see Fig. 1.3, the work of fracture is increased, presumably because of the different shear stress patterns in the two cases. Sometimes the Charpy test is viewed as an accelerated static test, but there is evidence that the energy stored to maximum load differs in the static and impact cases, with laminated specimens exhibiting a reduced modulus, and hence greater energy storage, in impact.12 A similar conclusion has been reached for sandwich panel specimens with composite skins. In this case quasi-static testing gave results 50–65% less than impact measurements.13 The physical cause is probably related to differences in the transverse shear behaviour at the different strain rates in the two cases. In parallel with the work on traditional impact tests the fracture mechanics approach was developed to describe composite fracture. This method is more complex theoretically and experimentally but arguably, for some materials, is more suitable for use in design.

IBF1 11/22/2000 4:13 PM Page 11

Impact behaviour of fibre-reinforced composites

11

Impact

Support

Impact

Support

1.3 Schematic diagram of Charpy specimens impacted in 3 and 4 point loading, respectively.

To some extent the effect of the notch is to reduce the sources of error due to stored energy. In this respect a chevron notch is often used in the Charpy test. This is formed by making two opposing cuts from the base of the specimen to the top, meeting at a point on the top surface. This leaves a triangular shaped cross section of material joining the two halves of the specimen, see Fig. 1.2. The argument is that if the specimen is struck at the back failure starts at the apex before significant energy storage due to bending occurs elsewhere in the specimen.Thus the recorded impact energy is more nearly the true value. Notches are also used to determine if the material is notch sensitive. If a scratch or surface flaw, acting as a stress raiser, severely reduces the impact strength of a component, because the stress concentration at the notch tip cannot be relieved, it is important to establish this prior to use. One method of expressing impact energy, for a plastic or a composite, is in terms of the formula U = E b(d - c )

[1.3]

where U is the impact energy, and E the energy registered in the test, for a specimen of breadth b, and depth d, containing a notch of depth c. This is a simple scaling formula. By adopting a fracture mechanics approach it can be shown2 that the fracture energy may be expressed thus: U = E fb( d - c)

[1.4]

IBF1 11/22/2000 4:14 PM Page 12

12

Impact behaviour of composite materials and structures Medium toughness

Force

Brittle

Ductile

Displacement

1.4 Idealised load displacement characteristics for brittle, medium toughness and ductile material. Note that the materials will differ in elastic properties – hence the different slopes. Real characteristics will be much less smooth.

where f is a calibration factor which depends on specimen and crack dimensions and compliance. In using either the Charpy or Izod test it is most important to specify the fibre direction in relation to the main stresses applied by the impact force. A trawl through the literature reveals that the Charpy test is much more widely used for composites than the Izod method. The variety of specimen shapes and notches is large – a typical specimen might be 6 ¥ 6 mm in cross section and 60 mm in length with a U, V or chevron notch, the former up to half the thickness of the specimen and for a V notch an angular opening of 30 or 45°. In another case the specimen was a laminate 2 mm thick, 13 mm wide, with a V notch on either side in the thickness. Pendulum strike velocities are typically ~2–4 ms-1 with energies, governed by the mass of the pendulum, of 0.4–15 J, and exceptionally up to 100 J. Some idealised load displacement traces, which could be obtained from machines with an instrumented striker head or tup, are shown in Fig. 1.4. Instrumenting the striker enables the force as a function of time into the impact, or displacement, to be obtained. The characteristics are for brittle, intermediate and tough materials, respectively. The difference in the areas under the curves in the three cases is obvious. Real traces tend to be a lot less clean because of ring in the system, possibly bouncing of the striker and repeated impact and complex material behaviour. A variety of impact tests using the DYNA3D FEA code were recently analysed and it was concluded that ringing or noise is due to local bending of plies around the tip of the impactor.14

IBF1 11/22/2000 4:14 PM Page 13

Impact behaviour of fibre-reinforced composites

13

By integrating the area under the load or force displacement curve, and noting the value up to the maximum load or the load at first failure, it is possible to deduce the energy required to start or initiate damage and relate it to the energy to propagate damage and the total energy involved, as indicated in Fig. 5.4 of Chapter 5 and Fig. 8.3 of Chapter 8. The ratio of the propagation energy, Ep, to the initiation energy, Ei, is known as the ductility index, D.15 D = E p Ei

[1.5]

Values range from zero upwards. The zero value indicates that, in this type of test, the material is behaving in a completely brittle manner. The larger D, the more energy is used in propagating failure compared with that to cause initiation. Note that a high index does not imply a material with high absolute toughness. What is required in practice is a large initiation energy and a large propagation energy. The reader should be aware that some authors define D as the ratio of propagation to total energy, Et. An analogous situation arises with G1c measurements where there is a relatively low initiation energy followed possibly by a higher propagation value. Some typical figures for G1c, for unidirectional sized and untreated glass fibre epoxy composites, are given by Krawczak and Pabiot.16 For crack initiation in the sized material the figure is 87 Jm-2 and 438 Jm-2 for propagation. For unsized fibre the figures are 224 and 185 Jm-2, respectively, indicating that in this case once a crack is initiated it propagates more easily.

1.4.2 Other methods of determining impact energy An increasingly popular method of assessing impact energy is the falling dart test,17 which was originally developed for rigid plastics. The standard covers both instrumented and uninstrumented testing procedures. The test piece, either 60 mm in diameter or 60 ¥ 60 mm square, and 1–4 mm thick, is supported on a hollow steel cylinder with an inside diameter of 40 mm. It may be clamped in position. The steel striker has a polished hemispherical head, either 10 or 20 mm in diameter, and is allowed to fall from a height of up to 2 m onto the specimen (equivalent to a maximum velocity of 6.3 ms-1). For a puncture test on a composite, a strike velocity of 4.4 ms-1 and a total striker mass of 5–20 kg (equivalent to energies of 48–193 J) are preferred. Many variants of the dropped weight test are described in the literature, with specimens ranging in size from 127 ¥ 127 mm square to 100 mm in diameter, and impactors with tip radii of 5–12.7 mm. Other variants are noted in Chapters 5 and 8. The impact velocity can be varied, within reason, to suit a particular requirement. Details of the impact testing of skinned sandwich panels, sometimes using specially shaped impactors, are

IBF1 11/22/2000 4:14 PM Page 14

14

Impact behaviour of composite materials and structures

1.5 C-scan of a laminated carbon fibre composite panel impacted at 50 ms-1 with a 6 mm diameter indenter. Note damage development along a diagonal.

given in Hildebrand.13 It was noted that pyramidal and hemispherical indenters gave different results and it was concluded that these different test methods are not even qualitatively comparable. Another way of assessing the impact energy in a Charpy, or falling weight, test is to repeatedly impact the same specimen, until failure occurs, under conditions which do not cause immediate failure, or to increase the impact energy on each successive blow until failure occurs. While this may be acceptable for ranking materials or designs, the build up of damage, which is not quantified before failure, makes the absolute interpretation of the results uncertain. To increase the impact velocity it is necessary to fire the projectile at the specimen. This may involve a conventional bullet, an anti-tank shell, a small ball ~1–40 g in weight fired by a gas gun, a soft projectile,18 or a liquid drop.19,20 See Chapters 7–9 for further details. The impact velocity can range from 20–100 ms-1 to 6000 ms-1 plus. Under certain conditions the projectile may penetrate the specimen cleanly or it may cause overall flexing, fibre break out at the back surface or considerable delamination. The latter can be assessed ultrasonically. In laminated specimens the damage pattern may show greater development in certain directions corresponding to less favourably oriented plies, see Fig. 1.5. One problem is having a specimen which is sufficiently large that the damage does not interact with the boundaries. One study of soft body impact involved firing a 3 g gelatine pellet at 90–190 ms-1 at a carbon thermoplastic matrix target. The damage was assessed by measuring the extent of delamination ultrasonically. The

IBF1 11/22/2000 4:14 PM Page 15

Impact behaviour of fibre-reinforced composites

15

damage was similar in form to that due to an aluminium projectile, though less extensive. The erosion, or impact damage of composites by repeated liquid impact, has been studied at velocities of 90 ms-1 upwards. A liquid or a soft body behaving compressibly exerts a pressure of rcV on the surface it strikes, where r is the density, V the impact velocity and c the stress wave velocity in the liquid. Liquid flowing outwards from under a curved surface causes considerable localised shear damage, particularly if the initial pressure has ruptured the surface. At high velocities, ~1000 ms-1, the compression wave generated by the liquid drop, on being reflected as a tension wave from the back surface of the specimen, causes scabbing, or the removal of material, if the transverse tensile strength is low. This has been observed in carbon fibre composite specimens. Fibres end-on to the direction of impact have an increased resistance to liquid erosion, probably due to the much better compressive properties of the fibre in the longitudinal, as compared with the transverse, direction. Practically, elastomer coatings (e.g. polyurethanes) are used to protect surfaces from liquid and solid particle erosion. In many of the cases involving high velocity impacts, with either hard or soft bodies, the experiment has been set up to test a special combination of projectile and material/design and the object is to determine the behaviour of the specimen rather than to derive a more fundamental impact energy; see Chapter 9. Three other areas of impact study involve: • • •

Barely visible impact damage (BVID). The measurement of a property after impact. The impacting of stressed bodies.

All are somewhat specialised and are related to damage tolerance, and the latter to the effects of superimposed stresses on impact behaviour. A general discussion of damage tolerant structural design is given in Chapter 4. BVID occurs when an object, such as a tool, is dropped accidentally onto a composite structure. For example, a thin shell-like, highly stressed aerospace component is particularly vulnerable in this respect. The danger is that the damage is so slight that it is not readily noticed by the naked eye but nevertheless compromises the load bearing capacity of the component. Apart from the obvious step of avoidance, possible solutions to this problem are the incorporation of sensitive sensors in the component and the use of damage tolerant matrices. An FEA analysis14 attributes back surface tensile damage in an impacted laminate, with little or no evidence of damage at the front, to localised bending in the vicinity of the impactor. If the back of the specimen is not visible this would be classified as a type of BVID. Since many crucial aerospace composite components are stressed in compression it is usually the compression strength that is evaluated after

IBF1 11/22/2000 4:14 PM Page 16

16

Impact behaviour of composite materials and structures

the impact. If the composite suffers debonding as a result of impact the compression strength will be affected because plies can act independently; limited microbuckling could occur on loading in compression and the strength would be reduced. Broken fibres would be an additional cause of a reduction in compression strength, possibly because of the complex stress field in the vicinity of the break. The compression strength after impact, CAI, is related to BVID, though the impact energies involved are probably greater than in the latter case. The approach to evaluating the damage is different, however. The crucial parameter is now how much a given energy or velocity impact reduces the strength of the material or component. Clearly the greater the strength retention, for given conditions, the better the material. As an illustration of the effect, a drop weight test with an impact energy of 30 J causes a reduction in the compressive stress of a laminate of ~30–40%.21 The authors developed a model based on the assumption that the change in compressive strength is related to the degradation of flexural stiffness in the impacted laminate. Fitting parameters are required and have to be determined experimentally but the model then gives a good fit to the data for the complete range of impact energies involved. Another, typical, account of the evaluation and analysis of the process for carbon fibre laminates is given in Ishai and Shragai.22 Generally the resulting degradation is influenced by clamping conditions and specimen geometry, since these can determine the nature of the damage produced under impact (e.g. shear delamination vs fibre failure). For similar studies see Chapter 5. The study of the impact of pre-stressed materials was initiated23 and more recently explored in a lengthy programme whose results have been summarised.24,25 The aim is to establish the combined effects of impact and a superimposed tensile or compressive stress. The combination is usually more damaging than either factor on its own. In the earlier work unidirectionally reinforced carbon and glass fibre specimens were stressed in tension up to 1.5–2.0 GPa and impacted with a wedge-shaped pendulum with a maximum energy of 4 J. The form of the results is shown in Fig. 1.6. The stress to cause failure, after impact in the unstressed state, falls linearly with increasing impact energy. This is equivalent to an ordinary notch sensitivity tensile test. Specimens stressed at the time of impact, however, require a lower stress to cause complete failure when tested to destruction after impact. It was noted that generally a high fibre strength and low fibre modulus lead to a higher impact performance. Later work investigated the effect of the wedge radius and role of delamination on the onset of failure – a low transverse strength could decrease the impact response. Rigidly supporting the back of the specimen caused different behaviour. Now the specimen could not bend when struck and no compressive fracture was

IBF1 11/22/2000 4:14 PM Page 17

17

0

Stress (GPa)

2

Impact behaviour of fibre-reinforced composites

0

Impact energy (J)

4

1.6 Effects of tensile prestress on impact energy. The upper line is for specimens impacted unstressed and then tested to failure in tension. The lower curve is for specimens impacted in the stressed state. In practice the prestress had to be adjusted to get impact on failure. The material was an intermediate modulus, unidirectional, carbon fibre/epoxy composite.

observed running in from the impacted face. There was also an optimum fibre volume loading ~67 v/o for maximum toughness. In the later work,24,25 carbon and glass fibre epoxy and thermoplastic laminates, prestrained in tension or compression up to 0.5%, were impacted at velocities ranging from a few meters per second up to 2.78 kms-1 using pendula, small projectiles and rifle bullets. The corresponding impact energies could be as high as 2.69 kJ. Damage was assessed visually and by using ultrasonic C scanning. Generally, impact with or without prestraining caused delamination, breakout of rear plies and sometimes complete penetration. The damage diameter, as determined by C scan, for different types of carbon fibre laminate as a function of prestrain, is shown in Fig. 1.7. Similar results were obtained with glass and aramid fibre panels. Compressive prestrain appeared more damaging than tensile prestrain, probably because the initial delamination allows the individual plies to buckle more easily under compression. Simultaneous strain and impact lowered the failure strain below that observed in the sequential case, see Fig. 1.8. Reasonable success was achieved in modelling the behaviour of cross ply laminates using the VEC-DYNA3D FEA code. It was possible to account for

C scan damage diameter (mm)

60

IBF1 11/22/2000 4:14 PM Page 18

More brittle resin

0

Less brittle resin –0.5

0

+0.5

Prestrain (%)

1.7 Delamination diameter, determined by C-scan, for carbon fibre composite laminated panels impacted at 50 ms-1 with a 6 mm diameter impacter at an energy of 1.1 J. Tensile prestrain has a minimal effect but compressive prestrain, combined with a more brittle epoxy resin leads to considerable damage.

Failure strain (%)

0.5

Woven

0

Unidirectional

0

0.25

0.5

Prestrain (%)

1.8 Effects of prestress on failure strain of a carbon fibre laminate. The figure shows the failure strain of the material impacted whilst prestrained and then, if required, strained to failure. The highest result is for a woven material. The impact velocity was 80 ms-1 and the impact energy 2.8 J.

IBF1 11/22/2000 4:14 PM Page 19

Impact behaviour of fibre-reinforced composites

19

penetration and the type and extent of damage. Overall it is important to use the correct boundary conditions. Potential failure mechanisms are complicated and interrelated and if one is not correctly assigned this may effect the predictions. Although much information on impact has been generated experimentally it is frequently very difficult to compare results because of differing specimen dimensions, boundary conditions, testing procedures, etc. The reader may be forgiven for thinking that the subject is poorly regulated and somewhat arbitrary. It has been suggested26 that specimen details seem to be resolved by a process of random choice. Certainly anyone perusing much of the literature on the impact properties of composites is struck by the way in which most papers approach the experimental side, appearing to use whatever materials and equipment are to hand rather than making a choice which fits in with other work. Having said that, the present author must confess to having tested specimens, 1 ¥ 1 m square ¥ 100 mm or more in thickness, by dropping steel cylinders, weighing up to 500 kg, onto the surface from a height of about a meter. The problem is that in many cases the modelling of the behaviour of a structure in an impact situation is so difficult that the best way to tackle the problem is to test the real structure in the most realistic way possible. No doubt as our knowledge and computational ability progress this will become less necessary but at present there is often nothing like a field trial.

1.5

Theoretical prediction of impact energy

Having discussed the methods for measuring impact energy and indicated the spread of results obtained it is necessary to develop a theoretical framework to describe the impact process. There are three approaches: • • •

Evaluate the bulk stored strain energy. Micromechanics – calculate the energy stored or dissipated in the fibre, resin and interface and in other failure processes. Linear elastic fracture mechanics (LEFM).

The first approach considers the elastically stored strain energy, while the second method covers dissipative processes. As was previously mentioned, because of energy storage in a specimen at the extremities, the first method will overestimate the energy required to create the two new surfaces resulting from the fracture of the specimen. LEFM is more mathematical and fibre composites do not always meet the assumptions made because of conditions at the crack tip leading to stress relief. While we shall mention fracture mechanics this approach will not be developed here.

IBF1 11/22/2000 4:14 PM Page 20

20

Impact behaviour of composite materials and structures

1.5.1 Strain energy If a body is stressed in tension, compression, flexure or shear, a simple strength of materials method27 can be used to calculate the stored strain energy. The area under a stress strain curve, up to the strain e, is equal to the energy, U, stored in the body, or e

U = Ú sde

[1.6]

0

If the material obeys Hooke’s law, s = Ee, the energy, per unit volume, is U = Ee 2 2 or s 2 2E

[1.7]

A similar expression applies for the energy in shear, per unit volume, viz.: U = t 2 2G

[1.8]

The following expressions for the strain energy in a rectangular beam of breadth, b, depth, d, and length, l, are useful: U t , U c = s lt2 bdl 2Elt , s lc2 bdl 2Elc (tension, compression)

[1.9]

U bc = 1 9 ¥ s bdl 2Elt (cantilever, beam 3 point loading)

[1.10]

U s = 4 15 ¥ t 2 bdl G (shear, 3 point loading)

[1.11]

2 lt

Note that in all of the formulae it is the maximum stress that is specified. A short span to depth ratio, Fmax > Fi F Fi

t Stage III-1: Fult = Fmax > Fi Fult F

t Stage III-2: Fult < Fmax F

t (a)

(b)

(c)

5.7 Three-stage damage sequence in thick laminate plates under lowvelocity impact described by (a) deformation sketches, (b) impact response curves and (c) C-scan graphs.

If a greater IKE was supplied, the top ply right underneath the impactor would be sheared through when the plate reached the maximum bending, as discussed earlier on the small plates and illustrated in Fig. 5.7. Because of this membrane stretching, the impacted large plates have shown much

IBF5 11/22/2000 4:54 PM Page 148

148

Impact behaviour of composite materials and structures

Table 5.2. Geometric effects on impact load-bearing capabilities of laminated composites Material

Laminate thickness (mm)

Impact force small plate (kN)

Impact force large plate (kN)

Percentage increase (%)

E-glass/polyester

10 25 150%

61 ± 1 124 ± 6 103%

92 144 57%

51 16

14 19 36%

117 ± 1 146 ± 2 25%

157 164 5%

34 12

Increased by S-glass/phenolic Increased by

greater load-bearing capability than the small plates as will be seen from Table 5.2. 5.4.1.2 Dominant damage mechanisms The use of the experimental techniques and processes described in Section 5.3.3 revealed that there were four types of damage mechanisms, on a macroscopic scale, operating during impact loading: matrix cracking, delamination, ply shear-out and fibre fracture. These failure modes would occur when stresses had exceeded the relevant strength values of the material. As these failure modes corresponded to strengths of very different magnitudes, they would be likely to occur sequentially and fibre breakage occurred only when a high IKE was provided. For example, matrix cracking usually took place first because its tensile strength in the region of 40– 90 MPa was the lowest and this was followed by delamination because of its low ILS strength, as shown in Fig. 5.4(b–c). Obviously, the damage mechanism such as matrix cracking dominated only at the lower end of the IKE spectrum. The other damage mechanisms were dominant at the central region and the upper end of the spectrum. Of course, the perforation of the laminate plates occurred at the upper end. In most of the impact and quasi-static tests, delamination and ply shear-out were the two dominant damage mechanisms. In order to ascertain these observations, extensive cross examination was carried out involving ultrasonic C-scanning, cross-sectioning and the use of impact force-time and/or quasi-static load-strain curves. Additional diagnostic impact as well as quasi-static tests on the small specimens were also conducted at several selected IKE levels aiming at generating the maximum forces slightly below and above the thresholds as identified previously. All

IBF5 11/22/2000 4:54 PM Page 149

Thick laminated woven roving GFRP plates

149

5.8 A through-the-thickness view of a single delamination in a 25 mm thick impacted E-glass/polyester panel (cut for CAI test).

these painstaking efforts19–21 have confirmed the following failure sequence for both composite systems, which is illustrated schematically in Fig. 5.7(a–d). Localised matrix cracking occurred in the contact area before the onset of delamination but it was insufficient to have a noticeable effect on the impact response curves.The initial load drop as indicated in Fig. 5.4(b–c) was caused by the onset of delamination and the final load drop in Fig. 5.4(c) corresponded to ply shear-out. After this load drop, shearing of plies continued through the thickness resulting in the growth of a truncated cone of sheared-out material. Ultimately this cone forced the remaining plies, close to the distal face, to fracture with an explosive bang as illustrated at the bottom of Fig. 5.7(a). The sequence of damage development is similar to observations on various CFRPs, reported in22–27 though some authors presented only quasi-static load-displacement curves. Because of the nature of woven roving reinforcement in a single ply, the current thick laminates were more likely to have a single delamination than those made of unidirectional prepregs, especially when impacted at low up to medium level of IKE. Such a single delamination usually occurred between one-quarter and three-quarters of the way through the laminate thickness as shown in a photograph taken from a sectioned impacted specimen in Fig. 5.8. Moreover, the projected contour of the delamination was usually close to a circle as a C-scan graph in Fig. 5.9 shows, though the difference of ILS strengths between the warp and the fill direction was around 20%. Obviously, at high IKE more than one delamination could be generated (see Fig. 5.26(a–b)), especially when the IKE was sufficient to induce ply shear-out. The through-thickness distribution of delamination was not investigated in all cases, but it is thought that a single, nearly circular delamination was the normal form of damage, at least in the early

IBF5 11/22/2000 4:54 PM Page 150

150

Impact behaviour of composite materials and structures

5.9 A C-scan graph showing a delamination in a 14 mm thick impacted S-glass/phenolic panel.

stages of the impact. In some thin UD-based quasi-isotropic carbon/epoxy laminates, it was often reported28–30 that a projected delamination of a nearly circular shape was due to an overlapping of multiple ‘peanut-shaped’ delaminations of similar sizes. This morphology results from the tendency of UD composites to delaminate along fibre directions, which seems not to apply to the woven rovings in the present investigation. Therefore, for the dominant damage mechanisms identified above, IDR comprises two separate elements: the resistance to the onset of delamination and its subsequent propagation and the resistance to ply shear-out or ultimate failure. In particular, resistance to delamination propagation in terms of IKE, as presented in Figs 5.10(a–b), is very much desired in the conventional impact damage tolerance assessment, as will be discussed in Section 5.5.4.

5.4.2 Effects of other parameters on impact damage resistance Since both composite systems could be strain-rate sensitive even at low impact velocities, the loading rate in addition to laminate geometry may affect the nature of the damage and thus the damage tolerance. Therefore the effect of varying these parameters on damage must be understood in terms of IKE, impact force and absorbed energy. Because of the different thicknesses used for the different composite systems, a direct comparison between them remains qualitative. Discussion on the strain-rate effect under high impact velocities is available in Chapter 3.

IBF5 11/22/2000 4:54 PM Page 151

Thick laminated woven roving GFRP plates

151

Damage area (mm2)

240 000 10 mm thick plates

200 000

25 mm thick plates 160 000 120 000 80 000 40 000 0 0

400

(a)

800

1200

1600

2000

2400

2800

3000

3500

Incident kinetic energy, IKE (J) 240 000

Damage area (mm2)

14 mm thick plates 200 000

19 mm thick plates

160 000 120 000 80 000 40 000 0

0

500

1000

1500

2000

2500

Incident kinetic energy, IKE (J)

(b)

5.10 (a) Damage area as a function of IKE for E-glass/polyester plates. (b) Damage area as a function of IKE for S-glass/phenolic plates.

5.4.2.1 Loading rate effect The effect of loading rate on damage was examined phenomenologically in two ways. One was to examine the variation of impactor mass (inertia) with impact velocity being kept constant; the other was to examine the variation of impact velocity by using the same impactor. The former has been neglected in most low-velocity impact investigations either due possibly to assumption that inertia effect plays no part in low-velocity impact or possibly because it is just easier to ignore it. The inertia effect examined

IBF5 11/22/2000 4:54 PM Page 152

152

Impact behaviour of composite materials and structures

Initial threshold impact force (kN)

100 10 mm thick 25 mm thick

80

14 mm thick 19 mm thick

60

40

20

0 0

10

20

30

40

50

60

70

80

Impactor mass (kg)

5.11 Initial threshold impact forces as a function of impactor mass for small E-glass/polyester and S-glass/phenolic plates.

here addressed half the problem as it arose only from the variation of impactor mass. The mass of the laminate plate during impact was not directly studied. Figure 5.11 presents the variation with impactor mass of the threshold forces corresponding to the onset of delamination for both composite systems. In this diagram, a higher impact force at specific impact mass corresponds to a higher impact velocity (thus IKE). It seems to show that the force at the onset of delamination was independent of impactor mass for both composite systems irrespective of laminate thickness, even when impactor mass was increased by nearly nine times. This finding seems also in accordance with one of the analytical predictions given.30 The inertia effect on delamination propagation was examined by increasing impactor mass while keeping impact velocity constant.As seen in Fig. 5.12, the growth of delamination area was sensitively related to an increase of impactor mass (and hence IKE) for both composite systems. Since IKE also increased with impactor mass in Fig. 5.12, this inertia effect on delamination area is further examined later by varying impactor mass and impact velocity simultaneously with IKE being kept constant. The effect of impact velocity on resistance to specific damage mechanisms has been examined using two methods.31 The effect was examined, in addition to the usual method in which impact velocity is varied, by directly comparing impact data with quasi-static. For delamination propagation, the examination procedure was quite involved as will be explained later. For the onset of delamination and ply shear-out, direct comparisons of the

IBF5 11/22/2000 4:54 PM Page 153

Thick laminated woven roving GFRP plates

153

Delamination area (mm2)

14 000 10 mm thick E-glass/polyester with 5.3ms-1 25 mm thick E-glass/polyester with 4.3ms-1 14 mm thick S-glass/phenolic with 4.3ms-1

12 000 10 000 8 000 6 000 4 000 2 000 0 0

100

200 300 400 500 600 700 Incident kinetic energy, IKE (J)

800

5.12 Delamination areas as a function of IKE with constant impact velocity for large laminate plates.

90 10 mm thick glass/polyester 25 mm thick glass/polyester 14 mm thick glass/phenolic 19 mm thick glass/phenolic

Initial threshold force (kN)

80 70 60 50 40 30 20 10 0 0

1

2

3

4

5

Impact velocity

6

7

8

9

(m s-1)

5.13 Initial threshold force for the onset of delamination as a function of impact velocity.

threshold forces were made between quasi-static and impact cases. In Fig. 5.13, both the quasi-static and impact threshold forces corresponding to the onset of delamination are plotted against velocity, which was varied from 8.3 ¥ 10-5 ms-1 (i.e. 5 mm/min) to 8 ms-1. It can be observed that the Eglass/polyester system seemed to be independent of impact velocity irre-

IBF5 11/22/2000 4:54 PM Page 154

154

Impact behaviour of composite materials and structures

Maximum force (kN)

180 160

Static data

140

Impact data 22%

120

19% 18%

100 80

36%

60 40 20 0

10 mm E-gl/po

25 mm E-gl/po

14 mm S-gl/ph

19 mm S-gl/ph

5.14 Comparison of load-bearing capabilities of small plates subjected to static and impact loadings.

Delamination area (mm2)

8000 10 mm thick E-glass/polyester 14 mm thick S-glass/phenolic 6000

4000

2000

0 0

30 60 90 120 Incident kinetic energy, IKE (J)

150

5.15 Delamination areas as a function of IKE with constant impactor mass of 8 kg.

spective of laminate thickness. However, the S-glass/phenolic system did show a modest increase in the threshold forces (over 20%) for both thicknesses with reference to the quasi-static values. For ply shear-out or laminate load-bearing capability, the results as summarised in Fig. 5.14 show that the effect of impact velocity was significant for the E-glass/polyester and was modest for the S-glass/phenolic. The effect of impact velocity on delamination propagation was examined with a constant impactor mass and the results are shown in Fig. 5.15. There, delamination area is seen to increase with impact velocity and thus IKE, as

IBF5 11/22/2000 4:54 PM Page 155

Thick laminated woven roving GFRP plates

155

Delamination area (mm2)

240 000 25mm thick large E-glass/polyester plates

200 000

68kg impactor mass 105kg impactor mass

160 000 120 000 80 000 40 000 0 0

500

1000

1500

2000

2500

Incident kinetic energy, IKE (J)

(a)

Delamination area (mm2)

240 000

68kg mass for 14mm thick plates 105kg mass for 14mm thick plates 68kg mass for 19mm thick plates 105kg mass for 19mm thick plates

200 000 160 000

S-glass/phenolic plates

120 000 80 000 40 000 0 0

(b)

500

1000

1500

2000

2500

Incident kinetic energy, IKE (J)

5.16 (a) and (b) Delamination areas as a function of two combinations of impactor mass and impact velocity for identical IKE.

expected. In order to separate out the effects of velocity, inertia and energy, it was also necessary to vary both impact velocity and impactor mass simultaneously while IKE was kept constant. In some cases appreciable variation of delamination area can occur.31 However, in the present investigation, as shown in Fig. 5.16(a–b), differences in delamination area produced in this way were small. In conjunction with the results in Fig. 5.12–15, this could be attributed to one of the following two reasons. One is that the 20% variation of impact velocity associated with a change of impactor mass from 68 kg to 105 kg was insufficient due to the physical constraints of the present drop-weight impact rig. The other is that, for an identical IKE, the effect of impact velocity on delamination propagation was likely to cancel out the inertia effect. That is, increasing impact velocity while holding impactor

IBF5 11/22/2000 4:54 PM Page 156

156

Impact behaviour of composite materials and structures Delamination area (mm2)

14 000 10 mm thick 25 mm thick

12 000 10 000 8 000 6 000 4 000 2 000 0 0

30

60

90

120

150

Impact force (kN)

5.17 Delamination area as a function of impact force for small E-glass/polyester plates.

mass constant may have produced a trend of delamination areas similar to that caused by increasing impactor mass while holding impact velocity constant. Consequently, the net effect caused by these combinations on delamination area for identical IKE would be small. 5.4.2.2 Laminate thickness effect In the present impact tests, the geometry of the laminate plates was varied to allow an examination of its effect on impact response and IDR over a large range of IKE for each composite system. The test results are summarised in Table 5.2 which shows clearly that, for specimens of a constant diameter, the impact resistance to ply shear-out increased with an increase of thickness as expected for both composite systems. In Fig. 5.13, the impact resistance to the onset of delamination increased by 216% with a thickness increase of 150% for small E-glass/polyester plates. For small S-glass/phenolic plates, a smaller increase of 36% in impact resistance was observed which was identical to the increase in thickness (36%). This appears to be independent of impact velocity. In Fig. 5.17, the thicker E-glass/polyester plates are seen to provide the greater impact resistance to delamination propagation for the same delamination area. In other words, for identical impact force, the delamination areas of the thicker plates were much smaller than those of the thin ones. Obviously, the penalty paid for this superior impact resistance was 150% weight increase. For Sglass/phenolic plates, however, there was little difference in the impact resistance to delamination propagation irrespective of plate diameter, as seen in Fig. 5.18(a–b). Interestingly, the resistance of this material to delamina-

IBF5 11/22/2000 4:54 PM Page 157

Thick laminated woven roving GFRP plates

157

Delamination area(mm2)

15 000 14 mm thick 19 mm thick

12 000 9 000 6 000 3 000 0 0

20

40

(a)

60 80 100 120 140 160 Impact force (kN)

Delamination area (mm2)

200 000 14 mm thick 19 mm thick

160 000 120 000 80 000 40 000 0 0

20

40

(b)

60 80 100 120 140 160 180 Impact force (kN)

5.18 (a) Delamination areas as a function of impact force for small S-glass/phenolic plates. (b) Delamination areas as a function of impact force for large S-glass/phenolic plates.

tion propagation, if measured by IKE, seemed to become lower for the thicker plates, as shown in Fig. 5.10(b). 5.4.2.3 Plate diameter effect Exploring the effect of plate diameter32 is possibly of greater practical importance than that of thickness. A realistic thickness is easily obtained in laboratory conditions for most full-scale composite structures. On the other hand, the in-plane dimensions of real structures normally need to be scaled down for test specimens. Scaling in impact testing is discussed elsewhere.32 A more general discussion is available, and33 relevant quasi-static data can also be found.34–36

IBF5 11/22/2000 4:54 PM Page 158

158

Impact behaviour of composite materials and structures

When the diameter of a laminate plate was increased from 100 mm to 500 mm, the increased membrane stretching was expected to contribute to IDR, especially in the relatively thin plates. In Table 5.2, the laminate loadbearing capabilities are clearly seen to increase rather than decrease as predicted by the static plate theory, while other experimental data based on carbon/epoxy plates34–36 have shown insensitivity to a change in plate diameter. The present dynamic enhancement of load-bearing capability was believed to be due to a change in the state of three-dimensional stresses in the contact area. This resulted from a significant contribution of membrane stretching to the in-plane stress components, manifested in part by the compression-to-tension switching of an impact strain gauge response in Fig. 5.6. The effect of this appears to be either a reduction in the local shear stress component which was responsible for ply shear-out, or possibly an increase in effective strength resulting from the triaxial stresses. Obviously, the thicker a laminate plate became, the less significant this enhancement would be, as shown in the table. Although an increase in plate diameter increased the degree of membrane stretching in the plate behaviour, it did not seem to affect the threshold forces corresponding to the onset of delamination17,27 and thus not the initial impact resistance. Moreover, the size of delamination areas from the small plates did not overlap in any way with that of the large plates, so unfortunately direct comparison of their impact resistance to delamination propagation was not feasible.

5.4.3 Energy-absorbing characteristics of damage mechanisms It was very likely that the damage mechanisms absorbing more IKE (such as delamination) had a greater effect on IDR and thus on damage tolerance. The onset of delamination was an unstable process associated with the sudden load drop and the jump in delamination area as described in Figs 5.17 and 5.18(a). Its subsequent propagation has been identified as the primary energy-absorbing damage mechanism. It appears to be a more desirable failure mode than ply shear-out, which could potentially lead to the plate perforation as illustrated in Fig. 5.19. In other words, the most effective process for completely absorbing a specified IKE in an impact event was through delamination propagation (OABCD) before the loadbearing capability was reached (at C or B¢). This was preferable to absorbing the energy by fibre fracture (OAB¢C¢), because more energy is absorbed and the delaminated plate still possessed a considerable amount of residual load-bearing capability as will be discussed later. It is not difficult to see that the region CDC¢E ought to be much greater than the region AB¢EB, although the position of C¢ is speculative. In Fig. 5.20(a–b) which sum-

IBF5 11/22/2000 4:54 PM Page 159

Thick laminated woven roving GFRP plates

159

A - Onset of delamination

Impact force

Fibre breakage

B¢

C

E A B

O

C¢

D

Time

5.19 Illustration of energy absorption with and without delamination.

marises the results of groups of impact tests, the IDR corresponding to delamination propagation increased nearly linearly with an increase of energy absorption (AE). When ply shear-out occurred, the IDR started to level off so that some of the IKE was absorbed by continued ply shear-out. It was shown that,37 when ply shear-out did not occur, an amount of AE (EAE) could be expressed by EIKE - ER = EAE = Emc + Eod + Epd = Emc + GIIcA

[5.1]

in which ER is rebound energy, Emc, Eod, and Epd denote an amount of AE from localised matrix cracking, onset of delamination, propagation of delamination, GIIc is mode-II strain energy release rate and A is delamination area with the assumption of a single delamination. If rebound velocity in an impact test was measured so that ER as well as EIKE (IKE) were known, the corresponding delamination area would be approximately estimated providing that GIIc was available and Emc was negligible. In the present case with GIIc = 4.2 kJ/m2 and 3.8 kJ/m2 for the E-glass/polyester and S-glass/phenolic systems, respectively, the predictions of equation [5.1] are demonstrated in Fig. 5.20(a–b) with arbitrary Emc as the latter was believed to be small and was impossible to quantify under the present impact conditions. When delamination areas were less than three-quarters of the small plate area, the predicted overall trends agreed reasonably well with the experimental data for both composite systems. An additional interesting feature was the effect of varying thickness on the relationship between delamination propagation and absorbed energy. For a given plate

IBF5 11/22/2000 4:54 PM Page 160

160

Impact behaviour of composite materials and structures

Delamination area (mm2)

14 000

Predictions of equation [5.1] with an arbitrary amount of matrix cracking

12 000 10 000 8 000 6 000 4 000

10 mm thick plate 25 mm thick plate

2 000 0 0

50 100 150 200 250 300 350 400 450 500 Absorbed energy, AE (J)

(a) 16 000

Predictions of equation [5.1] with an arbitrary amount of matrix cracking

Delamination area (mm2)

14 000 12 000 10 000 8 000 6 000 4 000

14 mm thick plate 19 mm thick plate

2 000 0 0

(b)

200 400 600 800 1000 1200 1400 1600 1800

Absorbed energy, AE (J)

5.20 (a) Delamination area as a function of AE for small Eglass/polyester plates. (b) Delamination area as a function of AE for small S-glass/phenolic plates.

diameter, delamination area seemed to decrease with increasing laminate thickness for identical AE. This suggested that some of the IKE in the thicker laminate was dissipated in other deformation mechanisms so that not all the IKE was absorbed in initiating and propagating delamination. A detailed discussion for the effect of GIIc on energy absorption is available in Chapter 1.

5.5

Impact damage tolerance and assessment

Naturally, for in-service load-bearing composite structures which also have a high risk of impact load, their damage tolerance holds the key to success.

IBF5 11/22/2000 4:54 PM Page 161

Thick laminated woven roving GFRP plates

161

The essence of damage tolerance is that the damaged composite structures are still capable of providing the desired performance, as defined by a set of mechanical requirements. As discussed in Section 5.1, the main measure of impact damage tolerance is the retention rate of compressive strength relative to the strength of the intact composite structure. The energy-based IDR alone provides only limited information. For a general damage tolerant structural design philosophy, see Chapter 4.

5.5.1 Compressive behaviour of intact and damaged panels In-plane compressive strength and stiffness were determined by testing rectangular panels quasi-statically. Generally, either damaged or intact panels needed to be supported laterally by using the anti-buckling device as described in Section 5.3.4 to avoid a premature buckling. The back-to-back strain gauges were bonded at a number of selected locations and an examination of their responses provided an important physical insight into the development of panel deformation mechanisms leading to ultimate failure. For intact panels, at least seven pairs of strain gauges were bonded across the panel width with one row (either two or three pairs per row) close to each end and one on the middle section. For damaged panels, three pairs were used, as shown in Fig. 5.3(b–c).The gauge response in terms of bending strain (i.e. difference between gauges on opposite sides of the panel at the same point) and mean strains was used to characterise panel behaviour. A positive panel bending strain here means that a panel buckles towards the distal surface while a negative panel bending strain corresponds to buckling toward the impact surface. The mean strain is relatively small if buckling occurs and is relatively large if delamination opening occurs. Equipped with this understanding, four major deformation mechanisms were identified in the compression of the present panels as illustrated in Fig. 5.21.38 Typical load-panel bending strain and load-mean strain curves are shown in Fig. 5.22(a–b) from a damaged 10 mm thick E-glass/polyester panel. Assuming a circular shape (as can be seen in Fig. 6 of Zhou17), the delamination area of 8961 mm2 was converted to a circle of 107 mm in diameter as shown in the inset of Fig. 5.22(a). Examining the 1/4 pair of strain gauges indicates that global buckling did not occur as the panel bending strain remained more or less zero until the ultimate failure was approached. Also, the fact that both panel bending and mean strains for the 2/5 pair were relatively large suggested that local buckling and delamination opening could have occurred simultaneously (case (2) in Fig. 5.21). The response of the 3/6 pair shows the similar behaviour to that of the 1/4 pair. The continuing local buckling eventually led to compression failure with a kink shear band as a photograph in Fig. 5.23 shows. This development must have been assisted

IBF5 11/22/2000 4:54 PM Page 162

162

Impact behaviour of composite materials and structures Pair 1/4

Pair 2/5

Pair 3/6

Bending Mean Bending Mean Bending Mean strain strain strain strain strain strain (1) Euler buckling

Large Small

Large Small

Large Small

(2) Delamination opening

Small Large

Small Large

Small Large

(3) Global-local mechanism

Large Small

Large Small

Small Large

Small Large

Large Small

(4) Compression with kink shear band

Small Large

5.21 Illustration of failure mechanisms of damaged panels in CAI tests with back-to-back strain gauges.

IBF5 11/22/2000 4:54 PM Page 163

Thick laminated woven roving GFRP plates

163

10 000

Bending microstrain

8 000

SG 1/4 SG 2/5 SG 3/6

1/4 3/6

6 000

2/5

4 000 2 000 0 -2 000 0

40

80

120

160

200

240

280

240

280

Compressive load (kN)

(a) 8000

SG 1/4 SG 2/5 SG 3/6

Mean microstrain

7000 6000 5000 4000 3000 2000 1000 0 0

(b)

40

80

120

160

200

Compressive load (kN)

5.22 (a) Compressive load-bending strain curves of a 10 mm thick damaged E-glass/polyester panel. (b) Compressive load-mean strain curves of a 10 mm thick damaged E-glass/polyester panel.

by the presence of the increased curvature of local fibres which made the damaged panel unsymmetrical locally thereby favouring local buckling. Sideways propagation of delamination was not very noticeable, but this may have been due to the fact that the orientation of the 2/5 and 3/6 pairs of the strain gauges was in the loading direction. With the benefit of hindsight, it may be speculated that additional strain gauges in the direction of the panel width could have been more useful for detecting width-wise delamination growth. In Fig. 5.24(a–b) from a damaged 14 mm thick S-glass/phenolic panel, some global buckling is visible though the response of all the strain gauges

IBF5 11/22/2000 4:54 PM Page 164

5.23 Compression failure with a kink shear band in a 10 mm thick Eglass/polyester CAI panel.

5.25 Compression failure with a kink shear band in a 14 mm thick Sglass/phenolic CAI panel.

IBF5 11/22/2000 4:54 PM Page 165

Thick laminated woven roving GFRP plates

165

30 000

Bending microstrain

25 000

1/4

SG 2/5

20 000

3/6 2/5

15 000 10 000

SG 3/6

5 000 0 -5 000

SG 1/4

-10 000 0

40

80

120

160

200

240

280

320

Compressive load (kN)

(a) 10 000 SG 1/4 SG 2/5 SG 3/6

Mean microstrain

8 000 6 000 4 000 2 000 0 0

(b)

50

100

150

200

250

300

Compressive load (kN)

5.24 (a) Compressive load-bending strain curves of a 14 mm thick damaged S-glass/phenolic panel. (b) Compressive load-mean strain curves of a 14 mm thick damaged S-glass/phenolic panel.

was similar. Judging from the developing trend of the 2/5 and 3/6 pairs, local buckling and delamination opening again occurred simultaneously. The final panel failure is shown in Fig. 5.25 with a clear kink shear band. This in conjunction with all three pairs of strain gauge readings suggested that the damaged panel twisted during loading in the form of the second buckling mode. Photographs in Fig. 5.26(a–b) show typical failed thicker damaged panels for both E-glass/polyester and S-glass/phenolic laminates. The only difference is that these thicker panels had multiple delaminations so that each sublaminate failed in compression through its own kink shear band. Therefore, the adjacent shear bands with often different orientations coalesced

IBF5 11/22/2000 4:54 PM Page 166

166

Impact behaviour of composite materials and structures

5.26 Compression failure with a kink shear band in (a) a 25 mm thick E-glass/polyester and (b) a 19 mm thick S-glass/phenolic CAI panels.

to form a saw-tooth shaped failure zone through the thickness. Other noticeable features are that the E-glass/polyester panel had a much greater shear angle formed between the loading direction and major kink band than the S-glass/phenolic panel. Also that the kink band was more jagged in the E-glass/polyester than in the S-glass/phenolic, possibly due to a stronger fibre/matrix interfacial bonding. As a whole, it seemed that compression failure with a kink shear band was predominant in the tests of the damaged panels. Ideally, both the intact and damaged compressive strengths used to calculate strength retention factor ought to be measured from panels which fail by similar mechanisms or at least at the middle section. Although the present damaged panels indeed failed consistently at the middle section with the combined mechanism of local buckling and shear as demonstrated, the intact panels always failed close to one end as shown in Fig. 5.27(a–b). Therefore the use of the compressive strengths from the intact panels as a

IBF5 11/22/2000 4:54 PM Page 167

Thick laminated woven roving GFRP plates

167

5.27 Compression failure with a kink shear band in (a) a 25 mm thick E-glass/polyester and (b) a 19 mm thick S-glass/phenolic intact panels.

reference was probably subject to a degree of systematic error. Nevertheless, this inherent feature is present in most of the published impact damage tolerance research works. Residual compressive stiffness could also be measured on the load-mean strain curve. This is important not only for a stiffness-sensitive structural component but also for its contribution to potential further propagation of impact damage.

5.5.2 Factors affecting strength retention factor Obviously, the strength retention factor decreased steadily as a severity of impact damage increased. Less obvious was its possible dependence on the panel geometry and local changes of fibre curvature in the vicinity of the impact contact area. Very little information exists on the panel geometry effect on residual and intact compressive strengths. In addition, an understanding of the contribution of local fibre curvature to a reduction of com-

IBF5 11/22/2000 4:54 PM Page 168

168

Impact behaviour of composite materials and structures

pressive strength may shed light on the true nature of compressive strength degradation. For example, it may provide an interesting physical insight into why a panel with an open hole (indirect assessment of residual strength) provided greater compressive strength than the impact-damaged panel with delamination area identical to the hole.39 Impact damage induced in the large plates had both local and global effects.40–41 Local damage consisted of matrix cracking, fibre/matrix debonding, surface microbuckling and fibre breakage (including both shear-out and tensile fracture for some plates), all surrounding the slightly dented impact contact area. Global damage refers to the extensive internal delamination or multiple delaminations, although, strictly, these are still local, but on a much larger scale. The local deformation (especially induced at relatively high IKE and involving ply shear-out) resulted in a local change in fibre curvature, which in turn acted as a pre-introduced misalignment, or region of fibre waviness, in the panel. In compressive loading this contributed to the initiation of local compression failure with a kink shear band. Another contribution to the loss in compressive strength was clearly the breakage of load-bearing fibres, but the failure mode is dominated by the impactinduced internal delamination. The delamination effectively divided the laminate locally into two or more sublaminates so that local flexural stiffness of these sublaminates was significantly reduced. As a result, these sublaminates may buckle locally causing an overall failure of the panel at a load level considerably lower than that of the intact panel.42 For thin damaged panels as demonstrated earlier, impact-induced delamination did not seem to propagate much in compressive loading. It is therefore thought that the large strains in the post-buckled part of the plate triggered in-plane compression failure. An increase of panel thickness by two and half times did not much alter either deformation mechanism or residual compressive strength as shown in Fig. 5.28(a–b). This finding is consistent with compression-after-impact (CAI) results of carbon/epoxy panels measured by Boeing method.43–44 Because failure is initiated locally, residual strength should not be affected by panel length. This was not investigated in the present study but work elsewhere on carbon/epoxy45 found a reduction of the length of damaged panels by 17% did not result in any significant change in residual compressive strength determined by the NASA method. On the other hand, variation of the geometry of intact panels, especially length, can have a greater effect on compressive strength so as to significantly affect strength retention factor. This was found, for example in.44 In the present investigation, the two-and-a-half-times increase of panel thickness between the two E-glass/polyester laminates led to a 12% decrease in undamaged compressive strength. This may partially account for the higher strength retention factors observed in the thicker plate.

IBF5 11/22/2000 4:54 PM Page 169

Thick laminated woven roving GFRP plates

169

18 000 SG 1/4 SG 2/5 SG 3/6

Bending microstrain

15 000 12 000 9 000 6 000 3 000 0 -3 000 -6 000 0

100

200

300

400

500

600

500

600

Compressive load (kN)

(a) 12 000

SG 1/4 SG 2/5 SG 3/6

Mean microstrain

10 000 8 000 6 000 4 000 2 000 0 -2 000 0

100

200

300

400

Compressive load (kN)

(b)

5.28 (a) Load-bending strain curves of a 25 mm thick damaged Eglass/polyester panel. (b) Load-mean strain curves of a 25 mm thick damaged E-glass/polyester panel.

5.5.3 Damage measures IKE, delamination area and depth of surface indent have all been used as the measures of damage in the tolerance assessment of impact damage. While the depth of a surface indent has been proved46 to bear no relation to the magnitude of interior damage and thus to a strength retention factor, IKE and delamination area also have inherent limitations, all involving the nature of impact damage. The only advantage of using IKE is its convenience as it can be readily defined to represent a degree of threat before an impact test is conducted. Disadvantages are that individual contributions

IBF5 11/22/2000 4:54 PM Page 170

170

Impact behaviour of composite materials and structures

of impact velocity (including quasi-static case) and impactor mass to damage and thus to damage tolerance cannot easily be examined separately. Therefore, an impact energy value could potentially yield a range of different strength retention factors. As discussed earlier, combinations of low velocity with large mass and high velocity with small mass have proved to result in two different delamination areas. Different orientations with regard to the loading direction of a single irregular delamination area of a given size have also been demonstrated both experimentally47 and numerically48 to be responsible for different strength retention factors. For example, residual compressive strength was shown to be higher when an elliptical damage area had the major axis in the loading direction. The reliability of using delamination area to assess likely residual strength is therefore questionable. The use of absorbed energy was suggested as a more relevant measure of damage.49 Quite recently, the use of impact force was shown to be a useful additional measure of damage17, 40–41 as it brought out some features of the panel compressive behaviour, which were less obvious when the other measures of damage were used. In particular, the identifiable impact force thresholds on a force-time history curve could be not only related to the dominant damage mechanisms occurring in laminate during impact but also compared directly to the static ones for examining the effect of loading rate in damage tolerance assessment.

5.5.4 Conventional damage tolerance assessment As described in Section 5.1, damage tolerance should embrace not only a load level or an IKE which a structure can sustain without suffering appreciable damage (IDR) but also a minimum level of residual load-bearing capability which the damaged structure can retain at the specified IKE or delamination area. The first part of the damage tolerance concept has already been established by the damage force and energy maps in the discussions of IDR (i.e. Figs 5.10(a–b), 5.17 and 5.28(a–b)). This is the idea of initial threshold force or IKE, below which there should be no damage. The estimated threshold will appear in the later diagrams as the end of the initial strength plateau on the grounds that if there is no damage, there should be no loss in residual compressive strength. The second part of the concept is addressed in the following through the variations of strength retention factor with IKE, delamination area and impact force. Figures 5.29–31 show the variations of strength retention factor for all four laminates in terms of damage area, IKE and impact force. As can be seen, once damage area started to increase or the initial threshold value of IKE or impact force was exceeded, residual strength was reduced very rapidly due to the presence of extensive delamination or multiple

IBF5 11/22/2000 4:54 PM Page 171

Thick laminated woven roving GFRP plates

171

1.1 1.0

10 mm glass/polyester 25 mm glass/polyester 14 mm glass/phenolic 19 mm glass/phenolic

Strength retention factor

0.9 0.8 0.7 0.6 0.5 0.4 0.3 0.2 0.1 0.0 0

40 000

80 000

120 000

160 000

200 000

Damage area (mm2)

5.29 Compressive strength retention factors as a function of damage area for composite panels.

1.1 1.0

10 mm glass/polyester 25 mm glass/polyester 14 mm glass/phenolic 19 mm glass/phenolic

Strength retention factor

0.9 0.8 0.7 0.6 0.5 0.4 0.3 0.2 0.1 0.0 0

400

800

1200 1600 2000 2400 2800 3200

Incident kinetic energy, IKE (J)

5.30 Compressive strength retention factors as a function of IKE for composite panels.

delaminations, prompting compression failure. It is noted that both types of the laminates could still retain 30% and 20% compressive strengths, respectively, even when they were completely delaminated. These asymptotes were largely due to the fact that the current panel width of 250 mm or the

IBF5 11/22/2000 4:54 PM Page 172

172

Impact behaviour of composite materials and structures 1.2 10 mm glass/polyester 25 mm glass/polyester 14 mm glass/phenolic 19 mm glass/phenolic

Strength retention factor

1.0 0.8 0.6 0.4 0.2 0.0 0

20

40

60

80

100

120

140

160

180

Impact force (kN)

5.31 Compressive strength retention factors as a function of impact force for composite panels.

equivalent circular area of 49 087 mm2 was not capable of differentiating compressive strengths from the panels containing a delamination area greater than that. Thickness did not seem to have much effect on residual strengths plotted against damage area or IKE once damage occurred or the initial IKE threshold was exceeded. However, plotting against impact force did reveal an effect of thickness. Another advantage of using impact force is that the initial plateau established in the damage force maps is readily recognised in the retained strength plots. The overall trends in degradation of residual strengths for the Sglass/phenolic laminates were similar to that of the E-glass/polyester laminates. The best performance from the 25 mm thick glass/polyester differed from the worst from the 14 mm thick glass/phenolic by less than 20%. For the same type of laminate, the thicker plates had fractionally higher residual strengths. The thickness effect on residual strength therefore did not seem to be significant on the basis of the present data. Sometimes the residual far-field compressive strain rather than strength is favoured in the conventional assessment of impact damage tolerance. Thus, the far-field compressive strain data for all four laminates are presented in terms of IKE in Figs 5.32–33(a–b), which also include strength retention data for comparison. These results indicate that both the overall downward trends were similar in magnitude and that the residual far-field compressive strain data gave higher retention factors than the residual strength data (except for the 10 mm thick E-glass/polyester panels). This

IBF5 11/22/2000 4:54 PM Page 173

1.2 Strain data Strength data

1.0 0.8 0.6 0.4 0.2 0.0 0

300

(a)

900

1200

1500

1800

1.2 Strain data

1.0

Strength data 0.8 0.6 0.4 0.2 0.0 500

1000

1500

2000

2500

Compressive strength retention factor

Compressive strain retention factor

Incident kinetic energy, IKE (J)

0

(b)

600

173

Compressive strength retention factor

Compressive strain retention factor

Thick laminated woven roving GFRP plates

3000

Incident kinetic energy, IKE (J)

5.32 (a) Comparison of far-field strain and strength retention factor data for 10 mm thick E-glass/polyester panels. (b) Comparison of far-field strain and strength retention factor data for 25 mm thick E-glass/polyester panels.

would be expected if the damage caused a reduction in stiffness and may indicate that the gauges were not truly in the far field. The impact damage did indeed cause a degradation in stiffness. For the present thick laminate panels, the reduction in compressive stiffness as shown in Figs 5.34–35 was much less severe than that in strength, as expected. The rate of degradation was nearly linear and the thicker panels suffered a lesser reduction. For example, the 25 mm thick E-glass/polyester panel suffered almost no loss in compressive stiffness after being impacted with an IKE of 334 J and having a delamination area of 163 mm in diameter, and lost only about 10% of stiffness at an IKE of 2000 J.

IBF5 11/22/2000 4:54 PM Page 174

1.2 Strain data Strength data

1.0 0.8 0.6 0.4 0.2 0.0 0

600

1800

2400

3000

3600

Compressive strain retention factor

1.2 Strain data Strength data

1.0 0.8 0.6 0.4 0.2 0.0 0

600

1200

1800

2400

3000

Compressive strength retention factor

Incident kinetic energy, IKE (J)

(a)

(b)

1200

Compressive strength retention factor

Impact behaviour of composite materials and structures Compressive strain retention factor

174

3600

Incident kinetic energy, IKE (J)

5.33 (a) Comparison of far-field strain and strength retention factor data for 14 mm thick S-glass/phenolic panels. (b) Comparison of far-field strain and strength retention factor data for 19 mm thick S-glass/phenolic panels.

5.5.5 Impact-force data based damage tolerance assessment As discussed earlier, the conventional assessment of impact damage tolerance is a complex, costly and time-consuming process. The use of strength retention factor in this process has been shown to have several inherent limitations, for example, sensitivity to different local topographic features around the impact contact area and different failure characteristics in addition to the uncertain effect of anti-buckling support on residual compressive strength. Therefore, it seems necessary to seek a simpler and more cost-effective alternative on both cost and lead time grounds.

IBF5 11/22/2000 4:54 PM Page 175

Compressive stiffness retention factor

Thick laminated woven roving GFRP plates

175

1.2 1.0 0.8 0.6 0.4 10 mm thick 0.2

25 mm thick

0.0 0

400

800

1200

1600

2000

2400

2800

Incident kinetic energy, IKE (J)

Compressive stiffness retention factor

5.34 Stiffness retention factor as a function of IKE for Eglass/polyester panels.

1.2 14 mm thick 1.0

19 mm thick

0.8 0.6 0.4 0.2 0.0 0

600

1200

1800

2400

3000

3600

Incident kinetic energy, IKE (J)

5.35 Stiffness retention factor as a function of IKE for S-glass/phenolic panels.

A novel method proposed recently50–51 was to use the ratio of two impact force thresholds identified on the recorded impact force-time history curves. One was the initial threshold force corresponding to the onset of delamination whereas the other was a peak impact force. It is advantageous if the data from the impact tests can be used directly for a preliminary assessment of damage tolerance. This method was developed on the basis of the fact that the dominant damage mechanisms such as delamination and

IBF5 11/22/2000 4:54 PM Page 176

Ratio of initial threshold force to max force

1.2 Force data of small plates Force data of large plates CAI data

1.0 0.8 0.6 0.4 0.2 0.0 0

2 000 4 000 6 000 8 000 10 000 12 000 14 000 Delamination area (mm2)

(a)

Ratio of initial threshold force to max force

1.2 Force data of small plates Force data of large plates CAI data

1.0 0.8 0.6 0.4 0.2 0.0 0

(b)

Compressive strength retention factor

Impact behaviour of composite materials and structures

40 000

80 000

Compressive strength retention factor

176

120 000 160 000 200 000

Delamination area (mm2)

5.36 (a) Comparison of force ratio and strength retention factor data for 10 mm thick E-glass/polyester panels. (b) Comparison of force ratio and strength retention factor data for 25 mm thick Eglass/polyester panels. (c) Comparison of force ratio and strength retention factor data for 14 mm thick S-glass/phenolic panels. (d) Comparison of force ratio and strength retention factor data for 19 mm thick S-glass/phenolic panels.

fibre breakage took place at different stages of impact loading and could be identified easily as demonstrated in Section 5.4.1. Consequently, the impact force-time curves from either large or small plates could be used for this purpose. In addition, the quasi-static force data may also be used. Figures 5.36–37(a–d) show impact force ratio data plotted against delamination area and IKE, respectively, for both large and small plates from all four laminates. Impact force ratio is defined here as initial damage

IBF5 11/22/2000 4:55 PM Page 177

Ratio of initial threshold force to max force

1.2 Force data of small plates Force data of large plates CAI data

1.0 0.8 0.6 0.4 0.2 0.0 0

177

Compressive strength retention factor

Thick laminated woven roving GFRP plates

20 000 40 000 60 000 80 000 100 000 120 000

Ratio of initial threshold force to max force

1.2 Force data of small plates Force data of large plates CAI data

1.0 0.8 0.6 0.4 0.2 0.0 0

Compressive strength retention factor

Delamination area (mm2)

(c)

30 000 60 000 90 000 120 000 150 000 180 000 Delamination area (mm2)

(d) 5.36 (cont.)

threshold divided by the maximum force that occurred during the impact, thus a low value of this ratio indicates a high maximum force. Compressive strength retention factor is also plotted on the same graphs. Two features can be readily observed from these diagrams. One is that the small plate data are in reasonably good agreement with the large plate data. The other is that impact force ratio and strength retention factor are approximately equal to each other for the 10 mm thick E-glass/polyester and both Sglass/phenolic panels. For the large 25 mm thick E-glass/polyester panels, the strength retention ratio is about 35% below the force ratio over the whole spectrum of damage. This difference is believed to be associated with the existence of a substantial amount of localised matrix cracking which contributed to a weakening of the panels.

IBF5 11/22/2000 4:55 PM Page 178

Ratio of initial threshold force to max force

1.2 CAI data of large plates Force ratio data of large plates Force ratio data of small plates

1.0 0.8 0.6 0.4 0.2 0.0 0

200 400 600 800 1000 1200 1400 1600 1800 Incident kinetic energy, IKE (J)

(a)

Ratio of initial threshold force to max force

1.2 CAI data of large plates Force ratio data of large plates Force ratio data of small plates

1.0 0.8 0.6 0.4 0.2 0.0 0

(b)

Compressive strength retention factor

Impact behaviour of composite materials and structures

400

800

Compressive strength retention factor

178

1200 1600 2000 2400 2800

Incident kinetic energy, IKE (J)

5.37 (a) Comparison of force ratio with strength retention factor in terms of IKE for 10 mm thick E-glass/polyester panels. (b) Comparison of force ratio with strength retention factor in terms of IKE for 25 mm thick E-glass/polyester panels. (c) Comparison of force ratio with strength retention factor in terms of IKE for 14 mm thick S-glass/phenolic panels. (d) Comparison of force ratio with strength retention factor in terms of IKE for 19 mm thick S-glass/phenolic panels.

Alternatively, as mentioned earlier, impact damage tolerance can be assessed in terms of the residual far-field compressive strain rather than strength. Strain retention factor is compared with force ratio and strength retention factor, all plotted against IKE in Fig. 5.38(a–d). It is noticeable from these diagrams that the far-field compressive strain factors are close to, but generally higher than, the force ratios. Therefore to assume that the

IBF5 11/22/2000 4:55 PM Page 179

Ratio of initial threshold force to max force

1.2 CAI data of large plates Force ratio data of large plates Force ratio data of small plates

1.0 0.8 0.6 0.4 0.2 0.0 0

179

Compressive strength retention factor

Thick laminated woven roving GFRP plates

400 800 1200 1600 2000 2400 2800 3200 3600

Ratio of initial threshold force to max force

1.2 CAI data of large plates Force ratio data of large plates Force ratio data of small plates

1.0 0.8 0.6 0.4 0.2 0.0 0

Compressive strength retention factor

Incident kinetic energy, IKE (J)

(c)

400 800 1200 1600 2000 2400 2800 3200 3600 Incident kinetic energy, IKE (J)

(d) 5.37 (cont.)

two were equal would normally give a conservative estimate of the strain retention factor. It should be noted that these results are based on only one size of CAI specimen, but the failure is thought to be controlled by the local damage and should therefore be independent of panel size. This observation that impact force ratio can be used as an estimate of strength retention ratio could have significant practical implications such that damage tolerance could be assessed by using the impact response curves of small plates alone. It would be necessary neither to carry out impact tests on large plates, nor to resort to expensive CAI tests. In addition, the use of the impact force data can allow the development of a unified effective scheme to assess simultaneously both IDR for the development of composite materials and impact damage tolerance for structural

IBF5 11/22/2000 4:55 PM Page 180

Ratio of initial threshold force to max force

1.2 Force data CAI data Far-field strain data

1.0 0.8 0.6 0.4 0.2 0.0 0

300

600

900

1200

1500

Compressive strength retention factor

Impact behaviour of composite materials and structures

1800

Incident kinetic energy, IKE (J)

(a)

Ratio of initial threshold force to max force

1.2 Force data CAI data Far-field strain data

1.0 0.8 0.6 0.4 0.2 0.0 0

500

1000

1500

2000

2500

Compressive strength retention factor

180

3000

Incident kinetic energy, IKE (J)

(b)

5.38 (a) Comparison of force ratio with strength and far-field strain retention factors for 10 mm thick large E-glass/polyester panels. (b) Comparison of force ratio with strength and far-field strain retention factors for 25 mm thick large E-glass/polyester panels. (c) Comparison of force ratio with strength and far-field strain retention factors for 14 mm thick large S-glass/phenolic panels. (d) Comparison of force ratio with strength and far-field strain retention factors for 19 mm thick large S-glass/phenolic panels.

analysis and design. This could lead to a considerable further saving of both time and experimentation cost. Further verification on different laminate systems would, however, be necessary.

5.6

Conclusions

Thick woven roving glass fibre-reinforced laminated plates of various dimensions were subjected to low-velocity and high-energy impact as well

IBF5 11/22/2000 4:55 PM Page 181

Ratio of initial threshold force to max force

1.2 Force data CAI data Far-field strain data

1.0 0.8 0.6 0.4 0.2 0.0 0

600

1200

1800

2400

3000

181

Compressive strength retention factor

Thick laminated woven roving GFRP plates

3600

(c)

Ratio of initial threshold force to max force

1.2 Force data CAI data Far-field strain data

1.0 0.8 0.6 0.4 0.2 0.0 0

600

1200

1800

2400

3000

Compressive strength retention factor

Incident kinetic energy, IKE (J)

3600

Incident kinetic energy, IKE (J)

(d) 5.38 (cont.)

as quasi-static loading. Their resistance and tolerance to impact damage have been thoroughly investigated. Delamination and ply shear-out were found to be the dominant damage mechanisms. The effect of varying impact velocity, impactor mass, plate thickness and diameter on these damage mechanisms was examined by using the recorded impact response curves, ultrasonic C-scanning and cross-sectioning. The resistance to (i.e. the threshold force for) the onset of delamination was shown to be insensitive to a change in either impactor mass or plate diameter for both E-glass/polyester and S-glass/phenolic systems. It was also insensitive to a change in velocity for the E-glass/polyester system but increased modestly with increasing velocity for the S-glass/phenolic system. Moreover, it was very sensitive to plate thickness and increased significantly for the thicker plates of the same diameter. The impact resistance to ply

IBF5 11/22/2000 4:55 PM Page 182

182

Impact behaviour of composite materials and structures

shear-out was enhanced significantly by an increase of velocity for the E-glass/polyester and modestly for the S-glass/phenolic and was found to be significantly affected by the variation of geometry especially for the E-glass/polyester system. The plate diameter-related enhancement was due to a significant contribution from membrane stretching which diminished considerably with an increase of thickness. It was demonstrated that an examination of the impact resistance to delamination propagation posed a very complex picture, being dependent on the parameter used to characterise the intensity of the impact. When impact force was used to characterise the impact, the resistance to delamination propagation was found to be insensitive to plate thickness for the S-glass/phenolic system, but it was much more sensitive for the thicker Eglass/polyester plates of the same diameter.When IKE was used, the thicker large plates had greater delamination areas. It was also found that the impacts of similar IKE gave similar amounts of delamination, regardless of whether the energy came from a high mass at low velocity or low mass at high velocity. Also, delamination propagation was found to be the primary energy-absorbing mechanism. The residual compressive strength of impact-damaged panels was found to deteriorate very rapidly due to a combined effect of a change of local fibre curvature in the vicinity of the contact area and the presence of extensive delamination(s) once the initial threshold value of IKE or impact force was exceeded. It was not sensitive to either panel thickness or variations of impact velocity and impactor mass (at fixed IKE). In addition, strength suffered more than residual stiffness or residual far-field strains. It was also found that the characteristic failure mechanism of the damaged panels in the compression tests was different from that of the intact. The damaged panels failed by a combination of local delamination buckling and kink band formation, while a near-end compression failure with a shear mechanism was found for the intact panels. The use of compressive strength retention factor along with IKE and delamination area in conventional impact damage tolerance assessment was reasonably satisfactory but was also complex, time-consuming and costly. In addition, strength retention factor, IKE and delamination area were all shown to have respective limitations. The novel alternative based on force data was demonstrated to be useful for the assessment of impact damage tolerance through direct comparisons with the conventional method in terms of both strength and far-field strain retention factors. In particular, it appeared possible to obtain a reasonable prediction of compression after impact performance using data from only impact tests on plates of an arbitrary size. If the composite system is not very strain rate sensitive, it should be possible to use quasi-static rather than impact loading. In addition, the use of impact force data can allow the development of a unified effective

IBF5 11/22/2000 4:55 PM Page 183

Thick laminated woven roving GFRP plates

183

scheme to assess simultaneously both IDR for the development of composite materials and impact damage tolerance for structural analysis and design. This could result in a considerable saving of both time and experimentation cost before resorting to the expensive conventional method.

Acknowledgements The authors are grateful to Professor G A O Davies of Imperial College (IC) for extensive and valuable interaction. The authors are also grateful to Mr J Churchward (Aeronautics of IC) for assistance and to Dr J M Hodgkinson and Mr E W Godwin (the Centre for Composite Materials of IC) for their generous assistance and discussions in the testing of mechanical properties and C-scanning. The work described here was supported by the Ministry of Defence.

References 1 Anon, ‘Joint airworthiness requirements’, JAR 25, ACJ 25.603, 1994. 2 Johnson A F and Marchant A, ‘Design and analysis of composite structures’, in Polymers and Polymer Composites in Construction, ed L C Hollaway, Thomas Telford, London, 1990. 3 Evans R E and Masters J E, ‘A new generation of epoxy composites for primary structural applications: materials and mechanics’, ASTM, 1985 STP 876 413–36. 4 Masters J E, ‘Correlation of impact and delamination resistance in interleafed laminates’, 6th ICCM/2nd ECCM, London, 3, 1987. 5 Mouritz A P, Leong K H and Herszberg I, ‘A review of the effect of stitching on the in-plane mechanical properties of fibre-reinforced polymer composites’, Composites, 1997 28A 979–91. 6 Freitas G, Magee C, Dardzinski P and Fusco T, ‘Fiber insertion process for improved damage tolerance in aircraft laminates’, J Advan Mater, 1994 36. 7 Dorey G, ‘Damage tolerance and damage assessment in advanced composites’, in Advanced Composites, ed I K Partridge, Elseview Applied Science Pub, Chapter 11, 369–98, 1989. 8 Abrate S, ‘Impact on laminated composite materials’, Appl Mech Rev, 1991 44(4) 155–90. 9 Cantwell W J and Morton J, ‘The impact resistance of composite materials – a review’, Composites, 1991 22(5) 347–62. 10 Abrate S, ‘Impact on laminated composites – recent advances’, Appl Mech Rev, 1994 47(11) 517–44. 11 Cantwell W J, Curtis P T and Morton J, ‘Post impact fatigue performance of carbon fibre laminates with non woven and mixed woven layers’, Composites, 1983 14 301–5. 12 Vedula M and Koczak M J, ‘Impact resistance of cross-plied polyphenylene sulfide composites’, J Thermoplastic Composite Materials, 1989 2 154–63. 13 Zhou G and Davies G A O, ‘Experimental determination of interlaminar shear strengths of thick GFRPs’, 6th ECCM – CTS2, Hamburg, 1994.

IBF5 11/22/2000 4:55 PM Page 184

184

Impact behaviour of composite materials and structures

14 Zhou G and Davies G A O, ‘Characterisation of thick glass woven roving/ polyester laminates: Part I, tension, compression and shear’, Composites, 1995 26(8) 579–86. 15 Zhou G and Davies G A O, ‘Characterisation of thick glass woven roving/ polyester laminates: Part II, flexure and statistical consideration’, Composites, 1995 26(8) 587–96. 16 Hodgkinson J M, Ayache S and Matthews F L, ‘In-plane and out-of-plane property measurements on thick woven glass/polyester laminates’, 5th ECCMCTS 1, Amsterdam, 1992. 17 Zhou G, ‘Static behaviour and damage of thick composite plates’, Composite Struct, 1996 36(1–2) 12–33. 18 Davies G A O, Hitchings D and Zhou G, ‘Impact damage and residual strengths of woven fabric glass/polyester laminates’, Composites, 1996 27A(8) 1147–56. 19 Zhou G and Davies G A O, ‘Impact response of thick glass fibre reinforced polyester laminates’, Int J of Impact Eng, 1995 16(3) 357–74. 20 Zhou G, ‘Damage mechanisms in composite laminates impacted by a flat-ended impactor’, Composites Sci and Tech, 1995 54(3) 267–73. 21 Zhou G, ‘Prediction of Impact damage thresholds in glass fibre reinforced laminates’, Composite Struct, 1995 31 185–93. 22 Sjoblom P, ‘Simple design approach against low-velocity impact damage’, 32nd Int SAMPE Symp, Anaheim, 529–39, 1987. 23 Lagace P A, Williamson J E, Tsang P H W, Wolf E and Thomas S, ‘The use of force as a (impact) damage resistance parameter’, 7th Tech Conf of American Society of Composites, PA, 1992. 24 Jakson W C and Poe Jr. C C, ‘The use of impact force as a scale parameter for the impact response of composite laminates’, J Composite Technol Res, 1993 15 282–9. 25 Lesser A J and Filippov A G, ‘Mechanisms governing the damage resistance of laminated composites subjected to low-velocity impacts’, Int J Damage Mech, 1994 3 408–32. 26 Rydin R W, Bushman M B and Karbhari V M, ‘The influence of velocity in low-velocity impact testing of composites using the drop weight impact tower’, J Reinforced Plastics Composites, 1995 14 113–27. 27 Delfosse D, Poursartip A, Coxon B R and Dost E F, ‘Non-penetrating impact behaviour of CFRP at low and intermediate velocities’, ASTM, 1995 STP 1230 333–50. 28 Liu D, ‘Impact induced delamination – a view of bending stiffness mismatching’, J Composite Mater, 1988 22 674–92. 29 Hull D and Shi Y B, ‘Damage mechanism characterization in composite damage tolerance investigations’, Composite Struct, 1993 23 99–120. 30 Davies G A O and Zhang X, ‘Impact damage prediction in carbon composite structures’, Int J Impact Eng, 1995 15(3) 357–74. 31 Zhou G, ‘Impact velocity effect on damage in laminated composites’, 7th ECCM – High Performance Composites, London, 1, 1996. 32 Zhou G, Impact damage resistance of thick glass woven roving fibre reinforced composites – geometric effects, Int Conf on Advanced Materials, Beijing, 1996. 33 Morton J, ‘Scaling of impact-loaded carbon fiber composites’, AIAA Journal, 1988 26 989–94.

IBF5 11/22/2000 4:55 PM Page 185

Thick laminated woven roving GFRP plates

185

34 Kwon Y S and Sankar B V, ‘Indentation-flexure and low-velocity impact damage in graphite epoxy laminates’, J Composite Technol Res, 1993 15 101. 35 Lee S W R and Sun C T, ‘Dynamic penetration of graphite/epoxy laminates impacted by a blunted-ended projectile’, Composites Sci Technol, 1993 49 369–80. 36 Zhou G, Lloyd J C and McGuirk, J J, ‘Experimental evaluation of geometric factors affecting damage mechanisms in carbon/epoxy plates’, accepted by Composites Part A. 37 Zhou G, ‘Characteristics of impact energy absorption during damage development in laminated composites’, 4th Int Conf Deformation and Fracture of Composites, Manchester, 1997. 38 Zhou G, ‘Compressive behaviour of large undamaged and damaged thick composite panels’, Composite Struct, 1997 38(1–4) 589–97. 39 Horton R E and McCarty J E, ‘Damage tolerance of composites’, in Engineering Materials Handbook, T J Reinhart, Ohio, USA, 1, ASM, 1987. 40 Zhou G and Davies G A O, ‘Damage tolerance of thick glass fibre reinforced laminate structures subjected to low-velocity impact’, ASME-WAM, Chicago, MD-vol. 51, 1994. 41 Zhou G, ‘Effect of impact damage on residual compressive strength of GFRP laminates’, Composite Struct, 1996 35(2) 171–81. 42 Lagace P A, ‘On delamination failures in composite laminates’, in Composite Structures Testing, Analysis, and Design, eds J N Reddy and A V K Murty, New Delhi, Spinger-Verlag/Narosa Publications, 1992. 43 Manders P W and Harris W C, ‘A parametric study of composite performance in compression-after-impact testing’, SAMPE J, 1986 Nov. 47–51. 44 Vedula M, Lee W M, Benedetto E E and Groleau M R, ‘Screening test for compression after impact strength evaluation of composites’, 7th Tech Conf of American Society of Composites, PA, 1992. 45 Ishikawa T, Sugimoto S, Matsushima M and Hayashi Y, ‘Some experimental findings in compression-after-impact (CAI) tests of CF/PEEK (APC-2) and conventional CF/epoxy flat plates’, Composites Sci Technol, 1995 55 349–63. 46 Wardle B L and Lagace P A, ‘On the use of dent depth as an impact damage metric for thin composite structures’, J Reinforced Plastics Composites, 1997 16 1093–110. 47 Lameris J, BRITE-EURAM 3159 CR, National Aerospace Lab., The Netherlands, 1993. 48 Xiong Y and Poon C, ‘Prediction of residual compressive strength of impactdamaged composite laminates’, 9th ICCM, Madrid, 1993. 49 Pintado P, Vogler T J and Morton J, ‘Impact damage tolerance of thick graphiteepoxy composite material systems’, 8th ICCM, Hawaii, 1993. 50 Zhou G, ‘The use of experimentally-determined impact force as a damage measure in impact damage resistance and tolerance of composite structures’, Composite Struct, 1998 42(4) 375–82. 51 Zhou G, ‘Replacing residual compressive strengths by impact force data in the damage tolerance assessment of composite structures’, 8th ECCM, Naples, 1998. © Crown copyright 2000. Published with the permission of the Defence Evaluation and Research Agency on behalf of the Controller of HMSO.

IBF6 11/22/2000 6:34 PM Page 186

6 Elastic impact stress analysis of composite plates and cylinders S R SWANSON

6.1

Introduction

Impact is a complicated topic, involving both structural and material response and damage formation. However, the stress analysis of the impact is fundamental to understanding the entire problem. The analysis can take many forms, such as nonlinear numerical analysis or linear analysis with closed form solutions, as some examples show in Chapter 7. In the following, the fundamentals of primarily linear analysis of laminated plates and cylinders will be discussed, and examples of work in the literature on these topics will be presented.

6.2

Impact regimes

It is possible to classify impact into various categories, depending on the characteristics of the impactor and target. A major category is those impact events where through-the-thickness stress wave effects are important. In impact of a structure by a foreign body, a through-the-thickness compressive stress wave will be initiated. In some circumstances, this wave will be reflected as a tensile wave from the free surface on the back side, introducing the possibility of through-the-thickness tensile failure.1 Calculation of the characteristics of the through-the-thickness wave may in general be difficult and require numerical treatment, however some limit cases will be informative. If the impactor is large with respect to the thickness of the target and both the target and impactor have parallel surfaces, the stressstate is that associated with one dimensional strain, and the wave speed will be in the order of c = Q33 r

and s = -aQ33v c

[6.1]

where Q33 is the diagonal term of the three-dimensional stress–strain matrix for the composite in the through-the-thickness direction, a is a constant depending on the properties of the impactor and target, and v is the 186

IBF6 11/22/2000 6:34 PM Page 187

Elastic impact stress analysis of composite plates and cylinders

187

impact velocity. For many composites Q33 is not greatly different from the through the thickness modulus, which is also comparable to the in-plane modulus E22 in a direction transverse to the fibers. The magnitude of the stress wave depends linearly on the ratio of the impactor velocity to the wave speed. Substituting values shows that through-the-thickness stress waves will be important in ballistic events and many simulations such as air-gun driven impactors, but are not likely to be significant in dropweight impacts. However the impactor and target surfaces are often not parallel, and the impactor may not be large. In this case the indentation of the impactor into the target will smear out the transverse wave so that detailed numerical computation is required, e.g. as carried out by Joshi and Sun.2 For those impact events in which through-the-thickness stress waves are not considered to be important, a further division is possible. Events in which the distributed mass of the target is negligible relative to the impactor mass are termed quasi-static. This assumption greatly simplifies the analysis of the impact event, as the target can then be characterised only by its static stiffness properties. Impact events that do not fall into this category will respond in a much more complex fashion, that can be considered to be a synthesis of a large number of natural frequencies and mode shapes of the target. Because of the simplicity of the quasi-static analysis, it is important to be able to determine when this assumption is applicable, and this topic is addressed further in the following. Impacts in which the quasistatic assumption is assumed to hold are sometimes termed ‘low-velocity’ impacts, but this is questionable terminology as the division between the structural dynamic and the quasi-static regimes is completely independent of the impact velocity itself, but depends on other characteristics of the impact.

6.3

Analysis of impact

The analysis of the stresses and strains resulting from impacts on laminated plates, beams, and cylinders will be discussed in this section, for impacts in which the structural dynamics of the target are important, but through-thethickness stress waves are not. The local deformations associated with the indentation of the target are first described, followed by several schemes for solving the dynamics problem of impact on plates and cylinders.

6.3.1 Contact stiffness and deformation The projectile indents the target to a greater or lesser extent, and this additional compliance influences the response. The usual treatment follows that of Sun et al.,3–5 who adapted the usual Hertz solution for contact between

IBF6 11/22/2000 6:34 PM Page 188

188

Impact behaviour of composite materials and structures

two bodies to the impact problem. The contact force is assumed to be related to the contact indentation by the following equation F = ka 3 2

with

k=

4 Rs E22 3

[6.2]

where F is the total contact force on the target, a is the local indentation, Rs is the radius of the spherical impactor, and E22 is the transverse Young’s modulus of the laminated target. The contact force is then related to the motion of the projectile by assuming rigid body dynamics for the projectile, that is F = -mü

[6.3]

where m is the mass and u is the displacement of the projectile. The relationship between the local indentation, projectile displacement and plate displacement at impact center is expressed by a(t ) = u(t ) - w(t , x, h)

[6.4]

where ξ and h give the location of the center of impact.

6.3.2 Structural dynamics of impact for plates The analysis of static and dynamic loadings of laminated composite plates has seen considerable development recently. Lekhnitskii,6 and Whitney and Leissa7 have presented analyses with infinite transverse rigidity while Whitney and Pagano8 have presented a theory including transverse shear deformations. The dynamic problems considered involved vibration of plates. Sun and Chattopadhyay3 and Dobyns9 used the plate equations developed by Whitney and Pagano8 to analyse a simply supported orthotropic plate subject to center impact. Dobyns assumed that the lateral force history was known, while Sun and Chattopadhyay noted that in impact by a foreign body, the force history must be computed as part of the problem. Thus Sun and Chattopadhyay integrated the equations of motion numerically. Birman and Bert10 obtained a closed-form solution for laminated angle-ply simply supported plates subject to blast loading, which again considers that the force history is known. Solutions of the impact problem for plates have been displayed in the literature, that solve for the force history as well as the resulting stresses, strains, and deformation. An analytical solution is available for plates with simply supported boundary conditions, using Fourier series expansion techniques combined with Laplace transform techniques. However, the contact stiffness must be linearised to permit this analytical solution. The solution for other boundary conditions has been addressed using Ritz solutions,

IBF6 11/22/2000 6:34 PM Page 189

Elastic impact stress analysis of composite plates and cylinders

189

combined with numerical time integration. These analysis techniques are illustrated in the following.

6.3.2.1 Equations of motion for plates The plate equations of motion developed by Whitney and Pagano8 reduced to specially orthotropic form (Bij = 0, A16 = A26 = D16 = D26 = 0), are given by Dobyns9 as D11

3 2 ∂2 yx ∂2 yx ∂ 2 yy Ê y + ∂w ˆ = rh ∂ y x ( ) + D + D + D kA 12 66 55 66 x Ë ∂x ∂ y ∂x ¯ 12 ∂t 2 ∂x 2 ∂ y2

( D12 + D66 ) [6.5] kA55

∂2 yx ∂ 2 yy ∂ 2 yy ∂w ˆ rh3 ∂ 2 yy + D66 + D22 - kA44 Ê y y + = 2 2 Ë ∂x ∂ y ∂y ¯ 12 ∂t 2 ∂x ∂y

2 ∂2w ˆ ∂2w Ê ∂y x ∂ w ˆ Ê ∂yy ( ) + + kA + + q x y t h , , = r 44 Ë ∂x Ë ∂y ∂x 2 ¯ ∂ y2 ¯ ∂t 2

[6.5]

where Dij and Aij are the stiffnesses, as defined by Whitney and Pagano,8 h is the plate thickness, t is time, r is material density, w is the plate displacement in the z direction at the plate midplane, yx and yy are the rotations in the x and y directions and k is a shear correction factor that is often taken to be p2/12.

6.3.2.2 Solution for simply-supported boundary conditions For plates with boundary conditions of simple support on all four edges, it is possible to use standard Fourier series expansion techniques to determine the response. Christoforou and Swanson11,12 have shown that it is possible to obtain an analytical solution to the impact problem by using Laplace transform techniques, if the nonlinear contact indentation is approximated by a linearised version. The solution is based on expansions of the loads, displacements, and rotations in Fourier series which satisfy the end boundary conditions of simple support. Each expression is assumed to be separable into a function of time and a function of position. Furthermore, following Bert and Birman,13 by neglecting in-plane and rotary inertia the problem becomes a second order ordinary differential equation in time for the Fourier coefficients of the lateral deflection. In the case of impact, the impact force is computed from the deceleration of the impactor mass. This involves the equilibrium equation between the impactor and the plate during contact. For a given dynamic load, solutions of the governing equations [6.5] that satisfy the boundary conditions of simple support are given by

IBF6 11/22/2000 6:34 PM Page 190

190

Impact behaviour of composite materials and structures F(t)/(uv)

x

h

U v

b

¡

a

y

6.1 Illustration of plate geometry used for analysis of simply supported plates.

yx = Â Â Amn (t ) cos m

n

yy = Â Â Bmn (t ) sin m

n

w = Â Â Wmn (t ) sin m

n

mpx npy sin a b

mpx npy cos a b

[6.6]

mpx npy sin a b

with the load function represented by q(x, y, t ) =

Â ÂQ

mn

m

n

(t ) sin

mpx npy sin a b

[6.7]

Equations [6.6] and [6.7] are the Fourier series representation of the rotations, lateral displacement and load. The coordinate system and geometry are illustrated in Fig. 6.1. The terms of the Fourier series representation for a uniform load over the rectangular area u, v with center at z, h is shown in Fig. 6.1 are Dobyns’.9 Qmn (t ) =

16F (t ) mpz nph mpu npv sin sin sin sin 2 a b 2a 2b p mn uv

[6.8]

Following the results of Bert and Chen,14 rotary inertia effects are neglected. Thus substituting equations [6.6] and [6.7] into equation [6.5]

IBF6 11/22/2000 6:34 PM Page 191

Elastic impact stress analysis of composite plates and cylinders

191

results in the independent sets of three equations for each set of modal parameters m and n: ÈC11 C12 C13 ˘ Ï Amn (t ) ¸ Ô Ô ÍC C 22 C 23 ˙ Ì Bmn (t ) ˝ = Í 12 ˙Ô ÍÎC13 C 23 C33 ˙˚ ÓWmn (t ) Ô˛

0 Ï ¸ Ô Ô 0 Ì ˝ ÔÓQ (t ) - rhW Ô ˙˙ mn mn (t ) ˛

[6.9]

where the elements of the symmetric matrix Cij are 2

2

mp ˆ np C11 = D11 Ê + D66 Ê ˆ + kA55 Ë a ¯ Ë b¯ mp ˆ Ê np ˆ C12 = (D12 + D66 )Ê Ë a ¯Ë b ¯ mp ˆ C13 = kA55 Ê Ë a ¯ 2

2

mp ˆ np C 22 = D66 Ê + D22 Ê ˆ + kA44 Ë a ¯ Ë b¯ np C 23 = kA44 Ê ˆ Ë b¯ 2

mp ˆ Ê np ˆ C33 = kA55 Ê + kA44 Ë b¯ Ë a ¯

[6.10]

2

Following Bert and Birman,13 equation [6.9] can be reduced to a single differential equation by the following transformation: Amn (t ) = K A Wmn (t ); Bmn (t ) = K BWmn (t )

[6.11]

where KA = KB =

C12C 23 - C13C 22 2

C11C 22 - C12 C12C13 - C11C 23 C11C 22 - C12

[6.12]

2

Substitution of equation [6.8] reduces the set [6.9] into the following: ab F (t ) 2 ˙˙ mn (t ) + w mn W Wmn (t ) = Pmn uv m1

[6.13]

C13 K A + C 23 K B + C33 are the squared fundamental frequenrh cies of the plate, and m1 is its mass. where w 2mn =

IBF6 11/22/2000 6:34 PM Page 192

192

Impact behaviour of composite materials and structures

For zero initial displacement and velocity, the solution of equation [6.13] is obtained using the convolution integral: Wmn (t )

Pmn ab uvm1w mn

t

Ú F (t) sin w 0

mn

(t - t )dt

[6.14]

The deflection of the plate at any point is given by w(x, y, t ) =

ab uvm1

Pmn

ÂÂw m

n

sin

mn

mpx npy t sin F (t ) sin w mn (t - t )dt a b Ú0

[6.15]

The response of a plate to impact by a foreign object may be computed from the transient response, equation [6.15], by computing the impact force from the deceleration of the impactor mass. The integral equilibrium equation between the impactor and the plate during contact is given by a b 1 wÊ , , t ˆ = V0 t Ë2 2 ¯ m2

t

Ú F ( t)(t - t)dt 0

F (t ) K2

[6.16]

Êa b ˆ where V0 is the initial velocity of the impactor with mass m2, w , , t is Ë2 2 ¯ the lateral deflection of the plate evaluated at the impact point as a function of time, F(t) is the impact force and K2 is the linearised contact area stiffness. As mentioned above, the contact problem must be linearised in order to be treated analytically using the present approach. This involves both replacing the nonlinear contact stiffness with an appropriate linearised value, as well as approximating the time varying contact area by a constant area. Combining equations [6.15] and [6.16] yields 1 t F (t ) F (t )(t - t )dt Ú 0 m2 K2 ab Pmn mp np t = sin sin F (t ) sin w mn (t - t )dt Â Â uv m1 m n w mn 2 2 Ú0

V0 t -

[6.17]

Taking the Laplace transform of equation [6.17] and after some rearranging yields F (s) =

m2 V0 m2 2 abm2 1+ s + K2 uvm1

mp np s2 Pmn sin sin Â Â 2 2 2 s 2 + w mn m n

[6.18]

Using the inverse theorem for Laplace transforms and following the procedure of Christoforou and Swanson11,12 yields

IBF6 11/22/2000 6:34 PM Page 193

Elastic impact stress analysis of composite plates and cylinders

193

0.0010 75 terms

Strain Ep X

0.0008

51 terms 25 terms

0.0006

0.0004

0.0002

0.0000 0

100

200

300

Time (ms)

6.2 Convergence of solution for strain behind the impact point. (After Christoforou and Swanson12.)

F (t ) =

Â F sinw t j

[6.19]

j

j

where ωj are the response frequencies or poles of expression [6.18] and Fj =

m2 V0 È m2 ab m2 w jÍ + Î K 2 uv m1

˘ w 2mn mp np sin Pmn sin ˙ Â Â 2 2 2 (w 2mn - w 2j ) ˚ m n

[6.20]

The impact response can be determined by combining the Laplace transforms of equations [6.14] and [6.19] Wmn (s) =

Pmn ab F jw j Â 2 2 m1uv j (s + w mn )(s 2 + w 2j )

[6.21]

Inverting as above gives Wmn (t ) =

Pmn ab Fj (w j sin w mnt - w mn sin w j t ) Â m1uv j w mn (w 2j - w 2mn )

[6.22]

The deflection and strain at any point can then be obtained by substituting [6.22] into equations [6.11] and [6.6]. An illustration of the convergence of the solution for strain is shown in Fig. 6.2, taken from Christoforou and Swanson.12 Further results will be shown subsequently.

IBF6 11/22/2000 6:34 PM Page 194

194

Impact behaviour of composite materials and structures

6.3.2.3 Plates with other boundary conditions As is the case with the static analysis of plates, boundary conditions other than simple support require techniques other than the double Fourier series expansion. An approximate but general technique is to use a Ritz analysis, combined with a numerical integration of the time variable. It is possible to include the nonlinear contact stiffness with this approach.The analysis shown here has been displayed by Cairns and Lagace15 and Qian and Swanson.16 The analysis is based on Lagrange’s equation of motion with the Lagrangian function L = T - V: d ∂L ∂L [6.23] =0 dt ∂ x ∂ x where x is the modal amplitude. Consider a laminated plate under dynamic lateral loading. The potential energy is given as V=

T 1 1 T k] [ D][k]dA + Ú Ú [ g ] [ A][ g ]dA - Ú Ú p(t , x, y) w(t , x, y)dA [ Ú Ú A 2 A 2 A [6.24]

where the first two terms are bending and transverse shear strain energy, respectively, and the third is the work done by the lateral load. The kinetic energy of the plate is given by T=

rh 2 w˙ (t , x, y) dA. Ú Ú A 2

[6.25]

Here again the in-plane and rotary inertia effects have been neglected, as suggested by Birman and Bert10 and Dobyns.9 The problem considered in Qian and Swanson16 has clamped boundary conditions on two opposing edges of the plate and free boundaries on the other two edges to correspond with experiments. The procedure followed is based on choosing two series of functions, or ‘mode shapes’, which satisfy the boundary conditions and give suitable expressions for deflection curves in x and y directions separately. The assumed deformed shape of the rectangular plate is then taken as a product of these functions. Therefore the series approximation for the planar rotations and transverse displacement can be taken as a (t , x, y) =

ÂÂA

(t ) X m¢ ( x)Yn ( y)

[6.26]

ÂÂB

(t ) X m ( x)Yn¢( y)

[6.27]

(t ) X m ( x)Yn ( y)

[6.28]

mn

m

b (t , x, y) =

mn

m

w(t , x, y) =

n

n

Â ÂC m

n

mn

IBF6 11/22/2000 6:34 PM Page 195

Elastic impact stress analysis of composite plates and cylinders

195

where Amn, Bmn, and Cmn are the modal amplitudes of the plate and are to be determined. Substituting the assumed mode shapes in the expressions for potential and kinetic energy, and then using Lagrange’s equation [6.23] gives three sets of equations with unknowns Amn, Bmn, and Cmn. Substituting Amn, Bmn in terms of Cmn yields a system of second order ordinary differential equations for the modal amplitudes Cmn

[ S ]{C˙˙} + [T ]{C} = {P}

[6.29]

In Qian and Swanson16 the assumed mode shapes were taken as beam functions, which are solutions for mode shapes of beams under the appropriate boundary conditions.17 The beam functions are orthogonal, permitting expansion of the load in terms of these functions. This expansion is of the form p(t , x, y) =

ÂÂ p

mn

m

(t ) X m ( x)Yn ( y)

[6.30]

n

with pmn (t ) =

ÚÚ

A

p(t , x, y)X m (x)Yn ( y)dxdy

ÚÚ

A

X m2 (x)Yn2 ( y)dxdy

[6.31]

The {P} in the right hand of equation [6.29] is a force term, and each component comes from taking the derivative of the work done by the lateral load to the relative mode amplitude, that is Pmn =

∂W = pmn Ú Ú X m2 (x)Yn2 ( y)dxdy A ∂ C mn

[6.32]

The contact force is assumed to be related to the contact indentation using the relations given previously above. The contact pressure p(t, x, y) is simply taken as the uniform distribution of the total contact force F(t) over a square area Ac. This area is determined by

[

Ac = p Rs2 - (Rs - a )

2

]

[6.33]

The equations above along with the contact laws were solved simultaneously. Due to the nonlinearity of the contact deformation relationship, the above equations were solved numerically, using the Newmark method with b = 1/4, which gives an unconditionally stable solution. A typical comparison of calculation with experimentally measured strain is shown in Fig. 6.3, taken from Qian and Swanson.16 It can be seen that the agreement is very reasonable.

IBF6 11/22/2000 6:34 PM Page 196

196

Impact behaviour of composite materials and structures 7000 Experiment Analysis

6000

e x at A (microstrain)

5000 4000 3000 2000 1000 0 -1000

0

200

400

600

800

1000

Time (ms)

6.3 Comparison of Ritz analysis with experiment for strain in impact of plate. (After Qian and Swanson16.)

6.3.2.4 Comparison of solution techniques It is possible to apply the second solution technique described above, that of using a Ritz analysis in conjunction with numerical time integration, to the problem of impact of a plate with simply-supported boundary conditions, and thus permit a comparison with the first technique, which used Laplace transforms. This comparison of solution techniques has been carried out by Qian and Swanson,18 and is reviewed in the following. The basic problem chosen to illustrate the techniques is based on geometry and properties used previously by Sun and Chen,19 and consists of center impact of a simply supported square composite plate. The material properties and geometry are given in Table 6.1. Analyses were also carried out on plates with two and four times the standard thickness. As mentioned above, the Rayleigh–Ritz technique used the Newmark method for time integration, and incorporated the nonlinear contact law with the contact area changing at each time step. The analytical solution with Laplace transforms was restricted to a linearisation of the contact law, with a constant contact area throughout the solution. The results of the computations presented in Qian and Swanson18 show the importance of using a sufficiently small time step in the numerical time integration used with the Ritz solution, and a time step of 0.1 ms was

IBF6 11/22/2000 6:34 PM Page 197

Elastic impact stress analysis of composite plates and cylinders

197

Table 6.1. Data for the plate impact problem used for comparison Plate:

[0/90/0/90/0]s T300/934 carbon/epoxy plate, simply supported plate size: 200 mm by 200 mm plate thickness: (a) h = 2.69 mm (0.269 mm/layer) (b) 2 h = 5.38 mm (0.538 mm/layer) (c) 4 h = 10.76 mm (1.076 mm/layer) E22 = 7.9 GPa E11 = 120 GPa υ12 = υ23 = 0.30 G12 = G23 = 5.5 GPa r = 1580 kg m-3

Impactor: 12.7 mm diameter steel ball, r = 7960 kg m-3 mass = 8.537 g, impact velocity = 3.0 m s-1 Hertzian contact stiffness kh = 8.394 ¥ 108 N m-3/2 Linearised contact stiffness kl = 5.866 ¥ 106 N m-1 Source: Qian and Swanson.18

employed. Comparisons of the contact force, and target displacement and strain between the two solution techniques were in general good. When the linearised contact law was used with both techniques, the agreement between the two methods was excellent. Using the nonlinear contact law with the Ritz technique and the linearised contact law with the Fourier series expansion technique gives results as shown in Fig. 6.4. Computations for the nominal plate thickness of the example problem showed reasonable agreement, but plates with thickness of two and four times this showed less good agreement, indicating the relative error involved in the linearisation of the contact law. A comparison with the dynamic finite element calculations of Sun and Chen19 is shown in Fig. 6.5, which shows reasonable agreement for displacement.

6.3.3 Impact of a cylinder Ramkumar and Thakar20 have presented an analysis of the dynamic response of curved laminated plates subjected to low-velocity impact. They use Donnell’s equations for thin shells, assume that the impact force varies linearly with time, and follow Dobyns’s9 procedure to solve for the response. Vinson and Chou21 presented a double Fourier series solution of an orthotropic cylindrical shell subjected to a lateral concentrated static load. A solution technique for impact of laminated cylinders has been presented by Christoforou and Swanson,11 and a comparison with experimental data has been given by Swanson et al.22 The solution uses Fourier series expansions and Laplace transform techniques, and requires linearisation of the contact stiffness. A review of this approach is given in the following.

IBF6 11/22/2000 6:34 PM Page 198

198

Impact behaviour of composite materials and structures 1400 Analytical solution

1200

Rayleigh–Ritz solution

Strain ex (microstrain)

1000 h 800

600

400 2h 200 0

4h

-200 0

50

100

150

200

250

Time (ms)

6.4 Comparison of Fourier series–Laplace transform solution with Ritz solution with numerical time integration, for strain behind the impact point in plate impact. (After Qian and Swanson18.)

This analysis is based on an expansion of the load, displacements, and rotations in a double Fourier series that satisfies the end boundary conditions of simple support. Each expansion is assumed to be separable into a function of time and a function of position. Furthermore, by neglecting in-plane and rotary inertia the problem becomes a second order ordinary differential equation in time for the Fourier coefficients of the radial deflection. On the right hand side of the differential equation are the Fourier coefficients of the loading function. For a given loading impulse the solution can be found by invoking the convolution integral. In the case of impact, the impact force is computed from the deceleration of the impactor mass.This basically involves the equilibrium equation between the impactor and the shell during contact. By neglecting the local contact area deformation, the resulting integral equation can be solved algebraically for the impact force by using Laplace transforms. The expressions for the impact response and force in time are obtained by using the inversion theorem of the Laplace transforms in conjunction with the Cauchy residue theorem.

IBF6 11/22/2000 6:34 PM Page 199

Elastic impact stress analysis of composite plates and cylinders

199

0.45 0.40

Plate centre displacement (mm)

0.35 0.30 0.25 0.20 0.15 0.10 Rayleigh–Ritz solution 0.05

Finite element solution6

0.00 0

400

800

1200

1600

Time (ms)

6.5 Comparison of Ritz solution with numerical time integration with dynamic finite solution,19 for center displacement in plate impact. (After Qian and Swanson18.)

6.3.3.1 Governing equations for cylinders Love’s equations of motion for a circular cylindrical shell of length L, radius R, and thickness h subject to lateral loads generalised to include shear deformations, combined with the constitutive equations for a specially orthotropic material, result in the equations given by Bert and Birman13 as: A66 A12 + A66 ˆ A12 u,qq + Ê v, xq + w, x = rhu˙˙ 2 Ë ¯ R R R Ê A12 + A66 ˆ u + A v + A22 v - A44 v 66 , xx ,qq Ë ¯ , xq R R2 R2 A22 + A44 ˆ A44 w ,q + +Ê bq = rhv˙˙ 2 Ë ¯ R R A12 A44 + A22 ˆ A44 A22 u, x - Ê v,q + A55 w , xx + 2 w ,qq - 2 w 2 Ë ¯ R R R R A44 ˙˙ + A55b x,x + bq,q + q( x, q, t ) = rhw R A11u, xx +

IBF6 11/22/2000 6:34 PM Page 200

200

Impact behaviour of composite materials and structures F z, w A l1

x, u

q, v bx

bq

l

Loaded area

A

2f1 t

Support conditions v = w = bq = 0 Nx = Mx = 0

R

Support conditions v = w = bq = 0 Nx = Mx = 0

6.6 Geometry of cylinder under transverse impact. (After Christoforou and Swanson11.)

D66 bx,qq - A55bx R2 D12 + D66 ˆ rh3 ˙˙ +Ê bq , xq = bx Ë ¯ R 12 A44 A44 D12 + D66 ˆ vw ,q + Ê b + D66bq , xx Ë ¯ x, xq R R R

- A55 w, x + D11bx, xx +

+

[6.34]

D22 rh3 ˙˙ b A b = bq q , qq 44 q 12 R2

where u, v, and w are the displacements along the axial x axis, circumferential θ axis and radial z axis, bx and bθ are bending slopes in the x - z and θ - z planes, q is lateral pressure loading, r is the mass per unit area, Aij and Dij are the standard lamination theory constants, and t is time. A comma denotes differentiation with respect to the space variables, and a dot denotes differentiation with respect to time. The geometry considered is illustrated in Fig. 6.6. The constitutive equations for a specially orthotropic

IBF6 11/22/2000 6:34 PM Page 201

Elastic impact stress analysis of composite plates and cylinders

201

material (Bij = 0, A16 = A26 = D16 = D26 = 0) have been used to relate the stress, moment, and shear resultants to the midsurface strains e0i , curvatures ki, and average transverse shear strains gxz and gθz. 6.3.3.2 Solution procedure for impact of cylinders A closed-form solution of the governing equations is given as follows. The boundary conditions for a cylindrical shell that is freely supported (simplysupported without in-surface restraint) along its curved edges are given by N x ( 0, q, t ) = N x (L, q, t ) = M x ( 0, q, t ) = M x (L, q, t ) = 0 w( 0, q, t ) = w(L, q, t ) = v( 0, q, t ) = v(L, q, t ) = 0 bq ( 0, q, t ) = bq (L, q, t ) = 0

[6.35]

For a given load, the solution to equation [6.34] that satisfies the boundary conditions, equation [6.35], can be separated into a function of time and a function of position as follows: mpx L mpx v = Vmn (t ) sin nq sin L mpx w = Wmn (t ) cos nq sin L mpx b x = Tmn (t ) cos nq cos L mpx bq = Bmn (t ) sin nq sin L u = U mn (t ) cos nq cos

[6.36]

and the load as q(x, q, t ) = Qmn (t ) cos nq sin

mpx L

[6.37]

Equations [6.36] and [6.37] are the double Fourier series expansions of the displacements, rotations and load, which are similar to the static case developed by Vinson and Chou.21 The effects of in-surface and rotary inertia will be assumed to be negligible. Bert and Birman13 mentioned these effects to be negligible in dynamic stability studies, while Dobyns,9 by referring to Mindlin’s23 finding made the same assumptions for the impact response of orthotropic plates. Thus, substituting equations [6.36] and [6.37] into equation [6.34] and neglecting in-surface and rotary inertia yields the following set of equations:

IBF6 11/22/2000 6:34 PM Page 202

202

Impact behaviour of composite materials and structures

ÈC11 Í Í Í Í Í Î

C13 C14 C15 ˘ ÏU mn (t ) ¸ C 23 C 24 C 25 ˙ ÔVmn (t ) Ô ˙ ÔÔ Ô C33 C34 C35 ˙ ÌWmn (t ) ˝ = sym C 44 C 45 ˙ Ô Bmn (t ) Ô Ô ˙Ô C55 ˚ ÔÓTmn (t ) Ô˛ C12 C 22

0 Ï ¸ Ô Ô 0 ÔÔ Ô ˙˙ mn (t ) - Qmn (t ) Ô˝ ÌrhW Ô Ô 0 Ô Ô ÔÓ Ô˛ 0

[6.38]

where Cij are given as 2

mp ˆ n C11 = - A11 Ê - A66 Ê ˆ Ë L ¯ Ë R¯ C12 = C 21

2

C 25 = C52 = 0

Ê n ˆ Ê mp ˆ = ( A12 + A66 ) Ë R¯Ë L ¯

C13 = C31 =

A12 Ê mp ˆ R Ë L ¯

C34

C14 = C15 = 0

C35 2

C 22 C 23

2

mp ˆ n A44 = - A66 Ê - A22 Ê ˆ - 2 Ë L ¯ Ë R¯ R A22 + A44 ˆ Ê n ˆ = -Ê Ë ¯Ë R¯ R

C 24 = C 42 =

A44 R

C33

C 44

2

2

2

2

mp ˆ n A22 = - A55 Ê - A44 Ê ˆ - 2 Ë L ¯ Ë R¯ R n = C 43 = A44 Ê ˆ Ë R¯ mp ˆ = - A55 Ê Ë L ¯ mp ˆ n = - D66 Ê - D22 Ê ˆ - A44 Ë L ¯ Ë R¯

Ê n ˆ Ê mp ˆ C 45 = -(D66 + D12 ) Ë R¯Ë L ¯ 2

2

mp ˆ n C55 = - D11 Ê - D66 Ê ˆ - A55 Ë L ¯ Ë R¯ [6.39]

Bert and Birman13 obtained equations similar to [6.38] for a dynamic stability problem, and showed that they can be reduced to a single linear second-order differential equation by the following transformation: U mn (t ) = KU Wmn (t ); Vmn (t ) = K V Wmn (t ) Bmn (t ) = K BWmn (t ); Tmn (t ) = KT Wmn (t ) where the coefficients Ki are given by Bert and Birman13 as KU = S1 + S 2 K B + S3 KT ; K V = S 4 + S5 K B + S 6 KT K B = D B D ; KT = D T D D B = (C35 + C15 S1 + C 25 S 4 )(C 45 + C14 S3 + C 24 S 6 ) - (C34 + C14 S1 + C 24 S 4 )(C55 + C15 S3 + C 25 S 6 ) D T = (C 45 + C15 S 2 + C 25 S5 )(C34 + C14 S1 + C 24 S 4 ) - (C 44 + C14 S 2 + C 24 S5 )(C35 + C15 S1 + C 25 S 4 )

[6.40]

IBF6 11/22/2000 6:35 PM Page 203

Elastic impact stress analysis of composite plates and cylinders D = (C 44 + C14 S 2 + C 24 S5 )(C55 + C15 S3 + C 25 S 6 ) - (C 45 + C14 S3 + C 24 S 6 )(C 45 + C15 S 2 + C 25 S5 ) S1 = (C12C 23 - C 22C13 ) S S 2 = (C12C 24 - C 22C14 ) S S3 = (C12C 25 - C 22C15 ) S S 4 = (C12C13 - C11C 23 ) S S5 = (C12C14 - C11C 24 ) S S 6 = (C12C15 - C11C 25 ) S

203

[6.41]

S = C11C 22 - C122 Substituting equation [6.40] into the third equation in [6.38] yields ˙˙ mn (t ) + K mn Wmn (t ) = 1 Qmn (t ) W rh rh

[6.42]

where the coefficients Kmn are given by K mn = -(C13 KU + C 23 K V + C33 + C34 K B + C35 KT )

[6.43]

The terms of the Fourier series representation for the load, applied uniformly over a small rectangular area, 2Rf1(l2 - l1), at the center of the cylindrical shell (L/2, 0) are Qmn (t ) = Pmn

F (t ) 2Rf1 (l 2 - l1 )

[6.44]

where Pmn =

mp mp 8 (l 2 + l1 ) sin (l 2 - l1 ) sin nf1 sin 2 2L 2L mnp

[6.45]

Substituting equation [6.44] into [6.42] and rearranging yields Pmn pRL F (t ) 2 ˙˙ mn (t ) + w mn W Wmn (t ) = Rf1 (l 2 - l1 ) m1

[6.46]

where ω2mn = Kmn/rh are the fundamental frequencies of the shell and m1 is the mass of the shell. For zero initial displacement and velocity, the solution of equation [6.46] is Wmn (t ) =

Pmn pRL Rf1 (l 2 - l1 )m1w mn

t

Ú F (t) sin w 0

mn

(t - t )dt

[6.47]

Using equations [6.47] and [6.40] with [6.36] results in expressions for the deformations in a shell under transverse loading, for example, the transverse deflection at any point of the shell is given by

IBF6 11/22/2000 6:35 PM Page 204

204

Impact behaviour of composite materials and structures w(x, q, t ) =

pRL Rf1 (l 2 - l1 )m1 ¥

Ú

t

0

Pmn

ÂÂw m

n

mn

sin

mpx cos nq L

[6.48]

F (t ) sin w mn (t - t )dt

6.3.3.3 Impact loading The response of a cylindrical shell to impact loading may be computed from the transient response, equation [6.48], by computing the impact force from the deceleration of the impactor mass. This procedure parallels that given previously above for plates in Section 3.2.2. The solution for the coefficients of the radial displacement are finally given by Wmn (t ) =

Pmn pRL Rf1 (l 2 - l1 ) m1

Âw j

Fj (w j sin w mnt - w mn sin w j t ) 2 2 mn (w j - w mn )

[6.49]

and by combining the above equations, the deflection and strain histories at any point of the shell can be evaluated. A series of impact experiments with transverse impact of laminated cylinders has been reported by Swanson et al.22 A typical comparison of a calculation made using the theory described above with three replicate experiments is shown in Fig. 6.7. It is seen that the comparison of calculated and measured strain is very reasonable.

6.4

The quasi-static approximation

The quasi-static calculation procedure involves treating the impact problem as an equivalent static problem with a static load applied to the impact site. By treating the impact mass and structure as a simple spring-mass system (neglecting the mass of the structure in comparison to the impact mass), the impact force can be obtained from the formula F = vi K st M i

[6.50]

where vi and Mi are velocity and mass of the impactor, and Kst is the static stiffness of the structure. This formula can equivalently be obtained by equating the kinetic energy of the impactor to the strain energy of the structure. The stresses and strains in the structure are then obtained from the static solution, using the force from equation [6.50]. It is possible to include the Hertzian contact law as developed by Sun et al.4,5 for anisotropic materials, to refine the above procedure.

IBF6 11/22/2000 6:35 PM Page 205

Elastic impact stress analysis of composite plates and cylinders

205

1000

500

Strain (10E-06)

0

-500

C6AV0D2 C8AV0D2

-1000 C9AV0D2 Predicted

-1500

-2000 -0.2

-0.0

0.2

0.4

0.6

0.8

1.0

1.2

1.4

1.6

Time (ms)

6.7 Comparison of analysis with strain gauge readings in impact of cylinders. The axial strains near the impact point in three separate experiments are shown. (After Swanson et al.22)

Clearly the quasi-static solution is much simpler to use than the structural dynamics solution. The question that arises is whether it is possible to determine the limits of applicability of the quasi-static solution, without recourse to a more complicated dynamic solution. A dimensionless parameter consisting of the ratio of the mass of the impactor to the ‘effective’ structure mass has been developed24 that permits identification of the range of applicability of the quasi-static solution. This procedure is briefly reviewed in the following.

6.4.1 Limits of quasi-static analysis An often employed rule-of-thumb is that the quasi-static approximation is valid if the frequency of the impact (say as defined by the contact duration) is less than 1/3 the lowest natural frequency of the structure.25 When dynamic effects in the structure do become important, the impact force and the resulting peak values of stresses and strains in the structure typically become larger than they would be for a given impact energy under quasistatic loading. This will be illustrated in calculations to be shown subsequently for impacts of plates and cylinders.

IBF6 11/22/2000 6:35 PM Page 206

206

Impact behaviour of composite materials and structures

The rule-of-thumb cited above does seem to be a reasonable method of ascertaining the limit of the quasi-static solution. However, it entails knowing at least the lowest natural frequency of the structure. This may be a significant drawback in some cases, as the point of the quasistatic approximation is to be able to analyse the impact event without knowledge of the dynamic solution. While it is easier to get a natural frequency of the structure than the entire dynamic response, there is still motivation for developing an alternative rule for the limits of the quasi-static approximation without knowing the structure’s natural frequency. This objective is pursued in the next section, following the work of Swanson.24

6.4.2 Alternative rule for limits of quasi-static approximation Intuitively it can be seen that if the impact mass is large with respect to the structure mass, the impact event can be treated as quasi-static. This idea can be simply related to the conventional rule for the ratio of natural frequencies given above. The approach taken is to develop an expression for an equivalent lumped mass, that can be used in conjunction with the static stiffness to approximate the lowest natural frequency of the structure. The definition of the equivalent mass will be given subsequently. The first premise to be advanced is that the lowest natural frequency of the structure can be approximated as wnª

K st meq

[6.51]

The impact frequency is given by wiª

K st meq + M i

[6.52]

Using the rule-of-thumb given above for the limits of quasi-static impact in terms of frequencies leads directly to the rule for the limits of validity of the quasi-static approximation as Mi ≥ 8meq 10meq

[6.53]

Thus a rule-of-thumb for the limits of the quasi-static approximation for impact problems has been formulated in terms of the ratio of impact mass to equivalent structure mass, which can be easily determined. The equivalent structure mass is defined here implicitly by the following formula,

IBF6 11/22/2000 6:35 PM Page 207

Elastic impact stress analysis of composite plates and cylinders 1 1 meq nc2 = Ú rn2 dVol 2 2 Vol

207 [6.54]

where meq is the equivalent lumped mass of the structure, vc is the peak velocity of the contact point for the impact, v is the peak velocity distribution throughout the impacted structure, and the integral is taken over the entire structure. The above expression is based on equating the energy of the equivalent lumped mass to the energy of the structure. If the assumption is made that the structure is undergoing motion in the mode determined by the quasi-static approximation, then the peak velocities are proportional to peak displacements, and the displacements are those calculated from a static application of load at the contact point.Thus, the above can be replaced by 1 1 meqd c2 = Ú rw 2 dVol 2 2 Vol

[6.55]

where here dc is the displacement at the point of impact, and w is the transverse displacement throughout the body as calculated by a static analysis. It is important to note that equation [6.55] enables the equivalent mass to be calculated from a knowledge of the static deformation of the body alone, without requiring access to a dynamic solution. The procedure given in [6.55] has been suggested for calculating lumped mass approximations, as presented by Steidel,26 for example, as an approximate method of calculating natural frequencies for beams and rods. The central issue at present is whether the equivalent lumped mass can be used to estimate the limits of suitability of a quasi-static solution for an impact problem. This is addressed in the following by comparing dynamic calculations with quasi-static calculations for various impact problems.

6.4.3 Comparison of dynamic and quasi-static impact response The calculations shown in this section will use solutions for impact problems of orthotropic plates and cylinders with various boundary conditions. Various example solutions for the impact response of structures were calculated using the procedures described above, for various values of impact mass. The equivalent masses of the structures were calculated using static solutions.55 The response quantities examined were the contact force, normal strains behind the impact point, and peak interlaminar shear stress values. In general, all of these response values start to increase relative to

IBF6 11/22/2000 6:35 PM Page 208

208

Impact behaviour of composite materials and structures

Ratio of dynamic to quasi-static solution

5

4

quasi-static (rule based on mass ratio = 10)

3

2

1

0 -2

-1

0

1

2

3

4

5

Log (projectile mass/effective structure mass)

6.8 Transition from quasi-static to dynamic response in impact of composite plates and cylinders. The variables shown are peak contact force, strain behind the impact point, and interlaminar shear stress. Plates are both simply supported and clampedclamped, free-free, and cylinders are of two lengths. (After Swanson24.)

the quasi-static solution when impact energy is held constant, as dynamic effects in the structure start to become important. A typical set of results for two different lengths of an orthotropic cylinder and plate solutions for two different sets of boundary conditions, using the calculational procedures discussed above, are shown in Fig. 6.8. These results have been normalised by dividing by the quasi-static solution, holding impact energy constant, and plotted as a function of the ratio of impact mass to equivalent structure mass as calculated by equation [6.55]. The critical ratio of impact mass to equivalent structure mass has been taken as 10 from [6.53], and is also shown. It can be seen that this rule is in fact a reasonable estimate of the limit of the validity of the quasi-static approximation. Qualitatively the results are quite comparable, as the value of 10 for the ratio of impact mass to equivalent structure mass appears to represent the limit of the quasi-static approximation for both the plates and cylinders reasonably well.

IBF6 11/22/2000 6:35 PM Page 209

Elastic impact stress analysis of composite plates and cylinders

209

3000 l=1 l=2 l=3 l=4 l=5

2500

ey at A (microstrain)

2000

1500

1000

500

0

-500 0

100

200

300

400

500

Time/l (ms)

6.9 Comparison of strain response in impact tests on five different plate sizes. Plates are scaled geometrically by the parameter l, and the analysis shows that time is also scaled by l. (After Qian and Swanson16.)

6.5

Issues of scaling in impact

The question of scaling, i.e. extrapolating from tests on small laboratory specimens to larger structures, is an important issue in impact. This issue has been addressed by a number of authors, including Morton,27 Sankar,28 Qian et al.,29 Qian and Swanson,16 Swanson et al.,22 and others. Analytical solutions such as those discussed in the above are very helpful in understanding the issues of scaling, as the governing equations can be manipulated to reveal the dimensionless parameters involved.An approach taken16,22,29 was to use geometric scaling, which also dictated the scaling of time. A typical result of scaled impact experiments on plates is shown in Fig. 6.9, where the linear response is found to scale within the basic reproducibility of the experiments for five sizes of plates. Scaling of the damage formation resulting from impact is more complicated. For example, Swanson30 found that the scaling associated with delamination resulting from impact is that characteristic of fracture mechanics. Christoforou and Yigit31,32 also address

IBF6 11/22/2000 6:35 PM Page 210

210

Impact behaviour of composite materials and structures

scaling of impact, and in addition develop dimensionless numbers characterising impact with respect to the relative importance of indentation, and the conditions for quasi-static analysis to be applicable.

6.6

Summary and conclusions

The fundamental equations and some solution procedures have been presented for elastic impact of laminated plates and cylinders. Issues of convergence and accuracy have been addressed, and comparisons with experimental data have been given. The results show that the linear response of these fundamental structural elements is reasonably well understood.

References 1 Zukas J A, et al., Impact Dynamics, New York, Wiley, 1982. 2 Joshi S P and Sun C T, ‘Impact induced fracture in a laminated composite’, J Composite Mater, 1985 19 51–66. 3 Sun C T and Chattopadhyay S, ‘Dynamic response of anisotropic laminate plates under initial stress to impact of a mass’, J Appl Mech, 1975 42 693–8. 4 Yang S H and Sun C T, ‘Indentation law for composite laminates’, Composite Materials: Testing and Design (Sixth Conference), ASTM STP 787, pp 425–49, 1982. 5 Tan T M and Sun C T, ‘Use of statical indentation laws in the impact analysis of laminated composite plates’, J Appl Mech, 1985 52 6–12. 6 Lekhnitskii S G Anisotropic Plates, transl S W Tsai and T Cheron, New York, Gordon and Breach Science, 1968. 7 Whitney J M and Leissa A W, ‘Analysis of a simply-supported laminated anisotropic rectangular plate’, AIAA J, 1970 7 28. 8 Whitney J M and Pagano N J, ‘Shear deformation in heterogeneous anisotropic plates’, J Appl Mech, 1970 37 1031. 9 Dobyns A L, ‘Analysis of simply-supported orthotropic plates subject to static and dynamic loads’, AIAA J, 1981 19 642. 10 Birman V and Bert C W, ‘Response of composite plates to blast loading’, in Proc ICCM & ECCM Conf, 5, Imperial College of Science and Technology, London, July 20–24, 5.192, 1987. 11 Christoforou A P and Swanson S R, ‘Analysis of simply-supported orthotropic cylindrical shells subject to lateral impact loads’, J Appl Mech, 1990 57 376–82. 12 Christoforou A P and Swanson S R, ‘Analysis of impact response in composite plates’, Intl J Solids Struct, 1991 27 161–70. 13 Bert C W and Birman V, ‘Dynamic stability of thick, orthotropic, circular cylindrical shells’, in Lecture Notes in Engineering: Refined Dynamic Theories of Beams, Plates and Shells and Their Applications, Springer-Verlag, Berlin, 235, 1987. 14 Bert C W and Chen T L C, ‘Effect of shear deformation on vibration of antisymmetric angle-ply laminated rectangular plates’, Int J Solid Struct, 1978 14 465.

IBF6 11/22/2000 6:35 PM Page 211

Elastic impact stress analysis of composite plates and cylinders

211

15 Cairns D S and Lagace P A, ‘Transient response of graphite/epoxy and kevlar/epoxy laminates subjected to impact’, presented at 29th Structures, Structural Dynamics and Materials Conference (not published in Proceedings), 1988. 16 Qian Y and Swanson S R, ‘Experimental measurement of impact response in carbon/epoxy plates’, AIAA J, 1990 28 1069–74. 17 Timoshenko S and Young D H, Vibration Problems in Engineering, 3rd edn, Van Nostrand, New York, 1955. 18 Qian Y and Swanson S R, ‘A comparison of solution techniques for impact response of composite plates’, Composite Struct, 1990 14 177–92. 19 Sun C T and Chen J K, ‘On the impact of initially stressed composite laminates’, J Composite Mater, 1985 19 490. 20 Ramkumar R L and Thakar Y R, ‘Dynamic response of curved laminated plates subjected to low velocity impact’, ASME J Eng Mater Technol, 1987 109 67–71. 21 Vinson J R and Chou T W, Composite Materials and Their Use in Structures, Applied Science, London, 1975. 22 Swanson S R, Smith N L and Qian Y, ‘Analytical and experimental strain response in impact of composite cylinders’, Composite Struct, 1991 18 95–108. 23 Mindlin R D, ‘Influence of rotary inertia and shear on flexural motions of isotropic elastic plates’, ASME J Appl Mech, 1951 18 31–8. 24 Swanson S R, ‘Limits of quasi-static solutions in impact of composite structures’, Composites Eng, 1992 2 261–7. 25 Cook R D, Malkus D S and Plesha M E, Concepts and Applications of Finite Element Analysis, 3rd edn, New York, Wiley, 1989. 26 Steidel R F, An Introduction to Mechanical Vibrations, 3rd edn, New York, Wiley, 1989. 27 Morton J, ‘Scaling of impact-loaded carbon-fiber composites’, AIAA J, 1988 26 989–94. 28 Sankar B V, ‘Scaling of low-velocity impact for symmetric composite laminates’, J Reinforced Plastics Composites, 1992 11 296–309. 29 Qian Y, Swanson S R, Nuismer R J and Bucinell R B, ‘An experimental study of scaling rules for impact damage in fiber composites’, J Composite Mater, 1990 24 559–70. 30 Swanson S R, ‘Scaling of impact damage in fiber composites from laboratory specimens to structures’, Composite Struct, 1993 25 249–55. 31 Yigit A S and Christoforou A P, ‘Impact dynamics of composite beams’, Composite Struct, 1995 32 187–95. 32 Christoforou A P and Yigit A S, ‘Characterization of impact in composite plates’, Composite Struct, 1998 43 15–24.

IBF7 11/22/2000 6:42 PM Page 212

7 Impact behaviour and analysis of CFRP laminated plates ENBOA WU AND CHENG-ZORN TSAI

7.1

Introduction

The low-velocity impact behaviour of composite laminates has been studied extensively in recent decades. As described in two review papers,1,2 experimental results reported in the literature have mainly focused on impactinduced damage mechanisms, such as matrix cracking, delamination and fiber breakage in different impact stages; on the other hand, most of the analytical methods have focused on elastic impact on laminates with perfect boundaries. Aside from direct investigation of the laminate damage using the naked eye, such as for glass/epoxy laminates that are partially light transparent,3–5 C-scan or X-ray has mostly been employed in damage assessment.6,7 A focused treatment of this topic is available in Chapter 2. The apparatus that has provided the impact energy has usually been a drop weight tower. Due to the limitation of the tower height, almost all the impact events have been conducted using a heavy impactor at a velocity of less than 10 m/s. The impact force has usually been recorded by a force transducer embedded in the impactor. The corresponding histories of energy, velocity, and displacement were then derived once the onset of contact between the impactor and the target was detected by Cantwell and Morton8 and others in Chapters 5 and 8. On the other hand, the higher-speed impact results published in the literature have been far fewer than those for lower-speed impact. One reason has been the need for a gas gun to provide the initial kinetic energy of the impactor. In this category, impact has generally been conducted using a lighter impactor, most of the time called a projectile, at a much higher initial velocity. Further, because it is very difficult to mount a sensor in a flying projectile,9,10 the data recorded during such an impact event has usually been only the initial and the final states of the projectile and the target. The history of impact, even if a high-speed camera was employed, was very hard to record. For example, Gupta and Davids back in 196611 used a rifle to launch projectiles which struck glass/epoxy laminates at impact speeds from 212

IBF7 11/22/2000 6:42 PM Page 213

Impact behaviour and analysis of CFRP laminated plates

213

305 to 387 m/s and found a linear relationship between the projectile energy loss and the target thickness.Takeda et al.12,13 studied the delamination crack propagation phenomena of glass/epoxy laminates for projectiles at initial speeds up to 83 m/s. Cantwell and Morton investigated the effects of laminate thickness, dimensions, and stacking sequence on the penetration energy threshold.14–16 Zhu et al. reported the impact phenomena for kevlar/polyester composites struck by cylindrically-conical projectiles.17 The results of impact on graphite/epoxy laminates by blunt projectiles were reported by Lee and Sun.18,19 The effect of the strain rate on the penetration behaviour was also uncovered by Jenq et al.20 and Wu and Chang.5 Other high-velocity impact studies can be found in Chapters 8 and 9. Meanwhile, as the composite laminated structures used in modern industry have rapidly increased, the need to more accurately predict the impact response of such advanced structures has become inevitable. In the past, most of the studies focused on the development of analytical or numerical methods to predict the elastic response of laminated beams,21 plates22–25 and shells,26 and the relationship between the impactor and the struck laminate was frequently modelled using the modified Hertz contact law,27 which was verified experimentally7,28 and analytically.29,30 A further example is available in Chapter 6. On the other hand, the inverse method was found to be able to detect the impact force, location, impactor mass and velocity using the response, which sometimes was even incomplete, of the struck plate.31–35 This method was also found to be able to reconstruct forces in bar-to-bar impact problems.36 However, most, if not all, of the experimental results reported in the literature for impact on graphite/epoxy composite laminates involving a gas gun, i.e. high-velocity impact, described only the final state, and in the analytical predictions, the laminates were all assumed to have perfect boundary conditions. In this chapter, the goal is to obtain the impact history of such advanced structures when they are struck by projectiles in a velocity range that is from very low to way above the ballistic limit of the targets, and to present an analytical method that can take boundary imperfection into consideration. In the experimental investigation, a gas gun was employed to launch a hemispherically tipped projectile to strike a 32-layered quasiisotropic graphite/epoxy laminate. Transient laser Doppler anemometry (TLDA), which was developed at the National Taiwan University and is a noncontact measurement method having a 1.0 ms sampling rate, was employed to extract the velocity history of the projectile while it was striking the target. This excellent technique has been successfully employed to uncover the impact process of metallic targets,37,38 glass/epoxy laminates39,40 and honeycombs.41 The force and the displacement histories were then subsequently derived. Thus, the terminal velocity, impact energy, absorbed energy, peak force and momentum change were obtained. The impact

IBF7 11/22/2000 6:42 PM Page 214

214

Impact behaviour of composite materials and structures

response of this laminated structure will be discussed in detail using these data and the measured laminate damage area. On the other hand, the Ritz method along with the Mindlin plate theory was employed to construct the governing equations of a laminated plate under impact conditions. In order to predict the impact response of a laminate under ‘imperfect’ boundary conditions, two beam functions, one satisfying simply supported conditions and the other satisfying fixed conditions, were employed, and a non-dimensional constant that represents the rotational spring constant of the physical clamp was used. The actual value of the rotational spring constant was obtained from the quasi-static contact test result. The correlation between the prediction and the measured data will be used to verify the presented method.

7.2

Experimental set-up and procedure

7.2.1 Specimen Fiberite Hy-E 1076E T300/976 graphite/epoxy prepregs were employed to fabricate the specimens using an autoclave. All the specimens were 32-ply (0/45/90/–45)4S quasi-isotropic laminates. The nominal thickness was 4.3 ± 0.1 mm. The in-plane dimensions were 152.4 mm by 101.6 mm. The 0° laminae were along the long dimension. Two types of boundary conditions were employed. In the first type, the plates were suspended by two light strings attached to two adjacent corners of the plate to simulate the free boundary condition, and was used for verification of the presented analytical method as the boundary can easily be made to be perfect. On the other hand, in most of the test runs, the laminates were tightly clamped on two opposite edges with the other two free of support, resulting in a clamped span of 101.6 mm and leaving the original short dimension of 101.6 mm as the free span. After the specimens were struck, they were C-scanned to uncover the delamination damage profile. In this study, the delamination area was defined as the area that was enclosed by the outermost crack fronts in all the interfaces along the thickness direction of the laminate.

7.2.2 Experimental procedure The transient laser Doppler anemometer (TLDA), which was developed in the Impact and Precision Measurement Laboratory of National Taiwan University, was employed for extraction of the quickly changing velocity history of a projectile during impact and penetration.38 This is a backscattering arrangement. It allows the Doppler signals to scatter backward to the optical devices through which the laser beams originally passed. The principle of laser Doppler anemometry is to intersect two coherent light beams to form a small measuring volume in an ellipsoidal shape, whose

IBF7 11/22/2000 6:42 PM Page 215

Impact behaviour and analysis of CFRP laminated plates

215

size depends upon the beam diameter and the light intersection angle, 2k, and is usually only a few mm in all three ellipsoidal axes. Because of light interference, fringes of spacing df are formed inside the measuring volume. When particles on the surface of a projectile travel across the fringes inside the measuring volume, light is scattered. By recording the history of this scattered light, the velocity history of the surface of the projectile can be obtained using the following equation:42,43 V=

l fD 2 sin k

[7.1]

where l is the wave length of the coherent light and fD is the frequency of the Doppler signal. In this study, l = 632.8 nm and k = tan-1 (1/20). Thus, df = l/(2 sin k) = 6.336 mm and V = 6.336 ¥ 10-6 fD m/s. A detailed description of the LDA principle can be found in Durst et al.42 and Drain.43 The experimental set-up for the impact test is schematically shown in Fig. 7.1. A gas gun was employed to launch a hemispherically tipped projectile, made of hard steel, of 12.7 mm diameter. The mass of the projectile was 35.6 g, and its length was 38.0 mm. The projectile was hardened to Rc60 to avoid possible plastic deformation during impact. The transient laser Doppler anemometer (TLDA) system included a 35 mW He–Ne laser light source, a series of optical devices for passage of the laser light and the scattered Doppler signals, a photomultiplier for conversion of the scattered Doppler signals into electric current, and a bandpassed filter for filtering out noises and pedestal signals carrying the Doppler signals. To simplify the process, the zero-crossing method was employed to extract the velocity history from the recorded Doppler signals. This was similar to the method used by Wu and Chang for impact on glass/epoxy laminates.4,5 On the other hand, a complete description of the implementation procedure for TLDA can be found in Tsai and Wu.38 After the velocity data were obtained, the acceleration history could be retrieved, in principle, by means of differentiation. In order to avoid errors from being induced in the acceleration due to direct differentiation, the smoothing cubic-spline method was employed. This method was a modification of the cubic-spline interpolation method, in which a function, f(x), in the following form is usually used:44 2

3

f (x) = a i + bi (x - x i ) + c i (x - x i ) + di (x - x i ) x i £ x £ x i+1 i = 1, 2, . . . , n - 1

[7.2]

where (xi, yi), i = 1, 2, . . . , n; n > 3 are the recorded discrete data points set and yi = f(xi). To suppress the noise, an objective function E is defined as i= N

E(a i , S ) =

Â (y i=1

2

i

- ai) + S Ú

xN

x1

2

[ f ¢¢(x)] dx

[7.3]

IBF7 11/22/2000 6:42 PM Page 216

Impact behaviour of composite materials and structures

7.1 A schematic of the experimental set-up for impact on composite laminates.

216

IBF7 11/22/2000 6:42 PM Page 217

Impact behaviour and analysis of CFRP laminated plates

217

where S is the smoothing parameter. The first term in [7.3] represents the deviation between f and the data point, and the second term is the smoothing level of f. A detailed description of the smoothing cubic-spline method can be found in de Boor.44 This method acts as a low-pass filter to the velocity data extracted from Doppler signals. The acceleration history was then obtained by means of direct differentiation of the function f. A detailed description of the implementation procedure can also be found in Tsai45 and examples shown in later sections. On the other hand, the displacement history was obtained by means of direct integration of the velocity data. The time for the onset of contact between the projectile and the target was precisely determined using a piezo-film attached at the center of the distal side of the laminated plate.37

7.3

Near-elastic impact behaviour

In this velocity range, no damage was found in laminates using both visual inspection by means of the naked eye and C-scan. The impact velocity of the projectile was lower than 20 m s-1. Typical velocity and force histories for the struck laminates in this category are shown in Fig. 7.2(a) and (b), which shows projectile impact results at 8.3 and 14.5 m s-1, respectively. Before the onset of contact, the velocity remained constant. This value dropped drastically once the projectile hit the target, and caused the projectile to indent the laminate in the contact region. The amount of indentation was equal to the difference of movement between the target and the projectile, and could be related to the impact force using the modified type of Hertz contact law.7 Thus, this indentation caused the impact force to increase drastically. In the meantime, the impact neighbourhood of the target started to move forward owing to the action of the projectile. This movement immediately decreased the indentation value, and the force dropped almost as sharply as in the rising part, thus forming the first peak. As impact proceeded, the velocity of the impact neighbourhood of the struck laminate was reduced due to the action of the bending stiffness of the laminate. As a result, the value of the indentation increased again. This resulted in a drastic increase of the force value. In this study, the second force peak was always observed when the laminate was not significantly damaged and occurred when the projectile velocity decreased to approximately zero, as typically shown in Fig. 7.2(a) and (b). It is interesting to note that a third force peak was also observed, and that the projectile physically separated from the target before the third peak occurred. Further, this phenomenon occurred when the projectile velocity was negative. Apparently, the projectile was hit by the target when the target bounced back. Due to the force exerted by the bouncing target,

IBF7 11/22/2000 6:42 PM Page 218

Impact behaviour of composite materials and structures 2.5 Vi = 8.3 ms–1 Vt = –6.4 ms–1 Fp = 2.30kN

2.0 1.5

0 1.0 –5

0.5

–10 –0.2

–0.0

0.2 0.4 Impact time (ms) (a)

0.6

0.0 0.8

4.0 Vi = 14.5 ms–1 Vt = –10.7 ms–1 Fp = 3.70kN

10 0

2.0

–10

1.0

–20 –0.2

–0.0

0.2 0.4 Impact time (ms) (b)

0.6

30 Velocity (ms–1)

3.0

Force (kN)

Velocity (ms–1)

20

0.0 0.8

5.0 Vi = 22.2 ms–1 Vt = –13.8 ms–1 Fp = 4.29kN

20 10

4.0 3.0

0

2.0

–10

1.0

–20 –0.2

–0.0

0.2 0.4 Impact time (ms) (c)

0.6

0.0 0.8

4.0

30 Velocity (ms–1)

Force (kN)

5

Force (kN)

Velocity (ms–1)

10

Vi = 24.4 ms–1 Vt = –15.2 ms–1 Fp = 3.27kN

20 10

3.0 2.0

0 1.0

–10 –20 –0.2

–0.0

0.2 0.4 Impact time (ms) (d)

0.6

Force (kN)

218

0.0 0.8

7.2 Velocity and force histories for laminates struck at (a) 8.3 m s-1; (b) 14.5 m s-1; (c) 22.2 m s-1; (d) 24.4 m s-1; (e) 31.8 m s-1; and (f) 36.2 m s-1.

IBF7 11/22/2000 6:42 PM Page 219

Impact behaviour and analysis of CFRP laminated plates 5.0 Vi = 31.8 ms–1 Vt = –5.1 ms–1 Fp = 4.23kN

30 20

4.0 3.0

10

2.0

0

1.0

–10 –0.4

–0.0

0.4

0.8

1.2

Force (kN)

Velocity (ms–1)

40

219

0.0 1.6

Impact time (ms) (e) 4.0 Vi = 36.2 ms–1 Vt = 10.0 ms–1 Fp = 3.63kN

30

3.0

20

2.0

10

1.0

0 –0.4

Force (kN)

Velocity (ms–1)

40

0.0 –0.0

0.4

0.8

1.2

1.6

Impact time (ms) (f)

7.2 (cont.)

the absolute value of the projectile velocity increased again, but in the negative direction.The impact process terminated when the bouncing target was pulled again in the forward direction due to its bending stiffness, at which point the projectile gained enough momentum from the bounced target and started to separate permanently from the target. The relationship between the impact and the terminal velocities for the event in which the struck laminates showed no delamination damage is illustrated in Fig. 7.3. A straight line was found to fit the relationship fairly well. Thus, the relationship between the absorbed energy, DE, and the impact velocity, Vi, was found to be quadratic, as shown in Fig. 7.4. On the other hand, a straight-line relationship is also observed in Fig. 7.5 between the impact velocity and the maximum force peak for each test run. Note that, in Fig. 7.2(a) and (b), the first peak in the multi-peak impact event always has the highest magnitude. This is because the largest indentation value between the projectile and the target always occurred very shortly after the onset of first contact. During this very short period the target did not deform extensively. As a result, the target response to impact was not similar to the target response to quasi-static loading because the peak force in the latter case always occurred when the deflection was largest.

IBF7 11/22/2000 6:43 PM Page 220

Impact behaviour of composite materials and structures 100 Measured Predicted

Terminal velocity (ms–1)

80

60

40

20

0 0

20

40

60

80

100

120

Impact velocity (ms ) -1

7.3 The relationship between the impact velocity, Vi and the terminal velocity, Vt of the projectile.

25

20 Absorbed energy (J)

220

15

10

5

0 0

20

40

60

80

100

120

Impact velocity (m s -1)

7.4 The relationship between the impact velocity, Vi of the projectile and the absorbed energy of the struck laminates.

IBF7 11/22/2000 6:43 PM Page 221

Impact behaviour and analysis of CFRP laminated plates

221

6

Peak impact force (kN)

5

4

3

2

1

0 0

20

40

60

80

100

120

Impact velocity (m s ) -1

7.5 The relationship between the impact velocity, Vi and the peak impact force of the projectile.

7.4

Prediction of elastic impact response

7.4.1 Governing equations The method presented in this section was derived using the Ritz method, and the Mindlin plate theory was adopted. The displacement field, by neglecting the in-plane deformation of the plate, reads u1 (x, y, z, t ) = za (x, y, t ) u2 (x, y, z, t ) = z b (x, y, t )

[7.4]

u3 (x, y, z, t ) = w (x, y, t ) where u1, u2 and u3 are the displacements in the x, y and z directions of the plate; a ¯ and b¯ are the rotations of the plate in the x and y directions, respectively; and w is the lateral deflection of the plate. The strain-displacement relations become Ê e xx ˆ Ê e1 ˆ Ê a ,x ˆ Á e yy ˜ = Á e 2 ˜ = zÁ b,y ˜ Á ˜ Á ˜ Á ˜ Ë 2 e xy ¯ Ë e 6 ¯ Ë a ,y + b, x ¯ Ê 2 e yz ˆ Ê e 4 ˆ Ê b + w ,y ˆ = = Ë 2 e zx ¯ Ë e 5 ¯ Ë a + w , x ¯

[7.5]

IBF7 11/22/2000 6:43 PM Page 222

222

Impact behaviour of composite materials and structures

For each lamina, the constitutive relations are Ê s xx ˆ Ê s1 ˆ ÈQ11 Q12 Q16 ˘ Ê e1 ˆ Á s yy ˜ = Á s 2 ˜ = ÍQ12 Q22 Q26 ˙ Á e 2 ˜ ˙Á ˜ Á ˜ Á ˜ Í Ë t xy ¯ Ë s 6 ¯ ÍÎQ16 Q26 Q66 ˙˚ Ë e 6 ¯

[7.6]

ÈQ44 Ê t yz ˆ Ê s 4 ˆ = = kÍ Ë t zx ¯ Ë s 5 ¯ ÎQ45

[7.7]

Q45 ˘ Ê e 4 ˆ Q55 ˙˚ Ë e 5 ¯

where Qij is the reduced elastic constant under the plane-stress conditions and k is the shear correction factor, whose value was taken to be 5/6. The kinetic and strain energy for the laminate is, respectively, h

T=

1 b a 2 r(u˙ 12 + u˙ 22 + u˙ 32 )dzdxdy 2 Ú0 Ú0 Ú-2h

V=

1 b a 2 (s1 e1 + s 2 e 2 + s 6 e 6 + s 4 e 4 + s 5 e 5 )dzdxdy 2 Ú0 Ú0 Ú-2h

[7.8]

and h

[7.9]

where r is the density of the laminate. On the other hand, the work done by the external force, P(x, y, t), applied normally to the plate is W =Ú

b

0

Ú

a

0

P(x, y, t )u3 dxdy.

[7.10]

In order to apply the Ritz method, beam functions that satisfy the geometric boundary conditions of the plate were adopted, and the three independent variables are expressed by the series expansion: a (x, y, t ) =

Âa

b (x, y, t ) =

Â b (t )x (x)h¢ ( y)

w (x, y, t ) =

Âw

ij

ij

ij

ij

(t )x ¢i (x)h j ( y)

ij

i

ij

j

[7.11]

(t )x i (x)h j ( y)

where x(x) and h(y) are beam functions in the x and y directions, respectively. Note also that x¢(x) and h¢(y) are included in the above equation in order to avoid the erroneous shear locking phenomenon when the plate becomes very thin.31 The governing equation in the form of

[ M ]{q˙˙} + [ K ]{q} = {P *}

[7.12]

can be derived by applying the Hamilton principle of t2

d Ú (T - V )dt = 0 t1

[7.13]

IBF7 11/22/2000 6:43 PM Page 223

Impact behaviour and analysis of CFRP laminated plates

223

where the generalised coordinates, q, are in the form of T

{q} = {a11 , a12 , . . . , a 21 , . . . ; b11 , b12 , . . . b 21 , . . . ; w11 , w12 , . . . , w 21 , . . .}. [7.14] On the other hand, the generalised force, P*, can be obtained from P. In this study, the area of contact between the projectile and the plate was small. Thus, a point load assumption is justified, and [7.10] is simplified as b

a

Â Ú Ú P(t )d(x - x )d( y - y ) ◊ w = P(t )(Â w (t )x (x )h ( y ))

W=

ij 0

0

0

ij

ij

0

i

T

0

ij

(t )x i (x)h j ( y)dxdy [7.15]

0

j

T

= P(t ){q} {Y *} = {q} {P *} where T

{Y *} = {0, 0, . . . , 0, 0, . . . , x1 h1 , . . . , x1 h2 , . . . , x 2 h1 , . . .}( x 0 ,y 0 ) . [7.16] Equation [7.12] can be further simplified by neglecting the effect of rotational inertia:31 È0 ÍÎ 0

0 ˘Ê q˙˙1 ˆ È K11 + M 22 ˙˚Ë q˙˙ 2 ¯ ÍÎ K 21

K12 ˘Ê q1 ˆ Ê 0 ˆ = K 22 ˙˚Ë q 2 ¯ Ë P2 ¯

[7.17]

* ]{q 2 } = {P2 } [ M22 ]{q˙˙ 2 } + [ K 22

[7.18]

where T

-1

[ K 22* ] = [ K 22 ] - [ K12 ] [ K11 ] [ K12 ]

[7.19]

and -1

{q1} = -[ K11 ] [ K12 ]{q 2 } T

{q 2 } = {a11 , a12 , . . . , a 21 , . . . ; b11 , b12 , . . . , b 21 . . .}

[7.20]

T

{q 2 } = {w11 , w12 , . . . , w 21 , . . .} T

{P2 } = P(t ){x1 h1 , x1 h2 , . . . , x 2 h1 , . . .}( x 0 ,y 0 ) = P(t ){Y }

T

7.4.2 Solution scheme The response of the projectile, on the other hand, is expressed in the form of mS˙˙(t ) = - P(t )

[7.21]

where m is the mass of the projectile and S is the projectile movement. The modified Hertz contact law, by assuming the projectile to be rigid, is then employed:7,28

IBF7 11/22/2000 6:43 PM Page 224

224

Impact behaviour of composite materials and structures f (a ) =

4 3 2 REz (a ) 3

[7.22]

where R is the radius of the projectile head and Ez is the Young’s modulus of the laminate in the thickness direction. In this equation, the indentation, a, is defined as the difference between s(t) and w0(t), and the impact force P(t) is equal to f(a), where w0(t) is the laminate deformation in the thickness direction at the contact location. In this study, the central difference method was employed. Thus, equations [7.18] and [7.21] can be expressed in the following discrete forms: 2

-1

2

-1

* ]{q 2 } {q 2 } j+1 = Pj (Dt ) [ M22 ] {Y } - (Dt ) (M22 ) [ K 22 j + 2{q 2 } j - {q 2 } j-1 2

S j+1 = Pj (Dt ) m + 2 S j - S j-1

[7.23] [7.24]

Comparisons between the prediction and the test results are shown in Fig. 7.6(a) and (b), in which the histories of the velocity and force are plotted. The initial striking velocity was 7.46 m s-1. The overall correlation is considered to be very satisfactory. Thus, the presented method has been demonstrated to be suitable for impact prediction of laminated structures.

7.4.3 Modeling of physically clamped boundaries As stated in the Introduction, the boundary of a laminated plate, except for one under free-free boundary conditions, can hardly be considered as being perfect due to elastic deformation and material and geometric imperfection of both the laminate and the clamped pads. Figure 7.7(a) and (b) shows typical results for a laminate that was physically clamped on two opposite sides and struck by a 35.6 g projectile at an impact velocity of 4.3 m/s. Also shown in these figures are two predictions made under the assumption that the boundary was simply supported and fully clamped. It is found that neither correlates with the experimental data. Thus, it is essential to develop a method that takes the physical boundary condition into consideration. In order to model the boundary of a laminated plate that is physically clamped on its two opposite sides with the other two free of support, this nearperfect clamped boundary was modeled as a simple support with an elastic restrained edge; i.e. a finite rotational angle was allowed on the clamped sides. Thus, using the Ritz approach, where the displacement field was constructed by means of a series of orthogonal beam functions, the eigenfunction of such a beam can be derived from the following equation: mü + EIu≤≤ = 0

[7.25]

IBF7 11/22/2000 6:43 PM Page 225

Impact behaviour and analysis of CFRP laminated plates

225

8 Experimental data Prediction

7

Impact velocity (m s -1)

6 5 4 3 2 1 0 -0.2

-0.1

-0.0

0.1

0.2

0.3

0.4

0.5

0.6

0.5

0.6

Impact time (ms) (a) 2.0 Experimental data Prediction

1.8

Impact force (kN)

1.5 1.3 1.0 0.8 0.5 0.3 0.0 -0.2

-0.1

-0.0

0.1

0.2

0.3

0.4

Impact time (ms) (b)

7.6 (a) The velocity history and (b) the force history for a 35.6 g projectile striking at 7.46 m s-1. Both the measurement data and the prediction using the Ritz method are plotted.

IBF7 11/22/2000 6:43 PM Page 226

226

Impact behaviour of composite materials and structures 6 Experimental data Prediction (Simple support) Prediction (Fixed-end)

Impact velocity (m s -1)

4

2

0

-2

-4 -0.1

-0.0

0.1

0.2

0.3

0.4

0.5

0.6

0.7

0.8

0.6

0.7

0.8

Impact time (ms) (a) 1.6 Experimental data Prediction (Simple support) Prediction (Fixed-end)

Impact force (kN)

1.2

0.8

0.4

0.0 -0.1

-0.0

0.1

0.2

0.3

0.4

0.5

Impact time (ms) (b)

7.7 The measured (a) velocity and (b) force histories for a laminated plate that was struck by a 35.6 g projectile at 4.3 m s-1 and was physically clamped on two opposite sides with the other two sides free of support. Also shown are the Ritz predictions, which treat the boundary as being simply supported and fully clamped.

IBF7 11/22/2000 6:43 PM Page 227

Impact behaviour and analysis of CFRP laminated plates

227

The corresponding boundary conditions are u(0, t ) = u(l , t ) = 0 u ¢¢(0, t ) =

K u ¢(0, t ) EI

u ¢¢(l , t ) = -

[7.26]

K u ¢(l , t ) EI

where m is the mass per unit length, u(x, t) is the transverse displacement, and E and I are the Young’s modulus and the moment of inertia, respectively, of such a beam. On the other hand, K is the stiffness of the rotational spring, and l is the length of the beam. The value of K represents the rotational stiffness of the boundary. In the two extreme cases when K reaches zero and infinity, the simply supported and the fixed end conditions are obtained, whose beam functions are f s (x) =

2 EIa (sinh al sin ax - sinh ax sin al ) (sinh al - sin al )

[7.27]

and f c (x) = (cosh ax - cos ax) -

cosh al - cos al (sinh ax - sin ax) sinh al - sin al [7.28]

respectively. On the other hand, when the value of K falls in between the two extremes, the beam function becomes a combination having the following form: f(x) = f s (x) K + f c (x)

[7.29]

and note that a must satisfy the following characteristic equation: 2

2

Ê K ˆ (cosh al cos al - 1) + 2Ê K ˆ (cos al sinh al - sin al cosh al ) Ë EIa ¯ Ë EIa ¯ [7.30] - 2 sinh al sin al = 0 By selecting a proper value of K, a real boundary condition that reflects the physically clamped condition can be obtained. In this study, the K value was determined from a quasi-static test result, in which the boundary conditions, the shape of the indentor, and the laminate being tested remained identical to those tested under impact conditions. The optimal K, by which the correlation between the predicted Ritz

IBF7 11/22/2000 6:43 PM Page 228

228

Impact behaviour of composite materials and structures

method and the experimental result was the best, was then searched. For analysis purposes, a non-dimensional value was employed: S Kl = 1 - S EI

0£S£1

[7.31]

Note that S ranges between 0 and 1. In this study, S = 0.93 was found to be optimal. The predictions obtained using S = 0.93 and the measured data are shown in Fig. 7.8(a) and (b). It is found that the correlation is much better. Other similar comparisons can be found in Tsai.45 This demonstrates that the developed method is capable of predicting the impact response of a laminate under physically clamped boundaries. On the other hand, the deviation between the measurement and the prediction is more noticeable in Fig. 7.8(a) and (b) as compared with the example shown in Fig. 7.6(a) and (b), in which the plate is subject to free-free boundary conditions. This might to be due to the assumption of the uniform boundary condition along the clamped boundary. Other factors contributing to the deviation include the assumptions that the boundary behaviours due to the quasi-static and to the impact loads are identical, that S remains unchanged during loading and unloading processes, etc.

7.5

Impact beyond the delamination threshold

7.5.1 Delamination damage Delamination damage was observed when the impact velocity increased to 20.3 m s-1, at which point the terminal velocity was -13.8 m s-1 and the area calculated based on the C-scan run was 2.90 cm2. Under this impact condition, no damage was found on either the front or the distal surfaces of the struck laminate. Thus, delamination should be the only observed damage mechanism. However, because the absorbed energy ratio of DE/Ei = 0.48 remained essentially identical to that for impact at Vi = 14.5 m s-1, under which condition no delamination damage was observed, this damage alone did not absorb a significant amount of the impact energy. As a result, the impact histories of the force and velocity have profiles very similar to the results shown in Fig. 7.2(a) and (b) and, thus, are not plotted again. Similarly, the impact velocity versus the terminal velocity of the projectile, shown in Fig. 7.3, continuously follows the same linear relationship, and the absorbed energy, shown in Fig. 7.4, follows the same quadratic curve. From these revealed impact results, it is found that the responses of the projectile remained the same regardless of whether or not the impact was beyond the delamination threshold of the laminates.

IBF7 11/22/2000 6:43 PM Page 229

Impact behaviour and analysis of CFRP laminated plates 6 Experimental data Ritz method, S = 0.93

Impact velocity (m s -1)

4

2

0

-2

-4 -0.1

0.1

0.5

0.3

0.7

Impact time (ms) (a)

1.2 Experimental data Ritz method, S = 0.93

Impact force (kN)

0.8

0.4

0.0 -0.1

-0.0

0.1

0.2

0.3

0.4

0.5

0.6

0.7

Impact time (ms) (b)

7.8 The (a) velocity and (b) force histories measured using the developed TLDA and predicted using the Ritz method with S = 0.93. The experimental data are identical to those shown in Fig. 7.7.

229

IBF7 11/22/2000 6:43 PM Page 230

230

Impact behaviour of composite materials and structures

16

Delamination area (cm 2)

12

8

4

0 0

10

20

30

40

50

60

Impact velocity (m s ) -1

7.9 The relationship between the projectile initial velocity and the delamination damage area.

7.5.2 Spalling damage When the impact velocity increased slightly to 22.2 m s-1, a patch of the lamina layers on the distal side of the struck specimen started to separate from the laminate. This phenomenon was different from that observed under the quasi-static loading condition. Thus, the damage was considered to have been induced by the reflected tensile waves that were induced by the dynamic loads applied by the striking projectile. This phenomenon, designated as spalling damage, was similarly observed for a brittle target, such as one made of concrete, under projectile impact. In this test run, the delamination area was found to enlarge to 4.52 cm2, as plotted in Fig. 7.9. This shows that graphite/epoxy laminates are brittle, and that the difference in the thresholds between the delamination damage and the spalling damage of such a laminated specimen is not significant. On the other hand, the absorbed energy ratio, DE/Ei, was found to jump significantly from 0.48 in a previous run to 0.61. This indicated that the spalling damage along with the enlargement of the delamination area consumed a significant amount of the impact energy. Still no damage was observed at the initial contact point between the projectile and the target. The velocity and the force histories for impact at 22.2 m s-1 are shown in

IBF7 11/22/2000 6:43 PM Page 231

Impact behaviour and analysis of CFRP laminated plates

231

Fig. 7.2(c). Compared to the results shown in Fig. 7.2(a) and (b) for the case that involved no impact-induced damage as revealed by both C-scan and visual inspection, the phenomenon is found to be significantly different. For example, the second force peak disappeared due to stiffness degradation of the struck laminate, which, in turn, was due to damage on the distal surface of the laminates. This degradation in laminate stiffness also prevented separation of the projectile from the struck target during impact. However, the residual stiffness of the struck laminate was still large enough to cause the laminate to strike the projectile when its velocity was close to zero during the impact process. This resulted in a peak force at around 0.4 ms after the onset of impact, and the projectile gained enough velocity in the negative direction to escape from contact with the struck target that bounced back due to the action of the residual stiffness. The terminal velocity was found to be Vt = -13.8 m s-1. Its absolute value, as expected, was found to be lower than that in the previous impact run of Vt = -14.7 m s-1 due to the more severe reduction of the stiffness in the struck laminate. Meanwhile, as shown in Fig. 7.3, the terminal velocity, Vt, was found to decrease as the impact velocity continuously increased. Thus, the spalling damage was considered to have caused significant degradation in laminate stiffness. It is found from Fig. 7.5 that the maximum force peak was 5.34 kN when the impact velocity was 20.3 m s-1. The force peak dropped and remained at a constant level as the impact velocity further increased. One possible explanation for this peculiar phenomenon was the occurrence of spallation, which reduced the stiffness of the laminate. Once spalling damage occurred on the distal side of the laminates, due to the sudden reduction of the laminate stiffness, the laminate moved much more easily with the projectile. As a result, the maximum indentation between the projectile and the laminate during the impact process, which corresponded to the maximum force peak, for the impact test run that involved spallation was smaller as compared to the test runs in which spallation was not observed.

7.5.3 Permanent indentation damage Permanent indentation damage on the impact side of the struck laminates was observed when the impact velocities became higher, and layers on the distal side of the laminates broke more seriously and separated from the remainder of the laminate. Two typical velocity and force histories for Vi = 24.4 m s-1 and Vi = 31.8 m s-1 are shown in Fig. 7.2(d) and (e). Due to the higher impact velocity, such as in the test run conducted at Vi = 31.8 m s-1, the laminate was damaged more seriously. As a result, it was not able to vibrate effectively enough to push the projectile further back in the reverse direction. Thus, the previously observed multiple force peak phenomenon

IBF7 11/22/2000 6:43 PM Page 232

232

Impact behaviour of composite materials and structures

was diminished, and there existed essentially only a single peak in the force history at the very beginning of the impact stage. The terminal velocity, Vt, was found to decrease at an approximately constant rate as the impact velocity became higher, as shown in Fig. 7.3. This value dropped finally to zero at the ballistic limit. On the other hand, as shown in Fig. 7.4, the absorbed energy, DE, was found to continuously follow the quadratic relationship and to reach the highest value also at the ballistic limit. Close investigation of the struck laminate reveals that the area of fiber bundle breakage increased when the impact velocity was slightly higher than the threshold, and that on the impact side of the fiber bundle, there was breakage due to permanent indentation of the laminate by the projectile. As the impact velocity became even higher, the fiber bundle breakage areas on both sides of the laminate remained approximately the same. However, comparing these areas with the delamination area, shown in Fig. 7.9, it was surprising to find that the delamination area was still proportional to the impact velocity even when the velocity was higher than the threshold corresponding to spalling damage. This demonstrates that it was not the delamination area that governed the residual stiffness of the struck laminate. Thus, the fiber bundle breakage associated with the spalling damage on the distal side of the laminate was considered to be the mechanism that affected the most of the residual stiffness of laminate.

7.6

Impact beyond the ballistic limit

7.6.1 Perforation The ballistic limit occurred when the projectile was struck at the laminate after impact, at which point the terminal velocity was equal to zero, and the impact period lasted forever. The force and velocity histories at the ballistic limit were very similar to that shown in Fig. 7.2(e) for Vi = 31.8 m s-1 except that the terminal velocity was equal to zero. When the impact velocity became higher than the ballistic limit, the terminal velocity was in the same direction as that of the impact velocity. Figure 7.2(f) shows a typical result for the case in which Vi = 36.2 m s-1. The velocity and force profiles were very similar to those shown in Fig. 7.2(e). The single force peak occurred right after the onset of contact between the projectile and the target, as expected. As impact proceeded, the velocity dropped quickly, but its rate of decrease became slower. It was found that the rate of decrease of the projectile velocity could be divided into two portions. In the first portion of the impact process, during roughly the first 0.5 ms after the onset of contact, the rate of decrease was very sharp. As the hemispherical part of the projectile perforated the laminate, the rate of decrease became much smaller, and the corresponding force was only several hundred Newtons.

IBF7 11/22/2000 6:43 PM Page 233

Impact behaviour and analysis of CFRP laminated plates

233

This force was considered to be the dynamic friction force between the projectile and the laminate, and was much smaller than the peak impact force. Meanwhile, the terminal velocity increased drastically again when the projectile velocity became even higher, as shown in Fig. 7.3. A simple equation was adopted to predict the terminal velocity of the projectile, Vt, when the initial striking velocity, Vi, was higher than the ballistic limit:19,20,46 0.5

Vt = (V02 - 2 * Es m)

[7.32]

where Es is the energy needed for an indentor to perforate a laminate under the quasi-static loading condition and m is the mass of the projectile. The predicted result is also plotted in Fig. 7.3. The correlation is considered to be satisfactory. As shown in Fig. 7.8, the absorbed energy was found to remain approximately the same regardless of the increasing velocity of the projectile. Thus, the laminate did not absorb extra energy in a perforated test run even if it was struck at a higher velocity.

7.6.2 Comparison with the quasi-static results To investigate the effect of the loading rate on the CFRP laminate when it is under lateral loading, results from both the impact test at the ballistic limit and the quasi-static contact test are plotted in Fig. 7.10. A similar comparison is also given in Fig. 8.5 of Chapter 8. A double peak phenomenon is observed in the quasi-static case. This is similar to the result observed by Lee and Sun and is attributed to delamination and the globally excessive deflection which occurred during the test.19 In Fig. 7.10, there is only a single peak for the impact test, and it is seen that the force increased at a much faster displacement rate before it reached the peak value. This is because the laminate deflection was very local when the laminate was struck by a projectile at a much higher loading rate. On the other hand, the relatively lower force peak shown for the impact case, as compared to the quasi-static counterpart, was considered to be due to the occurrence of spallation damage that reduced the laminate stiffness. This damage was induced by stress waves that reflected back from the distal side of the struck laminate immediately after the onset of contact between the projectile and the target. Thus, the loading rate effect is also considered to be noticeable for graphite/epoxy laminates under laterally applied loading.

7.7

Conclusions

A general overview for the impact behaviour of a projectile striking on a graphite/epoxy composite laminate has been reported. The laminates used were 6 inch ¥ 4 inch in their in-plane dimensions and 4.3 mm in thickness.

IBF7 11/22/2000 6:43 PM Page 234

234

Impact behaviour of composite materials and structures 5 Quasi-static Impact

Force (kN)

4

3

2

1

0 0

5

10

15

20

Displacement (mm)

7.10 The force vs displacement relationships for laminates under impact at the ballistic limit and under quasi-static loading conditions.

The projectiles employed had a hemispherical tip weighing 35.6 g in mass. The impact speeds were from 3.0 to 101.8 m s-1, where the ballistic limit of the laminates was found to be 35.5 m s-1. The kinetic energy of the projectile was provided by a gas gun. Two different boundary conditions were employed. The first one, which is considered to be perfect, was a free-free boundary. On the other hand, the second was clamping on two opposite sides of the laminate with the other two sides left free of support.This physically clamped boundary only approximated the perfect fixed-end condition although the boundary had been tightly clamped. When the laminate was struck, the velocity signals were measured in a non-contact manner by a developed transient laser Doppler anemometer (TLDA) system. The force and displacement histories for each impact run were then derived from the recorded velocity history, from which the initial and terminal velocities, the initial and the absorbed energy, and the force peak of the projectile were obtained.The struck laminates were then C-scanned to measure the delamination area. On the other hand, an analytical model has been presented in this chapter to predict the impact response of the projectile, and the effect of boundary imperfection was accounted for. Following is a summary of the revealed impact phenomena:

IBF7 11/22/2000 6:43 PM Page 235

Impact behaviour and analysis of CFRP laminated plates 1

235

Near elastic impact. When the impact velocity was low so that no damage was observed under visual inspection, even if a delamination damage area small in size was observed under C-scan when the velocity became higher, a multiple impact phenomenon was observed. The force history showed three peaks. The first had the highest value and occurred after the onset of contact between the projectile and the target, the second peak occurred when the projectile velocity reached zero, and the third peak happened when the laminate bounced back and struck the projectile. The terminal velocity of the projectile was linear to its impact velocity. Further, the maximum peak impact force in each test run also had a linear relationship with the impact velocity. 2 Prediction of projectile response under an imperfect boundary. An analytical method using the Ritz method along with the Mindlin plate theory was employed to predict the response of a laminated plate struck by projectiles at low velocities. The displacement field of the plate was represented by means of a series of beam functions that satisfied the boundary conditions of the plate. When the boundary conditions were perfect, such as a plate with a free boundary, the method could be experimentally verified, and the correlation was found to be very satisfactory. Then, when the laminated plate was physically clamped at two opposite sides, it has been found that the clamped boundary was neither fixed nor simply supported.To take this boundary imperfection into consideration, two beam functions corresponding to simple and fixed boundary conditions were combined, and a normalised rotational spring constant was employed to represent the actual rotational stiffness of the physically clamped boundary. In this study, this spring constant was obtained from the results of a quasi-static contact test. The satisfactory correlation between the prediction and the measured results demonstrates that the presented method is capable of predicting the impact response of a laminate with near-perfect boundaries. 3 Impact beyond the spallation threshold. When the impact velocity was higher than the spallation threshold, the laminae on the distal side of the struck laminates started to separate. This damage mechanism was considered to be due to stress waves reflected from the free surface on the distal side of the laminate, and was designated as spalling damage in this study. As the impact velocity continued to increase, a permanent indentation damage mechanism at the contact location was also observed in addition to spalling damage on the laminate distal side. A further increase of the impact velocity caused these two damage mechanisms to coincide, and the ballistic limit was observed at a speed of 35.5 m s-1. The three-force-peak phenomenon was found to gradually change to a single-force-peak impact phenomenon. This force peak occurred

IBF7 11/22/2000 6:43 PM Page 236

236

4

Impact behaviour of composite materials and structures

immediately after the onset of contact between the projectile and the target. The friction force between the cylindrical portion of the projectile and the perforated laminate was found to be only a small fraction of the peak impact force. On the other hand, the terminal velocity gradually decreased to zero as the impact velocity increased to the ballistic limit, whereas the force peak was found to remain essentially unchanged, and a linear relationship was observed between the delamination area and the impact velocity. Perforated impact. When the impact velocity became higher than the ballistic limit, perforation occurred. It was found that, whereas the terminal velocity increased drastically and approached the initial velocity of the projectile, other phenomena, such as the peak impact force and the delamination area, all remained the same regardless of the increase of the impact velocity. A simple equation was found to accurately predict the terminal velocity of the projectile.

In this study, the force versus the displacement relationships for laminates under impact and quasi-static loading conditions were also compared. The force peak for the laminate under impact occurred at a much lower displacement level. These different phenomena were considered to be mainly due to the more localised laminate response under impact conditions. Thus, the graphite/epoxy laminate was also sensitive to the rate of applied loading.

Acknowledgements This work was supported by the National Science Council of Taiwan, under Contract Numbers NSC 84-0424-E-002-004 and NSC 86-2212-E-002-087. It also represents a portion of the doctoral dissertation of the second author written in partial fulfillment of the requirements for the PhD degree at National Taiwan University. Supply of specimens and help in conducting the C-scan test provided by the Aeronautical Research Laboratory of the Chung-Shan Institute of Science and Technology, and especially by Mr Ming-Fa Shu, are gratefully acknowledged.

References 1 Abrate S, ‘Impact on laminated composite materials’, ASME Appl Mech Rev, 1991 44(2) 155–90. 2 Abrate S, ‘Impact on laminated composites: recent advances’, ASME Appl Mech Rev, 1994 47(11) 517–44. 3 Wu E and Liau J, ‘Impact of unstitched and stitched laminates by line loading’, J Composite Mater, 1994 28(17) 1640–58.

IBF7 11/22/2000 6:43 PM Page 237

Impact behaviour and analysis of CFRP laminated plates

237

4 Wu E and Wang J, ‘Behavior of stitched laminates under in-plane tensile and transverse impact loading’, J Composite Mater, 1995 29(11) 2254–79. 5 Wu E and Chang L C, ‘Loading rate effect on woven glass laminated plates by penetration force’, J Composite Mater, 1998 32(8) 702–21. 6 Liu D, ‘Impact-induced delamination – a view of bending stiffness mismatching’, J Composite Mater, 1988 22 674–92. 7 Wu E and Shyu K, ‘Response of composite laminates to contact loads and relationship to low-velocity impact’, J Composite Mater, 1993 27 1443–64. 8 Cantwell W J and Morton J, ‘The impact resistance of composite materials – a review’, Composites, 1991 22(5) 347–62. 9 Virostek S P, Dual J and Goldsmith W, ‘Direct force measurement in normal and oblique impact of plates by projectiles’, Int J Impact Eng, 1987 6 247–69. 10 Delfosse D, Pageau G, Bennett R and Poursartip A, ‘Instrumented impact testing at high velocities’, J Composites Technol Res, 1993 15(1) 38–45. 11 Gupta B P and Davids N, ‘Penetration experiments with fiberglass-reinforced plastic’, Exp Mech, 1966 6(9) 445–50. 12 Takeda N, Sierakowski R L and Malvern L E, ‘ Wave propagation experiments on ballistically impacted composite laminates’, J Composite Mater, 1981 15 157–74. 13 Takeda N, Sierakowski R L, Ross C A and Malvern L E, ‘ Delamination-crack propagation in ballistically impacted glass/epoxy composite laminates’, Exp Mech, 1982 22 19–25. 14 Cantwell W J and Morton J, ‘The influence of target geometry on the high velocity impact response of CFRP’, Composite Struct, 1988 10 247–65. 15 Cantwell W J and Morton J, ‘Comparison of the low and high velocity impact response of CFRP’, Composites, 1989 20(6) 545–55. 16 Cantwell W J and Morton J, ‘Impact perforation of carbon fibre-reinforced plastic’, Composites Sci Technol, 1990 38 119–41. 17 Zhu G, Goldsmith W and Dharan C K H, ‘Penetration of laminated kevlar by projectiles (I) experimental investigation’, Int J Solids Struct, 1992 29(4) 399–420. 18 Lee S-W R and Sun C T, ‘A quasi-static penetration model for composite laminates’, J Composite Mater, 1993 27 251–71. 19 Lee S-W R and Sun C T, ‘Dynamic penetration of graphite/epoxy laminates impacted by a blunt-ended projectile’, Composites Sci Technol, 1994 49 369–80. 20 Jenq S T, Jing H S and Chung C, ‘Prediction of the ballistic limit for plain woven glass/epoxy composite laminate’, Int J Impact Eng, 1994 15(4) 451–64. 21 Schonberg W P, Keer L M and Woo T K, ‘Low velocity impact of transversely isotropic beams and plates’, Int J Solids Struct, 1987 23(7) 871–96. 22 Cairns D S and Lagace P A, ‘Thick composite plates subjected to lateral loading’, ASME J Appl Mech, 1987 54 611–16. 23 Cairns D S and Lagace P A, ‘Transient response of graphite/epoxy and kevlar/epoxy laminates subjected to impact’, AIAA J, 1989 27(11) 1590–6. 24 Chao C C, Tung T P, Sheu C C and Tseng J H, ‘A consistent higher-order theory of lamimated plate with nonlinear impact modal analysis’, ASME J Vibrat Acoust, 1994 116 371–8. 25 Wu H Y T and Chang F K, ‘Transient dynamic analysis of laminate composite plates subjected to transverse impact’, Computer Struct, 1989 31(3) 453–66. 26 Lin H J and Lee Y J, ‘Impact-induced fracture in laminated plates and shells’, J Composite Mater, 1990 24 1179–99.

IBF7 11/22/2000 6:43 PM Page 238

238

Impact behaviour of composite materials and structures

27 Hertz H, ‘Uber die Beruhrung fester Elastischer Korper’, 1881 92 156–71, transl by Jones D E and Schott G A, London, MacMillan, 1896. 28 Tan T M and Sun C T, ‘Use of statical indentation laws in the impact analysis of laminated composite plates’, J Appl Mech, 1985 52 6–12. 29 Wu E, Chao J C and Yen C S, ‘Smooth contact of orthotropic laminates by rigid cylinders’, AIAA J, 1993 31(10) 1916–21. 30 Wu E and Yen C S, ‘The contact behavior between laminated composite plates and rigid spheres’, ASME J Appl Mech, 1994 61 60–6. 31 Yen C S and Wu E, ‘On the inverse problems of rectangular plates subjected to elastic impact, part 1: method development and numerical verification’, ASME J Appl Mech, 1995 62 692–8. 32 Yen C S and Wu E, ‘On the inverse problems of rectangular plates subjected to elastic impact, part 2: experimental verification and further applications’, ASME J Appl Mech, 1995 62 699–705. 33 Wu E, Yeh J C and Yen C S, ‘Impact on composite laminated plates: an inverse method’, Int J Impact Eng, 1994 15(4) 417–33. 34 Wu E, Yeh J C and Yen C S, ‘Identification of impact forces at multiple locations on laminated plates’, AIAA J, 1994 34(12) 2433–9. 35 Wu E, Tsai T D and Yen C S, ‘Two method for determining impact force history on elastic plates’, Exp Mech, 1995 35(1) 11–18. 36 Wu E, Tsai C Z and Tseng L H, ‘A deconvolution method for force reconstruction in rods under axial impact’, J Acoust Soc Am, 1998 104(3) 1418–26. 37 Wu E, Sheen H J, Chen Y C and Chang L C, ‘Penetration force measurement of thin plates by laser Doppler anemometry’, Exp Mech, 1994 38 93–9. 38 Tsai C Z and Wu E, ‘A transient laser Doppler anemometry to measure rapidly changed velocities of solid bodies’, Exp Mech, 1998 38 261–9. 39 Wu E, Tsai C Z and Chen Y C, ‘Penetration into glass/epoxy composite laminates’, J Composite Mater, 1994 28(18) 1783–802. 40 Wu E and Chang L C, ‘Woven glass/epoxy laminates subject to projectile impact’, Int J Impact Eng, 1995 16(4) 607–19. 41 Wu E and Jiang W S, ‘Axial crush of metallic honeycombs’, Int J Impact Eng, 1997 19(5–6) 439–56. 42 Durst F, Melling A and Whitelaw J M, Principles and Practice of Laser Doppler Anemometry, New York, Academic Press, 1976. 43 Drain L E, The Laser Doppler Technique, New York, Wiley, 1980. 44 de Boor C, A Practical Guide to Splines, Berlin, Springer, 1978. 45 Tsai C Z, ‘Development of the transient laser Doppler anemometry and applications to impact force measurements’, PhD dissertation, Institute of Applied Mechanics, National Taiwan University, Taiwan 1995. 46 Backman M E and Goldsmith W, ‘The mechanics of penetration of projectiles into targets’, Int J Engng Sci, 1978 16 1–99.

IBF8 11/22/2000 6:51 PM Page 239

8 Perforation of FRP laminates and sandwich panels subjected to missile impact S R REID AND H M WEN

8.1

Introduction

Composite structures such as fibre-reinforced plastic (FRP) laminates and sandwich panels made with such laminate skins and light-weight cores have great potential for use in aggressive environments. The high specific strength of composites can offer weight savings and their corrosion resistance gives advantage over traditional metallic materials. Such components, however, could be subjected to high speed impact by fragments resulting from the effects of the disintegration of nearby items of plant as well as low-velocity impact by dropped objects. Their response to such loading in the context of offshore applications has been studied extensively by the authors in recent years as part of the UK collaborative research programme on the Cost Effective Use of Fibre-Reinforced Composites Offshore. Most of this work has been summarised by the authors and their co-workers.1–3 Fibre-reinforced plastic laminates have also been considered for armour applications,4,5 glass fibres being more popular than other types of fibre such as Kevlar due to their cost advantage. The mechanics of deformation and failure of FRP laminates subjected to local impact loads is understood only for a few cases of simple geometrical form.4,5 Static indentation of thick composites with fibres in the form of woven fabrics by conical indenters has been modelled by Rutherford6 (see Reid et al.10) who used an energy approach to relate the force at a certain level of indentation to two strength parameters representing the in-plane and through-thickness strengths of the composites, respectively. A similar problem was also examined by Zhao et al.7 who employed transversely isotropic elastic analysis and rigid, perfectly-plastic material models. They showed that the latter led to a formula depending only on the in-plane strength of the material. This formula showed good agreement with tests on Scotch-ply laminates. The deformation mechanisms which occur during dynamic penetration and perforation of laminates have been examined by a number of authors.1–3,8–14 As indicated in Reid et al.,10 Greaves8,9 studied the deforma239

IBF8 11/22/2000 6:51 PM Page 240

240

Impact behaviour of composite materials and structures

tion mechanisms during ballistic perforation of thick S-2 glass/phenolic laminates by flat-faced projectiles and found that the failure can be divided into two phases. Phase 1 involves compression, shear, indentation and expulsion of debris. In phase 2 the formation of a cone of delaminations, fibre stretching and fracture occur and the projectile exits the back face. It was noted that the phase 1 indentation mechanism, said to be dominated by the through-thickness compressive resistance of the material, absorbed most of the impact energy and was therefore worthy of more detailed study. To this end, an investigation into the impact force-indentation characteristics of laminates at velocities of up to 200 m/s has been carried out by Reid et al.10 Zhu et al.11 investigated experimentally the penetration of laminated Kevlar29/polyester plates by conical-nosed projectiles and proposed a range of models for the various energy-absorbing mechanisms to estimate the target resistance to the projectile motion.12 The event of ballistic impact was divided into three consecutive stages: indentation, perforation and exit. The global structural deformations were determined using laminated plate theory. Dissipative mechanisms including indentation of the projectile tip, bulging of the back surface of the laminate, fibre failure, delamination and friction were described utilising certain simplifying assumptions. Good agreement was obtained between the model predictions and the experimental results. Lee and Sun13 carried out a combined experimental and numerical study on the dynamic penetration of clamped circular CFRP laminates by a 30 g, 14.5 mm diameter flat-ended projectile in the velocity range 24–91 m/s. The composite material examined was Hercules AS4/3501-6 graphite/epoxy and the stacking sequence of all the laminates was based on a basic pattern, namely [0/90/45/-45]s. Three types of impact tests were conducted on the graphite/epoxy laminates which had two thicknesses, 2 mm and 4 mm, and the ballistic limits were determined. The penetration process of composite laminates by a flat-ended missile consisted of three stages: predelamination, post-delamination before plugging and post-plugging. Based upon these three stages, a finite element model was established to simulate the static punch process. The material was modelled using effective moduli so that the details of the stacking sequence were not included in the model. The simulated static load-punch displacement curve was subsequently employed in the dynamic penetration analysis, and the displacements at certain specific checkpoints were adopted as the penetration criteria. It was shown that the computational results were in good agreement with the limited experimental data. More recently, Mines et al.14 conducted an experimental investigation into the high-velocity perforation behaviour of fully-clamped 200 mm ¥ 200 mm polymeric composite laminates at impact velocities of up to 571 m/s. Woven

IBF8 11/22/2000 6:51 PM Page 241

Perforation of FRP laminates and sandwich panels subjected

241

roving, z-stitched and through-thickness z-stitched glass polyester laminates for a number of laminate thicknesses (6, 12, 24 ply), three types of impactors (flat, hemispherical and conical), and two missile masses (6 g, 12 g) were examined. The results were presented in terms of static and impact perforation energies, and energy absorption mechanisms during high-velocity perforation were also discussed with a view to identifying improved combinations of materials. It was found that all types of construction behave in a similar manner. As far as sandwich structures are concerned, Moriarty and Goldsmith15 have recently conducted an experimental investigation into the dynamic energy absorption characteristics of sandwich shells, this work representing an extension of earlier work on flat sandwich panels.16 Aluminium or ABS (acrylonitrile–butadiene–styrene) were used for the skins and a variety of honeycomb materials for the cores of the sandwich constructions. The specimens were subjected to non-perforating impact by a 0.7045 kg, 76.2 mm diameter projectile with a slightly curved impact surface. The projectiles were fired pneumatically at speeds ranging from 16.5 to 19.05 m/s. At these low velocities, it was found that the core material dominates the response in the case of fully-clamped specimens. For the simply-supported samples, the skins (faceplates) dominated the performance characteristics, with the thicker aluminium skin giving significantly poorer results than either the thinner metal or the ABS facing. The effect of the core was more diffuse and was coupled more to the nature of the skin than for fully-clamped specimens. Other relevant investigations have been concerned primarily with the analysis and design of sandwich structures for quasi-static loading17–19 although Bernard and Lagace20 examined the impact resistance of composite sandwich panels and Kosza and Sayir21 studied failure patterns in the cores of sandwich beams and plates under impact loading. It is noted however that all of these studies of sandwich panels and components relate to relatively low impact velocities. This chapter presents some of the results of our own detailed study on the penetration and perforation of sandwich panels made of composite material skins with polymeric foam cores. Emphasis is placed on ballistic test results and associated deformation mechanisms are contrasted with those found in quasi-static penetration. General empirical models are given that provide the perforation energies of FRP laminates and sandwich panels consisting of FRP laminate skins and foam cores under lowvelocity impact by flat-faced, hemispherical-ended and conical-nosed indenters. A new model is developed for the so-called wave-dominated response/perforation of FRP laminates and sandwich panels with such laminates as skins and foam cores subjected to high-velocity impact by the three types of missile (flat, hemispherical and conical). The model predictions and the available test data are compared and discussed. The development

IBF8 11/22/2000 6:51 PM Page 242

242

Impact behaviour of composite materials and structures

of the high velocity perforation model complements and extends the discussion on the ballistic impact on FRP laminates and sandwich panels given recently in references.1–3

8.2

Experimental procedure

8.2.1 Materials and specimens E-glass woven roving (WR) cloth of 600 g/m2 area density with polyester resin (Crystic 491PA and Butanox M50 (1%) hardener) were chosen for the skins and expanded polymeric foam (e.g. PVC) cores were used, these being purchased in slab/sheet form. The manufacture of panels and preparation of specimens by hand lay-up and assembly are described in Wen et al.1 Square laminates and sandwich panels with side lengths of 0.9 m were prepared and some smaller panels of 0.3 m ¥ 0.3 m were cut from the larger panels for testing. Several triple-skinned (i.e. with a central laminate as well as the other skins) panels were manufactured using the same procedures. The behaviour of these latter panels is not discussed extensively herein (see Wen et al.1) but some of the test data will be included in the appropriate figures. Some of the properties of the materials used are given in Table 8.1 in which su, Es1, se and t13 are the tensile strength, Young’s modulus for inplane tension, the elastic limit for through-thickness compression and the transverse shear strength of the laminates, respectively, and sc, Ec, Gc and t are the compressive strength, Young’s modulus in compression, shear modulus and shear strength of the core materials, respectively. Typical nominal stress-strain curves for both GRP laminates and foam core are given in Fig. 8.1.

8.2.2 Loading and data recording In all the tests, panels were supported in specially designed frames, one with a 0.85 m square aperture (for the larger 0.9 m square panels) and the other with a 0.2 m square window (for smaller 0.3 m square panels). The supports were such that the out-of-plane movement of the edges of the panels was restrained but their in-plane movement was allowed (see Wen et al.1). Quasi-static indentation tests were conducted on a screw driven (RDP) testing machine operating under displacement control. Flat-ended, hemispherical-ended and conical-nosed indenters with different diameters (ranging from 5.25 mm up to 150 mm) were used in the experiments. All the indenters were case-hardened. The panels were loaded normal to their planes at the centre and the load versus punch displacement curves were

Source Scott Bader Source Strand Source Barracuda Barracuda Tensile tests

Resins Isopthalic polyester

Reinforcement E-Glass WR

Core material Divinycell H130 Divinycell HCP100

GRP skins

Table 8.1. Materials for sandwich panels

Average volume fraction = 43%

Density, thickness 130 kg m-3, 25 mm 400 kg m-3, 20 mm

Weight 600 g m-2

Type Crystic 491 PA

Ec 175 MPa 340 MPa Es1 = 24 GPa

sc 2.5 MPa 10.4 MPa su = 345 MPa se = 225 MPa

Cloth Woven roving

Catalyst/hardener Butanox M50 (1%)

t13 = 45 MPa

Gc 50 MPa 180 MPa

t 2 MPa 7.4 MPa

IBF8 11/22/2000 6:51 PM Page 243

Perforation of FRP laminates and sandwich panels subjected 243

IBF8 11/22/2000 6:51 PM Page 244

244

Impact behaviour of composite materials and structures 500

Stress (MPa)

400

300

200

100

0

1.6

0.8

2.4 3.2 Strain (%)

(a) 4

Stress (MPa)

3

2

1

0

0.1

0.2

0.3

0.4

0.5

0.6

Strain (b)

8.1 Nominal stress-strain curves: (a) GRP laminates in tension; (b) Divinycell H130 foam in compression; (c) GRP laminates in through-thickness compression.

recorded. The movements of the centres of the lower skins were also recorded on the larger panels during the tests using a suitable arrangement with an LVDT. The cross-head speed was 3 mm/minute for all the tests. Low-velocity impact tests were carried out using a drop weight apparatus. The tup was instrumented with an accelerometer (Bruel and Kjaer, type 4382) and the deceleration-time history was recorded using a Kontron digital event recorder (WW700) operating at a sampling rate of 106 samples

IBF8 11/22/2000 6:51 PM Page 245

Perforation of FRP laminates and sandwich panels subjected

245

500 450 400

Stress (MPa)

350 300 250 200 150 100 50 0 0.00

0.05

0.10

0.15

0.20

0.25

Strain (mm/mm) (c)

8.1 (cont.)

Pressure vessel

Solenold valve

Gun barrel

Specimen

Photocell unit

Holder Screens

Projectile catcher

Timer counters

8.2 Schematic diagram of the pneumatic gun facility.

per second. The direction of motion of the tup was controlled by pretensioned vertical guide ropes. The initial impact velocity was measured by means of a photocell system. Details of the results of these tests have been described elsewhere1 but some of the data are included in the relevant graphs to indicate the consistency in the behaviour of panels over a wide range of impact velocities. The fixtures for high speed ballistic impact tests and the pneumatic gun facility for firing the projectiles are shown schematically in Fig. 8.2. Three types of projectile end geometries referred to above were used but only two projectile diameters (10.5 mm and 45 mm) were chosen, the projectiles

IBF8 11/22/2000 6:51 PM Page 246

246

Impact behaviour of composite materials and structures

weighing approximately 18.0 g and 1.30 kg, respectively (see Wen et al.1 and Reddy et al.2 for details).

8.3

Experimental results

8.3.1 Quasi-static tests 8.3.1.1 Range of tests and general observations Details of the results of the quasi-static indentation experiments are given by Wen et al.1 It was found that most of the specimens failed by local indentation, penetration and perforation under the punches. One exception was the case of larger (0.9 m square) sandwich panels with 3.25 mm thick GRP skins and higher density foam core (Divinycell H100, density 400 kg/m3) loaded by 50 mm diameter flat or hemispherical indenters and those loaded by larger (150 mm) diameter indenters, all of which failed in a global bending mode. The other exception was the case of smaller (0.3 m square) sandwich panels with 3.25 mm thick GRP skins and higher density foam core (HCP100) loaded by a 20 mm flat-faced punch which failed by core shear. It was also found that sandwich panels loaded quasi-statically by hemispherical-ended indenters with radii equal to or greater than the thickness of the core required the least energy for complete penetration and for this reason particular emphasis was placed upon the results for this nose geometry.2 The details of the response to flat-ended indenters/projectiles are sufficiently different to warrant separate discussion and this has been given elsewhere.1,3 When the radii of the indenters were smaller than the core thickness, the energies for perforation by hemispherical, flat and conical punches were approximately the same. Flat-faced indenters Figure 8.3(a) shows typical quasi-static load-displacement characteristics for a 0.9 m square sandwich panel with 3.25 mm thick GRP skins and 25 mm thick Divinycell H130 foam core loaded centrally by a 50 mm diameter flatfaced indenter, which first failed by indentation. The load-punch displacement curve and the vertical moment of the bottom skin of the panel are indicated in the figure. The first part of the load-punch displacement trace (up to the top skin failure at the first peak load) is bilinear. Core crushing as evidenced by the difference between the punch and the bottom skin displacement starts just after the knee of this bilinear part. After top skin failure (by shear along the periphery of the punch) at the peak load, the load drops to about a third of its peak value, there was considerable further

IBF8 11/22/2000 6:51 PM Page 247

40 Flat

30

Load (kN)

Lower skin

20 Punch

10

0 0

20

40

60

80

100

120

Displacement (mm) (a) 40

Hemispherical

Load (kN)

30

Lower skin

Punch

20 F 10

0

20

40

60

80

100

Displacement (mm) (b)

8.3 Load-displacement characteristics for 0.9 m square 3.25 mm thick GRP skin sandwich panels loaded quasi-statically by 50 mm diameter indenters: (a) Twin-skinned panel with 25 mm thick H130 foam core; (b) twin-skinned panel with 25 mm thick H130 foam core; (c) twin-skinned panel with 50 mm thick H130 foam core; (d) triple-skinned panel with 25 mm thick H130 foam cores; (e) twinskinned panel with 25 mm thick H130 foam core; (f) cross-sectional view of identical panels loaded by flat-faced, hemispherical-ended and conical-nosed indenters (from bottom to top).

IBF8 11/22/2000 6:51 PM Page 248

248

Impact behaviour of composite materials and structures 20 Hemispherical Lower skin

15 Load (kN)

F

Punch

10

5

0

20

40

60

80

100

Displacement (mm) (c) Hemispherical B Lower skin

C Punch

Load (kN)

20

A 10

0

20

40

60 Displacement (mm) (d)

8.3 (cont.)

80

100

120

IBF8 11/22/2000 6:51 PM Page 249

Perforation of FRP laminates and sandwich panels subjected

249

30 Conical

Load (kN)

20 Punch

Lower skin

10

F

0 0

20

40

60

Displacement (mm) (e)

(f)

8.3 (cont.)

80

100

IBF8 11/22/2000 6:51 PM Page 250

250

Impact behaviour of composite materials and structures

deformation characterised by progressive core crushing, lower skin debonding and bending. The lower skin of the panel debonded gradually from the core and failed by fracturing due to bending of the debonded skin. Hemispherical-ended indenters Typical load-displacement characteristics for 0.9 m square sandwich panels with 3.25 mm thick GRP skins and 25 mm and 50 mm thick H130 foam cores loaded quasi-statically by a 50 mm diameter hemispherical-ended indenter are presented in Fig. 8.3(b) and (c), respectively. It can be seen that core crushing starts very soon after loading begins. The top skins failed by a central puncture causing four cruciform cracks, at points indicated by F in these two load-displacement curves. It is clear that the load-punch displacement responses are different. In Fig. 8.3(b) after the top skin failure, the load did not fall but rather increased steadily. This corresponded to the crushing of the core material, the lengthening of cracks in the top skin as well as bending of the flaps resulting from cracks. This was then followed by a more rapid rise in load until the bottom skin failed in bending. It should be noted here that in this test the core thickness was equal to the radius of the indenter so that the applied force directly acted on the lower skin before the indenter had completely penetrated the upper skin. By contrast the load-displacement curve in Fig. 8.3(c) shows double hump response. This response is associated with the larger ratios of core thickness, c, to punch diameter, D, (c/D > 0.5) which allows the top skin penetration to be completed before the bottom skin is loaded directly by the indenter through a layer of densified foam (Reddy et al.2). Good repeatability was observed for identical sandwich panels in terms of their load-displacement response. A typical example is shown in Fig. 8.3(b) in which the solid and broken lines represent the load versus punch displacement characteristics of two nominally identical panel tests. Figure 8.3(d) shows the load-displacement curve for a triple-skinned sandwich panel with three six-layer laminate skins of E-glass WR cloth reinforced polyester resin and two 25 mm thick H130 foam cores, loaded quasistatically by the 50 mm diameter hemispherical-ended indenter. Like the twin-skinned sandwich panels described above, core crushing occurs from the beginning of the loading process as can be seen from Fig. 8.3(d). The top skin failed by a central puncture causing four cruciform cracks at point A in the curve. After the top skin failure, the load dropped slightly and then increased steadily which corresponded to the crushing of the core, the lengthening of the cracks as well as the bending of the resulting petals in the top skin. This was then followed by a more rapid rise in load until the middle skin failed at point B. It is interesting to note here that up to the middle skin failure the load-displacement response of the triple-skinned

IBF8 11/22/2000 6:51 PM Page 251

Perforation of FRP laminates and sandwich panels subjected

251

panel was very similar to that of the double-skinned panel as shown in Fig. 8.3(c). After the middle skin failure, there was considerable further deformation which was characterised by progressive core crushing and the lower skin bending. At point C the lower skin fractured with the formation of four major cruciform cracks and perforation ensued. Conical-nosed punches Figure 8.3(e) shows typical load-displacement characteristics for a 0.9 m square sandwich panel with 3.25 mm thick GRP skins and 25 mm thick H130 foam core loaded quasi-statically by a 50 mm diameter conical-nosed indenter. After top skin failure just underneath the 2 mm radius nose tip (denoted by F in the figure), the load dropped slightly and then increased steadily to the maximum value. This second region was associated with the formation of major cruciform cracks and bending of the resulting flaps with bending hinges moving away from the loading point through the propagation of fractures and also overcoming the friction between the panel and the conical punch, all of which dissipated energy at an increasing rate. The bottom skin failed in bending accompanied by a small area of debonding. Figure 8.3(f) shows photographs of the cross-sectional views of the three identical 0.9 m square sandwich panels with 3.25 mm thick GRP skins and 25 mm thick H130 foam cores loaded quasi-statically by 50 mm diameter flat-faced, hemispherical-ended and conical-nosed indenters (from bottom to top). The top skin shear plugging and core crushing are evident with a flat punch, the other two look very similar to each other. All these cases are categorised as indentation failures. 8.3.1.2 Discussion Energies associated with three critical events in the penetration process of a twin-skinned sandwich panel loaded by flat-faced, hemispherical-ended and conical-nosed indenters can be found from the load-displacement curves as shown in Fig. 8.3(a), (b,c) and (e). These critical events are: (i) the energy to penetrate the top skin; (ii) the energy to penetrate (fracture) the bottom skin; and (iii) the energy to perforate the whole panel. It was found (Wen et al.1) that both the peak load at the failure of the top skin and the corresponding energy absorbed are approximately proportional to the weight of glass fibres in a skin, or equivalently, the thickness of the skin if the volume fraction is maintained the same. Similarly, the energies absorbed up to the failure (fracture) of the bottom skins of sandwich panels which fall into the same category (defined below) were also found to be linearly related to the weight of fibres or the thickness of skin (Wen et al.1 and

IBF8 11/22/2000 6:51 PM Page 252

252

Impact behaviour of composite materials and structures

Reddy et al.2). These observations indicate that laminate skins play a very important role in the failure and energy absorption of GRP skinned sandwich panels with foam cores, whilst the core thickness controls which category of behaviour occurs. The experimental results obtained for sandwich panels loaded quasistatically by hemispherical-ended indenters are presented in Fig. 8.4(a), which shows the plot of the non-dimensional penetration energy (Ef /suTD2) versus the non-dimensional geometric property (L/D). It is clear from Fig. 8.4(a) that, irrespective of panel side length (L), the quasistatic tests conducted on the sandwich panels using hemispherical-ended punches may be categorised into two groups, one group with H/D > 2, the other with H/D < 2, here H and D are the total panel thickness and the punch diameter, respectively. In the former case considerably more energy was absorbed as can be seen from Fig. 8.4(a). In order to dilineate the difference, panels were sectioned to study the mechanisms. The only obvious difference appeared to be that for the panels with H/D > 2 relatively more debonding between the lower skin and the foam core had occurred. This was found (Wen et al.1) generally to be one of the mechanisms enhancing the quasi-static energy absorbing capacity. On the other hand, the experimental data obtained for sandwich panels loaded quasi-statically by flat-faced punches are given in Fig. 8.4(b), which shows the plot of the non-dimensional global energy (Eg/suTD2) against the non-dimensional geometric property (L/D). It can be seen from Fig. 8.4(b) that all the data points follow the same trend irrespective of the ratios of H/D. Closer examination reveals that the plots of the non-dimensional global energy (Eg/suTD2) against the non-dimensional geometric property (L/D) for sandwich panels loaded quasi-statically by both flat-faced punches and hemispherical-ended indenters with H/D > 2 are almost identical, as can be deduced from Fig. 8.4(a) and (b). It may also be inferred from Fig. 8.4(b) that the energy absorbed by the global deformations of panels loaded by flat-faced punches is also approximately proportional to the thickness of the skin laminates. It should be mentioned here that the experimental results obtained for sandwich panels loaded quasi-statically by hemispherical-ended indenters can also be presented in terms of the plot of the non-dimensional global energy (Eg/suTD2) against the nondimensional geometric property (L/D), which is very similar to that given in Fig. 8.4(a). How to distinguish the global energy from the total penetration energy is discussed in Section 8.4.

8.3.2 Low-velocity impact tests Low-velocity tests will not be described or discussed in detail in this chapter (for details, see Wen et al.1). However, Fig. 8.5 shows a typical low-velocity

IBF8 11/22/2000 6:51 PM Page 253

Perforation of FRP laminates and sandwich panels subjected

253

Ef su TD 2 0.5

0.4

: t = 1.75 mm : t = 3.25 mm : t = 7.0 mm : Triple-skinned panel Open symbols: H/D < 2 Solid symbols: H/D > 2

0.3

Equation [8.5]

0.2

0.1

0

20

10

30

L D

40

(a) Eg su TD 2

0.6

D: t = 1.75 mm : t = 3.25 mm : t = 7.0 mm Open symbols: H D < 2 Solid symbols: H D > 2

0.4 Equation [8.7b]

0.2

0

10

20

30

40

L D

(b)

8.4 Variation of the non-dimensional penetration/global energies with the ratio of panel span to indenter diameter for sandwich panels loaded quasi-statically at the centre: (a) hemispherical-ended indenters; (b) flat-faced punches.

IBF8 11/22/2000 6:51 PM Page 254

254

Impact behaviour of composite materials and structures

30

Impact Load (kN)

20

10 Quasi-static

0

10

20

30

40

50

60

Displacement (mm)

8.5 Comparison between quasi-static and impact load-displacement characteristics for 0.9 m square sandwich panels with 3.25 mm thick GRP skins and 25 mm thick H130 foam core loaded by a 50 mm diameter hemispherical-ended punch.

impact load-displacement curve for a 3.25 mm thick GRP skin sandwich panel with 25 mm thick H130 foam core struck at 6.23 m/s by a 42.5 kg tup mass with an attached 50 mm diameter hemispherical indenter.1 Also shown in the figure is the corresponding quasi-static load-displacement curve for an identical panel. The lower skin of the panel subjected to dropped object loading fractured but was not completely penetrated. It was found that the fracture patterns as well as the load-deflection characteristics of the GRP skin sandwich panels loaded dynamically were similar to those observed in the corresponding quasi-static cases. It was also found that the extent of damage (judged by the extent of lower skin perforation) under dropped object loading was less than that observed in the identical panel under quasi-static loading even though the impact energy was about 20% higher than the corresponding quasi-static perforation energy. However, the extent of debonding between the lower skin and the core was larger in the impact tests. The dynamic load required to cause a given deflection is higher than the load required to cause the same deformation under quasi-static loading

IBF8 11/22/2000 6:51 PM Page 255

Perforation of FRP laminates and sandwich panels subjected

255

conditions (see Fig. 8.5). The changes are presumably the result of enhanced strengths and stiffnesses of the components due to rate-dependent material properties and inertia effects. The interplay between these and the core-skin bond strength will influence the balance between the various failure mechanisms in the panel and their respective contributions to energy absorption.

8.3.3 Ballistic impact tests 8.3.3.1 Range of tests and observations Ballistic impact tests were performed on 0.3 m square GRP laminates as well as sandwich panels with H130 foam core using 10.5 mm diameter projectiles with masses of approximately 19.0 g at impact velocities up to 305 m/s. Ballistic impact tests were also carried out on 0.9 m square twinskinned (as well as triple-skinned) panels using projectiles with a 45 mm diameter and masses of approximately 1.3 kg at impact velocities up to 102 m/s. Many tests were performed. Here we concentrate on presenting data for the critical impact conditions associated with the ballistic limit (velocity for full perforation of the projectile nose through the panel) for flat-faced, hemispherical-ended and conical-tipped projectiles. Figure 8.6(a) and (b) shows respectively the effects of total laminate skin thickness on the ballistic limits for 0.3 m and 0.9 m square sandwich panels struck by hemispherical-ended and conical-nosed missiles while Fig. 8.6(c) and (d) show respectively the same effects for 0.3 m and 0.9 m square sandwich panels struck by flat-faced projectiles. Plots of the variation in the residual velocity with impact velocity for 0.3 m square sandwich panels struck by hemispherical-ended conical-nosed projectiles are given in Fig. 8.6(e). It is seen from Fig. 8.6(a) to (d) that the ballistic limit is an increasing function of the total laminate thickness. Figure 8.6(a), (b) and (e) illustrates that the perforation processes for the hemispherical-ended and the conical-tipped projectiles used in the study are essentially the same in terms of ballistic limits and residual velocities. In order to observe the influence of skin thickness on the ballistic performance of sandwich panels, panels were sectioned. Figure 8.7(a) shows the cross-sectional view of 0.3 m square sandwich panels with 1.75 mm, 3.25 mm and 7.0 mm thick GRP skins and 25 mm thick H130 foam core, perforated by the 10.5 mm diameter hemispherical-ended missile at initial velocities well above their ballistic limits. It is evident from this figure that debonding between the lower skins and the core decreases with an increase in laminate thickness while delamination in the lower skins in particular increased with increasing laminate thickness. This is the reverse of the

IBF8 11/22/2000 6:51 PM Page 256

Vb (m s-1) D: conical : hemispherical

200

Equation [8.17] with G = 1.5

Equation [8.17] with G = 1.414 150 Equation [8.13] 100

50

0

4

8

12

16

T (mm) (a) Vb (m s-1) 100

: conical : hemispherical : triple-skinned panel

Equation [8.17] with G = 1.5

Equation [8.17] with G = 1.414

75

Equation [8.13] 50

25

0

4

8

12

16

T (mm) (b)

8.6 (a) Effects of total laminate thickness on the ballistic limits for 0.3 m square sandwich panels with GRP skins and 25 mm thick H130 foam core struck by 10.5 mm diameter hemispherical-ended and conical-nosed missiles. (b) Effects of total laminate thickness on the ballistic limits for 0.9 m square sandwich panels with GRP skins and 25 mm thick H130 foam core (two in the case of tripleskinned panel) struck by 10.5 mm diameter hemispherical-ended and conical-nosed missiles.

IBF8 11/22/2000 6:51 PM Page 257

Vb (ms-1) Flat 200

Equation [8.17]

Equation [8.13] 150

100

50

0

4

8

12

16

T (mm) (c) Vb (m s-1)

100

Flat

Equation [8.17]

70

Equation [8.13]

50

25

0

4

8

12

16

T (mm) (d)

8.6 (cont.) (c) Effects of total laminate thickness on the ballistic limits for 0.3 m square sandwich panels with GRP skins and 25 mm thick H130 foam core struck by a 10.5 mm diameter flat-faced projectile. (d) Effects of total laminate thickness on the ballistic limits for 0.9 m square sandwich panels with GRP skins and 25 mm thick H130 foam core struck by a 45 mm diameter flat-faced missile.

IBF8 11/22/2000 6:51 PM Page 258

258

Impact behaviour of composite materials and structures

Vr (ms-1)

200

D: t = 1.75 mm : t = 3.25 mm : t = 7.0 mm Open symbols: hemispherical Solid symbols: conical

150

100

50

0

50

100

150 Vi

200

250

300

(m s-1) (e)

8.6 (cont.) (e) Variation of the residual velocity with the initial impact velocity for 0.3 m square sandwich panels with GRP skins and 25 mm thick H130 foam core struck by 10.5 mm diameter hemispherical-ended and conical-nosed missiles.

behaviour of identical panels loaded quasi-statically by the same diameter punch, as shown in Fig. 8.7(b). The photographs in Fig. 8.8 show the effects of initial impact velocity on the behaviour of 0.3 m square sandwich panels with 1.75 mm thick GRP skins and 25 mm thick H130 foam core tested using the 10.5 mm diameter hemispherical-ended missile with impact velocities at and above the ballistic limit (approximately 100 m/s), as indicated in the figure. It is clear from this figure that debonding between the lower skins and the core decreased with increasing impact velocity whereas delamination within the lower skins increased with an increase in impact velocity. At an impact velocity of 163.9 m/s the delamination area was roughly circular in shape and its diameter was about eight times that of the missile, as can be seen from Fig. 8.8(d). 8.3.3.2 Discussion It was observed from the experiments described briefly in the previous sections that the dynamic perforation energies are higher than those under

IBF8 11/22/2000 6:51 PM Page 259

Perforation of FRP laminates and sandwich panels subjected

259

(a)

(b) 8.7 Cross-sectional views of 0.3 m square sandwich panels with GRP skins and 25 mm thick H130 foam core tested with a 10.5 mm diameter hemispherical-ended punch: (a) ballistic loading; (b) quasi-static loading, indicating the extent of delamination in the skins and debonding between the core and the bottom skin.

IBF8 11/22/2000 6:51 PM Page 260

260

Impact behaviour of composite materials and structures

(a)

(b)

(c)

(d)

8.8 Photographs of 0.3 m square sandwich panels with 1.75 mm thick GRP skins and 25 mm thick H130 foam core struck by a 10.5 mm diameter hemispherical-ended missile at different velocities. (a) Vi = 98 m s-1; (b) Vi = 120.5 m s-1; (c) Vi = 143.9 m s-1; (d) Vi = 163.9 m s-1.

quasi-static loading conditions. Figure 8.9(a), (b) and (c) shows plots of the dynamic enhancement factor, f, against impact velocity, Vi, for sandwich panels struck by hemispherical-ended projectiles for H/D ratios less than and greater than 2, and by flat-faced missiles (irrespective of the ratios of H/D), respectively. f is defined here as the ratio of the dynamic perforation energy for a panel to the energy absorbed up to the fracture of the lower skin of an identical panel under quasi-static loading. What it reflects is changes in energy absorbing mechanisms due to dynamic effects including inertia. Closer examination of Fig. 8.4(a) and Fig. 8.9(a) and (b) reveals that the products of the quasi-static penetration energy and the dynamic enhancement factor are nearly the same for sandwich panels with H/D > 2 and H/D < 2 especially at higher impact velocities. This means that at higher impact velocities the energy absorbing mechanisms are the same for sand-

IBF8 11/22/2000 6:51 PM Page 261

Perforation of FRP laminates and sandwich panels subjected f

261

: t = 1.75 mm : t = 3.25 mm : t = 7.0 mm Hemispherical

5

4

Equation [8.10]

3

2

1

0

25

50

75

100

125

Vi (m s-1) (a) f

D: t = 1.75 mm : t = 3.25 mm : t = 7.0 mm Hemispherical

3

Equation [8.10]

2

1

0

100

200 Vi ( m s

-1

)

(b)

8.9 Variation of the dynamic enhancement factors, f, with the initial impact velocity, Vi for sandwich panels. (a) Hemispherical-ended projectiles with H/D < 2; (b) hemispherical-ended projectiles with H/D > 2; (c) flat-faced missiles.

IBF8 11/22/2000 6:51 PM Page 262

262

Impact behaviour of composite materials and structures f

: t = 1.75 mm : t = 3.25 mm : t = 7.0 mm Flat

Equation [8.10]

3

2

1

0

150 Vi

300

(m s-1) (c)

8.9 (cont.)

wich panels irrespective of the H/D ratios and that the kinetic energy is mainly dissipated by the FRP laminate skins. The ratios of dynamic to quasi-static perforation energies versus impact velocity (in this case for 0.3 m square sandwich panels as noted above) are also given in Fig. 8.9(b) as open symbols. The latter illustrates the difference in the fracture and perforation energies for the smaller panels struck by hemispherical-ended projectiles when H/D > 2 which is why the fracture energies are used. It should be noted that for all the 0.9 m square panels loaded quasi-statically by a 50 mm diameter hemispherical-headed indenter the perforation energy and the energy absorbed up to the fracture of the lower skin of the panels are almost identical (Wen et al.1). Therefore, these two ratios are equivalent to each other in Fig. 8.9(a) as designated by the solid symbols. The half-solid symbols in this figure represent the experimental data for the 0.9 m square sandwich panels subjected to low speed impact (dropped object) loading, where the panels were not totally perforated, while the open symbol in Fig. 8.9(c) represent the test result for a 0.9 m square sandwich panel under dropped object loading, where the lower skin of the panel was not penetrated but debonded from the core in a large area (Wen et al.1). It is apparent from Fig. 8.9(a) and (c) that initially the dynamic enhancement factor increases with increasing impact velocities, while it is seen from Fig. 8.9(b) (where only the results of higher velocity impact tests are shown) that the dynamic enhancement factor is independent of the impact veloci-

IBF8 11/22/2000 6:51 PM Page 263

Perforation of FRP laminates and sandwich panels subjected

263

ties. These results imply that there exists a transition velocity below which the dynamic enhancement factor is linearly related to initial impact velocity and above which it is a constant. For the tests performed this velocity is approximately 80 m/s. It should be mentioned here that similar observations can be made for conical-nosed projectiles.

8.4

Model development

Based on the experimental observations and discussions made in the previous sections and elsewhere,1–3 ballistic impact on fibre-reinforced polymer laminates and sandwich panels with such laminates as skins and foam cores may be categorised into two regimes, namely, low velocity impact and wavedominated response. In the former case global response as well as local deformations/failure are simultaneously present while in the latter case local deformations/failure dominate. Two semi-empirical modelling methods are described. One uses the dynamic enhancement factor to scale the quasi-static behaviour and encompass the whole range of perforation/ballistic data. The other (wave-dominated) model is based upon a local mechanism alone and incorporates inertial effects in a simplified manner.

8.4.1 Low-velocity impact 8.4.1.1 Empirical formulas for quasi-static penetration energy The principle of dimensional analysis is used here to derive the empirical formulas for quasi-static penetration energies. Based on the observations made on the experimental data, it is reasonable to assume that the energy absorbed up to the fracture (penetration) of the lower skin by a sandwich panel with FRP laminate skins and foam core loaded quasi-statically by an indenter can be divided into two parts, in a similar manner to the procedure suggested by Wen and Jones.22 One part is associated with the energy absorbed by local deformations, El, and the other, Eg, is related to the energy dissipated by global deformations of the panel. Thus1–3 Ef = El + Eg

[8.1]

where Ef is the energy absorbed up to the fracture (penetration) of the lower skin of the sandwich panel. Hemispherical-ended indenters It is assumed that, in the case of a sandwich panel loaded by a hemispherical-ended indenter, the local energy, El, can be estimated by the fragmentation energy given by

IBF8 11/22/2000 6:51 PM Page 264

264

Impact behaviour of composite materials and structures E1 =

pD2Ts u e f 8

[8.2]

in which su, ef, D and T are the failure stress (UTS) and the fracture strain of the laminates in tension, indenter diameter and total laminate thickness, respectively. If the indenter diameter, D, is taken as a characteristic length, then standard techniques of dimensional analysis indicate that the energy absorbed by global structural response, Eg, when normalized with respect to suD3 can be related to the geometric properties of the punch and the panel by a relationship of the following form1–3 b1

Eg L T = AÊ ˆ Ê ˆ 3 Ë ¯ Ë D D¯ suD

b2

[8.3]

Substituting El and Eg in equations [8.2] and [8.3] into equation [8.1] and rearranging gives b1

Ef L T pe f Ê T ˆ = + AÊ ˆ Ê ˆ 3 Ë ¯ Ë ¯ Ë 8 D D D¯ suD

b2

[8.4]

here A, b1 and b2 are constants which are to be determined from experiments. For FRP skin sandwich panels with foam cores loaded quasi-statically by hemispherical-ended indenters it is found (Wen et al.,1 also see discussion in Section 8.3.1.2) that Ef is linearly related to the thickness of the skin laminates. Hence, b2 in equation [8.4] can be taken as unity. Equation [8.4] can thus be rewritten in the following form Ef L pe f = + AÊ ˆ 2 Ë 8 D¯ s uTD

b1

[8.5]

Flat-faced punches It is assumed that, in the case of a sandwich panel loaded by a flat-faced punch, the local energy, viz. the first term on the right hand side of equation [8.1], can be estimated by the following expression 2

E1 p Ks c ˆ Ê c ˆ p t13 ˆ Ê T ˆ Ê t ˆ pe f Ê t ˆ = Ê ed + Ê + 2 Ë ¯ Ë ¯ Ë ¯ Ë ¯ Ë ¯ 4 s T 2 s D T 8 ËT ¯ s uTD u u

[8.6]

in which the first, second and last terms on the right hand side of equation [8.6] represent the energies dissipated by the core crushing, the upper skin shear plugging and the fragmentation energy of the lower skin of the panel, respectively. K is the constraint factor usually taken to be 2 (Wen et al.1) and t13 and sc are the transverse shear strength of the skin laminates and

IBF8 11/22/2000 6:51 PM Page 265

Perforation of FRP laminates and sandwich panels subjected

265

the compressive strength of the core, respectively. ed is a measure of densification of the foam core, which may be determined experimentally, as discussed in Section 8.5. The energy dissipated by the global deformations of the panel may be estimated in a similar manner to that described above for a hemisphericalended indenter. Thus, b3

Eg L T = BÊ ˆ Ê ˆ 3 Ë ¯ Ë D D¯ suD

b4

[8.7a]

here B, b3 and b4 are constants which are to be determined from experiments. For FRP skin sandwich panels with foam cores loaded quasi-statically by flat-faced punches it is found (see discussion in Section 8.3.1.2) that Eg is approximately proportional to the thickness of the skin laminates. Therefore, b4 in equation [8.7a] can be taken as unity. Equation [8.7a] can thus be recast into the following form Eg L = BÊ ˆ Ë D¯ s uTD2

b3

[8.7b]

Substituting equations [8.6] and [8.7b] into equation [8.1] yields Ef p Ks c ˆ Ê c ˆ p t13 ˆ Ê T ˆ Ê t ˆ = Ê ed + Ê 2 4 Ë su ¯Ë T ¯ 2 Ë s u ¯ Ë D¯ Ë T ¯ s uTD +

pe f Ê t ˆ L + BÊ ˆ Ë ¯ Ë 8 T D¯

2

b3

[8.8]

8.4.1.2 Dynamic enhancement factor On the basis of the observations made regarding the experimental results (Section 8.3.3.2), the impact perforation energy, Epi, of a sandwich panel struck transversely by a projectile may be written as Epi = fEf

[8.9]

where f is the dynamic enhancement factor which may be expressed in the following form Vi f = 1 + bÊ ˆ Ë Vo ¯

(Vi < Vo )

[8.10a]

f = 1+b

(Vi > Vo )

[8.10b]

where b is an empirical constant. Here, Vo is the transition velocity. The data acquired in the test programme suggest that this is given by

IBF8 11/22/2000 6:51 PM Page 266

266

Impact behaviour of composite materials and structures Es1 ef rt

Vo = Ce f =

[8.10c]

in which C is the speed of sound in the laminates along the fibre direction; rt and Es1 are the density and the in-plane Young’s modulus of the laminates, respectively. Equation [8.10c] is the Karman critical velocity, the uniaxial impact velocity above which tensile deformation cannot be transmitted away from the loading point because the material has fractured and, perhaps coincidentally, is approximately 80 m/s for the material properties of the laminates used. The rationale for using this critical velocity for transverse impacts needs to be explored further. Combining equations [8.5], [8.8] and equation [8.9] yields Epi p L = e f + AÊ ˆ 2 Ë 8 D¯ fs uTD

b1

[8.11]

for hemispherical-ended projectiles, and Epi p Ks c ˆ Ê c ˆ p Ê t13 ˆ Ê T ˆ Ê t ˆ = Ê ed + 2 Ë ¯ Ë ¯ 4 su T 2 Ë s u ¯ Ë D¯ Ë T ¯ fs uTD L pe f Ê t ˆ + + BÊ ˆ Ë ¯ Ë 8 T D¯

b3

2

[8.12]

for flat-faced missiles. Finally, from the above equations an approximate expression can be obtained for the ballistic limit, Vb, by assuming that the critical projectile kinetic energy is equal to Epi, the energy for perforation. Thus, 1

2 Epi ˆ 2 Vb = Ê Ë G ¯

[8.13]

where G is the projectile mass.

8.4.2 Wave-dominated response 8.4.2.1 Assumption about the resistive pressure As discussed previously, for the wave-dominated response the deformations will be localised and the through-thickness strength of the FRP laminates will be enhanced by dynamic effects such as inertia and wave propagation. The nose shape of missiles also has an effect on the ballistic perforation process. In the following, a simple model is proposed for the high speed perforation of FRP laminates by missiles with different nose shapes. It is assumed that the mean pressure (s) applied normally to the surface of the missile provided by an FRP laminate target material to resist penetration

IBF8 11/22/2000 6:51 PM Page 267

Perforation of FRP laminates and sandwich panels subjected

267

and perforation by a missile can be decomposed into two parts, one part is the cohesive static resistive pressure (ss) due to the elastic-plastic deformations of the laminate material and the other is the dynamic resistive pressure (sd) arising from velocity effects. Thus23 s = ss + sd

[8.14]

If it is further assumed that the cohesive static resistive pressure is equal to the static linear elastic limit (se) in through-thickness compression of the FRP laminates,1,10 i.e. ss = se, and that the dynamic resistive pressure (sd) is a function of the parameter (rt/se)1/2Vi and is taken to be sd = G(rt/se)1/2Vise,23 then equation [8.14] can be rewritten as rt ˘ È s = Í1 + G Vi s e s e ˙˚ Î

[8.15]

Here rt and Vi are the density of the FRP laminates and the initial impact velocity of the missile, respectively. G is a constant which is determined empirically. In Wen,23 by curve-fitting the perforation data, G has been evaluated to be 2, 1.5 and 2 sin(q/2) for flat-faced, hemispherical-ended and conical-nosed missiles, respectively. Here q is the cone angle of a conical-nosed projectile.

8.4.2.2 Perforation of FRP laminates/sandwich panels The ballistic limit condition for FRP laminates and sandwich panels with such laminates as skins and with foam core struck transversely by a rigid missile with different nose shapes can be estimated from energy consideration. It is easy to show that Ek =

pD2Ts pD2T È rt ˘ = Vb s e 1+ G s e ˙˚ 4 4 ÍÎ

[8.16]

Substituting Ek = (1/2)GVb2 into the above equation and rearranging yields Vb =

pG r t s e D2T 4G

8G È ˘ ÍÎ1 + 1 + pG 2 r D2T ˙˚ t

[8.17]

where Vb is the critical impact velocity or ballistic limit.

8.5

Comparisons and discussion

The four constants, viz. A, b1 in equation [8.5] and B, b3 in equation [8.7] are determined by a curve-fitting technique using the test data obtained from the experimental programmes. As noted earlier in Section 8.3.1, all the quasi-static tests performed on sandwich panels by hemispherical-

IBF8 11/22/2000 6:51 PM Page 268

268

Impact behaviour of composite materials and structures

ended indenters thus far can be classed into two groups (see Fig. 8.4(a)) depending upon the ratio of the total panel thickness to punch diameter, H/D. ef in equation [8.5] is taken to be 0.021.1 For H/D < 2, A = 0.05, b1 = 1/3; for H/D > 2, A = 0.016, b1 = 1. Figure 4(a) shows how equation [8.5] correlates with the experimental data with these values of A and b1. On the other hand, all the quasi-static tests conducted on sandwich panels by flat-faced punches, as shown in Fig. 8.4(b), followed the same trend irrespective of the ratios of H/D. The data points for the global energy (Eg) presented in Fig. 8.4(b) are calculated using equation [8.1] and equation [8.6]. ed in equation [8.6] is taken to be 0.8 for H130 foam core employed in the tests, which may be estimated from the load-displacement characteristics as shown in Fig. 8.3(a) (from which it can be seen that the 25 mm thick foam core crushed about 20 mm when the bottom skin of the sandwich panel failed. Hence, ed = 20/25 = 0.8). It can be shown that the two constants, namely, B and b3 in equation [8.7] can be estimated to be B = 0.016 and b3 = 1. It should be noted here that these two values are the same as those for sandwich panels loaded by hemispherical-ended indenters with H/D > 2. It is seen from Fig. 8.4(b) that equation [8.7] with these two values is in good correlation with the experimental data. Equation [8.10] has been fitted to the available experimental results presented in Fig. 9(a), (b) and (c). rt and Es1 in equation [8.10c] are taken to be 1650 kg/m3 and 24 GPa, respectively (Wen et al.1). Substituting these values and ef = 0.021 into equation [8.10c] gives Vo = 80 m/s. The empirical constant, b, in the equation has been evaluated to be b = 4.5 and 1.5 for sandwich panels struck by hemispherical-ended projectiles with H/D < 2 and H/D > 2, respectively. For sandwich panels impacted by flat-faced missiles b has been evaluated to be b = 1.5. As can be seen from Fig. 8.9, with these values for b, there is good correspondence between equation [8.10] and the test data. Comparisons are made in Fig. 8.6(a) and (b) between the model predictions (equations [8.13 and [8.11]) and the experimental results obtained for GRP skin sandwich panels with H/D > 2 and H/D < 2 struck normally by hemispherical-ended projectiles. In Fig. 8.6(a) the solid line is the predictions of equation [8.13] with A = 0.016, b1 = 1 and b = 1.5, whilst in Fig. 8.6(b) the solid line represents equation [8.13] with A = 0.05, b1 = 1/3 and b = 4.5. It is clear from these two figures that the model predictions (equations [8.13] and [8.11]) fit the experimental results with good accuracy. Comparisons are also made in Fig. 8.6(c) and (d) between the model predictions (equations [8.13] and [8.12]) and the test data obtained for sandwich panels impacted by flat-faced missiles. The solid lines are the predictions of equation [8.13] with B = 0.016, b3 = 1 and b = 1.5. It is seen

IBF8 11/22/2000 6:51 PM Page 269

Perforation of FRP laminates and sandwich panels subjected

269

from Figs. 8.6(c) and (d) that the model (equations [8.13] and [8.12]) fits well with the experimental data. Figure 8.6(e) shows the experimental plots of the residual velocity versus impact velocity for 0.3 m square sandwich panels with H130 foam core impacted by a 10.5 mm diameter hemispherical-headed missile with a mass of 17.9 g at velocities up to 305 m/s. Also shown in Fig. 8.6(e) as solid lines are predictions based upon 1

Vr = (V 2i - V b2 ) 2

[8.18]

where Vr and Vi are the residual and incident impact velocities of the missile, respectively and Vb is the ballistic limit which is determined by equation [8.13]. It is evident from Fig. 8.6(e) that the model predictions are in good accord with the experimental observations. As noted earlier, the difference of the energies absorbed by identical sandwich panels loaded by hemispherical-ended indenters and conicalnosed punches are negligibly small and therefore the equations derived above for hemispherical indenters may also be applicable for conical punches. Indeed, as can be seen from Fig. 8.6(a), (b) and (e), good agreement is also obtained between the model predictions and the experimental data for sandwich panels struck by conical-nosed projectiles which are represented by the triangle (D) in Fig. 8.6(a) and (b) and the solid symbols in Fig. 8.6(e). Figures 8.10(a) and (b) show photographs of two identical panels with 7.0 mm thick GRP skins and 25 mm thick H130 foam core tested with 10.5 mm diameter hemispherical-ended and conical-nosed missiles at impact velocities of 199 m/s and 197 m/s, respectively which lend further support to the above argument. To a first approximation, the equations developed above may also be applied or adapted to monolithic FRP laminates subjected to missile impact and have been checked against published data on FRP laminates. For hemispherical-ended and conical-nosed projectiles the empirical constants in the appropriate equations are found to be A = 0.05, b1 = 1/3, b = 4.5 for simply-supported single laminates using the data presented above for panels with H/D < 2 and A = 0.016, b1 = 1, b = 4.5 for fully-clamped monolithic laminates using the data reported by Zhu et al.11 Figure 8.11(a) shows comparisons between equation [8.13] (solid line) and the test data for simply-supported GRP single laminates struck transversely by the 10.5 mm diameter hemispherical-ended projectile of 17.9 g mass. It is evident from Fig. 8.11(a) that the model predictions are in good agreement with the experimental data. Figure 8.11(b) demonstrates the comparison between equation [8.13] (solid line) and the experimental results for fully-clamped KFRP single laminates subjected to impact by a 12.7 mm diameter conical-nosed missile with a mass of 28.9 g, reported by

IBF8 11/22/2000 6:51 PM Page 270

(a)

(b) 8.10 Photographs of two 0.3 m square sandwich panels with 7.0 mm thick GRP skins and 25 mm thick H130 foam core tested with 10.5 mm diameter projectiles. (a) hemispherical-ended projectile at an impact velocity of 199 m s-1; (b) conical-nosed missile at an impact velocity of 197 m s-1.

IBF8 11/22/2000 6:51 PM Page 271

Perforation of FRP laminates and sandwich panels subjected

271

Vb (m s-1) Hemispherical

180

Equation [8.17]

120

Equation [8.13]

60

0

2

4

6

T (mm) (a) Vb (m s-1)

Conical

180

Equation [8.13]

Equation [8.17]

120

60

0

2

4

6

8

10 T (mm)

12

14

(b)

8.11 (a) Comparison of the model predictions with the experimental results for simply-supported GRP single laminates struck by a 17.9 g, 10.5 mm diameter hemispherical-ended missile. (b) Comparison of the model predictions with the test data for fully-clamped KFRP monolithic laminates impacted by a 28.9 g, 12.7 mm diameter conical-nosed missile. (After Zhu et al.11) (c) Comparison of the model predictions with the experimental data for simply-supported GRP single laminates struck by a 20.4 g, 10.5 mm diameter flat-faced missile.

IBF8 11/22/2000 6:51 PM Page 272

272

Impact behaviour of composite materials and structures Vb (m s-1) Flat

Equation [8.17]

100

Equation [8.13] 50

0

1

2

3 T (mm)

4

(c)

8.11 (cont.)

Zhu et al.11,12 It is seen from Fig. 8.11(b) that equation [8.13] gives a good fit to the test data reported by those authors when A = 0.016, b1 = 1 and b = 4.5 are used. For flat-faced missiles the appropriate equations developed previously for sandwich panels may be adapted directly to single FRP laminates. It has been observed experimentally that, depending upon the ratio of laminate thickness to missile diameter, either shear plugging (plus delamination) or shear plus tensile fracture (plus delamination) are the predominant failure mechanisms in the perforation of monolithic FRP laminates subjected to impact by flat-ended projectiles. It is further assumed that this critical value for T/D is to be determined empirically and may be taken as 1/4. Thus, one obtains Epi L p t13 ˆ Ê T ˆ = Ê + 0.016Ê ˆ 2 Ë ¯ Ë ¯ Ë 2 su D D¯ fs uTD

[8.19]

for T/D £ 1/4 (i.e. thin single FRP laminates), and Epi p t13 ˆ È 1 1 Ê D ˆ ˘ p e f = Ê + 2 2 Ë s u ¯ ÍÎ 2 16 Ë T ¯ ˙˚ 8 fs uTD

1 Ê Dˆ ˘ È Ê Lˆ ÍÎ1 - 4 Ë T ¯ ˙˚ + 0.016Ë D ¯ [8.20]

for T/D >1/4 (viz. thick monolithic FRP laminates). Figure 8.11(c) shows the comparison of equation [8.13] which incorporates equation [8.19] (solid line) with the limited test data obtained for simply-supported single GRP laminates struck by a 20.4 g, 10.5 mm diame-

IBF8 11/22/2000 6:51 PM Page 273

Perforation of FRP laminates and sandwich panels subjected

273

ter flat-faced projectile. It is seen from Fig. 8.11(c) that the model predictions are in good agreement with the limited experimental data. Figures 8.12–8.14 show comparisons of equation [8.13] with the recently obtained high velocity perforation data for glass fibre-reinforced polymeric laminates struck transversely by flat-faced, hemispherical-ended and conical-nosed (90° cone) missiles, respectively. It is seen from Fig. 8.12 that equation [8.13] incorporating equation [8.20] (solid line) predicts well the ballistic limits at relatively low velocities but underpredicts the ballistic limits at higher velocities for the GRP laminates subjected to impact by flat-faced missiles. It is also seen from Fig. 8.13 and 8.14 that equation [8.13] incorporating equation [8.11] (solid line) overpredicts the ballistic limits compared to the experimentally obtained values for the GRP laminates when struck by hemispherical-ended and conical-nosed projectiles. The predictions by the newly developed wave-dominated model for high velocity perforation of FRP laminates/sandwich panels are also presented in Fig. 8.6(a–d), Fig. 8.11(a) and (c) and Figs. 8.12–8.14. In the theoretical calculation,1 rt = 1650 kg/m3, se = 225 MPa and G has been evaluated to be G = 2, 1.5 and 2 sin(q/2) for flat-faced, hemispherical-ended and conicalnosed missiles, respectively.23 Here q is the cone angle of a conical-nosed missile. It is clear from Fig. 8.5(a–d) and Fig. 11(a) and (c) that the high velocity perforation model, equation [8.17], is in reasonable agreement with the experimental data.1 It is also clear from Fig. 8.12–8.14 that equation [8.17] predicts well the high velocity perforation of the GRP laminates examined in Mines et al.14 The high velocity perforation model is also compared in Fig. 8.11(b) with the ballistic perforation of KFRP laminates impacted by a 28.9 g, 12.7 mm diameter conical-nosed missile investigated in Zhu et al.11 In the theoretical calculation, rt = 1231 kg/m3, se = 145 MPa and q = 60°.11 It is seen from Fig. 8.11(b) that the model predictions (equation [8.17]) are in good agreement with the test results. The applicability of the models is dictated by the range of impact parameters examined in the present investigations. For example, the range of impact velocities studied lies between 0 and 305 m/s from which the empirical models have been derived. Furthermore, the empirical constants in the models have mainly been determined from the present experiments conducted on GRP laminates and sandwich panels with such laminates as skins and with foam cores and, strictly speaking, these constants are valid only for the material systems investigated. Therefore, care should be exercised when the model with these empirical constants is applied to other material systems though it has been shown to give good representation for KFRP laminates. From the comparisons between the empirical models and the high veloc-

IBF8 11/22/2000 6:51 PM Page 274

274

Impact behaviour of composite materials and structures

6 g Flat woven

700

6 g Flat Z-stitch

Vb (m s-1)

600 500

Equation [8.17]

400 300

Equation [8.13]

200 100 0

0

0.5

1.0

1.5 T/D

2.0

2.5

(a) 12 g Flat woven

500

12 g Flat Z-stitch

Vb (m s-1)

400

Equation [8.13]

300

200 Equation [8.17] 100

0

0

0.5

1.0

1.5

2.0

2.5

T/D (b)

8.12 Comparison of the model predictions with the experimental data for fully-clamped GRP single laminates struck by a 7.6 mm diameter flat-faced missile. (a) G = 6 g; (b) G = 12 g. (After Mines et al.14)

IBF8 11/22/2000 6:51 PM Page 275

Perforation of FRP laminates and sandwich panels subjected

700

275

6 g Hemisphere woven 6 g Hemisphere Z-stitch

600 Equation [8.13]

Vb (m s-1)

500 400

Equation [8.17]

300 200 100 0 0

0.5

1.0

1.5

2.0

2.5

T/D (a)

12 g Hemisphere woven

500

12 g Hemisphere Z-stitch

Vb (m s-1)

400

Equation [8.13]

300

200 Equation [8.17] 100

0 0

0.5

1.0

1.5

2.0

2.5

T/D (b)

8.13 Comparison of the model prediction with the experimental data for fully-clamped GRP single laminates struck by hemispherical missiles. (a) D = 10 mm; G = 6 g; (b) D = 7.6 mm, G = 12 g. (After Mines et al.14)

IBF8 11/22/2000 6:52 PM Page 276

276

Impact behaviour of composite materials and structures

700

6 g Cone woven 6 g Cone Z-stitch

600 Equation [8.13] Vb (m s-1)

500 400 300

Equation [8.17]

200 100 0

0

0.5

1.0

1.5

2.0

2.5

T/D (a)

12 g Cone woven 12 g Cone Z-stitch

500

Vb (m s-1)

400

Equation [8.13]

300

200 Equation [8.17] 100

0 0

0.5

1.0

1.5

2.0

2.5

T/D (b)

8.14 Comparison of the model predictions with the experimental data for fully-clamped GRP single laminates struck by a 7.6 mm diameter conical-nosed missile. (a) G = 6 g; (b) G = 12 g. (After Mines et al.14)

IBF8 11/22/2000 6:52 PM Page 277

Perforation of FRP laminates and sandwich panels subjected

277

ity perforation model and the available experimental data there exists a critical condition at which a change takes place in the mode of deformation from global response (low velocity impact) to localized deformation (wave-dominated response). It is very difficult to determine the critical condition either theoretically or experimentally, and this needs to be further investigated in a future study.

8.6

Conclusions

The results of quasi-static, drop-weight and ballistic impact tests performed on triple- as well as twin-skinned sandwich panels and single laminate skins using flat-faced, hemispherical-ended and conical-nosed indenters/projectiles with initial impact velocities up to 305 m/s have been briefly reported and discussed. Typical load-displacement characteristics under quasi-static and dropped object loading have been presented. Ballistic limits (perforation energies) have been determined and a classification of the responses deduced from the test data obtained. Experimental evidence has shown that ballistic impact on FRP laminates and sandwich panels with such laminates as skins and with foam cores may be categorized into two regimes, viz. low velocity impact and wavedominated response. Based on the experimental observations, dimensional analysis has been used to derive empirical equations that predict the penetration and perforation energies of fibre-reinforced plastic (FRP) laminates and sandwich panels with such laminates as skins and with foam cores subjected to quasistatic and impact loading by flat-faced and hemispherical-ended indenters. It is shown that the empirical formulas correlate well with the available data from experiments carried out by the authors and others. It is also shown that, to a first approximation, the formula obtained for hemisphericaltipped indenters is applicable to conical-nosed punches. A new model has also been developed for the high velocity perforation of FRP laminates and sandwich panels struck transversely by flat-faced, hemispherical-ended and conical-nosed missiles. It is found that the model predictions are in good agreement with the recently published14 high velocity perforation data. Future investigation should be directed towards clearly defining the respective ranges of impact parameters for which the models developed in Sections 8.4.1 (i.e. low velocity impact) and 8.4.2 (wave-dominated response/high velocity perforation) apply and engaging in detailed modelling of the range of failure mechanisms which control the failure of the laminates. Such investigation should lead to a methodology for optimising the design of FRP laminates and sandwich panels against impact loading.

IBF8 11/22/2000 6:52 PM Page 278

278

Impact behaviour of composite materials and structures

References 1 Wen H M, Reddy T Y, Reid S R and Soden P D, ‘Indentation penetration and perforation of composite laminates and sandwich panels under quasi-static and projectile loading’, Key Eng Mater, 1988 141–143 501–52. 2 Reddy T Y, Wen H M, Reid S R and Soden P D, ‘Penetration and perforation of composite sandwich panels by hemispherical and conical projectiles’, Trans ASME, J Pres Ves Technol, 1988 120 186–94. 3 Reid S R, Wen H M, Soden P D and Reddy T Y, ‘Response of single skin laminates and sandwich panels to projectile impact’, in Composite Materials for Offshore Operation – 2, (S S Wang, J J Williams and K H Lo, eds), pp 593–617. American Bureau of Shipping, 1999. 4 Abrate S, ‘Impact on laminated composite materials’, Appl Mech Rev, 1991 44(4) 155–90. 5 Abrate S, ‘Impact on laminated composites: recent advances’, Appl Mech Rev, 1994 47(11) 517–43. 6 Rutherford K L, ‘Indentation and penetration resistance of composite materials to pointed projectiles’, unpublished UK DRA Report, 1992. 7 Zhao Y, Pang S S and Griffin S A, ‘Force-indentation study of transversely isotropic composite materials using a conical-tip indenter’, Composites Eng, 1991 1(6) 393–402. 8 Greaves L J, ‘Failure mechanisms in GFRP armour’, unpublished UK DRA Report, 1992. 9 Greaves L J, ‘Progress in modelling the perforation of GFRP by ballistic projectiles’, unpublished UK DRA Report, 1994. 10 Reid S R, Reddy T Y, Ho H M, Crouch I G and Greaves L J, ‘Dynamic indentation of thick fibre-reinforced composites’, in High Rate Effects on Polymer, Metal and Ceramic Matrix Composites and Other Advanced Materials (Y D S Rajapakse and J R Vinson, eds), AD-Vol 48 ASME, 71–9, 1995. 11 Zhu G, Goldsmith W and Dharan C K H, ‘Penetration of laminated Kevlar by projectiles – I. Experimental investigation’, Int J Solids Struct, 1992 29(4) 399–420. 12 Zhu G, Goldsmith W and Dharan C K H, ‘Penetration of laminated Kevlar by projectiles – II. Analytical model’, Int J Solids Struct, 1992 29(4) 421–36. 13 Lee S-W R and Sun C T, ‘Dynamic penetration of graphite/epoxy laminates impacted by a blunt-ended projectile’, Composites Sci Technol, 1993 49 369– 80. 14 Mines R A W, Roach A M and Jones N, ‘High velocity perforation behaviour of polymer composite laminates’, Int J Impact Eng, 1999 22 561–88. 15 Moriarty K and Goldsmith W, ‘Dynamic energy absorption characteristics of sandwich shells’, Int J Impact Eng, 1993 13(2) 293–317. 16 Goldsmith W and Sackman J L, ‘An experimental study of energy absorption in impact on sandwich plates’, Int J Impact Eng, 1992 12 241–61. 17 Evans K E, ‘Design of doubly curved sandwich panels with honeycomb cores’, Composite Struct, 1990 17 95–111. 18 Allen H G, Analysis and Design of Sandwich Structures, Oxford, Pergamon Press, 1969. 19 Vinson J R, ‘Optimum design of composite sandwich panels subjected to uniaxial compression’, AIAA J, 1988 24 1690–6.

IBF8 11/22/2000 6:52 PM Page 279

Perforation of FRP laminates and sandwich panels subjected

279

20 Bernard M L and Lagace PA, ‘Impact resistance of composite sandwich panels’, J Reinforced Plastic Composites, 1989 8 432–45. 21 Kosza P and Sayir M B, ‘Failure patterns in the core of sandwich structures under impact loading’, Int J Impact Eng, 1994 15(4) 501–17. 22 Wen H M and Jones N, ‘Semi-empirical equations for the perforation of plates by a mass’, in Structures Under Shock and Impact – II, (P S Bulson, ed), pp 369–80. Computational Mechanics Publications, Southampton and Boston, Thomas Telford, London, 1992. 23 Wen H M, ‘Predicting the penetration and perforation of FRP laminates struck normally by a projectile with different noseshapes’, Composite Structures, 2000 49 321–9.

IBF9 11/22/2000 6:57 PM Page 280

9 High-velocity impact damage to polymer matrix composites R C TENNYSON AND C G LAMONTAGNE

9.1

Introduction

One of the major concerns involving the use of light-weight fibre-reinforced composites is their susceptibility to impact damage. Delamination (or interlaminar fracture), surface spallation and laminate penetration constitute various modes of failure resulting from impact loads. Low-velocity impacts are associated with delamination damage, especially that caused by bluntheaded projectiles. This inter-laminar debonding primarily reduces the local bending stiffness and thus can affect the bending and buckling behaviour of the structure. In the latter case, local buckling can induce further delamination growth which can lead to overall global weakening of the structure. Such damage has been reported to cause as much as a 40% reduction in static and fatigue strength.1,2 Low-velocity impacts have also been shown to reduce cylindrical shell buckling strengths by as much as 25 ~ 35%.3 As impact energy is increased, delamination coupled with surface spallation can occur, followed by penetration of the laminate. Figure 9.1 shows photomicrographs of front and rear face spallation damage to a graphite/PEEK laminate. An enlarged view of the damage associated with surface spallation and through-thickness delamination can be seen in Fig. 9.2. The ‘ballistic limit’ defines that energy which is required for a projectile to penetrate to the rear face of the laminate. Such cases are characterised by front face spallation, localised delamination below the surface (easily detected by ultrasonic C-scan) and an ‘impact hole’ just reaching the rear face. Beyond the ballistic limit, higher energy impacts produce all of the above features coupled with a crater hole, rear face spallation and ejecta plumes emanating from both sides of the laminate. Figure 9.3 presents photomicrographs of a crater hole viewed from the front and rear faces of a graphite/epoxy tube due to an actual micrometeoroid hypervelocity impact recorded on an experiment aboard a NASA satellite (LDEF, 1984–1990). Again, spallation damage is visible. 280

IBF9 11/22/2000 6:58 PM Page 281

High-velocity impact damage to polymer matrix composites

9.1 Impact damage on front/back faces.

281

IBF9 11/22/2000 6:58 PM Page 282

282

Impact behaviour of composite materials and structures

9.2 Impact damage on back face and through-thickness of graphite/epoxy laminate.

IBF9 11/22/2000 6:58 PM Page 283

High-velocity impact damage to polymer matrix composites

283

9.3 SEM Photographs of micrometeoroid/debris impact/exit holes for graphite/epoxy tube (SP-288/ T300, [±43°]4s).

IBF9 11/22/2000 6:58 PM Page 284

284

Impact behaviour of composite materials and structures

One of the dangerous features of hypervelocity impact is the debris plume emanating from the rear face. These ejecta particles can impact adjacent structures and components within the interior of the impacted structure. This of course includes human occupants residing inside a containment vessel such as the cylindrical habitat structures of the International Space Station (ISS), presently being deployed over the next several years. The ejecta from such hypervelocity impacts (i.e. at typical orbital velocities ≥7 km s-1) also travel at comparable speeds and can thus penetrate other structures causing much enhanced damage.4 Whereas the hypervelocity impacting particle produces an irregular shaped ‘hole’ or crater (typically 2.5–3 times larger than the particle diameter) on first hitting a laminate, the subsequent fracture of the particle and composite material at the impact site results in a debris plume containing 10–100 fold more particles that spread in a spherical or tear-drop pattern. Depending on the distance traveled and ‘cone’ angle, these particles produce an impact pattern and damage zone many times larger than the original crater. For composite shell structures, this secondary damage from the debris plume can lead to major structural failure.4 Hypervelocity impact conditions are most likely to occur on spacecraft in low earth orbit (LEO, 200–1000 km altitude). They are vulnerable to impact damage resulting from collisions with natural micrometeoroids (£1 cm diameter) and orbital debris (known as the MOD environment). Micrometeoroids originate from planetary or asteroidal collisions and cometary ejecta. Artificial space debris consists of everything from spent satellites and rockets to aluminum oxide fuel particles, paint chips and fragmentation objects from collisions of these bodies in orbit. A plot of the MOD environment as a function of altitude and particle size is presented in Fig. 9.4. This chart does not depict the enhanced micrometeoroid fluxes that occur when the earth passes through periodic ‘showers’ that can produce flux increases of 5–10 times that of the ‘natural’ background. In some isolated cases, these fluxes can reach as high as 105 times the background (such as the Leonid meteor storms in November 1998 and 1999). Fibre-reinforced polymer matrix composites are used extensively in spacecraft structures and satellite components such as antenna struts, panels and low distortion frames. The largest composite structure in space is the Canadian robot arm mounted on all of the Space Shuttles. A much more complex robot consisting of graphite IM7/PEEK cylinders has been assembled for the ISS Remote Manipulator System. Perhaps the greatest spacecraft application of composites is the Iridium telecommunications satellite constellation currently in orbit (~66 satellites) which employs carbon/epoxy laminates on the satellite exterior panels. Clearly, with the high cost of replacement of spacecraft, and particularly with the presence of humans in

IBF9 11/22/2000 6:58 PM Page 285

High-velocity impact damage to polymer matrix composites

285

1e3 1e2

Particle flux (#/m2 yr)

1e1 1e0 1e-1 Debris altitude (km)

1e-2 1e-3 1e-4 1e-5

100

0

Micrometeoroids 100–1000 km altitude

500 400 300

1e-6

100

1e-7 1e-8 0.001

0.01

0.1

1

10

Particle diameter (cm)

9.4 Micrometeoroid and orbital debris flux as a function of altitude (NASA CR # BB000883A, January 1991).

some cases, it is essential that the effects of hypervelocity impacts on materials and structures must be understood in order to evaluate risks and provide for the safe and reliable design of these systems. This is particularly true for composite materials where the data base is scarce and their utilisation is increasing. This chapter reviews hypervelocity impact damage to composites, with special emphasis on test data obtained on graphite epoxy and PEEK laminates. Sufficient data have been obtained to provide some insight on the major parameters governing the initial impact and debris damage that occurs.

9.2

Hypervelocity impact (HVI) tests on composites

Studies of HVI damage to composite materials and structures can be classified into three categories: flat plate laminates, tubes/cylinders, and composite laminate/sandwich structures. In the first category, a large number of graphite/epoxy, graphite/PEEK and Kevlar®/epoxy laminates have been investigated.5–13 Early work by Yew et al.5,6 on graphite/epoxy plates was done at the NASA Johnson Space Center (JSC), USA using their light gas gun facilities. A wide range of plate thicknesses was studied, including quasi-isotropic configurations. Later, Christiansen13 reported on a more detailed series of tests in which both high and low modulus graphite/epoxy laminates were tested, including tubes. Again, various target thicknesses were used and different impact angles

IBF9 11/22/2000 6:58 PM Page 286

286

Impact behaviour of composite materials and structures

employed. It was found that fibre modulus has a greater effect than lay-up. Lower energy impact tests were conducted on both graphite/epoxy and PEEK laminates,8 but the parametric range was small. A subsequent study focusing on PEEK/IM7 and AS-4 flat plates was reported,9 where varying thickness laminates of different lay-ups were tested. These experiments were conducted at JSC covering a wide range of projectile energies, including some cylinder tests as well. Most of the data reported to-date are for normal impact conditions, although some results have been obtained for oblique angles.12,13 In Lamontagne et al.,12 the experiments were undertaken at the University of Kent, UK using their light gas gun. It was observed that for oblique angle impacts, the debris cloud does not follow the line of flight of the projectile. Moreover, the cone angle associated with the debris cloud is not symmetric about the projectile impact velocity vector. Design charts derived from much of the test data reported in the above references will be described later. In comparison, HVI tests on composite tubes and cylinders are few in number.13–16 Of particular interest in these studies is the effect of the debris plume on the damage to the opposing wall. As noted earlier, the energy associated with the ejecta particles at orbital impact velocities is sufficiently high that structural failure of a cylinder under compressive loading can occur when the damage zone is large enough.4 Studies of HVI damage to composite laminate/sandwich panels have been reported for honeycomb17–20 and various heat shield materials.21 An extensive data base has been compiled for normal and oblique impacts on honeycomb/woven carbon fibre/epoxy structures.20 This data has been used to determine the ballistic limit which showed a strong dependence on impact angle. Additional data were published21 for graphite/epoxy laminates bonded to different types of heat shield material combinations subjected to normal hypervelocity impact conditions. Substantial data were obtained on the correlation of entry hole size and impactor energy. This chapter focuses on HVI damage to composite laminates only, with special emphasis on graphite/epoxy and PEEK materials.

9.3

Entry impact damage

The entry crater or hole size produced by the impact of a particle with a composite laminate can be correlated with the parameter (as suggested by Christiansen13) [Etrt/Dprp]1/3 where E is the projectile’s energy (J), t is the target thickness (mm), Dp is the projectile diameter (mm), rt and rp are the densities of the target and projectile, respectively.The entry crater is defined as Dc which is the equivalent diameter of a circle that encompasses the same area as the irregularly shaped hole. The projectile energy E is calculated as 1/2 m V n2 where Vn is the normal velocity component of the projectile

IBF9 11/22/2000 6:58 PM Page 287

High-velocity impact damage to polymer matrix composites Auburn GRE (SiC)

Auburn PEEK (SiC)

JSC PEEK (Al)

SwRl PEEK (Al)

USAF #1 PEEK (Al/Nylon)

Austin GRE (Al)

Eagle GRE (low E & Al)

USAF PEEK #2 (steel)

MSFC PEEK (Al)

SSRMS PEEK (Al)

UKC PEEK (Al)

Regression

287

Crater diameter (mm)

25 20 15 10 D c = 1.05

3

E

t rt Dp r p

5 0 0

5

10 3

15 t rt E Dp r p

20

[ J] 3

9.5 Equivalent crater diameter as a function of impact energy parameter.

velocity V and is given by V cos q, where q is the angle of V relative to the surface normal. Based on the AS-4 and IM7graphite/PEEK laminate test data described in Tennyson and Shortliffe,4,11 Fig. 9.5 illustrates the correlation between Dc and the energy parameter using a regression line forced to pass through zero. A variety of laminate lay-ups and thicknesses were tested under normal impact conditions using aluminum spheres of different diameters. Included in this plot are test results on AS-4graphite/PEEK cylinders16 and graphite/epoxy plates.13,8,5 In the latter case, some data from unpublished contract reports are also included. These results were obtained for a broad range of projectile diameters (0.4–9.13 mm), travelling at velocities from 4 to 7.5 km/s, for a variety of materials including glass, nylon, steel and SiC. More recent oblique angle impact tests were conducted on AS-4 graphite/PEEK flat plate laminates12 of different thicknesses using aluminum spheres of diameter 1–2 mm over a velocity range of 4.5–5.5 km/s. Impact angles of 0°, 30° and 45° were investigated. These results (UKC) are also plotted in Fig. 9.5 where it can be seen that reasonable correlation with normal impact data was found based on the normal velocity component.

IBF9 11/22/2000 6:58 PM Page 288

288

Impact behaviour of composite materials and structures

NASA JSC HIT-F shot #A2704 Target: SSRMS boom #1 Projectile diameter: 3.2 mm Velocity: 6.4 km s -1 Impact angle: 0°

9.6 Photograph of crater and front face spallation damage due to hypervelocity impact on graphite/PEEK laminate.

From a structural design point of view, the entry damage on the front face is an important parameter for assessing the overall reduction in stiffness, strength or long-term fatigue life due to crack propagation from this damaged region. The entry damage zone includes the crater hole and associated delamination/surface cracking area, as can be seen in the photograph shown in Fig. 9.6. As in the case of the hole diameter calculation, this region can also be defined by an ‘equivalent entry damage diameter’ parameter. Using earlier data,4,8,11 the entry damage diameter is plotted as a function of a reduced energy parameter in Fig. 9.7. Included in this graph is the regression curve based on C-scan measurements of the sub-surface damage zones. It can be seen that even though the delamination lies below the surface, the enhanced area is only about 20% greater than the visible surface area. To estimate probable damage for a given projectile impactor size, it is

IBF9 11/22/2000 6:58 PM Page 289

High-velocity impact damage to polymer matrix composites Auburn GRE (SiC)

Auburn PEEK (SiC)

JSC PEEK (AI)

SwRI PEEK (AI)

USAF #1 PEEK (AI/SiC)

Regression

C-Scan regression

UKC PEEK (AI)

289

Entry damage diameter (mm)

50 40 D C -scan = 4.043 E 30

t Dp

20 Dentry damage = 3.733 E 10

t Dp

0 0

2

4 3

E

6 t Dp

8

10

[ J] 3

9.7 Equivalent entry damage diameter as a function of impact energy parameter (visible and C-Scan).

useful to correlate the measured crater diameters with the known impactor diameters. Figure 9.8 presents this plot based on the above experiments. The regression curve was constructed only through the PEEK data. There appears to be no energy dependence when one considers complete penetration tests. However, for projectile diameters below 1 mm, it is apparent that the hole diameter can be taken as equal to the particle diameter. Rear face spallation damage on the impacted laminate is also an important parameter for assessing overall entry damage. Using the same data base, Fig. 9.9 illustrates the correlation of the equivalent damage diameter with the reduced energy parameter. The regression analysis indicates that this damage area is comparable to that observed on the front face for a given energy parameter.

9.4

Secondary debris cloud

Once the projectile has impacted and penetrated the laminate, two debris clouds are formed. These clouds or plumes of ejecta, formed by the disintegration of the wall material and the projectile, emanate from both the front and rear faces of the laminate. For high-velocity impacts, it has been found that the velocity of the ejecta is comparable to that of the impactor

IBF9 11/22/2000 6:58 PM Page 290

290

Impact behaviour of composite materials and structures

Auburn GRE (SiC)

Auburn PEEK (SiC)

JSC PEEK (Al)

SwRl PEEK (Al)

USAF #1 PEEK (Al/nylon)

Austin GRE (Al)

Eagle GRE (low E & Al)

Regression

UKC PEEK (Al)

Crater diameter (mm)

10 8 6 4 Dc = 2.67Dp 2 0 0

0.5

1

1.5 2 Projectile diameter (mm)

2.5

3

9.8 Equivalent crater diameter as a function of projectile diameter.

JSC PEEK (AI)

SwRI PEEK (AI)

Regression

UKC PEEK (AI)

USAF #1 PEEK (AI/SiC)

Spall damage diameter (mm)

30 25 20 15 10 Dspall = 3.123 E 5

t Dp

0 0

2

4 3

E

6 t Dp

8

10

[ J] 3

9.9 Equivalent rear face spall diameter as a function of impact energy parameter.

IBF9 11/22/2000 6:58 PM Page 291

High-velocity impact damage to polymer matrix composites

291

for the range of parameters studied.16 Consequently, the ejecta energy in the secondary debris cloud emanating from the rear face can be sufficiently high as to penetrate another adjacent composite laminate. Depending on the separation distance and the plume cone angle, damage areas much larger than the impact crater hole can occur. To demonstrate this process, consider the high speed photographs (Fig. 9.10) of an aluminum projectile (~9 mm diameter) impacting a composite cylindrical shell constructed of IM7/PEEK material, 19 plies thick (~2.7 mm) and 33 cm in diameter. The cylinder is a symmetric, balanced laminate (+/-43° with a single 0° centre ply). A Cordin high speed camera capable of snapping 80 frames over an elapsed time of 100 ms was used to record this impact.16 These frames show the early formation of the debris cloud and the subsequent growth of the spherical shaped plume of ejecta. Impact of the debris cloud with the rear wall of the cylinder results in the large damage area visible in the photograph of Fig. 9.11. Analysis of the debris plume velocity reveals that the cloud tip travelled at approximately the same velocity as the projectile. The damage resulting from this debris cloud impact (Fig. 9.11) contains many holes in the rear wall. This region is defined by a 200 mm diameter circle, thus yielding a damage cone angle of ~69.5°. Because of the multiple penetrations, cracks and spallation damage, the cylinder can be regarded as having a circular ‘cutout’ for structural analysis purposes. Analysis performed4 showed a compressive buckling strength loss for this cylinder of over 50%. Similar results were found in the flat plate IM7/PEEK tests.11 Using composite witness plates located 330 mm behind the primary impact sites, detailed mapping of the major debris impacts was performed to evaluate the ejecta plume damage and cone angles associated with the various laminate configurations tested. A plot of the semi-angles is presented in Fig. 9.12 as a function of the energy parameter. It is apparent that an average semi-cone angle of ~12.3° can be attributed to these experiments. Figure 9.13 depicts a schematic of one such plume impact where 87 craters were counted within a 120 mm diameter circle. The fact that these craters define holes in the laminate with associated spallation damage testifies to the ejecta energy. The typical projectile used in these tests was 2 mm in diameter and traveled at 6–7 km s-1. A series of oblique angle impact tests were conducted on 16 and 24-ply AS-4/PEEK plates12 to investigate plume damage using aluminum projectiles (1 and 2 mm in diameter) at velocities of 4.5–5.5 km/s. Analysis of the debris cloud impacts on adjacent aluminum witness plates showed that in fact there are two classes of damage. A primary damage zone was identified by large craters associated with projectile fragments, with a secondary area containing a larger number of smaller craters having carbon fibres imbedded in the aluminum plate. Figures 9.14 and 9.15 illustrate the

IBF9 11/22/2000 6:58 PM Page 292

292

Impact behaviour of composite materials and structures

9.10 High speed photographs of debris plume from hypervelocity impact on graphite/PEEK cylinder.

primary (a) and secondary (b) damage cone angles for normal and oblique impacts, respectively. In the latter case, the debris cloud exiting from the rear face of the laminates does not follow the line of flight of the projectile. Thus, a ‘turning’ angle (e) was defined as the angle between the initial

IBF9 11/22/2000 6:58 PM Page 293

High-velocity impact damage to polymer matrix composites

293

NASA JSC HIT-F shot #B934 Target: SSRMS boom #6 (Nextel AF-62 cable wrap) Projectile diameter: 9.13 mm Velocity: 6.55 km/s Impact angle: 0°

9.11 Photograph of crater, front face spallation and debris plume damage to rear wall due to hypervelocity impact on graphite/PEEK cylinder.

projectile velocity vector and the centre of mass of the primary damage zone (see Fig. 9.15). Furthermore, it was also observed that the primary and secondary cone angles for the oblique tests were not symmetric about the projectile flight line, thus accounting for the introduction of angles g and d in Fig. 9.15. Based on these experiments, a plot of the cone angles a and b are presented in Fig. 9.16 as a function of projectile impact angle. In addition, the cylinder secondary cone angle results are included for the normal impact case (~69.5°). In those experiments, one could not identify primary from secondary impacts. However, using the flat plate results from Fig. 9.12 for

IBF9 11/22/2000 6:58 PM Page 294

294

Impact behaviour of composite materials and structures

9.12 Plot of semi-cone angle of debris plume as a function of impact energy parameter.

87 distinct craters catalogued

Semi-cone angle = 11.6°

rinfluence ª 60 mm

9.13 Plot of secondary debris impact sites on flat plate.

IBF9 11/22/2000 6:58 PM Page 295

High-velocity impact damage to polymer matrix composites

295

Witness plate b a Primary damage cone Secondary damage cone

Guide rods

Target plate

Initial projectile vector

9.14 Schematic defining primary and secondary cone angles for debris plume (normal impact).

primary normal impacts (i.e. only those full penetration cases were plotted), an average primary cone angle of ~23.2° was also plotted. Thus, within the scatter indicated, all normal impact tests correlate reasonably well. Note that for the oblique tests on the 16-ply laminates using a 1 mm projectile, no evidence of primary impact debris was found. Figure 9.17 illustrates the variation of cone angles with the energy parameter using the normal projectile velocity component. Figure 9.18 presents a plot of the turning angle (e) as a function of the impact angle. For the limited data available, it appears that e is independent of ply thickness. This ‘turning’ effect, although small in magnitude, may well be important in predicting major impact damage relative to the location of critical spacecraft components and determining what protective measures it is necessary to implement.

9.5

Conclusions

This chapter presents an overview of high-velocity impact damage to composite laminates, with specific reference to test data obtained by UTIAS researchers using gun facilities at various laboratories in the USA and UK. Emphasis is placed on graphite/carbon fibre-reinforced epoxy/PEEK laminates of varying thickness and ply orientations. Where possible, pub-

IBF9 11/22/2000 6:58 PM Page 296

Witness plate

e

Center of mass, primary damage

Secondary damage cone

d

Primary damage cone

b Target plate

a g

Guide rods Initial projectile vector

9.15 Schematic defining oblique angle impact geometry associated with debris plume damage.

90 80

Cone angle (∞)

70 60 50 a, 16 ply, 1 mm a, 16 ply, 2 mm a, 24 ply, 2 mm b, 16 ply, 1 mm b, 16 ply, 2 mm b, 24 ply, 2 mm a, plate b, cylinder

40 30 20 10

0

10

20

30

40

50

Impact angle, qi (deg.)

9.16 Plot of primary and secondary debris cone angles for normal and oblique impacts on graphite/PEEK laminates.

IBF9 11/22/2000 6:58 PM Page 297

High-velocity impact damage to polymer matrix composites

297

90 80 70

Cone angle (∞)

60

b = 59.92E ¢ -164.72E ¢ 2 +182.41E ¢3 - 90.03E ¢ 4 +16.49E ¢5

50 40 30 a = -87.74E ¢ + 189.07E ¢ 2 -129.45E ¢3 + 29.02E ¢4

20

a b

10 0 2.2

3.2

4.2

(E ¢t

Dp )

(1/3 )

5.2

6.2

1/3

(J )

9.17 Plot of primary and secondary debris cone angles as a function of impact energy parameter.

14 16 ply 24 ply

12

Turning angle, e (∞)

10 8 e = 0.01e ( 0.16q ) i

6 4 2 0 0

10

20

30

40

50

Impact angle, qi (deg.)

9.18 Plot of primary turning angle as a function of impact angle.

IBF9 11/22/2000 6:58 PM Page 298

298

Impact behaviour of composite materials and structures

lished data from other researchers are included, although no results are presented on composite/sandwich construction. A variety of projectile materials are noted in the studies, but the bulk of the test data presented is based on aluminum spheres covering a wide range of impact energies. Most of the test results are derived from normal impact experiments, with a limited number of oblique tests also included. Despite the data base available from these studies, no predictive models are proposed. However, a number of observations can be made which might prove useful in the design of composite structures subject to hypervelocity impacts. First, a linear correlation of crater size and entry damage with an energy parameter has been established, which appears to be independent of laminate lay-up and valid for graphite/epoxy/PEEK materials. The damage resulting from secondary debris clouds has been amply demonstrated when the ejecta impact another laminate structure. Primary and secondary cone angles describing this debris plume have been identified for both normal and oblique angle impacts. Knowledge of the cone angles is essential in predicting the size of the plume impact area on adjacent structures. It has been shown that the energy of the debris particles can be sufficiently high as to result in major structural damage. Future research is necessary to enhance the data base, particularly for oblique impacts, and to develop predictive models capable of analysing the damage resulting from hypervelocity impacts on composite structures.

Acknowledgements The authors wish to acknowledge the significant contributions to the research referenced in this work by Mr G Shortliffe, Mr G Manuelpillai and Dr E A Taylor. It would have been impossible to undertake these studies without the collaboration of Dr J Crews, Dr E Christiansen, Mr J Kerr of the NASA Johnson Space Center, USA; Dr A Nolan of the NASA Marshall Space Flight Center, USA; and Dr J A M Mcdonnell of the University of Kent at Canterbury, UK.

References 1 Christoforou A P and Swanson S R, ‘Strength loss in composite cylinders under impact’, Trans ASME, 1988 110(2) 180–4. 2 Poe C C and Illg W, ‘Strength of a thick graphite/epoxy rocket motor case after impact by a blunt object’, 1987, NASA TM 89099. 3 Tennyson R C and Krishna Kumar S, ‘Delamination damage and its effect on buckling of laminated cylindrical shells’, AGARD Conf. Proc 530, Debonding/Delamination of Composites, 1989. 4 Tennyson R C and Shortliffe G, ‘MOD impact damage on composite materials in space’, Proc 7th Inter Symp, SP-399, Materials in Space Environment, 1997.

IBF9 11/22/2000 6:58 PM Page 299

High-velocity impact damage to polymer matrix composites

299

5 Yew C H, Yang C Y and Crews J, ‘A phenomenological study of the effect of hypervelocity impacts on graphite/epoxy plates’, Engineering Mechanics, University of Texas at Austin, and NASA JSC, 1986. 6 Yew C H and Kendrick R B, ‘A study of damage in composite panels produced by hypervelocity impact’, Int J Impact Eng, 1987. 7 Schonberg W P, ‘Hypervelocity impact response of spaced composite material structures’, Int J Impact Eng, 1990. 8 Tennyson R C, Manuelpillai G and Zimcik D G, ‘Model for predicting micrometeoroid/debris impacts and damage to composite materials’, 1st Eur Conf Orbital Debris SD-01, 1993. 9 Tennyson R C and Manuelpillai G, ‘Prediction of space hypervelocity impact damage in composite materials’, 8th CASI Conf Astronautics, 1994. 10 Silvestrov V V, Plastinin A V and Gorshkov N N, ‘Hypervelocity impact on laminate composite panels’, Int J Impact Eng, 1995. 11 Tennyson R C and Shortliffe G, ‘Hypervelocity impact damage to composite structures’, 1st Int Conf Composite Science and Technology, 1996. 12 Lamontagne C G, Manuelpillai G N, Taylor E A and Tennyson R C, ‘Normal and oblique hypervelocity impacts on carbon fibre/PEEK composites’, Proc Hypervelocity Impact Symp, 1998, Int J Impact Eng, 1999. 13 Christiansen E L, ‘Investigation of hypervelocity impact damage to space station truss tubes’, Int J Impact Eng, 1990. 14 Unda J, Weisz J, Uriarte A and Capitano R S, ‘Residual strength of CFRP tubes subjected to hypervelocity debris impact’, 45th Congr of the IAF, 1994. 15 Yasaka T, Meguro A and Watanabe M, ‘Debris impact damage and fragmentation of antenna structure in geostationary orbit’, 45th Congr of the IAF, 1994. 16 Shortliffe G D and Tennyson R C, ‘Hypervelocity impact tests on composite boom structures for space robot applications’, J Can Aeronauti Space Inst, 1997. 17 Taylor E A, Herbert M K, Gardner D J, Thomson R and Burchell M J, ‘Hypervelocity impact on spacecraft carbon fibre-reinforced plastic/aluminum honeycomb’, Proc Inst Mech Eng, 1997 211. 18 Taylor E A, Herbert M K and Kay L, ‘Hypervelocity impact on carbon fibrereinforced plastic/aluminum honeycomb at normal and oblique angles’, Proc 2nd Eur Space Debris Conf, ESA SD-02, 1997. 19 Frost C L and Rodriguez P I, ‘AXAF hypervelocity impact test results’, Proc 2nd Eur Space Debris Conf, ESA SD-02, 1997. 20 Taylor E A, Herbert M K, Vaughan A M and Mcdonnell J A M, ‘Hypervelocity Impact on carbon fibre-reinforced plastic/aluminum honeycomb: comparison with Whipple bumper shields’, Proc Hypervelocity Impact Symp, 1998. 21 Robinson J H, ‘Orbital debris impact damage to reusable launch vehicles’, Proc Hypervelocity Impact Symp, 1998.

IBF9 11/22/2000 6:58 PM Page 300

IBFINDEX 11/22/2000 7:03 PM Page 301

Index

accelerometer, 244 acoustic techniques backscattering, 51 emission, 60 microscopy, 52 adhesive bonding, 92–3 aerospace application, 280 ballistic, 266, 280 ballistic limit, 232, 255 barely visible impact damage, see damage beam, 9, 91 beam theory, 20 boundary conditions clamped, 123, 139, 194, 224, 242 simply supported, 189 brittle behaviour, 12, 17 buckling, 160–2 C-scan graph, 14, 150 carbon/epoxy, 17, 33, 86, 123, 197, 285 carbon/PEEK, 123 Charpy impact test, 9 classical plate theory, 189, 221 compression after impact (CAI) strength, see residual compressive strength compression after impact test, 123, 141 contact stiffness, 187–8 crater diameter, 287 critical strain energy release rate, 3–4, 102, 126, 159 cross-sectional micrograph, 36, 59, 281–3 crush strength, 26 damage, 6–8, 114 curing effects, 56–8 detection, 33, 140 indentation, 140, 231, 251 lay-up effects, 54 map, 37, 122, 151 measures, 169 mechanisms, 7, 148, 228–32, 246–63, 280–4

mechanics, 116 modelling, 99, 116 prediction, 114–23 source, 109 tolerance, 107, 160 tolerance assessment, 163, 172 damage tolerant structural design, 111 de-bonding, 7, 110, 255, 280 debris, 289 deflection-time curve, 97, 118, 199 delamination, 7, 33, 91–5, 148, 228, 258, 280–5 depth, 54 extent, 35–6, 54 propagation, 57, 151–9, 230 shape, 35, 150 de-ply technique, 34, 41 destructive techniques, 34, 140 drop weight impact test, 94, 123, 138, 186, 252 ductility index, 13 durability, 108 dynamic enhancement factor, 260 dynamic fracture, 1, 75 energy absorption, 13, 157, 220, 263 balance, 21, 157, 263 Charpy impact, 3 fracture, 21–2 perforation, 100, 246–66 entry diameter, see crater diameter failure criterion, 101 indentation, see damage modes, 6–7, 162 falling dart, see drop weight impact test fibre optics, 66 finite element modelling, 100, 117 foam core, 242 force-time curve, 96, 121, 144, 225–9

301

IBFINDEX 11/22/2000 7:03 PM Page 302

302

Index

fracture energy, see energy fracture mechanics, 22, 102 fracture toughness, 24 gas gun, 215, 245, 285 glass/epoxy, 17, 86 glass/phenolic, 133 glass/polyester, 133, 242 glass transition temperature, 2, 7 graphite/epoxy, 214, 285 graphite/PEEK, 285 Hertz contact law, 188, 224 high velocity impact, 212, 239 hybrid laminates, 87 hypervelocity impact, 285 impact damage, see damage damage resistance, 143 energy, see kinetic energy force ratio, 176–81 mass effects, 152 parameters, 134, 286 pre-stressed materials, 16 response, 91, 94, 143, 221 stress analysis, 91, 186 strength, 9 velocity effects, 153–4, 233, 254 impactor ball, 197 conical, 242–6 flat-ended, 139, 242–6 hemispherical, 242–6 wedge-ended, 95 incident kinetic energy, see kinetic energy indentation plates, 137 sandwich panels, 246 indentor conical, 251 flat-ended, 138, 246 hemispherical, 250 inertia effect, 152, 263 infrared thermography, 64 in-plane tests compression, 77 shear, 80 tension, 79 interface effect, 91 Izod impact test, 9

low velocity impact, 94, 123, 138, 186, 252 mass effects, see impact mass effects mechanical properties Aramid/epoxy, 4 carbon/epoxy, 4, 86, 197 carbon/glass hybrid, 86 E-glass/epoxy, 4, 86 E-glass/polyester, 137, 243 fibres, 2–3 foam core, 243 resins, 2–3 S-glass/phenolic, 137 membrane effect, 157 micromechanics, 19, 21 military application, 133 missile impact, 239 model development, 125, 263 nondestructive techniques, 33, 140, 214 nose shape, see impactor, indentor and projectile notch sensitivity, 10–12 oblique angle impact tests, 291 offshore application, 239 panel failure modes, 162 penetration process, 251 perforation, 232, 254, 283 plates circular, 137 diameter effect, 156 rectangular, 214 square, 197, 242 prediction of impact energy, 19 projectile characteristics, 96, 290 conical, 245 flat-ended, 245 gelatine pellet, 14 hemispherical, 215, 245 sphere, 14, 287 punch, see indentor quasi-static approximation, 204–7 tests, see indentation

Kevlar/epoxy, 285 kinetic energy, 21, 97, 287 kink shear band, 164–7

residual compressive properties, 113–14 stiffness, 175 strength, 16, 57, 115, 126, 170 residual impact velocity, 269

laser holography, 61 laser Doppler anemometry, 214–15 loading rate effect, see impact velocity effects

sandwich panels, 239 scaling, 99–100, 209 sensitivity of inspection techniques for impact damage, 68

IBFINDEX 11/22/2000 7:03 PM Page 303

Index shear out, 145–50 shearography, 63 skins, 242 spalling, 230, 290 split Hopkinson bar, 76–8 spring mass model, 204 stiffness retention factor, 127, 175 strain-gauged load cell, 95, 140 strain-time response, 146, 193–209 strain rate effects, 82 strain retention factor, 173–4 strength retention factor, 58, 165 stress-strain curve, 83–8, 244–5 striker, see impactor and projectile tap test, 38 terminal velocity, 233 thickness effects, 155, 253–7 threshold absorbed energy, 159 impact force, 156, 158, 171

impact velocity, 230 kinetic energy, 57, 145, 152–4 stiffness, 175 through-thickness tests compression, 81 interlaminar shear, 181 tension, 81 tube, 197, 287 tup, see impactor ultrasonic, 47 A-scan, 49 B-scan, 49 C-scan, 49, 140 wave propagation, 47, 77, 186, 266 weave pattern, 83–4, 135 woven fabrics, 82–3, 135 X-radiography, 39, 45

303

Our partners will collect data and use cookies for ad personalization and measurement. Learn how we and our ad partner Google, collect and use data. Agree & close